# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2024

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Sm2Mn074Ga51Ge09split
_database_code_depnum_ccdc_archive 'CCDC 2302493'
loop_
_audit_author_name
_audit_author_address
'Roman Khalaniya'
;Lomonosov Moscow State University
Russia
;
_audit_update_record             
;
2023-12-07 deposited with the CCDC.	2023-12-13 downloaded from the CCDC.
;
#=======================================================================

_audit_creation_method           'Jana2006 Version : 15/02/2021'

#=======================================================================

# 4. CHECKCIF RESPONSE 

# start Validation Reply Form

#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        Sm2Mn0.74Ga5.1Ge0.9
_chemical_name_common            ?
_chemical_formula_moiety         'Sm2 Mn0.736 Ga5.1 Ge0.9'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'Ga5.1 Ge0.9 Mn0.736 Sm2'
_chemical_formula_weight         762.1
_chemical_melting_point          ?
_chemical_compound_source        ?
_chemical_absolute_configuration .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'F m -3 m'
_symmetry_space_group_name_Hall  '-F 4;2;3'
_symmetry_Int_Tables_number      225

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -x,y,-z
4 x,-y,-z
5 z,x,y
6 z,-x,-y
7 -z,-x,y
8 -z,x,-y
9 y,z,x
10 -y,z,-x
11 y,-z,-x
12 -y,-z,x
13 y,x,-z
14 -y,-x,-z
15 y,-x,z
16 -y,x,z
17 x,z,-y
18 -x,z,y
19 -x,-z,-y
20 x,-z,y
21 z,y,-x
22 z,-y,x
23 -z,y,x
24 -z,-y,-x
25 -x,-y,-z
26 x,y,-z
27 x,-y,z
28 -x,y,z
29 -z,-x,-y
30 -z,x,y
31 z,x,-y
32 z,-x,y
33 -y,-z,-x
34 y,-z,x
35 -y,z,x
36 y,z,-x
37 -y,-x,z
38 y,x,z
39 -y,x,-z
40 y,-x,-z
41 -x,-z,y
42 x,-z,-y
43 x,z,y
44 -x,z,-y
45 -z,-y,x
46 -z,y,-x
47 z,-y,-x
48 z,y,x
49 x,y+1/2,z+1/2
50 -x,-y+1/2,z+1/2
51 -x,y+1/2,-z+1/2
52 x,-y+1/2,-z+1/2
53 z,x+1/2,y+1/2
54 z,-x+1/2,-y+1/2
55 -z,-x+1/2,y+1/2
56 -z,x+1/2,-y+1/2
57 y,z+1/2,x+1/2
58 -y,z+1/2,-x+1/2
59 y,-z+1/2,-x+1/2
60 -y,-z+1/2,x+1/2
61 y,x+1/2,-z+1/2
62 -y,-x+1/2,-z+1/2
63 y,-x+1/2,z+1/2
64 -y,x+1/2,z+1/2
65 x,z+1/2,-y+1/2
66 -x,z+1/2,y+1/2
67 -x,-z+1/2,-y+1/2
68 x,-z+1/2,y+1/2
69 z,y+1/2,-x+1/2
70 z,-y+1/2,x+1/2
71 -z,y+1/2,x+1/2
72 -z,-y+1/2,-x+1/2
73 -x,-y+1/2,-z+1/2
74 x,y+1/2,-z+1/2
75 x,-y+1/2,z+1/2
76 -x,y+1/2,z+1/2
77 -z,-x+1/2,-y+1/2
78 -z,x+1/2,y+1/2
79 z,x+1/2,-y+1/2
80 z,-x+1/2,y+1/2
81 -y,-z+1/2,-x+1/2
82 y,-z+1/2,x+1/2
83 -y,z+1/2,x+1/2
84 y,z+1/2,-x+1/2
85 -y,-x+1/2,z+1/2
86 y,x+1/2,z+1/2
87 -y,x+1/2,-z+1/2
88 y,-x+1/2,-z+1/2
89 -x,-z+1/2,y+1/2
90 x,-z+1/2,-y+1/2
91 x,z+1/2,y+1/2
92 -x,z+1/2,-y+1/2
93 -z,-y+1/2,x+1/2
94 -z,y+1/2,-x+1/2
95 z,-y+1/2,-x+1/2
96 z,y+1/2,x+1/2
97 x+1/2,y,z+1/2
98 -x+1/2,-y,z+1/2
99 -x+1/2,y,-z+1/2
100 x+1/2,-y,-z+1/2
101 z+1/2,x,y+1/2
102 z+1/2,-x,-y+1/2
103 -z+1/2,-x,y+1/2
104 -z+1/2,x,-y+1/2
105 y+1/2,z,x+1/2
106 -y+1/2,z,-x+1/2
107 y+1/2,-z,-x+1/2
108 -y+1/2,-z,x+1/2
109 y+1/2,x,-z+1/2
110 -y+1/2,-x,-z+1/2
111 y+1/2,-x,z+1/2
112 -y+1/2,x,z+1/2
113 x+1/2,z,-y+1/2
114 -x+1/2,z,y+1/2
115 -x+1/2,-z,-y+1/2
116 x+1/2,-z,y+1/2
117 z+1/2,y,-x+1/2
118 z+1/2,-y,x+1/2
119 -z+1/2,y,x+1/2
120 -z+1/2,-y,-x+1/2
121 -x+1/2,-y,-z+1/2
122 x+1/2,y,-z+1/2
123 x+1/2,-y,z+1/2
124 -x+1/2,y,z+1/2
125 -z+1/2,-x,-y+1/2
126 -z+1/2,x,y+1/2
127 z+1/2,x,-y+1/2
128 z+1/2,-x,y+1/2
129 -y+1/2,-z,-x+1/2
130 y+1/2,-z,x+1/2
131 -y+1/2,z,x+1/2
132 y+1/2,z,-x+1/2
133 -y+1/2,-x,z+1/2
134 y+1/2,x,z+1/2
135 -y+1/2,x,-z+1/2
136 y+1/2,-x,-z+1/2
137 -x+1/2,-z,y+1/2
138 x+1/2,-z,-y+1/2
139 x+1/2,z,y+1/2
140 -x+1/2,z,-y+1/2
141 -z+1/2,-y,x+1/2
142 -z+1/2,y,-x+1/2
143 z+1/2,-y,-x+1/2
144 z+1/2,y,x+1/2
145 x+1/2,y+1/2,z
146 -x+1/2,-y+1/2,z
147 -x+1/2,y+1/2,-z
148 x+1/2,-y+1/2,-z
149 z+1/2,x+1/2,y
150 z+1/2,-x+1/2,-y
151 -z+1/2,-x+1/2,y
152 -z+1/2,x+1/2,-y
153 y+1/2,z+1/2,x
154 -y+1/2,z+1/2,-x
155 y+1/2,-z+1/2,-x
156 -y+1/2,-z+1/2,x
157 y+1/2,x+1/2,-z
158 -y+1/2,-x+1/2,-z
159 y+1/2,-x+1/2,z
160 -y+1/2,x+1/2,z
161 x+1/2,z+1/2,-y
162 -x+1/2,z+1/2,y
163 -x+1/2,-z+1/2,-y
164 x+1/2,-z+1/2,y
165 z+1/2,y+1/2,-x
166 z+1/2,-y+1/2,x
167 -z+1/2,y+1/2,x
168 -z+1/2,-y+1/2,-x
169 -x+1/2,-y+1/2,-z
170 x+1/2,y+1/2,-z
171 x+1/2,-y+1/2,z
172 -x+1/2,y+1/2,z
173 -z+1/2,-x+1/2,-y
174 -z+1/2,x+1/2,y
175 z+1/2,x+1/2,-y
176 z+1/2,-x+1/2,y
177 -y+1/2,-z+1/2,-x
178 y+1/2,-z+1/2,x
179 -y+1/2,z+1/2,x
180 y+1/2,z+1/2,-x
181 -y+1/2,-x+1/2,z
182 y+1/2,x+1/2,z
183 -y+1/2,x+1/2,-z
184 y+1/2,-x+1/2,-z
185 -x+1/2,-z+1/2,y
186 x+1/2,-z+1/2,-y
187 x+1/2,z+1/2,y
188 -x+1/2,z+1/2,-y
189 -z+1/2,-y+1/2,x
190 -z+1/2,y+1/2,-x
191 z+1/2,-y+1/2,-x
192 z+1/2,y+1/2,x

_cell_length_a                   8.7126(3)
_cell_length_b                   8.7126(3)
_cell_length_c                   8.7126(3)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     661.37(4)

loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z            4

_cell_measurement_reflns_used    2654
_cell_measurement_theta_min      4.68
_cell_measurement_theta_max      55.47
_cell_measurement_temperature    100
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    7.6534
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             1317

_exptl_absorpt_coefficient_mu    43.138
_exptl_crystal_description       'rectangular cuboid'
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.1
_exptl_crystal_size_rad          ?
_exptl_crystal_colour            grey
_exptl_absorpt_correction_type   multi-scan,gaussian
_exptl_absorpt_process_details   
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_absorpt_correction_T_min  0.0047
_exptl_absorpt_correction_T_max  0.0242
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?

_diffrn_ambient_temperature      100
_diffrn_source                   ?
_diffrn_source_power             ?
_diffrn_source_voltage           ?
_diffrn_source_current           ?
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_detector                 ?
_diffrn_detector_area_resol_mean ?
_diffrn_measurement_method       'Bruker CCD'
_diffrn_measurement_specimen_support ?

_diffrn_reflns_number            3772
_diffrn_reflns_theta_min         4.05
_diffrn_reflns_theta_max         56.29
_diffrn_reflns_theta_full        56.29
_diffrn_measured_fraction_theta_max 0.98
_diffrn_measured_fraction_theta_full 0.98
_diffrn_reflns_av_R_equivalents  0.0774
_diffrn_reflns_av_unetI/netI     0.0341
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_reduction_process ?

_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?

_diffrn_radiation_probe          X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

_reflns_number_total             268
_reflns_number_gt                222
_reflns_threshold_expression     I>2σ(I)

_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0226
_refine_ls_wR_factor_gt          0.0245
_refine_ls_R_factor_all          0.0309
_refine_ls_wR_factor_ref         0.0257
_refine_ls_goodness_of_fit_ref   1.07
_refine_ls_goodness_of_fit_gt    1.13
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         268
_refine_ls_number_parameters     12
_refine_ls_number_restraints     0
_refine_ls_number_constraints    8
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0112
_refine_ls_shift/su_mean         0.0025
_refine_diff_density_max         2.43
_refine_diff_density_min         -2.03
_refine_ls_extinction_method     
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef       207(19)
_refine_ls_extinction_expression ?
_refine_ls_abs_structure_details ?
_refine_ls_abs_structure_Flack   ?
_refine_ls_abs_structure_Rogers  ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga 0.2307 1.6083 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Ge 0.1547 1.8001 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.3368 0.7283 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Sm -0.1638 3.4418 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?

loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?

loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?

loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sm1 Sm 0.25 0.25 0.25 Uani 0.00804(16) 8 1 d . . .
Mn1 Mn 0 0 0 Uiso 0.0086(4) 4 0.736(10) d . . .
Ga1 Ga 0.28453(13) 0 0 Uiso 0.00848(13) 24 0.657(3) d . . .
Ga1' Ga 0.2445(4) 0 0 Uiso 0.00848(13) 24 0.193(3) d . . .
Ge1 Ge 0.28453(13) 0 0 Uiso 0.00848(13) 24 0.1160(5) d . . .
Ge1' Ge 0.2445(4) 0 0 Uiso 0.00848(13) 24 0.0340(5) d . . .


loop_
_jana_atom_site_ADP_C_label
_jana_atom_site_ADP_C_type_symbol
_jana_atom_site_ADP_C_111
_jana_atom_site_ADP_C_112
_jana_atom_site_ADP_C_113
_jana_atom_site_ADP_C_122
_jana_atom_site_ADP_C_123
_jana_atom_site_ADP_C_133
_jana_atom_site_ADP_C_222
_jana_atom_site_ADP_C_223
_jana_atom_site_ADP_C_233
_jana_atom_site_ADP_C_333
Sm1 Sm 0 0 0 0 -0.00004(3) 0 0 0 0 0

loop_
_jana_atom_site_ADP_D_label
_jana_atom_site_ADP_D_type_symbol
_jana_atom_site_ADP_D_1111
_jana_atom_site_ADP_D_1112
_jana_atom_site_ADP_D_1113
_jana_atom_site_ADP_D_1122
_jana_atom_site_ADP_D_1123
_jana_atom_site_ADP_D_1133
_jana_atom_site_ADP_D_1222
_jana_atom_site_ADP_D_1223
_jana_atom_site_ADP_D_1233
_jana_atom_site_ADP_D_1333
_jana_atom_site_ADP_D_2222
_jana_atom_site_ADP_D_2223
_jana_atom_site_ADP_D_2233
_jana_atom_site_ADP_D_2333
_jana_atom_site_ADP_D_3333
Sm1 Sm 0.00013(4) 0 0 0.000061(12) 0 0.000061(12) 0 0 0 0 0.00013(4) 0
0.000061(12) 0 0.00013(4)

loop_
_jana_atom_site_ADP_E_label
_jana_atom_site_ADP_E_type_symbol
_jana_atom_site_ADP_E_11111
_jana_atom_site_ADP_E_11112
_jana_atom_site_ADP_E_11113
_jana_atom_site_ADP_E_11122
_jana_atom_site_ADP_E_11123
_jana_atom_site_ADP_E_11133
_jana_atom_site_ADP_E_11222
_jana_atom_site_ADP_E_11223
_jana_atom_site_ADP_E_11233
_jana_atom_site_ADP_E_11333
_jana_atom_site_ADP_E_12222
_jana_atom_site_ADP_E_12223
_jana_atom_site_ADP_E_12233
_jana_atom_site_ADP_E_12333
_jana_atom_site_ADP_E_13333
_jana_atom_site_ADP_E_22222
_jana_atom_site_ADP_E_22223
_jana_atom_site_ADP_E_22233
_jana_atom_site_ADP_E_22333
_jana_atom_site_ADP_E_23333
_jana_atom_site_ADP_E_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_F_label
_jana_atom_site_ADP_F_type_symbol
_jana_atom_site_ADP_F_111111
_jana_atom_site_ADP_F_111112
_jana_atom_site_ADP_F_111113
_jana_atom_site_ADP_F_111122
_jana_atom_site_ADP_F_111123
_jana_atom_site_ADP_F_111133
_jana_atom_site_ADP_F_111222
_jana_atom_site_ADP_F_111223
_jana_atom_site_ADP_F_111233
_jana_atom_site_ADP_F_111333
_jana_atom_site_ADP_F_112222
_jana_atom_site_ADP_F_112223
_jana_atom_site_ADP_F_112233
_jana_atom_site_ADP_F_112333
_jana_atom_site_ADP_F_113333
_jana_atom_site_ADP_F_122222
_jana_atom_site_ADP_F_122223
_jana_atom_site_ADP_F_122233
_jana_atom_site_ADP_F_122333
_jana_atom_site_ADP_F_123333
_jana_atom_site_ADP_F_133333
_jana_atom_site_ADP_F_222222
_jana_atom_site_ADP_F_222223
_jana_atom_site_ADP_F_222233
_jana_atom_site_ADP_F_222333
_jana_atom_site_ADP_F_223333
_jana_atom_site_ADP_F_233333
_jana_atom_site_ADP_F_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sm1 Mn1 . . 3.77267(15) ?
Sm1 Mn1 . 49_555 3.77267(15) ?
Sm1 Mn1 . 97_555 3.77267(15) ?
Sm1 Mn1 . 145_555 3.77267(15) ?
Sm1 Ga1 . . 3.09502(18) ?
Sm1 Ga1 . 49_555 3.09502(18) ?
Sm1 Ga1 . 98_555 3.09502(18) ?
Sm1 Ga1 . 146_555 3.09502(18) ?
Sm1 Ga1 . 5_555 3.09502(18) ?
Sm1 Ga1 . 101_555 3.09502(18) ?
Sm1 Ga1 . 54_555 3.09502(18) ?
Sm1 Ga1 . 150_555 3.09502(18) ?
Sm1 Ga1 . 9_555 3.09502(18) ?
Sm1 Ga1 . 153_555 3.09502(18) ?
Sm1 Ga1 . 58_555 3.09502(18) ?
Sm1 Ga1 . 106_555 3.09502(18) ?
Sm1 Ga1' . . 3.08075(16) ?
Sm1 Ga1' . 49_555 3.08075(16) ?
Sm1 Ga1' . 98_555 3.08075(16) ?
Sm1 Ga1' . 146_555 3.08075(16) ?
Sm1 Ga1' . 5_555 3.08075(16) ?
Sm1 Ga1' . 101_555 3.08075(16) ?
Sm1 Ga1' . 54_555 3.08075(16) ?
Sm1 Ga1' . 150_555 3.08075(16) ?
Sm1 Ga1' . 9_555 3.08075(16) ?
Sm1 Ga1' . 153_555 3.08075(16) ?
Sm1 Ga1' . 58_555 3.08075(16) ?
Sm1 Ga1' . 106_555 3.08075(16) ?
Sm1 Ge1 . . 3.09502(18) ?
Sm1 Ge1 . 49_555 3.09502(18) ?
Sm1 Ge1 . 98_555 3.09502(18) ?
Sm1 Ge1 . 146_555 3.09502(18) ?
Sm1 Ge1 . 5_555 3.09502(18) ?
Sm1 Ge1 . 101_555 3.09502(18) ?
Sm1 Ge1 . 54_555 3.09502(18) ?
Sm1 Ge1 . 150_555 3.09502(18) ?
Sm1 Ge1 . 9_555 3.09502(18) ?
Sm1 Ge1 . 153_555 3.09502(18) ?
Sm1 Ge1 . 58_555 3.09502(18) ?
Sm1 Ge1 . 106_555 3.09502(18) ?
Sm1 Ge1' . . 3.08075(16) ?
Sm1 Ge1' . 49_555 3.08075(16) ?
Sm1 Ge1' . 98_555 3.08075(16) ?
Sm1 Ge1' . 146_555 3.08075(16) ?
Sm1 Ge1' . 5_555 3.08075(16) ?
Sm1 Ge1' . 101_555 3.08075(16) ?
Sm1 Ge1' . 54_555 3.08075(16) ?
Sm1 Ge1' . 150_555 3.08075(16) ?
Sm1 Ge1' . 9_555 3.08075(16) ?
Sm1 Ge1' . 153_555 3.08075(16) ?
Sm1 Ge1' . 58_555 3.08075(16) ?
Sm1 Ge1' . 106_555 3.08075(16) ?
Mn1 Ga1 . . 2.4790(11) ?
Mn1 Ga1 . 2_555 2.4790(11) ?
Mn1 Ga1 . 5_555 2.4790(11) ?
Mn1 Ga1 . 6_555 2.4790(11) ?
Mn1 Ga1 . 9_555 2.4790(11) ?
Mn1 Ga1 . 10_555 2.4790(11) ?
Mn1 Ga1' . . 2.130(4) ?
Mn1 Ga1' . 2_555 2.130(4) ?
Mn1 Ga1' . 5_555 2.130(4) ?
Mn1 Ga1' . 6_555 2.130(4) ?
Mn1 Ga1' . 9_555 2.130(4) ?
Mn1 Ga1' . 10_555 2.130(4) ?
Mn1 Ge1 . . 2.4790(11) ?
Mn1 Ge1 . 2_555 2.4790(11) ?
Mn1 Ge1 . 5_555 2.4790(11) ?
Mn1 Ge1 . 6_555 2.4790(11) ?
Mn1 Ge1 . 9_555 2.4790(11) ?
Mn1 Ge1 . 10_555 2.4790(11) ?
Mn1 Ge1' . . 2.130(4) ?
Mn1 Ge1' . 2_555 2.130(4) ?
Mn1 Ge1' . 5_555 2.130(4) ?
Mn1 Ge1' . 6_555 2.130(4) ?
Mn1 Ge1' . 9_555 2.130(4) ?
Mn1 Ge1' . 10_555 2.130(4) ?
Ga1 Ga1 . 2_655 3.7547(16) ?
Ga1 Ga1 . 5_555 3.5058(11) ?
Ga1 Ga1 . 149_545 2.6549(11) ?
Ga1 Ga1 . 6_555 3.5058(11) ?
Ga1 Ga1 . 150_555 2.6549(11) ?
Ga1 Ga1 . 9_555 3.5058(11) ?
Ga1 Ga1 . 105_554 2.6549(11) ?
Ga1 Ga1 . 10_555 3.5058(11) ?
Ga1 Ga1 . 106_555 2.6549(11) ?
Ga1 Ga1' . . 0.349(4) ?
Ga1 Ga1' . 5_555 3.268(2) ?
Ga1 Ga1' . 149_545 2.912(3) ?
Ga1 Ga1' . 6_555 3.268(2) ?
Ga1 Ga1' . 150_555 2.912(3) ?
Ga1 Ga1' . 9_555 3.268(2) ?
Ga1 Ga1' . 105_554 2.912(3) ?
Ga1 Ga1' . 10_555 3.268(2) ?
Ga1 Ga1' . 106_555 2.912(3) ?
Ga1 Ge1 . 2_655 3.7547(16) ?
Ga1 Ge1 . 5_555 3.5058(11) ?
Ga1 Ge1 . 149_545 2.6549(11) ?
Ga1 Ge1 . 6_555 3.5058(11) ?
Ga1 Ge1 . 150_555 2.6549(11) ?
Ga1 Ge1 . 9_555 3.5058(11) ?
Ga1 Ge1 . 105_554 2.6549(11) ?
Ga1 Ge1 . 10_555 3.5058(11) ?
Ga1 Ge1 . 106_555 2.6549(11) ?
Ga1 Ge1' . . 0.349(4) ?
Ga1 Ge1' . 5_555 3.268(2) ?
Ga1 Ge1' . 149_545 2.912(3) ?
Ga1 Ge1' . 6_555 3.268(2) ?
Ga1 Ge1' . 150_555 2.912(3) ?
Ga1 Ge1' . 9_555 3.268(2) ?
Ga1 Ge1' . 105_554 2.912(3) ?
Ga1 Ge1' . 10_555 3.268(2) ?
Ga1 Ge1' . 106_555 2.912(3) ?
Ga1' Ga1' . 5_555 3.012(4) ?
Ga1' Ga1' . 149_545 3.149(4) ?
Ga1' Ga1' . 6_555 3.012(4) ?
Ga1' Ga1' . 150_555 3.149(4) ?
Ga1' Ga1' . 9_555 3.012(4) ?
Ga1' Ga1' . 105_554 3.149(4) ?
Ga1' Ga1' . 10_555 3.012(4) ?
Ga1' Ga1' . 106_555 3.149(4) ?
Ga1' Ge1 . . 0.349(4) ?
Ga1' Ge1 . 5_555 3.268(2) ?
Ga1' Ge1 . 149_545 2.912(3) ?
Ga1' Ge1 . 6_555 3.268(2) ?
Ga1' Ge1 . 150_555 2.912(3) ?
Ga1' Ge1 . 9_555 3.268(2) ?
Ga1' Ge1 . 105_554 2.912(3) ?
Ga1' Ge1 . 10_555 3.268(2) ?
Ga1' Ge1 . 106_555 2.912(3) ?
Ga1' Ge1' . 5_555 3.012(4) ?
Ga1' Ge1' . 149_545 3.149(4) ?
Ga1' Ge1' . 6_555 3.012(4) ?
Ga1' Ge1' . 150_555 3.149(4) ?
Ga1' Ge1' . 9_555 3.012(4) ?
Ga1' Ge1' . 105_554 3.149(4) ?
Ga1' Ge1' . 10_555 3.012(4) ?
Ga1' Ge1' . 106_555 3.149(4) ?
Ge1 Ge1 . 2_655 3.7547(16) ?
Ge1 Ge1 . 5_555 3.5058(11) ?
Ge1 Ge1 . 149_545 2.6549(11) ?
Ge1 Ge1 . 6_555 3.5058(11) ?
Ge1 Ge1 . 150_555 2.6549(11) ?
Ge1 Ge1 . 9_555 3.5058(11) ?
Ge1 Ge1 . 105_554 2.6549(11) ?
Ge1 Ge1 . 10_555 3.5058(11) ?
Ge1 Ge1 . 106_555 2.6549(11) ?
Ge1 Ge1' . . 0.349(4) ?
Ge1 Ge1' . 5_555 3.268(2) ?
Ge1 Ge1' . 149_545 2.912(3) ?
Ge1 Ge1' . 6_555 3.268(2) ?
Ge1 Ge1' . 150_555 2.912(3) ?
Ge1 Ge1' . 9_555 3.268(2) ?
Ge1 Ge1' . 105_554 2.912(3) ?
Ge1 Ge1' . 10_555 3.268(2) ?
Ge1 Ge1' . 106_555 2.912(3) ?
Ge1' Ge1' . 5_555 3.012(4) ?
Ge1' Ge1' . 149_545 3.149(4) ?
Ge1' Ge1' . 6_555 3.012(4) ?
Ge1' Ge1' . 150_555 3.149(4) ?
Ge1' Ge1' . 9_555 3.012(4) ?
Ge1' Ge1' . 105_554 3.149(4) ?
Ge1' Ge1' . 10_555 3.012(4) ?
Ge1' Ge1' . 106_555 3.149(4) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Mn1 Sm1 Mn1 . . 49_555 109.471(2) ?
Mn1 Sm1 Mn1 . . 97_555 109.471(2) ?
Mn1 Sm1 Mn1 . . 145_555 109.471(2) ?
Mn1 Sm1 Ga1 . . . 40.84(2) ?
Mn1 Sm1 Ga1 . . 49_555 150.31(2) ?
Mn1 Sm1 Ga1 . . 98_555 86.783(12) ?
Mn1 Sm1 Ga1 . . 146_555 86.783(12) ?
Mn1 Sm1 Ga1 . . 5_555 40.84(2) ?
Mn1 Sm1 Ga1 . . 101_555 150.31(2) ?
Mn1 Sm1 Ga1 . . 54_555 86.783(12) ?
Mn1 Sm1 Ga1 . . 150_555 86.783(12) ?
Mn1 Sm1 Ga1 . . 9_555 40.84(2) ?
Mn1 Sm1 Ga1 . . 153_555 150.31(2) ?
Mn1 Sm1 Ga1 . . 58_555 86.783(12) ?
Mn1 Sm1 Ga1 . . 106_555 86.783(12) ?
Mn1 Sm1 Ga1' . . . 34.37(7) ?
Mn1 Sm1 Ga1' . . 49_555 143.84(7) ?
Mn1 Sm1 Ga1' . . 98_555 90.52(4) ?
Mn1 Sm1 Ga1' . . 146_555 90.52(4) ?
Mn1 Sm1 Ga1' . . 5_555 34.37(7) ?
Mn1 Sm1 Ga1' . . 101_555 143.84(7) ?
Mn1 Sm1 Ga1' . . 54_555 90.52(4) ?
Mn1 Sm1 Ga1' . . 150_555 90.52(4) ?
Mn1 Sm1 Ga1' . . 9_555 34.37(7) ?
Mn1 Sm1 Ga1' . . 153_555 143.84(7) ?
Mn1 Sm1 Ga1' . . 58_555 90.52(4) ?
Mn1 Sm1 Ga1' . . 106_555 90.52(4) ?
Mn1 Sm1 Ge1 . . . 40.84(2) ?
Mn1 Sm1 Ge1 . . 49_555 150.31(2) ?
Mn1 Sm1 Ge1 . . 98_555 86.783(12) ?
Mn1 Sm1 Ge1 . . 146_555 86.783(12) ?
Mn1 Sm1 Ge1 . . 5_555 40.84(2) ?
Mn1 Sm1 Ge1 . . 101_555 150.31(2) ?
Mn1 Sm1 Ge1 . . 54_555 86.783(12) ?
Mn1 Sm1 Ge1 . . 150_555 86.783(12) ?
Mn1 Sm1 Ge1 . . 9_555 40.84(2) ?
Mn1 Sm1 Ge1 . . 153_555 150.31(2) ?
Mn1 Sm1 Ge1 . . 58_555 86.783(12) ?
Mn1 Sm1 Ge1 . . 106_555 86.783(12) ?
Mn1 Sm1 Ge1' . . . 34.37(7) ?
Mn1 Sm1 Ge1' . . 49_555 143.84(7) ?
Mn1 Sm1 Ge1' . . 98_555 90.52(4) ?
Mn1 Sm1 Ge1' . . 146_555 90.52(4) ?
Mn1 Sm1 Ge1' . . 5_555 34.37(7) ?
Mn1 Sm1 Ge1' . . 101_555 143.84(7) ?
Mn1 Sm1 Ge1' . . 54_555 90.52(4) ?
Mn1 Sm1 Ge1' . . 150_555 90.52(4) ?
Mn1 Sm1 Ge1' . . 9_555 34.37(7) ?
Mn1 Sm1 Ge1' . . 153_555 143.84(7) ?
Mn1 Sm1 Ge1' . . 58_555 90.52(4) ?
Mn1 Sm1 Ge1' . . 106_555 90.52(4) ?
Mn1 Sm1 Mn1 49_555 . 97_555 109.471(2) ?
Mn1 Sm1 Mn1 49_555 . 145_555 109.471(2) ?
Mn1 Sm1 Ga1 49_555 . . 150.31(2) ?
Mn1 Sm1 Ga1 49_555 . 49_555 40.84(2) ?
Mn1 Sm1 Ga1 49_555 . 98_555 86.783(12) ?
Mn1 Sm1 Ga1 49_555 . 146_555 86.783(12) ?
Mn1 Sm1 Ga1 49_555 . 5_555 86.783(12) ?
Mn1 Sm1 Ga1 49_555 . 101_555 86.783(12) ?
Mn1 Sm1 Ga1 49_555 . 54_555 40.84(2) ?
Mn1 Sm1 Ga1 49_555 . 150_555 150.31(2) ?
Mn1 Sm1 Ga1 49_555 . 9_555 86.783(12) ?
Mn1 Sm1 Ga1 49_555 . 153_555 86.783(12) ?
Mn1 Sm1 Ga1 49_555 . 58_555 40.84(2) ?
Mn1 Sm1 Ga1 49_555 . 106_555 150.31(2) ?
Mn1 Sm1 Ga1' 49_555 . . 143.84(7) ?
Mn1 Sm1 Ga1' 49_555 . 49_555 34.37(7) ?
Mn1 Sm1 Ga1' 49_555 . 98_555 90.52(4) ?
Mn1 Sm1 Ga1' 49_555 . 146_555 90.52(4) ?
Mn1 Sm1 Ga1' 49_555 . 5_555 90.52(4) ?
Mn1 Sm1 Ga1' 49_555 . 101_555 90.52(4) ?
Mn1 Sm1 Ga1' 49_555 . 54_555 34.37(7) ?
Mn1 Sm1 Ga1' 49_555 . 150_555 143.84(7) ?
Mn1 Sm1 Ga1' 49_555 . 9_555 90.52(4) ?
Mn1 Sm1 Ga1' 49_555 . 153_555 90.52(4) ?
Mn1 Sm1 Ga1' 49_555 . 58_555 34.37(7) ?
Mn1 Sm1 Ga1' 49_555 . 106_555 143.84(7) ?
Mn1 Sm1 Ge1 49_555 . . 150.31(2) ?
Mn1 Sm1 Ge1 49_555 . 49_555 40.84(2) ?
Mn1 Sm1 Ge1 49_555 . 98_555 86.783(12) ?
Mn1 Sm1 Ge1 49_555 . 146_555 86.783(12) ?
Mn1 Sm1 Ge1 49_555 . 5_555 86.783(12) ?
Mn1 Sm1 Ge1 49_555 . 101_555 86.783(12) ?
Mn1 Sm1 Ge1 49_555 . 54_555 40.84(2) ?
Mn1 Sm1 Ge1 49_555 . 150_555 150.31(2) ?
Mn1 Sm1 Ge1 49_555 . 9_555 86.783(12) ?
Mn1 Sm1 Ge1 49_555 . 153_555 86.783(12) ?
Mn1 Sm1 Ge1 49_555 . 58_555 40.84(2) ?
Mn1 Sm1 Ge1 49_555 . 106_555 150.31(2) ?
Mn1 Sm1 Ge1' 49_555 . . 143.84(7) ?
Mn1 Sm1 Ge1' 49_555 . 49_555 34.37(7) ?
Mn1 Sm1 Ge1' 49_555 . 98_555 90.52(4) ?
Mn1 Sm1 Ge1' 49_555 . 146_555 90.52(4) ?
Mn1 Sm1 Ge1' 49_555 . 5_555 90.52(4) ?
Mn1 Sm1 Ge1' 49_555 . 101_555 90.52(4) ?
Mn1 Sm1 Ge1' 49_555 . 54_555 34.37(7) ?
Mn1 Sm1 Ge1' 49_555 . 150_555 143.84(7) ?
Mn1 Sm1 Ge1' 49_555 . 9_555 90.52(4) ?
Mn1 Sm1 Ge1' 49_555 . 153_555 90.52(4) ?
Mn1 Sm1 Ge1' 49_555 . 58_555 34.37(7) ?
Mn1 Sm1 Ge1' 49_555 . 106_555 143.84(7) ?
Mn1 Sm1 Mn1 97_555 . 145_555 109.471(2) ?
Mn1 Sm1 Ga1 97_555 . . 86.783(12) ?
Mn1 Sm1 Ga1 97_555 . 49_555 86.783(12) ?
Mn1 Sm1 Ga1 97_555 . 98_555 40.84(2) ?
Mn1 Sm1 Ga1 97_555 . 146_555 150.31(2) ?
Mn1 Sm1 Ga1 97_555 . 5_555 150.31(2) ?
Mn1 Sm1 Ga1 97_555 . 101_555 40.84(2) ?
Mn1 Sm1 Ga1 97_555 . 54_555 86.783(12) ?
Mn1 Sm1 Ga1 97_555 . 150_555 86.783(12) ?
Mn1 Sm1 Ga1 97_555 . 9_555 86.783(12) ?
Mn1 Sm1 Ga1 97_555 . 153_555 86.783(12) ?
Mn1 Sm1 Ga1 97_555 . 58_555 150.31(2) ?
Mn1 Sm1 Ga1 97_555 . 106_555 40.84(2) ?
Mn1 Sm1 Ga1' 97_555 . . 90.52(4) ?
Mn1 Sm1 Ga1' 97_555 . 49_555 90.52(4) ?
Mn1 Sm1 Ga1' 97_555 . 98_555 34.37(7) ?
Mn1 Sm1 Ga1' 97_555 . 146_555 143.84(7) ?
Mn1 Sm1 Ga1' 97_555 . 5_555 143.84(7) ?
Mn1 Sm1 Ga1' 97_555 . 101_555 34.37(7) ?
Mn1 Sm1 Ga1' 97_555 . 54_555 90.52(4) ?
Mn1 Sm1 Ga1' 97_555 . 150_555 90.52(4) ?
Mn1 Sm1 Ga1' 97_555 . 9_555 90.52(4) ?
Mn1 Sm1 Ga1' 97_555 . 153_555 90.52(4) ?
Mn1 Sm1 Ga1' 97_555 . 58_555 143.84(7) ?
Mn1 Sm1 Ga1' 97_555 . 106_555 34.37(7) ?
Mn1 Sm1 Ge1 97_555 . . 86.783(12) ?
Mn1 Sm1 Ge1 97_555 . 49_555 86.783(12) ?
Mn1 Sm1 Ge1 97_555 . 98_555 40.84(2) ?
Mn1 Sm1 Ge1 97_555 . 146_555 150.31(2) ?
Mn1 Sm1 Ge1 97_555 . 5_555 150.31(2) ?
Mn1 Sm1 Ge1 97_555 . 101_555 40.84(2) ?
Mn1 Sm1 Ge1 97_555 . 54_555 86.783(12) ?
Mn1 Sm1 Ge1 97_555 . 150_555 86.783(12) ?
Mn1 Sm1 Ge1 97_555 . 9_555 86.783(12) ?
Mn1 Sm1 Ge1 97_555 . 153_555 86.783(12) ?
Mn1 Sm1 Ge1 97_555 . 58_555 150.31(2) ?
Mn1 Sm1 Ge1 97_555 . 106_555 40.84(2) ?
Mn1 Sm1 Ge1' 97_555 . . 90.52(4) ?
Mn1 Sm1 Ge1' 97_555 . 49_555 90.52(4) ?
Mn1 Sm1 Ge1' 97_555 . 98_555 34.37(7) ?
Mn1 Sm1 Ge1' 97_555 . 146_555 143.84(7) ?
Mn1 Sm1 Ge1' 97_555 . 5_555 143.84(7) ?
Mn1 Sm1 Ge1' 97_555 . 101_555 34.37(7) ?
Mn1 Sm1 Ge1' 97_555 . 54_555 90.52(4) ?
Mn1 Sm1 Ge1' 97_555 . 150_555 90.52(4) ?
Mn1 Sm1 Ge1' 97_555 . 9_555 90.52(4) ?
Mn1 Sm1 Ge1' 97_555 . 153_555 90.52(4) ?
Mn1 Sm1 Ge1' 97_555 . 58_555 143.84(7) ?
Mn1 Sm1 Ge1' 97_555 . 106_555 34.37(7) ?
Mn1 Sm1 Ga1 145_555 . . 86.783(12) ?
Mn1 Sm1 Ga1 145_555 . 49_555 86.783(12) ?
Mn1 Sm1 Ga1 145_555 . 98_555 150.31(2) ?
Mn1 Sm1 Ga1 145_555 . 146_555 40.84(2) ?
Mn1 Sm1 Ga1 145_555 . 5_555 86.783(12) ?
Mn1 Sm1 Ga1 145_555 . 101_555 86.783(12) ?
Mn1 Sm1 Ga1 145_555 . 54_555 150.31(2) ?
Mn1 Sm1 Ga1 145_555 . 150_555 40.84(2) ?
Mn1 Sm1 Ga1 145_555 . 9_555 150.31(2) ?
Mn1 Sm1 Ga1 145_555 . 153_555 40.84(2) ?
Mn1 Sm1 Ga1 145_555 . 58_555 86.783(12) ?
Mn1 Sm1 Ga1 145_555 . 106_555 86.783(12) ?
Mn1 Sm1 Ga1' 145_555 . . 90.52(4) ?
Mn1 Sm1 Ga1' 145_555 . 49_555 90.52(4) ?
Mn1 Sm1 Ga1' 145_555 . 98_555 143.84(7) ?
Mn1 Sm1 Ga1' 145_555 . 146_555 34.37(7) ?
Mn1 Sm1 Ga1' 145_555 . 5_555 90.52(4) ?
Mn1 Sm1 Ga1' 145_555 . 101_555 90.52(4) ?
Mn1 Sm1 Ga1' 145_555 . 54_555 143.84(7) ?
Mn1 Sm1 Ga1' 145_555 . 150_555 34.37(7) ?
Mn1 Sm1 Ga1' 145_555 . 9_555 143.84(7) ?
Mn1 Sm1 Ga1' 145_555 . 153_555 34.37(7) ?
Mn1 Sm1 Ga1' 145_555 . 58_555 90.52(4) ?
Mn1 Sm1 Ga1' 145_555 . 106_555 90.52(4) ?
Mn1 Sm1 Ge1 145_555 . . 86.783(12) ?
Mn1 Sm1 Ge1 145_555 . 49_555 86.783(12) ?
Mn1 Sm1 Ge1 145_555 . 98_555 150.31(2) ?
Mn1 Sm1 Ge1 145_555 . 146_555 40.84(2) ?
Mn1 Sm1 Ge1 145_555 . 5_555 86.783(12) ?
Mn1 Sm1 Ge1 145_555 . 101_555 86.783(12) ?
Mn1 Sm1 Ge1 145_555 . 54_555 150.31(2) ?
Mn1 Sm1 Ge1 145_555 . 150_555 40.84(2) ?
Mn1 Sm1 Ge1 145_555 . 9_555 150.31(2) ?
Mn1 Sm1 Ge1 145_555 . 153_555 40.84(2) ?
Mn1 Sm1 Ge1 145_555 . 58_555 86.783(12) ?
Mn1 Sm1 Ge1 145_555 . 106_555 86.783(12) ?
Mn1 Sm1 Ge1' 145_555 . . 90.52(4) ?
Mn1 Sm1 Ge1' 145_555 . 49_555 90.52(4) ?
Mn1 Sm1 Ge1' 145_555 . 98_555 143.84(7) ?
Mn1 Sm1 Ge1' 145_555 . 146_555 34.37(7) ?
Mn1 Sm1 Ge1' 145_555 . 5_555 90.52(4) ?
Mn1 Sm1 Ge1' 145_555 . 101_555 90.52(4) ?
Mn1 Sm1 Ge1' 145_555 . 54_555 143.84(7) ?
Mn1 Sm1 Ge1' 145_555 . 150_555 34.37(7) ?
Mn1 Sm1 Ge1' 145_555 . 9_555 143.84(7) ?
Mn1 Sm1 Ge1' 145_555 . 153_555 34.37(7) ?
Mn1 Sm1 Ge1' 145_555 . 58_555 90.52(4) ?
Mn1 Sm1 Ge1' 145_555 . 106_555 90.52(4) ?
Ga1 Sm1 Ga1 . . 49_555 168.84(3) ?
Ga1 Sm1 Ga1 . . 98_555 90.541(4) ?
Ga1 Sm1 Ga1 . . 146_555 90.541(4) ?
Ga1 Sm1 Ga1 . . 5_555 68.99(2) ?
Ga1 Sm1 Ga1 . . 101_555 119.69(2) ?
Ga1 Sm1 Ga1 . . 54_555 119.69(2) ?
Ga1 Sm1 Ga1 . . 150_555 50.80(2) ?
Ga1 Sm1 Ga1 . . 9_555 68.99(2) ?
Ga1 Sm1 Ga1 . . 153_555 119.69(2) ?
Ga1 Sm1 Ga1 . . 58_555 119.69(2) ?
Ga1 Sm1 Ga1 . . 106_555 50.80(2) ?
Ga1 Sm1 Ga1' . . . 6.48(7) ?
Ga1 Sm1 Ga1' . . 49_555 175.32(7) ?
Ga1 Sm1 Ga1' . . 98_555 89.913(7) ?
Ga1 Sm1 Ga1' . . 146_555 89.913(7) ?
Ga1 Sm1 Ga1' . . 5_555 63.90(5) ?
Ga1 Sm1 Ga1' . . 101_555 114.70(5) ?
Ga1 Sm1 Ga1' . . 54_555 125.26(6) ?
Ga1 Sm1 Ga1' . . 150_555 56.27(6) ?
Ga1 Sm1 Ga1' . . 9_555 63.90(5) ?
Ga1 Sm1 Ga1' . . 153_555 114.70(5) ?
Ga1 Sm1 Ga1' . . 58_555 125.26(6) ?
Ga1 Sm1 Ga1' . . 106_555 56.27(6) ?
Ga1 Sm1 Ge1 . . . 0 ?
Ga1 Sm1 Ge1 . . 49_555 168.84(3) ?
Ga1 Sm1 Ge1 . . 98_555 90.541(4) ?
Ga1 Sm1 Ge1 . . 146_555 90.541(4) ?
Ga1 Sm1 Ge1 . . 5_555 68.99(2) ?
Ga1 Sm1 Ge1 . . 101_555 119.69(2) ?
Ga1 Sm1 Ge1 . . 54_555 119.69(2) ?
Ga1 Sm1 Ge1 . . 150_555 50.80(2) ?
Ga1 Sm1 Ge1 . . 9_555 68.99(2) ?
Ga1 Sm1 Ge1 . . 153_555 119.69(2) ?
Ga1 Sm1 Ge1 . . 58_555 119.69(2) ?
Ga1 Sm1 Ge1 . . 106_555 50.80(2) ?
Ga1 Sm1 Ge1' . . . 6.48(7) ?
Ga1 Sm1 Ge1' . . 49_555 175.32(7) ?
Ga1 Sm1 Ge1' . . 98_555 89.913(7) ?
Ga1 Sm1 Ge1' . . 146_555 89.913(7) ?
Ga1 Sm1 Ge1' . . 5_555 63.90(5) ?
Ga1 Sm1 Ge1' . . 101_555 114.70(5) ?
Ga1 Sm1 Ge1' . . 54_555 125.26(6) ?
Ga1 Sm1 Ge1' . . 150_555 56.27(6) ?
Ga1 Sm1 Ge1' . . 9_555 63.90(5) ?
Ga1 Sm1 Ge1' . . 153_555 114.70(5) ?
Ga1 Sm1 Ge1' . . 58_555 125.26(6) ?
Ga1 Sm1 Ge1' . . 106_555 56.27(6) ?
Ga1 Sm1 Ga1 49_555 . 98_555 90.541(4) ?
Ga1 Sm1 Ga1 49_555 . 146_555 90.541(4) ?
Ga1 Sm1 Ga1 49_555 . 5_555 119.69(2) ?
Ga1 Sm1 Ga1 49_555 . 101_555 50.80(2) ?
Ga1 Sm1 Ga1 49_555 . 54_555 68.99(2) ?
Ga1 Sm1 Ga1 49_555 . 150_555 119.69(2) ?
Ga1 Sm1 Ga1 49_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ga1 49_555 . 153_555 50.80(2) ?
Ga1 Sm1 Ga1 49_555 . 58_555 68.99(2) ?
Ga1 Sm1 Ga1 49_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ga1' 49_555 . . 175.32(7) ?
Ga1 Sm1 Ga1' 49_555 . 49_555 6.48(7) ?
Ga1 Sm1 Ga1' 49_555 . 98_555 89.913(7) ?
Ga1 Sm1 Ga1' 49_555 . 146_555 89.913(7) ?
Ga1 Sm1 Ga1' 49_555 . 5_555 125.26(6) ?
Ga1 Sm1 Ga1' 49_555 . 101_555 56.27(6) ?
Ga1 Sm1 Ga1' 49_555 . 54_555 63.90(5) ?
Ga1 Sm1 Ga1' 49_555 . 150_555 114.70(5) ?
Ga1 Sm1 Ga1' 49_555 . 9_555 125.26(6) ?
Ga1 Sm1 Ga1' 49_555 . 153_555 56.27(6) ?
Ga1 Sm1 Ga1' 49_555 . 58_555 63.90(5) ?
Ga1 Sm1 Ga1' 49_555 . 106_555 114.70(5) ?
Ga1 Sm1 Ge1 49_555 . . 168.84(3) ?
Ga1 Sm1 Ge1 49_555 . 49_555 0 ?
Ga1 Sm1 Ge1 49_555 . 98_555 90.541(4) ?
Ga1 Sm1 Ge1 49_555 . 146_555 90.541(4) ?
Ga1 Sm1 Ge1 49_555 . 5_555 119.69(2) ?
Ga1 Sm1 Ge1 49_555 . 101_555 50.80(2) ?
Ga1 Sm1 Ge1 49_555 . 54_555 68.99(2) ?
Ga1 Sm1 Ge1 49_555 . 150_555 119.69(2) ?
Ga1 Sm1 Ge1 49_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ge1 49_555 . 153_555 50.80(2) ?
Ga1 Sm1 Ge1 49_555 . 58_555 68.99(2) ?
Ga1 Sm1 Ge1 49_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ge1' 49_555 . . 175.32(7) ?
Ga1 Sm1 Ge1' 49_555 . 49_555 6.48(7) ?
Ga1 Sm1 Ge1' 49_555 . 98_555 89.913(7) ?
Ga1 Sm1 Ge1' 49_555 . 146_555 89.913(7) ?
Ga1 Sm1 Ge1' 49_555 . 5_555 125.26(6) ?
Ga1 Sm1 Ge1' 49_555 . 101_555 56.27(6) ?
Ga1 Sm1 Ge1' 49_555 . 54_555 63.90(5) ?
Ga1 Sm1 Ge1' 49_555 . 150_555 114.70(5) ?
Ga1 Sm1 Ge1' 49_555 . 9_555 125.26(6) ?
Ga1 Sm1 Ge1' 49_555 . 153_555 56.27(6) ?
Ga1 Sm1 Ge1' 49_555 . 58_555 63.90(5) ?
Ga1 Sm1 Ge1' 49_555 . 106_555 114.70(5) ?
Ga1 Sm1 Ga1 98_555 . 146_555 168.84(3) ?
Ga1 Sm1 Ga1 98_555 . 5_555 119.69(2) ?
Ga1 Sm1 Ga1 98_555 . 101_555 68.99(2) ?
Ga1 Sm1 Ga1 98_555 . 54_555 50.80(2) ?
Ga1 Sm1 Ga1 98_555 . 150_555 119.69(2) ?
Ga1 Sm1 Ga1 98_555 . 9_555 50.80(2) ?
Ga1 Sm1 Ga1 98_555 . 153_555 119.69(2) ?
Ga1 Sm1 Ga1 98_555 . 58_555 119.69(2) ?
Ga1 Sm1 Ga1 98_555 . 106_555 68.99(2) ?
Ga1 Sm1 Ga1' 98_555 . . 89.913(7) ?
Ga1 Sm1 Ga1' 98_555 . 49_555 89.913(7) ?
Ga1 Sm1 Ga1' 98_555 . 98_555 6.48(7) ?
Ga1 Sm1 Ga1' 98_555 . 146_555 175.32(7) ?
Ga1 Sm1 Ga1' 98_555 . 5_555 114.70(5) ?
Ga1 Sm1 Ga1' 98_555 . 101_555 63.90(5) ?
Ga1 Sm1 Ga1' 98_555 . 54_555 56.27(6) ?
Ga1 Sm1 Ga1' 98_555 . 150_555 125.26(6) ?
Ga1 Sm1 Ga1' 98_555 . 9_555 56.27(6) ?
Ga1 Sm1 Ga1' 98_555 . 153_555 125.26(6) ?
Ga1 Sm1 Ga1' 98_555 . 58_555 114.70(5) ?
Ga1 Sm1 Ga1' 98_555 . 106_555 63.90(5) ?
Ga1 Sm1 Ge1 98_555 . . 90.541(4) ?
Ga1 Sm1 Ge1 98_555 . 49_555 90.541(4) ?
Ga1 Sm1 Ge1 98_555 . 98_555 0 ?
Ga1 Sm1 Ge1 98_555 . 146_555 168.84(3) ?
Ga1 Sm1 Ge1 98_555 . 5_555 119.69(2) ?
Ga1 Sm1 Ge1 98_555 . 101_555 68.99(2) ?
Ga1 Sm1 Ge1 98_555 . 54_555 50.80(2) ?
Ga1 Sm1 Ge1 98_555 . 150_555 119.69(2) ?
Ga1 Sm1 Ge1 98_555 . 9_555 50.80(2) ?
Ga1 Sm1 Ge1 98_555 . 153_555 119.69(2) ?
Ga1 Sm1 Ge1 98_555 . 58_555 119.69(2) ?
Ga1 Sm1 Ge1 98_555 . 106_555 68.99(2) ?
Ga1 Sm1 Ge1' 98_555 . . 89.913(7) ?
Ga1 Sm1 Ge1' 98_555 . 49_555 89.913(7) ?
Ga1 Sm1 Ge1' 98_555 . 98_555 6.48(7) ?
Ga1 Sm1 Ge1' 98_555 . 146_555 175.32(7) ?
Ga1 Sm1 Ge1' 98_555 . 5_555 114.70(5) ?
Ga1 Sm1 Ge1' 98_555 . 101_555 63.90(5) ?
Ga1 Sm1 Ge1' 98_555 . 54_555 56.27(6) ?
Ga1 Sm1 Ge1' 98_555 . 150_555 125.26(6) ?
Ga1 Sm1 Ge1' 98_555 . 9_555 56.27(6) ?
Ga1 Sm1 Ge1' 98_555 . 153_555 125.26(6) ?
Ga1 Sm1 Ge1' 98_555 . 58_555 114.70(5) ?
Ga1 Sm1 Ge1' 98_555 . 106_555 63.90(5) ?
Ga1 Sm1 Ga1 146_555 . 5_555 50.80(2) ?
Ga1 Sm1 Ga1 146_555 . 101_555 119.69(2) ?
Ga1 Sm1 Ga1 146_555 . 54_555 119.69(2) ?
Ga1 Sm1 Ga1 146_555 . 150_555 68.99(2) ?
Ga1 Sm1 Ga1 146_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ga1 146_555 . 153_555 68.99(2) ?
Ga1 Sm1 Ga1 146_555 . 58_555 50.80(2) ?
Ga1 Sm1 Ga1 146_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ga1' 146_555 . . 89.913(7) ?
Ga1 Sm1 Ga1' 146_555 . 49_555 89.913(7) ?
Ga1 Sm1 Ga1' 146_555 . 98_555 175.32(7) ?
Ga1 Sm1 Ga1' 146_555 . 146_555 6.48(7) ?
Ga1 Sm1 Ga1' 146_555 . 5_555 56.27(6) ?
Ga1 Sm1 Ga1' 146_555 . 101_555 125.26(6) ?
Ga1 Sm1 Ga1' 146_555 . 54_555 114.70(5) ?
Ga1 Sm1 Ga1' 146_555 . 150_555 63.90(5) ?
Ga1 Sm1 Ga1' 146_555 . 9_555 114.70(5) ?
Ga1 Sm1 Ga1' 146_555 . 153_555 63.90(5) ?
Ga1 Sm1 Ga1' 146_555 . 58_555 56.27(6) ?
Ga1 Sm1 Ga1' 146_555 . 106_555 125.26(6) ?
Ga1 Sm1 Ge1 146_555 . . 90.541(4) ?
Ga1 Sm1 Ge1 146_555 . 49_555 90.541(4) ?
Ga1 Sm1 Ge1 146_555 . 98_555 168.84(3) ?
Ga1 Sm1 Ge1 146_555 . 146_555 0 ?
Ga1 Sm1 Ge1 146_555 . 5_555 50.80(2) ?
Ga1 Sm1 Ge1 146_555 . 101_555 119.69(2) ?
Ga1 Sm1 Ge1 146_555 . 54_555 119.69(2) ?
Ga1 Sm1 Ge1 146_555 . 150_555 68.99(2) ?
Ga1 Sm1 Ge1 146_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ge1 146_555 . 153_555 68.99(2) ?
Ga1 Sm1 Ge1 146_555 . 58_555 50.80(2) ?
Ga1 Sm1 Ge1 146_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ge1' 146_555 . . 89.913(7) ?
Ga1 Sm1 Ge1' 146_555 . 49_555 89.913(7) ?
Ga1 Sm1 Ge1' 146_555 . 98_555 175.32(7) ?
Ga1 Sm1 Ge1' 146_555 . 146_555 6.48(7) ?
Ga1 Sm1 Ge1' 146_555 . 5_555 56.27(6) ?
Ga1 Sm1 Ge1' 146_555 . 101_555 125.26(6) ?
Ga1 Sm1 Ge1' 146_555 . 54_555 114.70(5) ?
Ga1 Sm1 Ge1' 146_555 . 150_555 63.90(5) ?
Ga1 Sm1 Ge1' 146_555 . 9_555 114.70(5) ?
Ga1 Sm1 Ge1' 146_555 . 153_555 63.90(5) ?
Ga1 Sm1 Ge1' 146_555 . 58_555 56.27(6) ?
Ga1 Sm1 Ge1' 146_555 . 106_555 125.26(6) ?
Ga1 Sm1 Ga1 5_555 . 101_555 168.84(3) ?
Ga1 Sm1 Ga1 5_555 . 54_555 90.541(4) ?
Ga1 Sm1 Ga1 5_555 . 150_555 90.541(4) ?
Ga1 Sm1 Ga1 5_555 . 9_555 68.99(2) ?
Ga1 Sm1 Ga1 5_555 . 153_555 119.69(2) ?
Ga1 Sm1 Ga1 5_555 . 58_555 50.80(2) ?
Ga1 Sm1 Ga1 5_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ga1' 5_555 . . 63.90(5) ?
Ga1 Sm1 Ga1' 5_555 . 49_555 114.70(5) ?
Ga1 Sm1 Ga1' 5_555 . 98_555 125.26(6) ?
Ga1 Sm1 Ga1' 5_555 . 146_555 56.27(6) ?
Ga1 Sm1 Ga1' 5_555 . 5_555 6.48(7) ?
Ga1 Sm1 Ga1' 5_555 . 101_555 175.32(7) ?
Ga1 Sm1 Ga1' 5_555 . 54_555 89.913(7) ?
Ga1 Sm1 Ga1' 5_555 . 150_555 89.913(7) ?
Ga1 Sm1 Ga1' 5_555 . 9_555 63.90(5) ?
Ga1 Sm1 Ga1' 5_555 . 153_555 114.70(5) ?
Ga1 Sm1 Ga1' 5_555 . 58_555 56.27(6) ?
Ga1 Sm1 Ga1' 5_555 . 106_555 125.26(6) ?
Ga1 Sm1 Ge1 5_555 . . 68.99(2) ?
Ga1 Sm1 Ge1 5_555 . 49_555 119.69(2) ?
Ga1 Sm1 Ge1 5_555 . 98_555 119.69(2) ?
Ga1 Sm1 Ge1 5_555 . 146_555 50.80(2) ?
Ga1 Sm1 Ge1 5_555 . 5_555 0 ?
Ga1 Sm1 Ge1 5_555 . 101_555 168.84(3) ?
Ga1 Sm1 Ge1 5_555 . 54_555 90.541(4) ?
Ga1 Sm1 Ge1 5_555 . 150_555 90.541(4) ?
Ga1 Sm1 Ge1 5_555 . 9_555 68.99(2) ?
Ga1 Sm1 Ge1 5_555 . 153_555 119.69(2) ?
Ga1 Sm1 Ge1 5_555 . 58_555 50.80(2) ?
Ga1 Sm1 Ge1 5_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ge1' 5_555 . . 63.90(5) ?
Ga1 Sm1 Ge1' 5_555 . 49_555 114.70(5) ?
Ga1 Sm1 Ge1' 5_555 . 98_555 125.26(6) ?
Ga1 Sm1 Ge1' 5_555 . 146_555 56.27(6) ?
Ga1 Sm1 Ge1' 5_555 . 5_555 6.48(7) ?
Ga1 Sm1 Ge1' 5_555 . 101_555 175.32(7) ?
Ga1 Sm1 Ge1' 5_555 . 54_555 89.913(7) ?
Ga1 Sm1 Ge1' 5_555 . 150_555 89.913(7) ?
Ga1 Sm1 Ge1' 5_555 . 9_555 63.90(5) ?
Ga1 Sm1 Ge1' 5_555 . 153_555 114.70(5) ?
Ga1 Sm1 Ge1' 5_555 . 58_555 56.27(6) ?
Ga1 Sm1 Ge1' 5_555 . 106_555 125.26(6) ?
Ga1 Sm1 Ga1 101_555 . 54_555 90.541(4) ?
Ga1 Sm1 Ga1 101_555 . 150_555 90.541(4) ?
Ga1 Sm1 Ga1 101_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ga1 101_555 . 153_555 50.80(2) ?
Ga1 Sm1 Ga1 101_555 . 58_555 119.69(2) ?
Ga1 Sm1 Ga1 101_555 . 106_555 68.99(2) ?
Ga1 Sm1 Ga1' 101_555 . . 125.26(6) ?
Ga1 Sm1 Ga1' 101_555 . 49_555 56.27(6) ?
Ga1 Sm1 Ga1' 101_555 . 98_555 63.90(5) ?
Ga1 Sm1 Ga1' 101_555 . 146_555 114.70(5) ?
Ga1 Sm1 Ga1' 101_555 . 5_555 175.32(7) ?
Ga1 Sm1 Ga1' 101_555 . 101_555 6.48(7) ?
Ga1 Sm1 Ga1' 101_555 . 54_555 89.913(7) ?
Ga1 Sm1 Ga1' 101_555 . 150_555 89.913(7) ?
Ga1 Sm1 Ga1' 101_555 . 9_555 125.26(6) ?
Ga1 Sm1 Ga1' 101_555 . 153_555 56.27(6) ?
Ga1 Sm1 Ga1' 101_555 . 58_555 114.70(5) ?
Ga1 Sm1 Ga1' 101_555 . 106_555 63.90(5) ?
Ga1 Sm1 Ge1 101_555 . . 119.69(2) ?
Ga1 Sm1 Ge1 101_555 . 49_555 50.80(2) ?
Ga1 Sm1 Ge1 101_555 . 98_555 68.99(2) ?
Ga1 Sm1 Ge1 101_555 . 146_555 119.69(2) ?
Ga1 Sm1 Ge1 101_555 . 5_555 168.84(3) ?
Ga1 Sm1 Ge1 101_555 . 101_555 0 ?
Ga1 Sm1 Ge1 101_555 . 54_555 90.541(4) ?
Ga1 Sm1 Ge1 101_555 . 150_555 90.541(4) ?
Ga1 Sm1 Ge1 101_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ge1 101_555 . 153_555 50.80(2) ?
Ga1 Sm1 Ge1 101_555 . 58_555 119.69(2) ?
Ga1 Sm1 Ge1 101_555 . 106_555 68.99(2) ?
Ga1 Sm1 Ge1' 101_555 . . 125.26(6) ?
Ga1 Sm1 Ge1' 101_555 . 49_555 56.27(6) ?
Ga1 Sm1 Ge1' 101_555 . 98_555 63.90(5) ?
Ga1 Sm1 Ge1' 101_555 . 146_555 114.70(5) ?
Ga1 Sm1 Ge1' 101_555 . 5_555 175.32(7) ?
Ga1 Sm1 Ge1' 101_555 . 101_555 6.48(7) ?
Ga1 Sm1 Ge1' 101_555 . 54_555 89.913(7) ?
Ga1 Sm1 Ge1' 101_555 . 150_555 89.913(7) ?
Ga1 Sm1 Ge1' 101_555 . 9_555 125.26(6) ?
Ga1 Sm1 Ge1' 101_555 . 153_555 56.27(6) ?
Ga1 Sm1 Ge1' 101_555 . 58_555 114.70(5) ?
Ga1 Sm1 Ge1' 101_555 . 106_555 63.90(5) ?
Ga1 Sm1 Ga1 54_555 . 150_555 168.84(3) ?
Ga1 Sm1 Ga1 54_555 . 9_555 50.80(2) ?
Ga1 Sm1 Ga1 54_555 . 153_555 119.69(2) ?
Ga1 Sm1 Ga1 54_555 . 58_555 68.99(2) ?
Ga1 Sm1 Ga1 54_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ga1' 54_555 . . 114.70(5) ?
Ga1 Sm1 Ga1' 54_555 . 49_555 63.90(5) ?
Ga1 Sm1 Ga1' 54_555 . 98_555 56.27(6) ?
Ga1 Sm1 Ga1' 54_555 . 146_555 125.26(6) ?
Ga1 Sm1 Ga1' 54_555 . 5_555 89.913(7) ?
Ga1 Sm1 Ga1' 54_555 . 101_555 89.913(7) ?
Ga1 Sm1 Ga1' 54_555 . 54_555 6.48(7) ?
Ga1 Sm1 Ga1' 54_555 . 150_555 175.32(7) ?
Ga1 Sm1 Ga1' 54_555 . 9_555 56.27(6) ?
Ga1 Sm1 Ga1' 54_555 . 153_555 125.26(6) ?
Ga1 Sm1 Ga1' 54_555 . 58_555 63.90(5) ?
Ga1 Sm1 Ga1' 54_555 . 106_555 114.70(5) ?
Ga1 Sm1 Ge1 54_555 . . 119.69(2) ?
Ga1 Sm1 Ge1 54_555 . 49_555 68.99(2) ?
Ga1 Sm1 Ge1 54_555 . 98_555 50.80(2) ?
Ga1 Sm1 Ge1 54_555 . 146_555 119.69(2) ?
Ga1 Sm1 Ge1 54_555 . 5_555 90.541(4) ?
Ga1 Sm1 Ge1 54_555 . 101_555 90.541(4) ?
Ga1 Sm1 Ge1 54_555 . 54_555 0 ?
Ga1 Sm1 Ge1 54_555 . 150_555 168.84(3) ?
Ga1 Sm1 Ge1 54_555 . 9_555 50.80(2) ?
Ga1 Sm1 Ge1 54_555 . 153_555 119.69(2) ?
Ga1 Sm1 Ge1 54_555 . 58_555 68.99(2) ?
Ga1 Sm1 Ge1 54_555 . 106_555 119.69(2) ?
Ga1 Sm1 Ge1' 54_555 . . 114.70(5) ?
Ga1 Sm1 Ge1' 54_555 . 49_555 63.90(5) ?
Ga1 Sm1 Ge1' 54_555 . 98_555 56.27(6) ?
Ga1 Sm1 Ge1' 54_555 . 146_555 125.26(6) ?
Ga1 Sm1 Ge1' 54_555 . 5_555 89.913(7) ?
Ga1 Sm1 Ge1' 54_555 . 101_555 89.913(7) ?
Ga1 Sm1 Ge1' 54_555 . 54_555 6.48(7) ?
Ga1 Sm1 Ge1' 54_555 . 150_555 175.32(7) ?
Ga1 Sm1 Ge1' 54_555 . 9_555 56.27(6) ?
Ga1 Sm1 Ge1' 54_555 . 153_555 125.26(6) ?
Ga1 Sm1 Ge1' 54_555 . 58_555 63.90(5) ?
Ga1 Sm1 Ge1' 54_555 . 106_555 114.70(5) ?
Ga1 Sm1 Ga1 150_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ga1 150_555 . 153_555 68.99(2) ?
Ga1 Sm1 Ga1 150_555 . 58_555 119.69(2) ?
Ga1 Sm1 Ga1 150_555 . 106_555 50.80(2) ?
Ga1 Sm1 Ga1' 150_555 . . 56.27(6) ?
Ga1 Sm1 Ga1' 150_555 . 49_555 125.26(6) ?
Ga1 Sm1 Ga1' 150_555 . 98_555 114.70(5) ?
Ga1 Sm1 Ga1' 150_555 . 146_555 63.90(5) ?
Ga1 Sm1 Ga1' 150_555 . 5_555 89.913(7) ?
Ga1 Sm1 Ga1' 150_555 . 101_555 89.913(7) ?
Ga1 Sm1 Ga1' 150_555 . 54_555 175.32(7) ?
Ga1 Sm1 Ga1' 150_555 . 150_555 6.48(7) ?
Ga1 Sm1 Ga1' 150_555 . 9_555 114.70(5) ?
Ga1 Sm1 Ga1' 150_555 . 153_555 63.90(5) ?
Ga1 Sm1 Ga1' 150_555 . 58_555 125.26(6) ?
Ga1 Sm1 Ga1' 150_555 . 106_555 56.27(6) ?
Ga1 Sm1 Ge1 150_555 . . 50.80(2) ?
Ga1 Sm1 Ge1 150_555 . 49_555 119.69(2) ?
Ga1 Sm1 Ge1 150_555 . 98_555 119.69(2) ?
Ga1 Sm1 Ge1 150_555 . 146_555 68.99(2) ?
Ga1 Sm1 Ge1 150_555 . 5_555 90.541(4) ?
Ga1 Sm1 Ge1 150_555 . 101_555 90.541(4) ?
Ga1 Sm1 Ge1 150_555 . 54_555 168.84(3) ?
Ga1 Sm1 Ge1 150_555 . 150_555 0 ?
Ga1 Sm1 Ge1 150_555 . 9_555 119.69(2) ?
Ga1 Sm1 Ge1 150_555 . 153_555 68.99(2) ?
Ga1 Sm1 Ge1 150_555 . 58_555 119.69(2) ?
Ga1 Sm1 Ge1 150_555 . 106_555 50.80(2) ?
Ga1 Sm1 Ge1' 150_555 . . 56.27(6) ?
Ga1 Sm1 Ge1' 150_555 . 49_555 125.26(6) ?
Ga1 Sm1 Ge1' 150_555 . 98_555 114.70(5) ?
Ga1 Sm1 Ge1' 150_555 . 146_555 63.90(5) ?
Ga1 Sm1 Ge1' 150_555 . 5_555 89.913(7) ?
Ga1 Sm1 Ge1' 150_555 . 101_555 89.913(7) ?
Ga1 Sm1 Ge1' 150_555 . 54_555 175.32(7) ?
Ga1 Sm1 Ge1' 150_555 . 150_555 6.48(7) ?
Ga1 Sm1 Ge1' 150_555 . 9_555 114.70(5) ?
Ga1 Sm1 Ge1' 150_555 . 153_555 63.90(5) ?
Ga1 Sm1 Ge1' 150_555 . 58_555 125.26(6) ?
Ga1 Sm1 Ge1' 150_555 . 106_555 56.27(6) ?
Ga1 Sm1 Ga1 9_555 . 153_555 168.84(3) ?
Ga1 Sm1 Ga1 9_555 . 58_555 90.541(4) ?
Ga1 Sm1 Ga1 9_555 . 106_555 90.541(4) ?
Ga1 Sm1 Ga1' 9_555 . . 63.90(5) ?
Ga1 Sm1 Ga1' 9_555 . 49_555 114.70(5) ?
Ga1 Sm1 Ga1' 9_555 . 98_555 56.27(6) ?
Ga1 Sm1 Ga1' 9_555 . 146_555 125.26(6) ?
Ga1 Sm1 Ga1' 9_555 . 5_555 63.90(5) ?
Ga1 Sm1 Ga1' 9_555 . 101_555 114.70(5) ?
Ga1 Sm1 Ga1' 9_555 . 54_555 56.27(6) ?
Ga1 Sm1 Ga1' 9_555 . 150_555 125.26(6) ?
Ga1 Sm1 Ga1' 9_555 . 9_555 6.48(7) ?
Ga1 Sm1 Ga1' 9_555 . 153_555 175.32(7) ?
Ga1 Sm1 Ga1' 9_555 . 58_555 89.913(7) ?
Ga1 Sm1 Ga1' 9_555 . 106_555 89.913(7) ?
Ga1 Sm1 Ge1 9_555 . . 68.99(2) ?
Ga1 Sm1 Ge1 9_555 . 49_555 119.69(2) ?
Ga1 Sm1 Ge1 9_555 . 98_555 50.80(2) ?
Ga1 Sm1 Ge1 9_555 . 146_555 119.69(2) ?
Ga1 Sm1 Ge1 9_555 . 5_555 68.99(2) ?
Ga1 Sm1 Ge1 9_555 . 101_555 119.69(2) ?
Ga1 Sm1 Ge1 9_555 . 54_555 50.80(2) ?
Ga1 Sm1 Ge1 9_555 . 150_555 119.69(2) ?
Ga1 Sm1 Ge1 9_555 . 9_555 0 ?
Ga1 Sm1 Ge1 9_555 . 153_555 168.84(3) ?
Ga1 Sm1 Ge1 9_555 . 58_555 90.541(4) ?
Ga1 Sm1 Ge1 9_555 . 106_555 90.541(4) ?
Ga1 Sm1 Ge1' 9_555 . . 63.90(5) ?
Ga1 Sm1 Ge1' 9_555 . 49_555 114.70(5) ?
Ga1 Sm1 Ge1' 9_555 . 98_555 56.27(6) ?
Ga1 Sm1 Ge1' 9_555 . 146_555 125.26(6) ?
Ga1 Sm1 Ge1' 9_555 . 5_555 63.90(5) ?
Ga1 Sm1 Ge1' 9_555 . 101_555 114.70(5) ?
Ga1 Sm1 Ge1' 9_555 . 54_555 56.27(6) ?
Ga1 Sm1 Ge1' 9_555 . 150_555 125.26(6) ?
Ga1 Sm1 Ge1' 9_555 . 9_555 6.48(7) ?
Ga1 Sm1 Ge1' 9_555 . 153_555 175.32(7) ?
Ga1 Sm1 Ge1' 9_555 . 58_555 89.913(7) ?
Ga1 Sm1 Ge1' 9_555 . 106_555 89.913(7) ?
Ga1 Sm1 Ga1 153_555 . 58_555 90.541(4) ?
Ga1 Sm1 Ga1 153_555 . 106_555 90.541(4) ?
Ga1 Sm1 Ga1' 153_555 . . 125.26(6) ?
Ga1 Sm1 Ga1' 153_555 . 49_555 56.27(6) ?
Ga1 Sm1 Ga1' 153_555 . 98_555 114.70(5) ?
Ga1 Sm1 Ga1' 153_555 . 146_555 63.90(5) ?
Ga1 Sm1 Ga1' 153_555 . 5_555 125.26(6) ?
Ga1 Sm1 Ga1' 153_555 . 101_555 56.27(6) ?
Ga1 Sm1 Ga1' 153_555 . 54_555 114.70(5) ?
Ga1 Sm1 Ga1' 153_555 . 150_555 63.90(5) ?
Ga1 Sm1 Ga1' 153_555 . 9_555 175.32(7) ?
Ga1 Sm1 Ga1' 153_555 . 153_555 6.48(7) ?
Ga1 Sm1 Ga1' 153_555 . 58_555 89.913(7) ?
Ga1 Sm1 Ga1' 153_555 . 106_555 89.913(7) ?
Ga1 Sm1 Ge1 153_555 . . 119.69(2) ?
Ga1 Sm1 Ge1 153_555 . 49_555 50.80(2) ?
Ga1 Sm1 Ge1 153_555 . 98_555 119.69(2) ?
Ga1 Sm1 Ge1 153_555 . 146_555 68.99(2) ?
Ga1 Sm1 Ge1 153_555 . 5_555 119.69(2) ?
Ga1 Sm1 Ge1 153_555 . 101_555 50.80(2) ?
Ga1 Sm1 Ge1 153_555 . 54_555 119.69(2) ?
Ga1 Sm1 Ge1 153_555 . 150_555 68.99(2) ?
Ga1 Sm1 Ge1 153_555 . 9_555 168.84(3) ?
Ga1 Sm1 Ge1 153_555 . 153_555 0 ?
Ga1 Sm1 Ge1 153_555 . 58_555 90.541(4) ?
Ga1 Sm1 Ge1 153_555 . 106_555 90.541(4) ?
Ga1 Sm1 Ge1' 153_555 . . 125.26(6) ?
Ga1 Sm1 Ge1' 153_555 . 49_555 56.27(6) ?
Ga1 Sm1 Ge1' 153_555 . 98_555 114.70(5) ?
Ga1 Sm1 Ge1' 153_555 . 146_555 63.90(5) ?
Ga1 Sm1 Ge1' 153_555 . 5_555 125.26(6) ?
Ga1 Sm1 Ge1' 153_555 . 101_555 56.27(6) ?
Ga1 Sm1 Ge1' 153_555 . 54_555 114.70(5) ?
Ga1 Sm1 Ge1' 153_555 . 150_555 63.90(5) ?
Ga1 Sm1 Ge1' 153_555 . 9_555 175.32(7) ?
Ga1 Sm1 Ge1' 153_555 . 153_555 6.48(7) ?
Ga1 Sm1 Ge1' 153_555 . 58_555 89.913(7) ?
Ga1 Sm1 Ge1' 153_555 . 106_555 89.913(7) ?
Ga1 Sm1 Ga1 58_555 . 106_555 168.84(3) ?
Ga1 Sm1 Ga1' 58_555 . . 114.70(5) ?
Ga1 Sm1 Ga1' 58_555 . 49_555 63.90(5) ?
Ga1 Sm1 Ga1' 58_555 . 98_555 125.26(6) ?
Ga1 Sm1 Ga1' 58_555 . 146_555 56.27(6) ?
Ga1 Sm1 Ga1' 58_555 . 5_555 56.27(6) ?
Ga1 Sm1 Ga1' 58_555 . 101_555 125.26(6) ?
Ga1 Sm1 Ga1' 58_555 . 54_555 63.90(5) ?
Ga1 Sm1 Ga1' 58_555 . 150_555 114.70(5) ?
Ga1 Sm1 Ga1' 58_555 . 9_555 89.913(7) ?
Ga1 Sm1 Ga1' 58_555 . 153_555 89.913(7) ?
Ga1 Sm1 Ga1' 58_555 . 58_555 6.48(7) ?
Ga1 Sm1 Ga1' 58_555 . 106_555 175.32(7) ?
Ga1 Sm1 Ge1 58_555 . . 119.69(2) ?
Ga1 Sm1 Ge1 58_555 . 49_555 68.99(2) ?
Ga1 Sm1 Ge1 58_555 . 98_555 119.69(2) ?
Ga1 Sm1 Ge1 58_555 . 146_555 50.80(2) ?
Ga1 Sm1 Ge1 58_555 . 5_555 50.80(2) ?
Ga1 Sm1 Ge1 58_555 . 101_555 119.69(2) ?
Ga1 Sm1 Ge1 58_555 . 54_555 68.99(2) ?
Ga1 Sm1 Ge1 58_555 . 150_555 119.69(2) ?
Ga1 Sm1 Ge1 58_555 . 9_555 90.541(4) ?
Ga1 Sm1 Ge1 58_555 . 153_555 90.541(4) ?
Ga1 Sm1 Ge1 58_555 . 58_555 0 ?
Ga1 Sm1 Ge1 58_555 . 106_555 168.84(3) ?
Ga1 Sm1 Ge1' 58_555 . . 114.70(5) ?
Ga1 Sm1 Ge1' 58_555 . 49_555 63.90(5) ?
Ga1 Sm1 Ge1' 58_555 . 98_555 125.26(6) ?
Ga1 Sm1 Ge1' 58_555 . 146_555 56.27(6) ?
Ga1 Sm1 Ge1' 58_555 . 5_555 56.27(6) ?
Ga1 Sm1 Ge1' 58_555 . 101_555 125.26(6) ?
Ga1 Sm1 Ge1' 58_555 . 54_555 63.90(5) ?
Ga1 Sm1 Ge1' 58_555 . 150_555 114.70(5) ?
Ga1 Sm1 Ge1' 58_555 . 9_555 89.913(7) ?
Ga1 Sm1 Ge1' 58_555 . 153_555 89.913(7) ?
Ga1 Sm1 Ge1' 58_555 . 58_555 6.48(7) ?
Ga1 Sm1 Ge1' 58_555 . 106_555 175.32(7) ?
Ga1 Sm1 Ga1' 106_555 . . 56.27(6) ?
Ga1 Sm1 Ga1' 106_555 . 49_555 125.26(6) ?
Ga1 Sm1 Ga1' 106_555 . 98_555 63.90(5) ?
Ga1 Sm1 Ga1' 106_555 . 146_555 114.70(5) ?
Ga1 Sm1 Ga1' 106_555 . 5_555 114.70(5) ?
Ga1 Sm1 Ga1' 106_555 . 101_555 63.90(5) ?
Ga1 Sm1 Ga1' 106_555 . 54_555 125.26(6) ?
Ga1 Sm1 Ga1' 106_555 . 150_555 56.27(6) ?
Ga1 Sm1 Ga1' 106_555 . 9_555 89.913(7) ?
Ga1 Sm1 Ga1' 106_555 . 153_555 89.913(7) ?
Ga1 Sm1 Ga1' 106_555 . 58_555 175.32(7) ?
Ga1 Sm1 Ga1' 106_555 . 106_555 6.48(7) ?
Ga1 Sm1 Ge1 106_555 . . 50.80(2) ?
Ga1 Sm1 Ge1 106_555 . 49_555 119.69(2) ?
Ga1 Sm1 Ge1 106_555 . 98_555 68.99(2) ?
Ga1 Sm1 Ge1 106_555 . 146_555 119.69(2) ?
Ga1 Sm1 Ge1 106_555 . 5_555 119.69(2) ?
Ga1 Sm1 Ge1 106_555 . 101_555 68.99(2) ?
Ga1 Sm1 Ge1 106_555 . 54_555 119.69(2) ?
Ga1 Sm1 Ge1 106_555 . 150_555 50.80(2) ?
Ga1 Sm1 Ge1 106_555 . 9_555 90.541(4) ?
Ga1 Sm1 Ge1 106_555 . 153_555 90.541(4) ?
Ga1 Sm1 Ge1 106_555 . 58_555 168.84(3) ?
Ga1 Sm1 Ge1 106_555 . 106_555 0 ?
Ga1 Sm1 Ge1' 106_555 . . 56.27(6) ?
Ga1 Sm1 Ge1' 106_555 . 49_555 125.26(6) ?
Ga1 Sm1 Ge1' 106_555 . 98_555 63.90(5) ?
Ga1 Sm1 Ge1' 106_555 . 146_555 114.70(5) ?
Ga1 Sm1 Ge1' 106_555 . 5_555 114.70(5) ?
Ga1 Sm1 Ge1' 106_555 . 101_555 63.90(5) ?
Ga1 Sm1 Ge1' 106_555 . 54_555 125.26(6) ?
Ga1 Sm1 Ge1' 106_555 . 150_555 56.27(6) ?
Ga1 Sm1 Ge1' 106_555 . 9_555 89.913(7) ?
Ga1 Sm1 Ge1' 106_555 . 153_555 89.913(7) ?
Ga1 Sm1 Ge1' 106_555 . 58_555 175.32(7) ?
Ga1 Sm1 Ge1' 106_555 . 106_555 6.48(7) ?
Ga1' Sm1 Ga1' . . 49_555 178.20(9) ?
Ga1' Sm1 Ga1' . . 98_555 90.014(3) ?
Ga1' Sm1 Ga1' . . 146_555 90.014(3) ?
Ga1' Sm1 Ga1' . . 5_555 58.53(8) ?
Ga1' Sm1 Ga1' . . 101_555 119.99(8) ?
Ga1' Sm1 Ga1' . . 54_555 119.99(8) ?
Ga1' Sm1 Ga1' . . 150_555 61.47(8) ?
Ga1' Sm1 Ga1' . . 9_555 58.53(8) ?
Ga1' Sm1 Ga1' . . 153_555 119.99(8) ?
Ga1' Sm1 Ga1' . . 58_555 119.99(8) ?
Ga1' Sm1 Ga1' . . 106_555 61.47(8) ?
Ga1' Sm1 Ge1 . . . 6.48(7) ?
Ga1' Sm1 Ge1 . . 49_555 175.32(7) ?
Ga1' Sm1 Ge1 . . 98_555 89.913(7) ?
Ga1' Sm1 Ge1 . . 146_555 89.913(7) ?
Ga1' Sm1 Ge1 . . 5_555 63.90(5) ?
Ga1' Sm1 Ge1 . . 101_555 125.26(6) ?
Ga1' Sm1 Ge1 . . 54_555 114.70(5) ?
Ga1' Sm1 Ge1 . . 150_555 56.27(6) ?
Ga1' Sm1 Ge1 . . 9_555 63.90(5) ?
Ga1' Sm1 Ge1 . . 153_555 125.26(6) ?
Ga1' Sm1 Ge1 . . 58_555 114.70(5) ?
Ga1' Sm1 Ge1 . . 106_555 56.27(6) ?
Ga1' Sm1 Ge1' . . . 0 ?
Ga1' Sm1 Ge1' . . 49_555 178.20(9) ?
Ga1' Sm1 Ge1' . . 98_555 90.014(3) ?
Ga1' Sm1 Ge1' . . 146_555 90.014(3) ?
Ga1' Sm1 Ge1' . . 5_555 58.53(8) ?
Ga1' Sm1 Ge1' . . 101_555 119.99(8) ?
Ga1' Sm1 Ge1' . . 54_555 119.99(8) ?
Ga1' Sm1 Ge1' . . 150_555 61.47(8) ?
Ga1' Sm1 Ge1' . . 9_555 58.53(8) ?
Ga1' Sm1 Ge1' . . 153_555 119.99(8) ?
Ga1' Sm1 Ge1' . . 58_555 119.99(8) ?
Ga1' Sm1 Ge1' . . 106_555 61.47(8) ?
Ga1' Sm1 Ga1' 49_555 . 98_555 90.014(3) ?
Ga1' Sm1 Ga1' 49_555 . 146_555 90.014(3) ?
Ga1' Sm1 Ga1' 49_555 . 5_555 119.99(8) ?
Ga1' Sm1 Ga1' 49_555 . 101_555 61.47(8) ?
Ga1' Sm1 Ga1' 49_555 . 54_555 58.53(8) ?
Ga1' Sm1 Ga1' 49_555 . 150_555 119.99(8) ?
Ga1' Sm1 Ga1' 49_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ga1' 49_555 . 153_555 61.47(8) ?
Ga1' Sm1 Ga1' 49_555 . 58_555 58.53(8) ?
Ga1' Sm1 Ga1' 49_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ge1 49_555 . . 175.32(7) ?
Ga1' Sm1 Ge1 49_555 . 49_555 6.48(7) ?
Ga1' Sm1 Ge1 49_555 . 98_555 89.913(7) ?
Ga1' Sm1 Ge1 49_555 . 146_555 89.913(7) ?
Ga1' Sm1 Ge1 49_555 . 5_555 114.70(5) ?
Ga1' Sm1 Ge1 49_555 . 101_555 56.27(6) ?
Ga1' Sm1 Ge1 49_555 . 54_555 63.90(5) ?
Ga1' Sm1 Ge1 49_555 . 150_555 125.26(6) ?
Ga1' Sm1 Ge1 49_555 . 9_555 114.70(5) ?
Ga1' Sm1 Ge1 49_555 . 153_555 56.27(6) ?
Ga1' Sm1 Ge1 49_555 . 58_555 63.90(5) ?
Ga1' Sm1 Ge1 49_555 . 106_555 125.26(6) ?
Ga1' Sm1 Ge1' 49_555 . . 178.20(9) ?
Ga1' Sm1 Ge1' 49_555 . 49_555 0 ?
Ga1' Sm1 Ge1' 49_555 . 98_555 90.014(3) ?
Ga1' Sm1 Ge1' 49_555 . 146_555 90.014(3) ?
Ga1' Sm1 Ge1' 49_555 . 5_555 119.99(8) ?
Ga1' Sm1 Ge1' 49_555 . 101_555 61.47(8) ?
Ga1' Sm1 Ge1' 49_555 . 54_555 58.53(8) ?
Ga1' Sm1 Ge1' 49_555 . 150_555 119.99(8) ?
Ga1' Sm1 Ge1' 49_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ge1' 49_555 . 153_555 61.47(8) ?
Ga1' Sm1 Ge1' 49_555 . 58_555 58.53(8) ?
Ga1' Sm1 Ge1' 49_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ga1' 98_555 . 146_555 178.20(9) ?
Ga1' Sm1 Ga1' 98_555 . 5_555 119.99(8) ?
Ga1' Sm1 Ga1' 98_555 . 101_555 58.53(8) ?
Ga1' Sm1 Ga1' 98_555 . 54_555 61.47(8) ?
Ga1' Sm1 Ga1' 98_555 . 150_555 119.99(8) ?
Ga1' Sm1 Ga1' 98_555 . 9_555 61.47(8) ?
Ga1' Sm1 Ga1' 98_555 . 153_555 119.99(8) ?
Ga1' Sm1 Ga1' 98_555 . 58_555 119.99(8) ?
Ga1' Sm1 Ga1' 98_555 . 106_555 58.53(8) ?
Ga1' Sm1 Ge1 98_555 . . 89.913(7) ?
Ga1' Sm1 Ge1 98_555 . 49_555 89.913(7) ?
Ga1' Sm1 Ge1 98_555 . 98_555 6.48(7) ?
Ga1' Sm1 Ge1 98_555 . 146_555 175.32(7) ?
Ga1' Sm1 Ge1 98_555 . 5_555 125.26(6) ?
Ga1' Sm1 Ge1 98_555 . 101_555 63.90(5) ?
Ga1' Sm1 Ge1 98_555 . 54_555 56.27(6) ?
Ga1' Sm1 Ge1 98_555 . 150_555 114.70(5) ?
Ga1' Sm1 Ge1 98_555 . 9_555 56.27(6) ?
Ga1' Sm1 Ge1 98_555 . 153_555 114.70(5) ?
Ga1' Sm1 Ge1 98_555 . 58_555 125.26(6) ?
Ga1' Sm1 Ge1 98_555 . 106_555 63.90(5) ?
Ga1' Sm1 Ge1' 98_555 . . 90.014(3) ?
Ga1' Sm1 Ge1' 98_555 . 49_555 90.014(3) ?
Ga1' Sm1 Ge1' 98_555 . 98_555 0 ?
Ga1' Sm1 Ge1' 98_555 . 146_555 178.20(9) ?
Ga1' Sm1 Ge1' 98_555 . 5_555 119.99(8) ?
Ga1' Sm1 Ge1' 98_555 . 101_555 58.53(8) ?
Ga1' Sm1 Ge1' 98_555 . 54_555 61.47(8) ?
Ga1' Sm1 Ge1' 98_555 . 150_555 119.99(8) ?
Ga1' Sm1 Ge1' 98_555 . 9_555 61.47(8) ?
Ga1' Sm1 Ge1' 98_555 . 153_555 119.99(8) ?
Ga1' Sm1 Ge1' 98_555 . 58_555 119.99(8) ?
Ga1' Sm1 Ge1' 98_555 . 106_555 58.53(8) ?
Ga1' Sm1 Ga1' 146_555 . 5_555 61.47(8) ?
Ga1' Sm1 Ga1' 146_555 . 101_555 119.99(8) ?
Ga1' Sm1 Ga1' 146_555 . 54_555 119.99(8) ?
Ga1' Sm1 Ga1' 146_555 . 150_555 58.53(8) ?
Ga1' Sm1 Ga1' 146_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ga1' 146_555 . 153_555 58.53(8) ?
Ga1' Sm1 Ga1' 146_555 . 58_555 61.47(8) ?
Ga1' Sm1 Ga1' 146_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ge1 146_555 . . 89.913(7) ?
Ga1' Sm1 Ge1 146_555 . 49_555 89.913(7) ?
Ga1' Sm1 Ge1 146_555 . 98_555 175.32(7) ?
Ga1' Sm1 Ge1 146_555 . 146_555 6.48(7) ?
Ga1' Sm1 Ge1 146_555 . 5_555 56.27(6) ?
Ga1' Sm1 Ge1 146_555 . 101_555 114.70(5) ?
Ga1' Sm1 Ge1 146_555 . 54_555 125.26(6) ?
Ga1' Sm1 Ge1 146_555 . 150_555 63.90(5) ?
Ga1' Sm1 Ge1 146_555 . 9_555 125.26(6) ?
Ga1' Sm1 Ge1 146_555 . 153_555 63.90(5) ?
Ga1' Sm1 Ge1 146_555 . 58_555 56.27(6) ?
Ga1' Sm1 Ge1 146_555 . 106_555 114.70(5) ?
Ga1' Sm1 Ge1' 146_555 . . 90.014(3) ?
Ga1' Sm1 Ge1' 146_555 . 49_555 90.014(3) ?
Ga1' Sm1 Ge1' 146_555 . 98_555 178.20(9) ?
Ga1' Sm1 Ge1' 146_555 . 146_555 0 ?
Ga1' Sm1 Ge1' 146_555 . 5_555 61.47(8) ?
Ga1' Sm1 Ge1' 146_555 . 101_555 119.99(8) ?
Ga1' Sm1 Ge1' 146_555 . 54_555 119.99(8) ?
Ga1' Sm1 Ge1' 146_555 . 150_555 58.53(8) ?
Ga1' Sm1 Ge1' 146_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ge1' 146_555 . 153_555 58.53(8) ?
Ga1' Sm1 Ge1' 146_555 . 58_555 61.47(8) ?
Ga1' Sm1 Ge1' 146_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ga1' 5_555 . 101_555 178.20(9) ?
Ga1' Sm1 Ga1' 5_555 . 54_555 90.014(3) ?
Ga1' Sm1 Ga1' 5_555 . 150_555 90.014(3) ?
Ga1' Sm1 Ga1' 5_555 . 9_555 58.53(8) ?
Ga1' Sm1 Ga1' 5_555 . 153_555 119.99(8) ?
Ga1' Sm1 Ga1' 5_555 . 58_555 61.47(8) ?
Ga1' Sm1 Ga1' 5_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ge1 5_555 . . 63.90(5) ?
Ga1' Sm1 Ge1 5_555 . 49_555 125.26(6) ?
Ga1' Sm1 Ge1 5_555 . 98_555 114.70(5) ?
Ga1' Sm1 Ge1 5_555 . 146_555 56.27(6) ?
Ga1' Sm1 Ge1 5_555 . 5_555 6.48(7) ?
Ga1' Sm1 Ge1 5_555 . 101_555 175.32(7) ?
Ga1' Sm1 Ge1 5_555 . 54_555 89.913(7) ?
Ga1' Sm1 Ge1 5_555 . 150_555 89.913(7) ?
Ga1' Sm1 Ge1 5_555 . 9_555 63.90(5) ?
Ga1' Sm1 Ge1 5_555 . 153_555 125.26(6) ?
Ga1' Sm1 Ge1 5_555 . 58_555 56.27(6) ?
Ga1' Sm1 Ge1 5_555 . 106_555 114.70(5) ?
Ga1' Sm1 Ge1' 5_555 . . 58.53(8) ?
Ga1' Sm1 Ge1' 5_555 . 49_555 119.99(8) ?
Ga1' Sm1 Ge1' 5_555 . 98_555 119.99(8) ?
Ga1' Sm1 Ge1' 5_555 . 146_555 61.47(8) ?
Ga1' Sm1 Ge1' 5_555 . 5_555 0 ?
Ga1' Sm1 Ge1' 5_555 . 101_555 178.20(9) ?
Ga1' Sm1 Ge1' 5_555 . 54_555 90.014(3) ?
Ga1' Sm1 Ge1' 5_555 . 150_555 90.014(3) ?
Ga1' Sm1 Ge1' 5_555 . 9_555 58.53(8) ?
Ga1' Sm1 Ge1' 5_555 . 153_555 119.99(8) ?
Ga1' Sm1 Ge1' 5_555 . 58_555 61.47(8) ?
Ga1' Sm1 Ge1' 5_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ga1' 101_555 . 54_555 90.014(3) ?
Ga1' Sm1 Ga1' 101_555 . 150_555 90.014(3) ?
Ga1' Sm1 Ga1' 101_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ga1' 101_555 . 153_555 61.47(8) ?
Ga1' Sm1 Ga1' 101_555 . 58_555 119.99(8) ?
Ga1' Sm1 Ga1' 101_555 . 106_555 58.53(8) ?
Ga1' Sm1 Ge1 101_555 . . 114.70(5) ?
Ga1' Sm1 Ge1 101_555 . 49_555 56.27(6) ?
Ga1' Sm1 Ge1 101_555 . 98_555 63.90(5) ?
Ga1' Sm1 Ge1 101_555 . 146_555 125.26(6) ?
Ga1' Sm1 Ge1 101_555 . 5_555 175.32(7) ?
Ga1' Sm1 Ge1 101_555 . 101_555 6.48(7) ?
Ga1' Sm1 Ge1 101_555 . 54_555 89.913(7) ?
Ga1' Sm1 Ge1 101_555 . 150_555 89.913(7) ?
Ga1' Sm1 Ge1 101_555 . 9_555 114.70(5) ?
Ga1' Sm1 Ge1 101_555 . 153_555 56.27(6) ?
Ga1' Sm1 Ge1 101_555 . 58_555 125.26(6) ?
Ga1' Sm1 Ge1 101_555 . 106_555 63.90(5) ?
Ga1' Sm1 Ge1' 101_555 . . 119.99(8) ?
Ga1' Sm1 Ge1' 101_555 . 49_555 61.47(8) ?
Ga1' Sm1 Ge1' 101_555 . 98_555 58.53(8) ?
Ga1' Sm1 Ge1' 101_555 . 146_555 119.99(8) ?
Ga1' Sm1 Ge1' 101_555 . 5_555 178.20(9) ?
Ga1' Sm1 Ge1' 101_555 . 101_555 0 ?
Ga1' Sm1 Ge1' 101_555 . 54_555 90.014(3) ?
Ga1' Sm1 Ge1' 101_555 . 150_555 90.014(3) ?
Ga1' Sm1 Ge1' 101_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ge1' 101_555 . 153_555 61.47(8) ?
Ga1' Sm1 Ge1' 101_555 . 58_555 119.99(8) ?
Ga1' Sm1 Ge1' 101_555 . 106_555 58.53(8) ?
Ga1' Sm1 Ga1' 54_555 . 150_555 178.20(9) ?
Ga1' Sm1 Ga1' 54_555 . 9_555 61.47(8) ?
Ga1' Sm1 Ga1' 54_555 . 153_555 119.99(8) ?
Ga1' Sm1 Ga1' 54_555 . 58_555 58.53(8) ?
Ga1' Sm1 Ga1' 54_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ge1 54_555 . . 125.26(6) ?
Ga1' Sm1 Ge1 54_555 . 49_555 63.90(5) ?
Ga1' Sm1 Ge1 54_555 . 98_555 56.27(6) ?
Ga1' Sm1 Ge1 54_555 . 146_555 114.70(5) ?
Ga1' Sm1 Ge1 54_555 . 5_555 89.913(7) ?
Ga1' Sm1 Ge1 54_555 . 101_555 89.913(7) ?
Ga1' Sm1 Ge1 54_555 . 54_555 6.48(7) ?
Ga1' Sm1 Ge1 54_555 . 150_555 175.32(7) ?
Ga1' Sm1 Ge1 54_555 . 9_555 56.27(6) ?
Ga1' Sm1 Ge1 54_555 . 153_555 114.70(5) ?
Ga1' Sm1 Ge1 54_555 . 58_555 63.90(5) ?
Ga1' Sm1 Ge1 54_555 . 106_555 125.26(6) ?
Ga1' Sm1 Ge1' 54_555 . . 119.99(8) ?
Ga1' Sm1 Ge1' 54_555 . 49_555 58.53(8) ?
Ga1' Sm1 Ge1' 54_555 . 98_555 61.47(8) ?
Ga1' Sm1 Ge1' 54_555 . 146_555 119.99(8) ?
Ga1' Sm1 Ge1' 54_555 . 5_555 90.014(3) ?
Ga1' Sm1 Ge1' 54_555 . 101_555 90.014(3) ?
Ga1' Sm1 Ge1' 54_555 . 54_555 0 ?
Ga1' Sm1 Ge1' 54_555 . 150_555 178.20(9) ?
Ga1' Sm1 Ge1' 54_555 . 9_555 61.47(8) ?
Ga1' Sm1 Ge1' 54_555 . 153_555 119.99(8) ?
Ga1' Sm1 Ge1' 54_555 . 58_555 58.53(8) ?
Ga1' Sm1 Ge1' 54_555 . 106_555 119.99(8) ?
Ga1' Sm1 Ga1' 150_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ga1' 150_555 . 153_555 58.53(8) ?
Ga1' Sm1 Ga1' 150_555 . 58_555 119.99(8) ?
Ga1' Sm1 Ga1' 150_555 . 106_555 61.47(8) ?
Ga1' Sm1 Ge1 150_555 . . 56.27(6) ?
Ga1' Sm1 Ge1 150_555 . 49_555 114.70(5) ?
Ga1' Sm1 Ge1 150_555 . 98_555 125.26(6) ?
Ga1' Sm1 Ge1 150_555 . 146_555 63.90(5) ?
Ga1' Sm1 Ge1 150_555 . 5_555 89.913(7) ?
Ga1' Sm1 Ge1 150_555 . 101_555 89.913(7) ?
Ga1' Sm1 Ge1 150_555 . 54_555 175.32(7) ?
Ga1' Sm1 Ge1 150_555 . 150_555 6.48(7) ?
Ga1' Sm1 Ge1 150_555 . 9_555 125.26(6) ?
Ga1' Sm1 Ge1 150_555 . 153_555 63.90(5) ?
Ga1' Sm1 Ge1 150_555 . 58_555 114.70(5) ?
Ga1' Sm1 Ge1 150_555 . 106_555 56.27(6) ?
Ga1' Sm1 Ge1' 150_555 . . 61.47(8) ?
Ga1' Sm1 Ge1' 150_555 . 49_555 119.99(8) ?
Ga1' Sm1 Ge1' 150_555 . 98_555 119.99(8) ?
Ga1' Sm1 Ge1' 150_555 . 146_555 58.53(8) ?
Ga1' Sm1 Ge1' 150_555 . 5_555 90.014(3) ?
Ga1' Sm1 Ge1' 150_555 . 101_555 90.014(3) ?
Ga1' Sm1 Ge1' 150_555 . 54_555 178.20(9) ?
Ga1' Sm1 Ge1' 150_555 . 150_555 0 ?
Ga1' Sm1 Ge1' 150_555 . 9_555 119.99(8) ?
Ga1' Sm1 Ge1' 150_555 . 153_555 58.53(8) ?
Ga1' Sm1 Ge1' 150_555 . 58_555 119.99(8) ?
Ga1' Sm1 Ge1' 150_555 . 106_555 61.47(8) ?
Ga1' Sm1 Ga1' 9_555 . 153_555 178.20(9) ?
Ga1' Sm1 Ga1' 9_555 . 58_555 90.014(3) ?
Ga1' Sm1 Ga1' 9_555 . 106_555 90.014(3) ?
Ga1' Sm1 Ge1 9_555 . . 63.90(5) ?
Ga1' Sm1 Ge1 9_555 . 49_555 125.26(6) ?
Ga1' Sm1 Ge1 9_555 . 98_555 56.27(6) ?
Ga1' Sm1 Ge1 9_555 . 146_555 114.70(5) ?
Ga1' Sm1 Ge1 9_555 . 5_555 63.90(5) ?
Ga1' Sm1 Ge1 9_555 . 101_555 125.26(6) ?
Ga1' Sm1 Ge1 9_555 . 54_555 56.27(6) ?
Ga1' Sm1 Ge1 9_555 . 150_555 114.70(5) ?
Ga1' Sm1 Ge1 9_555 . 9_555 6.48(7) ?
Ga1' Sm1 Ge1 9_555 . 153_555 175.32(7) ?
Ga1' Sm1 Ge1 9_555 . 58_555 89.913(7) ?
Ga1' Sm1 Ge1 9_555 . 106_555 89.913(7) ?
Ga1' Sm1 Ge1' 9_555 . . 58.53(8) ?
Ga1' Sm1 Ge1' 9_555 . 49_555 119.99(8) ?
Ga1' Sm1 Ge1' 9_555 . 98_555 61.47(8) ?
Ga1' Sm1 Ge1' 9_555 . 146_555 119.99(8) ?
Ga1' Sm1 Ge1' 9_555 . 5_555 58.53(8) ?
Ga1' Sm1 Ge1' 9_555 . 101_555 119.99(8) ?
Ga1' Sm1 Ge1' 9_555 . 54_555 61.47(8) ?
Ga1' Sm1 Ge1' 9_555 . 150_555 119.99(8) ?
Ga1' Sm1 Ge1' 9_555 . 9_555 0 ?
Ga1' Sm1 Ge1' 9_555 . 153_555 178.20(9) ?
Ga1' Sm1 Ge1' 9_555 . 58_555 90.014(3) ?
Ga1' Sm1 Ge1' 9_555 . 106_555 90.014(3) ?
Ga1' Sm1 Ga1' 153_555 . 58_555 90.014(3) ?
Ga1' Sm1 Ga1' 153_555 . 106_555 90.014(3) ?
Ga1' Sm1 Ge1 153_555 . . 114.70(5) ?
Ga1' Sm1 Ge1 153_555 . 49_555 56.27(6) ?
Ga1' Sm1 Ge1 153_555 . 98_555 125.26(6) ?
Ga1' Sm1 Ge1 153_555 . 146_555 63.90(5) ?
Ga1' Sm1 Ge1 153_555 . 5_555 114.70(5) ?
Ga1' Sm1 Ge1 153_555 . 101_555 56.27(6) ?
Ga1' Sm1 Ge1 153_555 . 54_555 125.26(6) ?
Ga1' Sm1 Ge1 153_555 . 150_555 63.90(5) ?
Ga1' Sm1 Ge1 153_555 . 9_555 175.32(7) ?
Ga1' Sm1 Ge1 153_555 . 153_555 6.48(7) ?
Ga1' Sm1 Ge1 153_555 . 58_555 89.913(7) ?
Ga1' Sm1 Ge1 153_555 . 106_555 89.913(7) ?
Ga1' Sm1 Ge1' 153_555 . . 119.99(8) ?
Ga1' Sm1 Ge1' 153_555 . 49_555 61.47(8) ?
Ga1' Sm1 Ge1' 153_555 . 98_555 119.99(8) ?
Ga1' Sm1 Ge1' 153_555 . 146_555 58.53(8) ?
Ga1' Sm1 Ge1' 153_555 . 5_555 119.99(8) ?
Ga1' Sm1 Ge1' 153_555 . 101_555 61.47(8) ?
Ga1' Sm1 Ge1' 153_555 . 54_555 119.99(8) ?
Ga1' Sm1 Ge1' 153_555 . 150_555 58.53(8) ?
Ga1' Sm1 Ge1' 153_555 . 9_555 178.20(9) ?
Ga1' Sm1 Ge1' 153_555 . 153_555 0 ?
Ga1' Sm1 Ge1' 153_555 . 58_555 90.014(3) ?
Ga1' Sm1 Ge1' 153_555 . 106_555 90.014(3) ?
Ga1' Sm1 Ga1' 58_555 . 106_555 178.20(9) ?
Ga1' Sm1 Ge1 58_555 . . 125.26(6) ?
Ga1' Sm1 Ge1 58_555 . 49_555 63.90(5) ?
Ga1' Sm1 Ge1 58_555 . 98_555 114.70(5) ?
Ga1' Sm1 Ge1 58_555 . 146_555 56.27(6) ?
Ga1' Sm1 Ge1 58_555 . 5_555 56.27(6) ?
Ga1' Sm1 Ge1 58_555 . 101_555 114.70(5) ?
Ga1' Sm1 Ge1 58_555 . 54_555 63.90(5) ?
Ga1' Sm1 Ge1 58_555 . 150_555 125.26(6) ?
Ga1' Sm1 Ge1 58_555 . 9_555 89.913(7) ?
Ga1' Sm1 Ge1 58_555 . 153_555 89.913(7) ?
Ga1' Sm1 Ge1 58_555 . 58_555 6.48(7) ?
Ga1' Sm1 Ge1 58_555 . 106_555 175.32(7) ?
Ga1' Sm1 Ge1' 58_555 . . 119.99(8) ?
Ga1' Sm1 Ge1' 58_555 . 49_555 58.53(8) ?
Ga1' Sm1 Ge1' 58_555 . 98_555 119.99(8) ?
Ga1' Sm1 Ge1' 58_555 . 146_555 61.47(8) ?
Ga1' Sm1 Ge1' 58_555 . 5_555 61.47(8) ?
Ga1' Sm1 Ge1' 58_555 . 101_555 119.99(8) ?
Ga1' Sm1 Ge1' 58_555 . 54_555 58.53(8) ?
Ga1' Sm1 Ge1' 58_555 . 150_555 119.99(8) ?
Ga1' Sm1 Ge1' 58_555 . 9_555 90.014(3) ?
Ga1' Sm1 Ge1' 58_555 . 153_555 90.014(3) ?
Ga1' Sm1 Ge1' 58_555 . 58_555 0 ?
Ga1' Sm1 Ge1' 58_555 . 106_555 178.20(9) ?
Ga1' Sm1 Ge1 106_555 . . 56.27(6) ?
Ga1' Sm1 Ge1 106_555 . 49_555 114.70(5) ?
Ga1' Sm1 Ge1 106_555 . 98_555 63.90(5) ?
Ga1' Sm1 Ge1 106_555 . 146_555 125.26(6) ?
Ga1' Sm1 Ge1 106_555 . 5_555 125.26(6) ?
Ga1' Sm1 Ge1 106_555 . 101_555 63.90(5) ?
Ga1' Sm1 Ge1 106_555 . 54_555 114.70(5) ?
Ga1' Sm1 Ge1 106_555 . 150_555 56.27(6) ?
Ga1' Sm1 Ge1 106_555 . 9_555 89.913(7) ?
Ga1' Sm1 Ge1 106_555 . 153_555 89.913(7) ?
Ga1' Sm1 Ge1 106_555 . 58_555 175.32(7) ?
Ga1' Sm1 Ge1 106_555 . 106_555 6.48(7) ?
Ga1' Sm1 Ge1' 106_555 . . 61.47(8) ?
Ga1' Sm1 Ge1' 106_555 . 49_555 119.99(8) ?
Ga1' Sm1 Ge1' 106_555 . 98_555 58.53(8) ?
Ga1' Sm1 Ge1' 106_555 . 146_555 119.99(8) ?
Ga1' Sm1 Ge1' 106_555 . 5_555 119.99(8) ?
Ga1' Sm1 Ge1' 106_555 . 101_555 58.53(8) ?
Ga1' Sm1 Ge1' 106_555 . 54_555 119.99(8) ?
Ga1' Sm1 Ge1' 106_555 . 150_555 61.47(8) ?
Ga1' Sm1 Ge1' 106_555 . 9_555 90.014(3) ?
Ga1' Sm1 Ge1' 106_555 . 153_555 90.014(3) ?
Ga1' Sm1 Ge1' 106_555 . 58_555 178.20(9) ?
Ga1' Sm1 Ge1' 106_555 . 106_555 0 ?
Ge1 Sm1 Ge1 . . 49_555 168.84(3) ?
Ge1 Sm1 Ge1 . . 98_555 90.541(4) ?
Ge1 Sm1 Ge1 . . 146_555 90.541(4) ?
Ge1 Sm1 Ge1 . . 5_555 68.99(2) ?
Ge1 Sm1 Ge1 . . 101_555 119.69(2) ?
Ge1 Sm1 Ge1 . . 54_555 119.69(2) ?
Ge1 Sm1 Ge1 . . 150_555 50.80(2) ?
Ge1 Sm1 Ge1 . . 9_555 68.99(2) ?
Ge1 Sm1 Ge1 . . 153_555 119.69(2) ?
Ge1 Sm1 Ge1 . . 58_555 119.69(2) ?
Ge1 Sm1 Ge1 . . 106_555 50.80(2) ?
Ge1 Sm1 Ge1' . . . 6.48(7) ?
Ge1 Sm1 Ge1' . . 49_555 175.32(7) ?
Ge1 Sm1 Ge1' . . 98_555 89.913(7) ?
Ge1 Sm1 Ge1' . . 146_555 89.913(7) ?
Ge1 Sm1 Ge1' . . 5_555 63.90(5) ?
Ge1 Sm1 Ge1' . . 101_555 114.70(5) ?
Ge1 Sm1 Ge1' . . 54_555 125.26(6) ?
Ge1 Sm1 Ge1' . . 150_555 56.27(6) ?
Ge1 Sm1 Ge1' . . 9_555 63.90(5) ?
Ge1 Sm1 Ge1' . . 153_555 114.70(5) ?
Ge1 Sm1 Ge1' . . 58_555 125.26(6) ?
Ge1 Sm1 Ge1' . . 106_555 56.27(6) ?
Ge1 Sm1 Ge1 49_555 . 98_555 90.541(4) ?
Ge1 Sm1 Ge1 49_555 . 146_555 90.541(4) ?
Ge1 Sm1 Ge1 49_555 . 5_555 119.69(2) ?
Ge1 Sm1 Ge1 49_555 . 101_555 50.80(2) ?
Ge1 Sm1 Ge1 49_555 . 54_555 68.99(2) ?
Ge1 Sm1 Ge1 49_555 . 150_555 119.69(2) ?
Ge1 Sm1 Ge1 49_555 . 9_555 119.69(2) ?
Ge1 Sm1 Ge1 49_555 . 153_555 50.80(2) ?
Ge1 Sm1 Ge1 49_555 . 58_555 68.99(2) ?
Ge1 Sm1 Ge1 49_555 . 106_555 119.69(2) ?
Ge1 Sm1 Ge1' 49_555 . . 175.32(7) ?
Ge1 Sm1 Ge1' 49_555 . 49_555 6.48(7) ?
Ge1 Sm1 Ge1' 49_555 . 98_555 89.913(7) ?
Ge1 Sm1 Ge1' 49_555 . 146_555 89.913(7) ?
Ge1 Sm1 Ge1' 49_555 . 5_555 125.26(6) ?
Ge1 Sm1 Ge1' 49_555 . 101_555 56.27(6) ?
Ge1 Sm1 Ge1' 49_555 . 54_555 63.90(5) ?
Ge1 Sm1 Ge1' 49_555 . 150_555 114.70(5) ?
Ge1 Sm1 Ge1' 49_555 . 9_555 125.26(6) ?
Ge1 Sm1 Ge1' 49_555 . 153_555 56.27(6) ?
Ge1 Sm1 Ge1' 49_555 . 58_555 63.90(5) ?
Ge1 Sm1 Ge1' 49_555 . 106_555 114.70(5) ?
Ge1 Sm1 Ge1 98_555 . 146_555 168.84(3) ?
Ge1 Sm1 Ge1 98_555 . 5_555 119.69(2) ?
Ge1 Sm1 Ge1 98_555 . 101_555 68.99(2) ?
Ge1 Sm1 Ge1 98_555 . 54_555 50.80(2) ?
Ge1 Sm1 Ge1 98_555 . 150_555 119.69(2) ?
Ge1 Sm1 Ge1 98_555 . 9_555 50.80(2) ?
Ge1 Sm1 Ge1 98_555 . 153_555 119.69(2) ?
Ge1 Sm1 Ge1 98_555 . 58_555 119.69(2) ?
Ge1 Sm1 Ge1 98_555 . 106_555 68.99(2) ?
Ge1 Sm1 Ge1' 98_555 . . 89.913(7) ?
Ge1 Sm1 Ge1' 98_555 . 49_555 89.913(7) ?
Ge1 Sm1 Ge1' 98_555 . 98_555 6.48(7) ?
Ge1 Sm1 Ge1' 98_555 . 146_555 175.32(7) ?
Ge1 Sm1 Ge1' 98_555 . 5_555 114.70(5) ?
Ge1 Sm1 Ge1' 98_555 . 101_555 63.90(5) ?
Ge1 Sm1 Ge1' 98_555 . 54_555 56.27(6) ?
Ge1 Sm1 Ge1' 98_555 . 150_555 125.26(6) ?
Ge1 Sm1 Ge1' 98_555 . 9_555 56.27(6) ?
Ge1 Sm1 Ge1' 98_555 . 153_555 125.26(6) ?
Ge1 Sm1 Ge1' 98_555 . 58_555 114.70(5) ?
Ge1 Sm1 Ge1' 98_555 . 106_555 63.90(5) ?
Ge1 Sm1 Ge1 146_555 . 5_555 50.80(2) ?
Ge1 Sm1 Ge1 146_555 . 101_555 119.69(2) ?
Ge1 Sm1 Ge1 146_555 . 54_555 119.69(2) ?
Ge1 Sm1 Ge1 146_555 . 150_555 68.99(2) ?
Ge1 Sm1 Ge1 146_555 . 9_555 119.69(2) ?
Ge1 Sm1 Ge1 146_555 . 153_555 68.99(2) ?
Ge1 Sm1 Ge1 146_555 . 58_555 50.80(2) ?
Ge1 Sm1 Ge1 146_555 . 106_555 119.69(2) ?
Ge1 Sm1 Ge1' 146_555 . . 89.913(7) ?
Ge1 Sm1 Ge1' 146_555 . 49_555 89.913(7) ?
Ge1 Sm1 Ge1' 146_555 . 98_555 175.32(7) ?
Ge1 Sm1 Ge1' 146_555 . 146_555 6.48(7) ?
Ge1 Sm1 Ge1' 146_555 . 5_555 56.27(6) ?
Ge1 Sm1 Ge1' 146_555 . 101_555 125.26(6) ?
Ge1 Sm1 Ge1' 146_555 . 54_555 114.70(5) ?
Ge1 Sm1 Ge1' 146_555 . 150_555 63.90(5) ?
Ge1 Sm1 Ge1' 146_555 . 9_555 114.70(5) ?
Ge1 Sm1 Ge1' 146_555 . 153_555 63.90(5) ?
Ge1 Sm1 Ge1' 146_555 . 58_555 56.27(6) ?
Ge1 Sm1 Ge1' 146_555 . 106_555 125.26(6) ?
Ge1 Sm1 Ge1 5_555 . 101_555 168.84(3) ?
Ge1 Sm1 Ge1 5_555 . 54_555 90.541(4) ?
Ge1 Sm1 Ge1 5_555 . 150_555 90.541(4) ?
Ge1 Sm1 Ge1 5_555 . 9_555 68.99(2) ?
Ge1 Sm1 Ge1 5_555 . 153_555 119.69(2) ?
Ge1 Sm1 Ge1 5_555 . 58_555 50.80(2) ?
Ge1 Sm1 Ge1 5_555 . 106_555 119.69(2) ?
Ge1 Sm1 Ge1' 5_555 . . 63.90(5) ?
Ge1 Sm1 Ge1' 5_555 . 49_555 114.70(5) ?
Ge1 Sm1 Ge1' 5_555 . 98_555 125.26(6) ?
Ge1 Sm1 Ge1' 5_555 . 146_555 56.27(6) ?
Ge1 Sm1 Ge1' 5_555 . 5_555 6.48(7) ?
Ge1 Sm1 Ge1' 5_555 . 101_555 175.32(7) ?
Ge1 Sm1 Ge1' 5_555 . 54_555 89.913(7) ?
Ge1 Sm1 Ge1' 5_555 . 150_555 89.913(7) ?
Ge1 Sm1 Ge1' 5_555 . 9_555 63.90(5) ?
Ge1 Sm1 Ge1' 5_555 . 153_555 114.70(5) ?
Ge1 Sm1 Ge1' 5_555 . 58_555 56.27(6) ?
Ge1 Sm1 Ge1' 5_555 . 106_555 125.26(6) ?
Ge1 Sm1 Ge1 101_555 . 54_555 90.541(4) ?
Ge1 Sm1 Ge1 101_555 . 150_555 90.541(4) ?
Ge1 Sm1 Ge1 101_555 . 9_555 119.69(2) ?
Ge1 Sm1 Ge1 101_555 . 153_555 50.80(2) ?
Ge1 Sm1 Ge1 101_555 . 58_555 119.69(2) ?
Ge1 Sm1 Ge1 101_555 . 106_555 68.99(2) ?
Ge1 Sm1 Ge1' 101_555 . . 125.26(6) ?
Ge1 Sm1 Ge1' 101_555 . 49_555 56.27(6) ?
Ge1 Sm1 Ge1' 101_555 . 98_555 63.90(5) ?
Ge1 Sm1 Ge1' 101_555 . 146_555 114.70(5) ?
Ge1 Sm1 Ge1' 101_555 . 5_555 175.32(7) ?
Ge1 Sm1 Ge1' 101_555 . 101_555 6.48(7) ?
Ge1 Sm1 Ge1' 101_555 . 54_555 89.913(7) ?
Ge1 Sm1 Ge1' 101_555 . 150_555 89.913(7) ?
Ge1 Sm1 Ge1' 101_555 . 9_555 125.26(6) ?
Ge1 Sm1 Ge1' 101_555 . 153_555 56.27(6) ?
Ge1 Sm1 Ge1' 101_555 . 58_555 114.70(5) ?
Ge1 Sm1 Ge1' 101_555 . 106_555 63.90(5) ?
Ge1 Sm1 Ge1 54_555 . 150_555 168.84(3) ?
Ge1 Sm1 Ge1 54_555 . 9_555 50.80(2) ?
Ge1 Sm1 Ge1 54_555 . 153_555 119.69(2) ?
Ge1 Sm1 Ge1 54_555 . 58_555 68.99(2) ?
Ge1 Sm1 Ge1 54_555 . 106_555 119.69(2) ?
Ge1 Sm1 Ge1' 54_555 . . 114.70(5) ?
Ge1 Sm1 Ge1' 54_555 . 49_555 63.90(5) ?
Ge1 Sm1 Ge1' 54_555 . 98_555 56.27(6) ?
Ge1 Sm1 Ge1' 54_555 . 146_555 125.26(6) ?
Ge1 Sm1 Ge1' 54_555 . 5_555 89.913(7) ?
Ge1 Sm1 Ge1' 54_555 . 101_555 89.913(7) ?
Ge1 Sm1 Ge1' 54_555 . 54_555 6.48(7) ?
Ge1 Sm1 Ge1' 54_555 . 150_555 175.32(7) ?
Ge1 Sm1 Ge1' 54_555 . 9_555 56.27(6) ?
Ge1 Sm1 Ge1' 54_555 . 153_555 125.26(6) ?
Ge1 Sm1 Ge1' 54_555 . 58_555 63.90(5) ?
Ge1 Sm1 Ge1' 54_555 . 106_555 114.70(5) ?
Ge1 Sm1 Ge1 150_555 . 9_555 119.69(2) ?
Ge1 Sm1 Ge1 150_555 . 153_555 68.99(2) ?
Ge1 Sm1 Ge1 150_555 . 58_555 119.69(2) ?
Ge1 Sm1 Ge1 150_555 . 106_555 50.80(2) ?
Ge1 Sm1 Ge1' 150_555 . . 56.27(6) ?
Ge1 Sm1 Ge1' 150_555 . 49_555 125.26(6) ?
Ge1 Sm1 Ge1' 150_555 . 98_555 114.70(5) ?
Ge1 Sm1 Ge1' 150_555 . 146_555 63.90(5) ?
Ge1 Sm1 Ge1' 150_555 . 5_555 89.913(7) ?
Ge1 Sm1 Ge1' 150_555 . 101_555 89.913(7) ?
Ge1 Sm1 Ge1' 150_555 . 54_555 175.32(7) ?
Ge1 Sm1 Ge1' 150_555 . 150_555 6.48(7) ?
Ge1 Sm1 Ge1' 150_555 . 9_555 114.70(5) ?
Ge1 Sm1 Ge1' 150_555 . 153_555 63.90(5) ?
Ge1 Sm1 Ge1' 150_555 . 58_555 125.26(6) ?
Ge1 Sm1 Ge1' 150_555 . 106_555 56.27(6) ?
Ge1 Sm1 Ge1 9_555 . 153_555 168.84(3) ?
Ge1 Sm1 Ge1 9_555 . 58_555 90.541(4) ?
Ge1 Sm1 Ge1 9_555 . 106_555 90.541(4) ?
Ge1 Sm1 Ge1' 9_555 . . 63.90(5) ?
Ge1 Sm1 Ge1' 9_555 . 49_555 114.70(5) ?
Ge1 Sm1 Ge1' 9_555 . 98_555 56.27(6) ?
Ge1 Sm1 Ge1' 9_555 . 146_555 125.26(6) ?
Ge1 Sm1 Ge1' 9_555 . 5_555 63.90(5) ?
Ge1 Sm1 Ge1' 9_555 . 101_555 114.70(5) ?
Ge1 Sm1 Ge1' 9_555 . 54_555 56.27(6) ?
Ge1 Sm1 Ge1' 9_555 . 150_555 125.26(6) ?
Ge1 Sm1 Ge1' 9_555 . 9_555 6.48(7) ?
Ge1 Sm1 Ge1' 9_555 . 153_555 175.32(7) ?
Ge1 Sm1 Ge1' 9_555 . 58_555 89.913(7) ?
Ge1 Sm1 Ge1' 9_555 . 106_555 89.913(7) ?
Ge1 Sm1 Ge1 153_555 . 58_555 90.541(4) ?
Ge1 Sm1 Ge1 153_555 . 106_555 90.541(4) ?
Ge1 Sm1 Ge1' 153_555 . . 125.26(6) ?
Ge1 Sm1 Ge1' 153_555 . 49_555 56.27(6) ?
Ge1 Sm1 Ge1' 153_555 . 98_555 114.70(5) ?
Ge1 Sm1 Ge1' 153_555 . 146_555 63.90(5) ?
Ge1 Sm1 Ge1' 153_555 . 5_555 125.26(6) ?
Ge1 Sm1 Ge1' 153_555 . 101_555 56.27(6) ?
Ge1 Sm1 Ge1' 153_555 . 54_555 114.70(5) ?
Ge1 Sm1 Ge1' 153_555 . 150_555 63.90(5) ?
Ge1 Sm1 Ge1' 153_555 . 9_555 175.32(7) ?
Ge1 Sm1 Ge1' 153_555 . 153_555 6.48(7) ?
Ge1 Sm1 Ge1' 153_555 . 58_555 89.913(7) ?
Ge1 Sm1 Ge1' 153_555 . 106_555 89.913(7) ?
Ge1 Sm1 Ge1 58_555 . 106_555 168.84(3) ?
Ge1 Sm1 Ge1' 58_555 . . 114.70(5) ?
Ge1 Sm1 Ge1' 58_555 . 49_555 63.90(5) ?
Ge1 Sm1 Ge1' 58_555 . 98_555 125.26(6) ?
Ge1 Sm1 Ge1' 58_555 . 146_555 56.27(6) ?
Ge1 Sm1 Ge1' 58_555 . 5_555 56.27(6) ?
Ge1 Sm1 Ge1' 58_555 . 101_555 125.26(6) ?
Ge1 Sm1 Ge1' 58_555 . 54_555 63.90(5) ?
Ge1 Sm1 Ge1' 58_555 . 150_555 114.70(5) ?
Ge1 Sm1 Ge1' 58_555 . 9_555 89.913(7) ?
Ge1 Sm1 Ge1' 58_555 . 153_555 89.913(7) ?
Ge1 Sm1 Ge1' 58_555 . 58_555 6.48(7) ?
Ge1 Sm1 Ge1' 58_555 . 106_555 175.32(7) ?
Ge1 Sm1 Ge1' 106_555 . . 56.27(6) ?
Ge1 Sm1 Ge1' 106_555 . 49_555 125.26(6) ?
Ge1 Sm1 Ge1' 106_555 . 98_555 63.90(5) ?
Ge1 Sm1 Ge1' 106_555 . 146_555 114.70(5) ?
Ge1 Sm1 Ge1' 106_555 . 5_555 114.70(5) ?
Ge1 Sm1 Ge1' 106_555 . 101_555 63.90(5) ?
Ge1 Sm1 Ge1' 106_555 . 54_555 125.26(6) ?
Ge1 Sm1 Ge1' 106_555 . 150_555 56.27(6) ?
Ge1 Sm1 Ge1' 106_555 . 9_555 89.913(7) ?
Ge1 Sm1 Ge1' 106_555 . 153_555 89.913(7) ?
Ge1 Sm1 Ge1' 106_555 . 58_555 175.32(7) ?
Ge1 Sm1 Ge1' 106_555 . 106_555 6.48(7) ?
Ge1' Sm1 Ge1' . . 49_555 178.20(9) ?
Ge1' Sm1 Ge1' . . 98_555 90.014(3) ?
Ge1' Sm1 Ge1' . . 146_555 90.014(3) ?
Ge1' Sm1 Ge1' . . 5_555 58.53(8) ?
Ge1' Sm1 Ge1' . . 101_555 119.99(8) ?
Ge1' Sm1 Ge1' . . 54_555 119.99(8) ?
Ge1' Sm1 Ge1' . . 150_555 61.47(8) ?
Ge1' Sm1 Ge1' . . 9_555 58.53(8) ?
Ge1' Sm1 Ge1' . . 153_555 119.99(8) ?
Ge1' Sm1 Ge1' . . 58_555 119.99(8) ?
Ge1' Sm1 Ge1' . . 106_555 61.47(8) ?
Ge1' Sm1 Ge1' 49_555 . 98_555 90.014(3) ?
Ge1' Sm1 Ge1' 49_555 . 146_555 90.014(3) ?
Ge1' Sm1 Ge1' 49_555 . 5_555 119.99(8) ?
Ge1' Sm1 Ge1' 49_555 . 101_555 61.47(8) ?
Ge1' Sm1 Ge1' 49_555 . 54_555 58.53(8) ?
Ge1' Sm1 Ge1' 49_555 . 150_555 119.99(8) ?
Ge1' Sm1 Ge1' 49_555 . 9_555 119.99(8) ?
Ge1' Sm1 Ge1' 49_555 . 153_555 61.47(8) ?
Ge1' Sm1 Ge1' 49_555 . 58_555 58.53(8) ?
Ge1' Sm1 Ge1' 49_555 . 106_555 119.99(8) ?
Ge1' Sm1 Ge1' 98_555 . 146_555 178.20(9) ?
Ge1' Sm1 Ge1' 98_555 . 5_555 119.99(8) ?
Ge1' Sm1 Ge1' 98_555 . 101_555 58.53(8) ?
Ge1' Sm1 Ge1' 98_555 . 54_555 61.47(8) ?
Ge1' Sm1 Ge1' 98_555 . 150_555 119.99(8) ?
Ge1' Sm1 Ge1' 98_555 . 9_555 61.47(8) ?
Ge1' Sm1 Ge1' 98_555 . 153_555 119.99(8) ?
Ge1' Sm1 Ge1' 98_555 . 58_555 119.99(8) ?
Ge1' Sm1 Ge1' 98_555 . 106_555 58.53(8) ?
Ge1' Sm1 Ge1' 146_555 . 5_555 61.47(8) ?
Ge1' Sm1 Ge1' 146_555 . 101_555 119.99(8) ?
Ge1' Sm1 Ge1' 146_555 . 54_555 119.99(8) ?
Ge1' Sm1 Ge1' 146_555 . 150_555 58.53(8) ?
Ge1' Sm1 Ge1' 146_555 . 9_555 119.99(8) ?
Ge1' Sm1 Ge1' 146_555 . 153_555 58.53(8) ?
Ge1' Sm1 Ge1' 146_555 . 58_555 61.47(8) ?
Ge1' Sm1 Ge1' 146_555 . 106_555 119.99(8) ?
Ge1' Sm1 Ge1' 5_555 . 101_555 178.20(9) ?
Ge1' Sm1 Ge1' 5_555 . 54_555 90.014(3) ?
Ge1' Sm1 Ge1' 5_555 . 150_555 90.014(3) ?
Ge1' Sm1 Ge1' 5_555 . 9_555 58.53(8) ?
Ge1' Sm1 Ge1' 5_555 . 153_555 119.99(8) ?
Ge1' Sm1 Ge1' 5_555 . 58_555 61.47(8) ?
Ge1' Sm1 Ge1' 5_555 . 106_555 119.99(8) ?
Ge1' Sm1 Ge1' 101_555 . 54_555 90.014(3) ?
Ge1' Sm1 Ge1' 101_555 . 150_555 90.014(3) ?
Ge1' Sm1 Ge1' 101_555 . 9_555 119.99(8) ?
Ge1' Sm1 Ge1' 101_555 . 153_555 61.47(8) ?
Ge1' Sm1 Ge1' 101_555 . 58_555 119.99(8) ?
Ge1' Sm1 Ge1' 101_555 . 106_555 58.53(8) ?
Ge1' Sm1 Ge1' 54_555 . 150_555 178.20(9) ?
Ge1' Sm1 Ge1' 54_555 . 9_555 61.47(8) ?
Ge1' Sm1 Ge1' 54_555 . 153_555 119.99(8) ?
Ge1' Sm1 Ge1' 54_555 . 58_555 58.53(8) ?
Ge1' Sm1 Ge1' 54_555 . 106_555 119.99(8) ?
Ge1' Sm1 Ge1' 150_555 . 9_555 119.99(8) ?
Ge1' Sm1 Ge1' 150_555 . 153_555 58.53(8) ?
Ge1' Sm1 Ge1' 150_555 . 58_555 119.99(8) ?
Ge1' Sm1 Ge1' 150_555 . 106_555 61.47(8) ?
Ge1' Sm1 Ge1' 9_555 . 153_555 178.20(9) ?
Ge1' Sm1 Ge1' 9_555 . 58_555 90.014(3) ?
Ge1' Sm1 Ge1' 9_555 . 106_555 90.014(3) ?
Ge1' Sm1 Ge1' 153_555 . 58_555 90.014(3) ?
Ge1' Sm1 Ge1' 153_555 . 106_555 90.014(3) ?
Ge1' Sm1 Ge1' 58_555 . 106_555 178.20(9) ?
Sm1 Mn1 Sm1 . . 49_544 109.471(2) ?
Sm1 Mn1 Sm1 . . 97_454 109.471(2) ?
Sm1 Mn1 Sm1 . . 145_445 109.471(2) ?
Sm1 Mn1 Sm1 . . 13_555 70.529(2) ?
Sm1 Mn1 Sm1 . . 61_545 70.529(2) ?
Sm1 Mn1 Sm1 . . 109_455 70.529(2) ?
Sm1 Mn1 Sm1 . . 157_445 180 ?
Sm1 Mn1 Ga1 . . . 54.7356(11) ?
Sm1 Mn1 Ga1 . . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 . . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 . . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 . . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 . . 10_555 125.2644(11) ?
Sm1 Mn1 Ga1' . . . 54.7356(11) ?
Sm1 Mn1 Ga1' . . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1' . . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1' . . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1' . . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1' . . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 . . . 54.7356(11) ?
Sm1 Mn1 Ge1 . . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 . . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 . . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 . . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 . . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1' . . . 54.7356(11) ?
Sm1 Mn1 Ge1' . . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1' . . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1' . . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1' . . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1' . . 10_555 125.2644(11) ?
Sm1 Mn1 Sm1 49_544 . 97_454 109.471(2) ?
Sm1 Mn1 Sm1 49_544 . 145_445 109.471(2) ?
Sm1 Mn1 Sm1 49_544 . 13_555 70.529(2) ?
Sm1 Mn1 Sm1 49_544 . 61_545 70.529(2) ?
Sm1 Mn1 Sm1 49_544 . 109_455 180 ?
Sm1 Mn1 Sm1 49_544 . 157_445 70.529(2) ?
Sm1 Mn1 Ga1 49_544 . . 54.7356(11) ?
Sm1 Mn1 Ga1 49_544 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 49_544 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 49_544 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 49_544 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 49_544 . 10_555 54.7356(11) ?
Sm1 Mn1 Ga1' 49_544 . . 54.7356(11) ?
Sm1 Mn1 Ga1' 49_544 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1' 49_544 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1' 49_544 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1' 49_544 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1' 49_544 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 49_544 . . 54.7356(11) ?
Sm1 Mn1 Ge1 49_544 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 49_544 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 49_544 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 49_544 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 49_544 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1' 49_544 . . 54.7356(11) ?
Sm1 Mn1 Ge1' 49_544 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1' 49_544 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1' 49_544 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1' 49_544 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1' 49_544 . 10_555 54.7356(11) ?
Sm1 Mn1 Sm1 97_454 . 145_445 109.471(2) ?
Sm1 Mn1 Sm1 97_454 . 13_555 70.529(2) ?
Sm1 Mn1 Sm1 97_454 . 61_545 180 ?
Sm1 Mn1 Sm1 97_454 . 109_455 70.529(2) ?
Sm1 Mn1 Sm1 97_454 . 157_445 70.529(2) ?
Sm1 Mn1 Ga1 97_454 . . 125.2644(11) ?
Sm1 Mn1 Ga1 97_454 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 97_454 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 97_454 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 97_454 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 97_454 . 10_555 54.7356(11) ?
Sm1 Mn1 Ga1' 97_454 . . 125.2644(11) ?
Sm1 Mn1 Ga1' 97_454 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1' 97_454 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1' 97_454 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1' 97_454 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1' 97_454 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 97_454 . . 125.2644(11) ?
Sm1 Mn1 Ge1 97_454 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 97_454 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 97_454 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 97_454 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 97_454 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1' 97_454 . . 125.2644(11) ?
Sm1 Mn1 Ge1' 97_454 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1' 97_454 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1' 97_454 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1' 97_454 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1' 97_454 . 10_555 54.7356(11) ?
Sm1 Mn1 Sm1 145_445 . 13_555 180 ?
Sm1 Mn1 Sm1 145_445 . 61_545 70.529(2) ?
Sm1 Mn1 Sm1 145_445 . 109_455 70.529(2) ?
Sm1 Mn1 Sm1 145_445 . 157_445 70.529(2) ?
Sm1 Mn1 Ga1 145_445 . . 125.2644(11) ?
Sm1 Mn1 Ga1 145_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 145_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 145_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 145_445 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 145_445 . 10_555 125.2644(11) ?
Sm1 Mn1 Ga1' 145_445 . . 125.2644(11) ?
Sm1 Mn1 Ga1' 145_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1' 145_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1' 145_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1' 145_445 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1' 145_445 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 145_445 . . 125.2644(11) ?
Sm1 Mn1 Ge1 145_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 145_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 145_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 145_445 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 145_445 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1' 145_445 . . 125.2644(11) ?
Sm1 Mn1 Ge1' 145_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1' 145_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1' 145_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1' 145_445 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1' 145_445 . 10_555 125.2644(11) ?
Sm1 Mn1 Sm1 13_555 . 61_545 109.471(2) ?
Sm1 Mn1 Sm1 13_555 . 109_455 109.471(2) ?
Sm1 Mn1 Sm1 13_555 . 157_445 109.471(2) ?
Sm1 Mn1 Ga1 13_555 . . 54.7356(11) ?
Sm1 Mn1 Ga1 13_555 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 13_555 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 13_555 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 13_555 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 13_555 . 10_555 54.7356(11) ?
Sm1 Mn1 Ga1' 13_555 . . 54.7356(11) ?
Sm1 Mn1 Ga1' 13_555 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1' 13_555 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1' 13_555 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1' 13_555 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1' 13_555 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 13_555 . . 54.7356(11) ?
Sm1 Mn1 Ge1 13_555 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 13_555 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 13_555 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 13_555 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 13_555 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1' 13_555 . . 54.7356(11) ?
Sm1 Mn1 Ge1' 13_555 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1' 13_555 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1' 13_555 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1' 13_555 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1' 13_555 . 10_555 54.7356(11) ?
Sm1 Mn1 Sm1 61_545 . 109_455 109.471(2) ?
Sm1 Mn1 Sm1 61_545 . 157_445 109.471(2) ?
Sm1 Mn1 Ga1 61_545 . . 54.7356(11) ?
Sm1 Mn1 Ga1 61_545 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 61_545 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 61_545 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 61_545 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 61_545 . 10_555 125.2644(11) ?
Sm1 Mn1 Ga1' 61_545 . . 54.7356(11) ?
Sm1 Mn1 Ga1' 61_545 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1' 61_545 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1' 61_545 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1' 61_545 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1' 61_545 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 61_545 . . 54.7356(11) ?
Sm1 Mn1 Ge1 61_545 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 61_545 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 61_545 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 61_545 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 61_545 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1' 61_545 . . 54.7356(11) ?
Sm1 Mn1 Ge1' 61_545 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1' 61_545 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1' 61_545 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1' 61_545 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1' 61_545 . 10_555 125.2644(11) ?
Sm1 Mn1 Sm1 109_455 . 157_445 109.471(2) ?
Sm1 Mn1 Ga1 109_455 . . 125.2644(11) ?
Sm1 Mn1 Ga1 109_455 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 109_455 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 109_455 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 109_455 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 109_455 . 10_555 125.2644(11) ?
Sm1 Mn1 Ga1' 109_455 . . 125.2644(11) ?
Sm1 Mn1 Ga1' 109_455 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1' 109_455 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1' 109_455 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1' 109_455 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1' 109_455 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 109_455 . . 125.2644(11) ?
Sm1 Mn1 Ge1 109_455 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 109_455 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 109_455 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 109_455 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 109_455 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1' 109_455 . . 125.2644(11) ?
Sm1 Mn1 Ge1' 109_455 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1' 109_455 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1' 109_455 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1' 109_455 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1' 109_455 . 10_555 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . . 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 157_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 157_445 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . 10_555 54.7356(11) ?
Sm1 Mn1 Ga1' 157_445 . . 125.2644(11) ?
Sm1 Mn1 Ga1' 157_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1' 157_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1' 157_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1' 157_445 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1' 157_445 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 157_445 . . 125.2644(11) ?
Sm1 Mn1 Ge1 157_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 157_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 157_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 157_445 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 157_445 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1' 157_445 . . 125.2644(11) ?
Sm1 Mn1 Ge1' 157_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1' 157_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1' 157_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1' 157_445 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1' 157_445 . 10_555 54.7356(11) ?
Ga1 Mn1 Ga1 . . 2_555 180 ?
Ga1 Mn1 Ga1 . . 5_555 90 ?
Ga1 Mn1 Ga1 . . 6_555 90 ?
Ga1 Mn1 Ga1 . . 9_555 90 ?
Ga1 Mn1 Ga1 . . 10_555 90 ?
Ga1 Mn1 Ga1' . . . 0 ?
Ga1 Mn1 Ga1' . . 2_555 180 ?
Ga1 Mn1 Ga1' . . 5_555 90 ?
Ga1 Mn1 Ga1' . . 6_555 90 ?
Ga1 Mn1 Ga1' . . 9_555 90 ?
Ga1 Mn1 Ga1' . . 10_555 90 ?
Ga1 Mn1 Ge1 . . . 0 ?
Ga1 Mn1 Ge1 . . 2_555 180 ?
Ga1 Mn1 Ge1 . . 5_555 90 ?
Ga1 Mn1 Ge1 . . 6_555 90 ?
Ga1 Mn1 Ge1 . . 9_555 90 ?
Ga1 Mn1 Ge1 . . 10_555 90 ?
Ga1 Mn1 Ge1' . . . 0 ?
Ga1 Mn1 Ge1' . . 2_555 180 ?
Ga1 Mn1 Ge1' . . 5_555 90 ?
Ga1 Mn1 Ge1' . . 6_555 90 ?
Ga1 Mn1 Ge1' . . 9_555 90 ?
Ga1 Mn1 Ge1' . . 10_555 90 ?
Ga1 Mn1 Ga1 2_555 . 5_555 90 ?
Ga1 Mn1 Ga1 2_555 . 6_555 90 ?
Ga1 Mn1 Ga1 2_555 . 9_555 90 ?
Ga1 Mn1 Ga1 2_555 . 10_555 90 ?
Ga1 Mn1 Ga1' 2_555 . . 180 ?
Ga1 Mn1 Ga1' 2_555 . 2_555 0 ?
Ga1 Mn1 Ga1' 2_555 . 5_555 90 ?
Ga1 Mn1 Ga1' 2_555 . 6_555 90 ?
Ga1 Mn1 Ga1' 2_555 . 9_555 90 ?
Ga1 Mn1 Ga1' 2_555 . 10_555 90 ?
Ga1 Mn1 Ge1 2_555 . . 180 ?
Ga1 Mn1 Ge1 2_555 . 2_555 0 ?
Ga1 Mn1 Ge1 2_555 . 5_555 90 ?
Ga1 Mn1 Ge1 2_555 . 6_555 90 ?
Ga1 Mn1 Ge1 2_555 . 9_555 90 ?
Ga1 Mn1 Ge1 2_555 . 10_555 90 ?
Ga1 Mn1 Ge1' 2_555 . . 180 ?
Ga1 Mn1 Ge1' 2_555 . 2_555 0 ?
Ga1 Mn1 Ge1' 2_555 . 5_555 90 ?
Ga1 Mn1 Ge1' 2_555 . 6_555 90 ?
Ga1 Mn1 Ge1' 2_555 . 9_555 90 ?
Ga1 Mn1 Ge1' 2_555 . 10_555 90 ?
Ga1 Mn1 Ga1 5_555 . 6_555 180 ?
Ga1 Mn1 Ga1 5_555 . 9_555 90 ?
Ga1 Mn1 Ga1 5_555 . 10_555 90 ?
Ga1 Mn1 Ga1' 5_555 . . 90 ?
Ga1 Mn1 Ga1' 5_555 . 2_555 90 ?
Ga1 Mn1 Ga1' 5_555 . 5_555 0 ?
Ga1 Mn1 Ga1' 5_555 . 6_555 180 ?
Ga1 Mn1 Ga1' 5_555 . 9_555 90 ?
Ga1 Mn1 Ga1' 5_555 . 10_555 90 ?
Ga1 Mn1 Ge1 5_555 . . 90 ?
Ga1 Mn1 Ge1 5_555 . 2_555 90 ?
Ga1 Mn1 Ge1 5_555 . 5_555 0 ?
Ga1 Mn1 Ge1 5_555 . 6_555 180 ?
Ga1 Mn1 Ge1 5_555 . 9_555 90 ?
Ga1 Mn1 Ge1 5_555 . 10_555 90 ?
Ga1 Mn1 Ge1' 5_555 . . 90 ?
Ga1 Mn1 Ge1' 5_555 . 2_555 90 ?
Ga1 Mn1 Ge1' 5_555 . 5_555 0 ?
Ga1 Mn1 Ge1' 5_555 . 6_555 180 ?
Ga1 Mn1 Ge1' 5_555 . 9_555 90 ?
Ga1 Mn1 Ge1' 5_555 . 10_555 90 ?
Ga1 Mn1 Ga1 6_555 . 9_555 90 ?
Ga1 Mn1 Ga1 6_555 . 10_555 90 ?
Ga1 Mn1 Ga1' 6_555 . . 90 ?
Ga1 Mn1 Ga1' 6_555 . 2_555 90 ?
Ga1 Mn1 Ga1' 6_555 . 5_555 180 ?
Ga1 Mn1 Ga1' 6_555 . 6_555 0 ?
Ga1 Mn1 Ga1' 6_555 . 9_555 90 ?
Ga1 Mn1 Ga1' 6_555 . 10_555 90 ?
Ga1 Mn1 Ge1 6_555 . . 90 ?
Ga1 Mn1 Ge1 6_555 . 2_555 90 ?
Ga1 Mn1 Ge1 6_555 . 5_555 180 ?
Ga1 Mn1 Ge1 6_555 . 6_555 0 ?
Ga1 Mn1 Ge1 6_555 . 9_555 90 ?
Ga1 Mn1 Ge1 6_555 . 10_555 90 ?
Ga1 Mn1 Ge1' 6_555 . . 90 ?
Ga1 Mn1 Ge1' 6_555 . 2_555 90 ?
Ga1 Mn1 Ge1' 6_555 . 5_555 180 ?
Ga1 Mn1 Ge1' 6_555 . 6_555 0 ?
Ga1 Mn1 Ge1' 6_555 . 9_555 90 ?
Ga1 Mn1 Ge1' 6_555 . 10_555 90 ?
Ga1 Mn1 Ga1 9_555 . 10_555 180 ?
Ga1 Mn1 Ga1' 9_555 . . 90 ?
Ga1 Mn1 Ga1' 9_555 . 2_555 90 ?
Ga1 Mn1 Ga1' 9_555 . 5_555 90 ?
Ga1 Mn1 Ga1' 9_555 . 6_555 90 ?
Ga1 Mn1 Ga1' 9_555 . 9_555 0 ?
Ga1 Mn1 Ga1' 9_555 . 10_555 180 ?
Ga1 Mn1 Ge1 9_555 . . 90 ?
Ga1 Mn1 Ge1 9_555 . 2_555 90 ?
Ga1 Mn1 Ge1 9_555 . 5_555 90 ?
Ga1 Mn1 Ge1 9_555 . 6_555 90 ?
Ga1 Mn1 Ge1 9_555 . 9_555 0 ?
Ga1 Mn1 Ge1 9_555 . 10_555 180 ?
Ga1 Mn1 Ge1' 9_555 . . 90 ?
Ga1 Mn1 Ge1' 9_555 . 2_555 90 ?
Ga1 Mn1 Ge1' 9_555 . 5_555 90 ?
Ga1 Mn1 Ge1' 9_555 . 6_555 90 ?
Ga1 Mn1 Ge1' 9_555 . 9_555 0 ?
Ga1 Mn1 Ge1' 9_555 . 10_555 180 ?
Ga1 Mn1 Ga1' 10_555 . . 90 ?
Ga1 Mn1 Ga1' 10_555 . 2_555 90 ?
Ga1 Mn1 Ga1' 10_555 . 5_555 90 ?
Ga1 Mn1 Ga1' 10_555 . 6_555 90 ?
Ga1 Mn1 Ga1' 10_555 . 9_555 180 ?
Ga1 Mn1 Ga1' 10_555 . 10_555 0 ?
Ga1 Mn1 Ge1 10_555 . . 90 ?
Ga1 Mn1 Ge1 10_555 . 2_555 90 ?
Ga1 Mn1 Ge1 10_555 . 5_555 90 ?
Ga1 Mn1 Ge1 10_555 . 6_555 90 ?
Ga1 Mn1 Ge1 10_555 . 9_555 180 ?
Ga1 Mn1 Ge1 10_555 . 10_555 0 ?
Ga1 Mn1 Ge1' 10_555 . . 90 ?
Ga1 Mn1 Ge1' 10_555 . 2_555 90 ?
Ga1 Mn1 Ge1' 10_555 . 5_555 90 ?
Ga1 Mn1 Ge1' 10_555 . 6_555 90 ?
Ga1 Mn1 Ge1' 10_555 . 9_555 180 ?
Ga1 Mn1 Ge1' 10_555 . 10_555 0 ?
Ga1' Mn1 Ga1' . . 2_555 180 ?
Ga1' Mn1 Ga1' . . 5_555 90 ?
Ga1' Mn1 Ga1' . . 6_555 90 ?
Ga1' Mn1 Ga1' . . 9_555 90 ?
Ga1' Mn1 Ga1' . . 10_555 90 ?
Ga1' Mn1 Ge1 . . . 0 ?
Ga1' Mn1 Ge1 . . 2_555 180 ?
Ga1' Mn1 Ge1 . . 5_555 90 ?
Ga1' Mn1 Ge1 . . 6_555 90 ?
Ga1' Mn1 Ge1 . . 9_555 90 ?
Ga1' Mn1 Ge1 . . 10_555 90 ?
Ga1' Mn1 Ge1' . . . 0 ?
Ga1' Mn1 Ge1' . . 2_555 180 ?
Ga1' Mn1 Ge1' . . 5_555 90 ?
Ga1' Mn1 Ge1' . . 6_555 90 ?
Ga1' Mn1 Ge1' . . 9_555 90 ?
Ga1' Mn1 Ge1' . . 10_555 90 ?
Ga1' Mn1 Ga1' 2_555 . 5_555 90 ?
Ga1' Mn1 Ga1' 2_555 . 6_555 90 ?
Ga1' Mn1 Ga1' 2_555 . 9_555 90 ?
Ga1' Mn1 Ga1' 2_555 . 10_555 90 ?
Ga1' Mn1 Ge1 2_555 . . 180 ?
Ga1' Mn1 Ge1 2_555 . 2_555 0 ?
Ga1' Mn1 Ge1 2_555 . 5_555 90 ?
Ga1' Mn1 Ge1 2_555 . 6_555 90 ?
Ga1' Mn1 Ge1 2_555 . 9_555 90 ?
Ga1' Mn1 Ge1 2_555 . 10_555 90 ?
Ga1' Mn1 Ge1' 2_555 . . 180 ?
Ga1' Mn1 Ge1' 2_555 . 2_555 0 ?
Ga1' Mn1 Ge1' 2_555 . 5_555 90 ?
Ga1' Mn1 Ge1' 2_555 . 6_555 90 ?
Ga1' Mn1 Ge1' 2_555 . 9_555 90 ?
Ga1' Mn1 Ge1' 2_555 . 10_555 90 ?
Ga1' Mn1 Ga1' 5_555 . 6_555 180 ?
Ga1' Mn1 Ga1' 5_555 . 9_555 90 ?
Ga1' Mn1 Ga1' 5_555 . 10_555 90 ?
Ga1' Mn1 Ge1 5_555 . . 90 ?
Ga1' Mn1 Ge1 5_555 . 2_555 90 ?
Ga1' Mn1 Ge1 5_555 . 5_555 0 ?
Ga1' Mn1 Ge1 5_555 . 6_555 180 ?
Ga1' Mn1 Ge1 5_555 . 9_555 90 ?
Ga1' Mn1 Ge1 5_555 . 10_555 90 ?
Ga1' Mn1 Ge1' 5_555 . . 90 ?
Ga1' Mn1 Ge1' 5_555 . 2_555 90 ?
Ga1' Mn1 Ge1' 5_555 . 5_555 0 ?
Ga1' Mn1 Ge1' 5_555 . 6_555 180 ?
Ga1' Mn1 Ge1' 5_555 . 9_555 90 ?
Ga1' Mn1 Ge1' 5_555 . 10_555 90 ?
Ga1' Mn1 Ga1' 6_555 . 9_555 90 ?
Ga1' Mn1 Ga1' 6_555 . 10_555 90 ?
Ga1' Mn1 Ge1 6_555 . . 90 ?
Ga1' Mn1 Ge1 6_555 . 2_555 90 ?
Ga1' Mn1 Ge1 6_555 . 5_555 180 ?
Ga1' Mn1 Ge1 6_555 . 6_555 0 ?
Ga1' Mn1 Ge1 6_555 . 9_555 90 ?
Ga1' Mn1 Ge1 6_555 . 10_555 90 ?
Ga1' Mn1 Ge1' 6_555 . . 90 ?
Ga1' Mn1 Ge1' 6_555 . 2_555 90 ?
Ga1' Mn1 Ge1' 6_555 . 5_555 180 ?
Ga1' Mn1 Ge1' 6_555 . 6_555 0 ?
Ga1' Mn1 Ge1' 6_555 . 9_555 90 ?
Ga1' Mn1 Ge1' 6_555 . 10_555 90 ?
Ga1' Mn1 Ga1' 9_555 . 10_555 180 ?
Ga1' Mn1 Ge1 9_555 . . 90 ?
Ga1' Mn1 Ge1 9_555 . 2_555 90 ?
Ga1' Mn1 Ge1 9_555 . 5_555 90 ?
Ga1' Mn1 Ge1 9_555 . 6_555 90 ?
Ga1' Mn1 Ge1 9_555 . 9_555 0 ?
Ga1' Mn1 Ge1 9_555 . 10_555 180 ?
Ga1' Mn1 Ge1' 9_555 . . 90 ?
Ga1' Mn1 Ge1' 9_555 . 2_555 90 ?
Ga1' Mn1 Ge1' 9_555 . 5_555 90 ?
Ga1' Mn1 Ge1' 9_555 . 6_555 90 ?
Ga1' Mn1 Ge1' 9_555 . 9_555 0 ?
Ga1' Mn1 Ge1' 9_555 . 10_555 180 ?
Ga1' Mn1 Ge1 10_555 . . 90 ?
Ga1' Mn1 Ge1 10_555 . 2_555 90 ?
Ga1' Mn1 Ge1 10_555 . 5_555 90 ?
Ga1' Mn1 Ge1 10_555 . 6_555 90 ?
Ga1' Mn1 Ge1 10_555 . 9_555 180 ?
Ga1' Mn1 Ge1 10_555 . 10_555 0 ?
Ga1' Mn1 Ge1' 10_555 . . 90 ?
Ga1' Mn1 Ge1' 10_555 . 2_555 90 ?
Ga1' Mn1 Ge1' 10_555 . 5_555 90 ?
Ga1' Mn1 Ge1' 10_555 . 6_555 90 ?
Ga1' Mn1 Ge1' 10_555 . 9_555 180 ?
Ga1' Mn1 Ge1' 10_555 . 10_555 0 ?
Ge1 Mn1 Ge1 . . 2_555 180 ?
Ge1 Mn1 Ge1 . . 5_555 90 ?
Ge1 Mn1 Ge1 . . 6_555 90 ?
Ge1 Mn1 Ge1 . . 9_555 90 ?
Ge1 Mn1 Ge1 . . 10_555 90 ?
Ge1 Mn1 Ge1' . . . 0 ?
Ge1 Mn1 Ge1' . . 2_555 180 ?
Ge1 Mn1 Ge1' . . 5_555 90 ?
Ge1 Mn1 Ge1' . . 6_555 90 ?
Ge1 Mn1 Ge1' . . 9_555 90 ?
Ge1 Mn1 Ge1' . . 10_555 90 ?
Ge1 Mn1 Ge1 2_555 . 5_555 90 ?
Ge1 Mn1 Ge1 2_555 . 6_555 90 ?
Ge1 Mn1 Ge1 2_555 . 9_555 90 ?
Ge1 Mn1 Ge1 2_555 . 10_555 90 ?
Ge1 Mn1 Ge1' 2_555 . . 180 ?
Ge1 Mn1 Ge1' 2_555 . 2_555 0 ?
Ge1 Mn1 Ge1' 2_555 . 5_555 90 ?
Ge1 Mn1 Ge1' 2_555 . 6_555 90 ?
Ge1 Mn1 Ge1' 2_555 . 9_555 90 ?
Ge1 Mn1 Ge1' 2_555 . 10_555 90 ?
Ge1 Mn1 Ge1 5_555 . 6_555 180 ?
Ge1 Mn1 Ge1 5_555 . 9_555 90 ?
Ge1 Mn1 Ge1 5_555 . 10_555 90 ?
Ge1 Mn1 Ge1' 5_555 . . 90 ?
Ge1 Mn1 Ge1' 5_555 . 2_555 90 ?
Ge1 Mn1 Ge1' 5_555 . 5_555 0 ?
Ge1 Mn1 Ge1' 5_555 . 6_555 180 ?
Ge1 Mn1 Ge1' 5_555 . 9_555 90 ?
Ge1 Mn1 Ge1' 5_555 . 10_555 90 ?
Ge1 Mn1 Ge1 6_555 . 9_555 90 ?
Ge1 Mn1 Ge1 6_555 . 10_555 90 ?
Ge1 Mn1 Ge1' 6_555 . . 90 ?
Ge1 Mn1 Ge1' 6_555 . 2_555 90 ?
Ge1 Mn1 Ge1' 6_555 . 5_555 180 ?
Ge1 Mn1 Ge1' 6_555 . 6_555 0 ?
Ge1 Mn1 Ge1' 6_555 . 9_555 90 ?
Ge1 Mn1 Ge1' 6_555 . 10_555 90 ?
Ge1 Mn1 Ge1 9_555 . 10_555 180 ?
Ge1 Mn1 Ge1' 9_555 . . 90 ?
Ge1 Mn1 Ge1' 9_555 . 2_555 90 ?
Ge1 Mn1 Ge1' 9_555 . 5_555 90 ?
Ge1 Mn1 Ge1' 9_555 . 6_555 90 ?
Ge1 Mn1 Ge1' 9_555 . 9_555 0 ?
Ge1 Mn1 Ge1' 9_555 . 10_555 180 ?
Ge1 Mn1 Ge1' 10_555 . . 90 ?
Ge1 Mn1 Ge1' 10_555 . 2_555 90 ?
Ge1 Mn1 Ge1' 10_555 . 5_555 90 ?
Ge1 Mn1 Ge1' 10_555 . 6_555 90 ?
Ge1 Mn1 Ge1' 10_555 . 9_555 180 ?
Ge1 Mn1 Ge1' 10_555 . 10_555 0 ?
Ge1' Mn1 Ge1' . . 2_555 180 ?
Ge1' Mn1 Ge1' . . 5_555 90 ?
Ge1' Mn1 Ge1' . . 6_555 90 ?
Ge1' Mn1 Ge1' . . 9_555 90 ?
Ge1' Mn1 Ge1' . . 10_555 90 ?
Ge1' Mn1 Ge1' 2_555 . 5_555 90 ?
Ge1' Mn1 Ge1' 2_555 . 6_555 90 ?
Ge1' Mn1 Ge1' 2_555 . 9_555 90 ?
Ge1' Mn1 Ge1' 2_555 . 10_555 90 ?
Ge1' Mn1 Ge1' 5_555 . 6_555 180 ?
Ge1' Mn1 Ge1' 5_555 . 9_555 90 ?
Ge1' Mn1 Ge1' 5_555 . 10_555 90 ?
Ge1' Mn1 Ge1' 6_555 . 9_555 90 ?
Ge1' Mn1 Ge1' 6_555 . 10_555 90 ?
Ge1' Mn1 Ge1' 9_555 . 10_555 180 ?
Sm1 Ga1 Sm1 . . 49_544 168.84(4) ?
Sm1 Ga1 Sm1 . . 13_555 89.459(5) ?
Sm1 Ga1 Sm1 . . 61_545 89.459(5) ?
Sm1 Ga1 Mn1 . . . 84.42(2) ?
Sm1 Ga1 Ga1 . . 2_655 95.58(2) ?
Sm1 Ga1 Ga1 . . 5_555 55.503(12) ?
Sm1 Ga1 Ga1 . . 149_545 124.50(3) ?
Sm1 Ga1 Ga1 . . 6_555 115.40(3) ?
Sm1 Ga1 Ga1 . . 150_555 64.602(13) ?
Sm1 Ga1 Ga1 . . 9_555 55.503(12) ?
Sm1 Ga1 Ga1 . . 105_554 124.50(3) ?
Sm1 Ga1 Ga1 . . 10_555 115.40(3) ?
Sm1 Ga1 Ga1 . . 106_555 64.602(13) ?
Sm1 Ga1 Ga1' . . . 84.42(2) ?
Sm1 Ga1 Ga1' . . 5_555 57.84(3) ?
Sm1 Ga1 Ga1' . . 149_545 126.92(3) ?
Sm1 Ga1 Ga1' . . 6_555 112.64(4) ?
Sm1 Ga1 Ga1' . . 150_555 61.62(3) ?
Sm1 Ga1 Ga1' . . 9_555 57.84(3) ?
Sm1 Ga1 Ga1' . . 105_554 126.92(3) ?
Sm1 Ga1 Ga1' . . 10_555 112.64(4) ?
Sm1 Ga1 Ga1' . . 106_555 61.62(3) ?
Sm1 Ga1 Ge1 . . 2_655 95.58(2) ?
Sm1 Ga1 Ge1 . . 5_555 55.503(12) ?
Sm1 Ga1 Ge1 . . 149_545 124.50(3) ?
Sm1 Ga1 Ge1 . . 6_555 115.40(3) ?
Sm1 Ga1 Ge1 . . 150_555 64.602(13) ?
Sm1 Ga1 Ge1 . . 9_555 55.503(12) ?
Sm1 Ga1 Ge1 . . 105_554 124.50(3) ?
Sm1 Ga1 Ge1 . . 10_555 115.40(3) ?
Sm1 Ga1 Ge1 . . 106_555 64.602(13) ?
Sm1 Ga1 Ge1' . . . 84.42(2) ?
Sm1 Ga1 Ge1' . . 5_555 57.84(3) ?
Sm1 Ga1 Ge1' . . 149_545 126.92(3) ?
Sm1 Ga1 Ge1' . . 6_555 112.64(4) ?
Sm1 Ga1 Ge1' . . 150_555 61.62(3) ?
Sm1 Ga1 Ge1' . . 9_555 57.84(3) ?
Sm1 Ga1 Ge1' . . 105_554 126.92(3) ?
Sm1 Ga1 Ge1' . . 10_555 112.64(4) ?
Sm1 Ga1 Ge1' . . 106_555 61.62(3) ?
Sm1 Ga1 Sm1 49_544 . 13_555 89.459(5) ?
Sm1 Ga1 Sm1 49_544 . 61_545 89.459(5) ?
Sm1 Ga1 Mn1 49_544 . . 84.42(2) ?
Sm1 Ga1 Ga1 49_544 . 2_655 95.58(2) ?
Sm1 Ga1 Ga1 49_544 . 5_555 115.40(3) ?
Sm1 Ga1 Ga1 49_544 . 149_545 64.602(13) ?
Sm1 Ga1 Ga1 49_544 . 6_555 55.503(12) ?
Sm1 Ga1 Ga1 49_544 . 150_555 124.50(3) ?
Sm1 Ga1 Ga1 49_544 . 9_555 115.40(3) ?
Sm1 Ga1 Ga1 49_544 . 105_554 64.602(13) ?
Sm1 Ga1 Ga1 49_544 . 10_555 55.503(12) ?
Sm1 Ga1 Ga1 49_544 . 106_555 124.50(3) ?
Sm1 Ga1 Ga1' 49_544 . . 84.42(2) ?
Sm1 Ga1 Ga1' 49_544 . 5_555 112.64(4) ?
Sm1 Ga1 Ga1' 49_544 . 149_545 61.62(3) ?
Sm1 Ga1 Ga1' 49_544 . 6_555 57.84(3) ?
Sm1 Ga1 Ga1' 49_544 . 150_555 126.92(3) ?
Sm1 Ga1 Ga1' 49_544 . 9_555 112.64(4) ?
Sm1 Ga1 Ga1' 49_544 . 105_554 61.62(3) ?
Sm1 Ga1 Ga1' 49_544 . 10_555 57.84(3) ?
Sm1 Ga1 Ga1' 49_544 . 106_555 126.92(3) ?
Sm1 Ga1 Ge1 49_544 . 2_655 95.58(2) ?
Sm1 Ga1 Ge1 49_544 . 5_555 115.40(3) ?
Sm1 Ga1 Ge1 49_544 . 149_545 64.602(13) ?
Sm1 Ga1 Ge1 49_544 . 6_555 55.503(12) ?
Sm1 Ga1 Ge1 49_544 . 150_555 124.50(3) ?
Sm1 Ga1 Ge1 49_544 . 9_555 115.40(3) ?
Sm1 Ga1 Ge1 49_544 . 105_554 64.602(13) ?
Sm1 Ga1 Ge1 49_544 . 10_555 55.503(12) ?
Sm1 Ga1 Ge1 49_544 . 106_555 124.50(3) ?
Sm1 Ga1 Ge1' 49_544 . . 84.42(2) ?
Sm1 Ga1 Ge1' 49_544 . 5_555 112.64(4) ?
Sm1 Ga1 Ge1' 49_544 . 149_545 61.62(3) ?
Sm1 Ga1 Ge1' 49_544 . 6_555 57.84(3) ?
Sm1 Ga1 Ge1' 49_544 . 150_555 126.92(3) ?
Sm1 Ga1 Ge1' 49_544 . 9_555 112.64(4) ?
Sm1 Ga1 Ge1' 49_544 . 105_554 61.62(3) ?
Sm1 Ga1 Ge1' 49_544 . 10_555 57.84(3) ?
Sm1 Ga1 Ge1' 49_544 . 106_555 126.92(3) ?
Sm1 Ga1 Sm1 13_555 . 61_545 168.84(4) ?
Sm1 Ga1 Mn1 13_555 . . 84.42(2) ?
Sm1 Ga1 Ga1 13_555 . 2_655 95.58(2) ?
Sm1 Ga1 Ga1 13_555 . 5_555 55.503(12) ?
Sm1 Ga1 Ga1 13_555 . 149_545 124.50(3) ?
Sm1 Ga1 Ga1 13_555 . 6_555 115.40(3) ?
Sm1 Ga1 Ga1 13_555 . 150_555 64.602(13) ?
Sm1 Ga1 Ga1 13_555 . 9_555 115.40(3) ?
Sm1 Ga1 Ga1 13_555 . 105_554 64.602(13) ?
Sm1 Ga1 Ga1 13_555 . 10_555 55.503(12) ?
Sm1 Ga1 Ga1 13_555 . 106_555 124.50(3) ?
Sm1 Ga1 Ga1' 13_555 . . 84.42(2) ?
Sm1 Ga1 Ga1' 13_555 . 5_555 57.84(3) ?
Sm1 Ga1 Ga1' 13_555 . 149_545 126.92(3) ?
Sm1 Ga1 Ga1' 13_555 . 6_555 112.64(4) ?
Sm1 Ga1 Ga1' 13_555 . 150_555 61.62(3) ?
Sm1 Ga1 Ga1' 13_555 . 9_555 112.64(4) ?
Sm1 Ga1 Ga1' 13_555 . 105_554 61.62(3) ?
Sm1 Ga1 Ga1' 13_555 . 10_555 57.84(3) ?
Sm1 Ga1 Ga1' 13_555 . 106_555 126.92(3) ?
Sm1 Ga1 Ge1 13_555 . 2_655 95.58(2) ?
Sm1 Ga1 Ge1 13_555 . 5_555 55.503(12) ?
Sm1 Ga1 Ge1 13_555 . 149_545 124.50(3) ?
Sm1 Ga1 Ge1 13_555 . 6_555 115.40(3) ?
Sm1 Ga1 Ge1 13_555 . 150_555 64.602(13) ?
Sm1 Ga1 Ge1 13_555 . 9_555 115.40(3) ?
Sm1 Ga1 Ge1 13_555 . 105_554 64.602(13) ?
Sm1 Ga1 Ge1 13_555 . 10_555 55.503(12) ?
Sm1 Ga1 Ge1 13_555 . 106_555 124.50(3) ?
Sm1 Ga1 Ge1' 13_555 . . 84.42(2) ?
Sm1 Ga1 Ge1' 13_555 . 5_555 57.84(3) ?
Sm1 Ga1 Ge1' 13_555 . 149_545 126.92(3) ?
Sm1 Ga1 Ge1' 13_555 . 6_555 112.64(4) ?
Sm1 Ga1 Ge1' 13_555 . 150_555 61.62(3) ?
Sm1 Ga1 Ge1' 13_555 . 9_555 112.64(4) ?
Sm1 Ga1 Ge1' 13_555 . 105_554 61.62(3) ?
Sm1 Ga1 Ge1' 13_555 . 10_555 57.84(3) ?
Sm1 Ga1 Ge1' 13_555 . 106_555 126.92(3) ?
Sm1 Ga1 Mn1 61_545 . . 84.42(2) ?
Sm1 Ga1 Ga1 61_545 . 2_655 95.58(2) ?
Sm1 Ga1 Ga1 61_545 . 5_555 115.40(3) ?
Sm1 Ga1 Ga1 61_545 . 149_545 64.602(13) ?
Sm1 Ga1 Ga1 61_545 . 6_555 55.503(12) ?
Sm1 Ga1 Ga1 61_545 . 150_555 124.50(3) ?
Sm1 Ga1 Ga1 61_545 . 9_555 55.503(12) ?
Sm1 Ga1 Ga1 61_545 . 105_554 124.50(3) ?
Sm1 Ga1 Ga1 61_545 . 10_555 115.40(3) ?
Sm1 Ga1 Ga1 61_545 . 106_555 64.602(13) ?
Sm1 Ga1 Ga1' 61_545 . . 84.42(2) ?
Sm1 Ga1 Ga1' 61_545 . 5_555 112.64(4) ?
Sm1 Ga1 Ga1' 61_545 . 149_545 61.62(3) ?
Sm1 Ga1 Ga1' 61_545 . 6_555 57.84(3) ?
Sm1 Ga1 Ga1' 61_545 . 150_555 126.92(3) ?
Sm1 Ga1 Ga1' 61_545 . 9_555 57.84(3) ?
Sm1 Ga1 Ga1' 61_545 . 105_554 126.92(3) ?
Sm1 Ga1 Ga1' 61_545 . 10_555 112.64(4) ?
Sm1 Ga1 Ga1' 61_545 . 106_555 61.62(3) ?
Sm1 Ga1 Ge1 61_545 . 2_655 95.58(2) ?
Sm1 Ga1 Ge1 61_545 . 5_555 115.40(3) ?
Sm1 Ga1 Ge1 61_545 . 149_545 64.602(13) ?
Sm1 Ga1 Ge1 61_545 . 6_555 55.503(12) ?
Sm1 Ga1 Ge1 61_545 . 150_555 124.50(3) ?
Sm1 Ga1 Ge1 61_545 . 9_555 55.503(12) ?
Sm1 Ga1 Ge1 61_545 . 105_554 124.50(3) ?
Sm1 Ga1 Ge1 61_545 . 10_555 115.40(3) ?
Sm1 Ga1 Ge1 61_545 . 106_555 64.602(13) ?
Sm1 Ga1 Ge1' 61_545 . . 84.42(2) ?
Sm1 Ga1 Ge1' 61_545 . 5_555 112.64(4) ?
Sm1 Ga1 Ge1' 61_545 . 149_545 61.62(3) ?
Sm1 Ga1 Ge1' 61_545 . 6_555 57.84(3) ?
Sm1 Ga1 Ge1' 61_545 . 150_555 126.92(3) ?
Sm1 Ga1 Ge1' 61_545 . 9_555 57.84(3) ?
Sm1 Ga1 Ge1' 61_545 . 105_554 126.92(3) ?
Sm1 Ga1 Ge1' 61_545 . 10_555 112.64(4) ?
Sm1 Ga1 Ge1' 61_545 . 106_555 61.62(3) ?
Mn1 Ga1 Ga1 . . 2_655 180 ?
Mn1 Ga1 Ga1 . . 5_555 45.000(18) ?
Mn1 Ga1 Ga1 . . 149_545 135.00(2) ?
Mn1 Ga1 Ga1 . . 6_555 45.000(18) ?
Mn1 Ga1 Ga1 . . 150_555 135.00(2) ?
Mn1 Ga1 Ga1 . . 9_555 45.000(18) ?
Mn1 Ga1 Ga1 . . 105_554 135.00(2) ?
Mn1 Ga1 Ga1 . . 10_555 45.000(18) ?
Mn1 Ga1 Ga1 . . 106_555 135.00(2) ?
Mn1 Ga1 Ga1' . . . 0 ?
Mn1 Ga1 Ga1' . . 5_555 40.67(5) ?
Mn1 Ga1 Ga1' . . 149_545 130.14(5) ?
Mn1 Ga1 Ga1' . . 6_555 40.67(5) ?
Mn1 Ga1 Ga1' . . 150_555 130.14(5) ?
Mn1 Ga1 Ga1' . . 9_555 40.67(5) ?
Mn1 Ga1 Ga1' . . 105_554 130.14(5) ?
Mn1 Ga1 Ga1' . . 10_555 40.67(5) ?
Mn1 Ga1 Ga1' . . 106_555 130.14(5) ?
Mn1 Ga1 Ge1 . . 2_655 180 ?
Mn1 Ga1 Ge1 . . 5_555 45.000(18) ?
Mn1 Ga1 Ge1 . . 149_545 135.00(2) ?
Mn1 Ga1 Ge1 . . 6_555 45.000(18) ?
Mn1 Ga1 Ge1 . . 150_555 135.00(2) ?
Mn1 Ga1 Ge1 . . 9_555 45.000(18) ?
Mn1 Ga1 Ge1 . . 105_554 135.00(2) ?
Mn1 Ga1 Ge1 . . 10_555 45.000(18) ?
Mn1 Ga1 Ge1 . . 106_555 135.00(2) ?
Mn1 Ga1 Ge1' . . . 0 ?
Mn1 Ga1 Ge1' . . 5_555 40.67(5) ?
Mn1 Ga1 Ge1' . . 149_545 130.14(5) ?
Mn1 Ga1 Ge1' . . 6_555 40.67(5) ?
Mn1 Ga1 Ge1' . . 150_555 130.14(5) ?
Mn1 Ga1 Ge1' . . 9_555 40.67(5) ?
Mn1 Ga1 Ge1' . . 105_554 130.14(5) ?
Mn1 Ga1 Ge1' . . 10_555 40.67(5) ?
Mn1 Ga1 Ge1' . . 106_555 130.14(5) ?
Ga1 Ga1 Ga1 2_655 . 5_555 135.000(18) ?
Ga1 Ga1 Ga1 2_655 . 149_545 45.00(2) ?
Ga1 Ga1 Ga1 2_655 . 6_555 135.000(18) ?
Ga1 Ga1 Ga1 2_655 . 150_555 45.00(2) ?
Ga1 Ga1 Ga1 2_655 . 9_555 135.000(18) ?
Ga1 Ga1 Ga1 2_655 . 105_554 45.00(2) ?
Ga1 Ga1 Ga1 2_655 . 10_555 135.000(18) ?
Ga1 Ga1 Ga1 2_655 . 106_555 45.00(2) ?
Ga1 Ga1 Ga1' 2_655 . . 180 ?
Ga1 Ga1 Ga1' 2_655 . 5_555 139.33(5) ?
Ga1 Ga1 Ga1' 2_655 . 149_545 49.86(5) ?
Ga1 Ga1 Ga1' 2_655 . 6_555 139.33(5) ?
Ga1 Ga1 Ga1' 2_655 . 150_555 49.86(5) ?
Ga1 Ga1 Ga1' 2_655 . 9_555 139.33(5) ?
Ga1 Ga1 Ga1' 2_655 . 105_554 49.86(5) ?
Ga1 Ga1 Ga1' 2_655 . 10_555 139.33(5) ?
Ga1 Ga1 Ga1' 2_655 . 106_555 49.86(5) ?
Ga1 Ga1 Ge1 2_655 . 2_655 0 ?
Ga1 Ga1 Ge1 2_655 . 5_555 135.000(18) ?
Ga1 Ga1 Ge1 2_655 . 149_545 45.00(2) ?
Ga1 Ga1 Ge1 2_655 . 6_555 135.000(18) ?
Ga1 Ga1 Ge1 2_655 . 150_555 45.00(2) ?
Ga1 Ga1 Ge1 2_655 . 9_555 135.000(18) ?
Ga1 Ga1 Ge1 2_655 . 105_554 45.00(2) ?
Ga1 Ga1 Ge1 2_655 . 10_555 135.000(18) ?
Ga1 Ga1 Ge1 2_655 . 106_555 45.00(2) ?
Ga1 Ga1 Ge1' 2_655 . . 180 ?
Ga1 Ga1 Ge1' 2_655 . 5_555 139.33(5) ?
Ga1 Ga1 Ge1' 2_655 . 149_545 49.86(5) ?
Ga1 Ga1 Ge1' 2_655 . 6_555 139.33(5) ?
Ga1 Ga1 Ge1' 2_655 . 150_555 49.86(5) ?
Ga1 Ga1 Ge1' 2_655 . 9_555 139.33(5) ?
Ga1 Ga1 Ge1' 2_655 . 105_554 49.86(5) ?
Ga1 Ga1 Ge1' 2_655 . 10_555 139.33(5) ?
Ga1 Ga1 Ge1' 2_655 . 106_555 49.86(5) ?
Ga1 Ga1 Ga1 5_555 . 149_545 180 ?
Ga1 Ga1 Ga1 5_555 . 6_555 90.00(3) ?
Ga1 Ga1 Ga1 5_555 . 150_555 90.00(2) ?
Ga1 Ga1 Ga1 5_555 . 9_555 60.000(18) ?
Ga1 Ga1 Ga1 5_555 . 105_554 120.000(13) ?
Ga1 Ga1 Ga1 5_555 . 10_555 60.000(18) ?
Ga1 Ga1 Ga1 5_555 . 106_555 120.000(13) ?
Ga1 Ga1 Ga1' 5_555 . . 45.000(18) ?
Ga1 Ga1 Ga1' 5_555 . 5_555 4.33(5) ?
Ga1 Ga1 Ga1' 5_555 . 149_545 175.14(6) ?
Ga1 Ga1 Ga1' 5_555 . 6_555 85.67(6) ?
Ga1 Ga1 Ga1' 5_555 . 150_555 85.14(5) ?
Ga1 Ga1 Ga1' 5_555 . 9_555 57.56(3) ?
Ga1 Ga1 Ga1' 5_555 . 105_554 117.12(3) ?
Ga1 Ga1 Ga1' 5_555 . 10_555 57.56(3) ?
Ga1 Ga1 Ga1' 5_555 . 106_555 117.12(3) ?
Ga1 Ga1 Ge1 5_555 . 2_655 135.000(18) ?
Ga1 Ga1 Ge1 5_555 . 5_555 0 ?
Ga1 Ga1 Ge1 5_555 . 149_545 180 ?
Ga1 Ga1 Ge1 5_555 . 6_555 90.00(3) ?
Ga1 Ga1 Ge1 5_555 . 150_555 90.00(2) ?
Ga1 Ga1 Ge1 5_555 . 9_555 60.000(18) ?
Ga1 Ga1 Ge1 5_555 . 105_554 120.000(13) ?
Ga1 Ga1 Ge1 5_555 . 10_555 60.000(18) ?
Ga1 Ga1 Ge1 5_555 . 106_555 120.000(13) ?
Ga1 Ga1 Ge1' 5_555 . . 45.000(18) ?
Ga1 Ga1 Ge1' 5_555 . 5_555 4.33(5) ?
Ga1 Ga1 Ge1' 5_555 . 149_545 175.14(6) ?
Ga1 Ga1 Ge1' 5_555 . 6_555 85.67(6) ?
Ga1 Ga1 Ge1' 5_555 . 150_555 85.14(5) ?
Ga1 Ga1 Ge1' 5_555 . 9_555 57.56(3) ?
Ga1 Ga1 Ge1' 5_555 . 105_554 117.12(3) ?
Ga1 Ga1 Ge1' 5_555 . 10_555 57.56(3) ?
Ga1 Ga1 Ge1' 5_555 . 106_555 117.12(3) ?
Ga1 Ga1 Ga1 149_545 . 6_555 90.00(2) ?
Ga1 Ga1 Ga1 149_545 . 150_555 90.00(4) ?
Ga1 Ga1 Ga1 149_545 . 9_555 120.000(13) ?
Ga1 Ga1 Ga1 149_545 . 105_554 60.00(2) ?
Ga1 Ga1 Ga1 149_545 . 10_555 120.000(13) ?
Ga1 Ga1 Ga1 149_545 . 106_555 60.00(2) ?
Ga1 Ga1 Ga1' 149_545 . . 135.00(2) ?
Ga1 Ga1 Ga1' 149_545 . 5_555 175.67(6) ?
Ga1 Ga1 Ga1' 149_545 . 149_545 4.86(5) ?
Ga1 Ga1 Ga1' 149_545 . 6_555 94.33(5) ?
Ga1 Ga1 Ga1' 149_545 . 150_555 94.86(6) ?
Ga1 Ga1 Ga1' 149_545 . 9_555 122.44(3) ?
Ga1 Ga1 Ga1' 149_545 . 105_554 62.88(3) ?
Ga1 Ga1 Ga1' 149_545 . 10_555 122.44(3) ?
Ga1 Ga1 Ga1' 149_545 . 106_555 62.88(3) ?
Ga1 Ga1 Ge1 149_545 . 2_655 45.00(2) ?
Ga1 Ga1 Ge1 149_545 . 5_555 180 ?
Ga1 Ga1 Ge1 149_545 . 149_545 0 ?
Ga1 Ga1 Ge1 149_545 . 6_555 90.00(2) ?
Ga1 Ga1 Ge1 149_545 . 150_555 90.00(4) ?
Ga1 Ga1 Ge1 149_545 . 9_555 120.000(13) ?
Ga1 Ga1 Ge1 149_545 . 105_554 60.00(2) ?
Ga1 Ga1 Ge1 149_545 . 10_555 120.000(13) ?
Ga1 Ga1 Ge1 149_545 . 106_555 60.00(2) ?
Ga1 Ga1 Ge1' 149_545 . . 135.00(2) ?
Ga1 Ga1 Ge1' 149_545 . 5_555 175.67(6) ?
Ga1 Ga1 Ge1' 149_545 . 149_545 4.86(5) ?
Ga1 Ga1 Ge1' 149_545 . 6_555 94.33(5) ?
Ga1 Ga1 Ge1' 149_545 . 150_555 94.86(6) ?
Ga1 Ga1 Ge1' 149_545 . 9_555 122.44(3) ?
Ga1 Ga1 Ge1' 149_545 . 105_554 62.88(3) ?
Ga1 Ga1 Ge1' 149_545 . 10_555 122.44(3) ?
Ga1 Ga1 Ge1' 149_545 . 106_555 62.88(3) ?
Ga1 Ga1 Ga1 6_555 . 150_555 180 ?
Ga1 Ga1 Ga1 6_555 . 9_555 60.000(18) ?
Ga1 Ga1 Ga1 6_555 . 105_554 120.000(13) ?
Ga1 Ga1 Ga1 6_555 . 10_555 60.000(18) ?
Ga1 Ga1 Ga1 6_555 . 106_555 120.000(13) ?
Ga1 Ga1 Ga1' 6_555 . . 45.000(18) ?
Ga1 Ga1 Ga1' 6_555 . 5_555 85.67(6) ?
Ga1 Ga1 Ga1' 6_555 . 149_545 85.14(5) ?
Ga1 Ga1 Ga1' 6_555 . 6_555 4.33(5) ?
Ga1 Ga1 Ga1' 6_555 . 150_555 175.14(6) ?
Ga1 Ga1 Ga1' 6_555 . 9_555 57.56(3) ?
Ga1 Ga1 Ga1' 6_555 . 105_554 117.12(3) ?
Ga1 Ga1 Ga1' 6_555 . 10_555 57.56(3) ?
Ga1 Ga1 Ga1' 6_555 . 106_555 117.12(3) ?
Ga1 Ga1 Ge1 6_555 . 2_655 135.000(18) ?
Ga1 Ga1 Ge1 6_555 . 5_555 90.00(3) ?
Ga1 Ga1 Ge1 6_555 . 149_545 90.00(2) ?
Ga1 Ga1 Ge1 6_555 . 6_555 0 ?
Ga1 Ga1 Ge1 6_555 . 150_555 180 ?
Ga1 Ga1 Ge1 6_555 . 9_555 60.000(18) ?
Ga1 Ga1 Ge1 6_555 . 105_554 120.000(13) ?
Ga1 Ga1 Ge1 6_555 . 10_555 60.000(18) ?
Ga1 Ga1 Ge1 6_555 . 106_555 120.000(13) ?
Ga1 Ga1 Ge1' 6_555 . . 45.000(18) ?
Ga1 Ga1 Ge1' 6_555 . 5_555 85.67(6) ?
Ga1 Ga1 Ge1' 6_555 . 149_545 85.14(5) ?
Ga1 Ga1 Ge1' 6_555 . 6_555 4.33(5) ?
Ga1 Ga1 Ge1' 6_555 . 150_555 175.14(6) ?
Ga1 Ga1 Ge1' 6_555 . 9_555 57.56(3) ?
Ga1 Ga1 Ge1' 6_555 . 105_554 117.12(3) ?
Ga1 Ga1 Ge1' 6_555 . 10_555 57.56(3) ?
Ga1 Ga1 Ge1' 6_555 . 106_555 117.12(3) ?
Ga1 Ga1 Ga1 150_555 . 9_555 120.000(13) ?
Ga1 Ga1 Ga1 150_555 . 105_554 60.00(2) ?
Ga1 Ga1 Ga1 150_555 . 10_555 120.000(13) ?
Ga1 Ga1 Ga1 150_555 . 106_555 60.00(2) ?
Ga1 Ga1 Ga1' 150_555 . . 135.00(2) ?
Ga1 Ga1 Ga1' 150_555 . 5_555 94.33(5) ?
Ga1 Ga1 Ga1' 150_555 . 149_545 94.86(6) ?
Ga1 Ga1 Ga1' 150_555 . 6_555 175.67(6) ?
Ga1 Ga1 Ga1' 150_555 . 150_555 4.86(5) ?
Ga1 Ga1 Ga1' 150_555 . 9_555 122.44(3) ?
Ga1 Ga1 Ga1' 150_555 . 105_554 62.88(3) ?
Ga1 Ga1 Ga1' 150_555 . 10_555 122.44(3) ?
Ga1 Ga1 Ga1' 150_555 . 106_555 62.88(3) ?
Ga1 Ga1 Ge1 150_555 . 2_655 45.00(2) ?
Ga1 Ga1 Ge1 150_555 . 5_555 90.00(2) ?
Ga1 Ga1 Ge1 150_555 . 149_545 90.00(4) ?
Ga1 Ga1 Ge1 150_555 . 6_555 180 ?
Ga1 Ga1 Ge1 150_555 . 150_555 0 ?
Ga1 Ga1 Ge1 150_555 . 9_555 120.000(13) ?
Ga1 Ga1 Ge1 150_555 . 105_554 60.00(2) ?
Ga1 Ga1 Ge1 150_555 . 10_555 120.000(13) ?
Ga1 Ga1 Ge1 150_555 . 106_555 60.00(2) ?
Ga1 Ga1 Ge1' 150_555 . . 135.00(2) ?
Ga1 Ga1 Ge1' 150_555 . 5_555 94.33(5) ?
Ga1 Ga1 Ge1' 150_555 . 149_545 94.86(6) ?
Ga1 Ga1 Ge1' 150_555 . 6_555 175.67(6) ?
Ga1 Ga1 Ge1' 150_555 . 150_555 4.86(5) ?
Ga1 Ga1 Ge1' 150_555 . 9_555 122.44(3) ?
Ga1 Ga1 Ge1' 150_555 . 105_554 62.88(3) ?
Ga1 Ga1 Ge1' 150_555 . 10_555 122.44(3) ?
Ga1 Ga1 Ge1' 150_555 . 106_555 62.88(3) ?
Ga1 Ga1 Ga1 9_555 . 105_554 180 ?
Ga1 Ga1 Ga1 9_555 . 10_555 90.00(3) ?
Ga1 Ga1 Ga1 9_555 . 106_555 90.00(2) ?
Ga1 Ga1 Ga1' 9_555 . . 45.000(18) ?
Ga1 Ga1 Ga1' 9_555 . 5_555 57.56(3) ?
Ga1 Ga1 Ga1' 9_555 . 149_545 117.12(3) ?
Ga1 Ga1 Ga1' 9_555 . 6_555 57.56(3) ?
Ga1 Ga1 Ga1' 9_555 . 150_555 117.12(3) ?
Ga1 Ga1 Ga1' 9_555 . 9_555 4.33(5) ?
Ga1 Ga1 Ga1' 9_555 . 105_554 175.14(6) ?
Ga1 Ga1 Ga1' 9_555 . 10_555 85.67(6) ?
Ga1 Ga1 Ga1' 9_555 . 106_555 85.14(5) ?
Ga1 Ga1 Ge1 9_555 . 2_655 135.000(18) ?
Ga1 Ga1 Ge1 9_555 . 5_555 60.000(18) ?
Ga1 Ga1 Ge1 9_555 . 149_545 120.000(13) ?
Ga1 Ga1 Ge1 9_555 . 6_555 60.000(18) ?
Ga1 Ga1 Ge1 9_555 . 150_555 120.000(13) ?
Ga1 Ga1 Ge1 9_555 . 9_555 0 ?
Ga1 Ga1 Ge1 9_555 . 105_554 180 ?
Ga1 Ga1 Ge1 9_555 . 10_555 90.00(3) ?
Ga1 Ga1 Ge1 9_555 . 106_555 90.00(2) ?
Ga1 Ga1 Ge1' 9_555 . . 45.000(18) ?
Ga1 Ga1 Ge1' 9_555 . 5_555 57.56(3) ?
Ga1 Ga1 Ge1' 9_555 . 149_545 117.12(3) ?
Ga1 Ga1 Ge1' 9_555 . 6_555 57.56(3) ?
Ga1 Ga1 Ge1' 9_555 . 150_555 117.12(3) ?
Ga1 Ga1 Ge1' 9_555 . 9_555 4.33(5) ?
Ga1 Ga1 Ge1' 9_555 . 105_554 175.14(6) ?
Ga1 Ga1 Ge1' 9_555 . 10_555 85.67(6) ?
Ga1 Ga1 Ge1' 9_555 . 106_555 85.14(5) ?
Ga1 Ga1 Ga1 105_554 . 10_555 90.00(2) ?
Ga1 Ga1 Ga1 105_554 . 106_555 90.00(4) ?
Ga1 Ga1 Ga1' 105_554 . . 135.00(2) ?
Ga1 Ga1 Ga1' 105_554 . 5_555 122.44(3) ?
Ga1 Ga1 Ga1' 105_554 . 149_545 62.88(3) ?
Ga1 Ga1 Ga1' 105_554 . 6_555 122.44(3) ?
Ga1 Ga1 Ga1' 105_554 . 150_555 62.88(3) ?
Ga1 Ga1 Ga1' 105_554 . 9_555 175.67(6) ?
Ga1 Ga1 Ga1' 105_554 . 105_554 4.86(5) ?
Ga1 Ga1 Ga1' 105_554 . 10_555 94.33(5) ?
Ga1 Ga1 Ga1' 105_554 . 106_555 94.86(6) ?
Ga1 Ga1 Ge1 105_554 . 2_655 45.00(2) ?
Ga1 Ga1 Ge1 105_554 . 5_555 120.000(13) ?
Ga1 Ga1 Ge1 105_554 . 149_545 60.00(2) ?
Ga1 Ga1 Ge1 105_554 . 6_555 120.000(13) ?
Ga1 Ga1 Ge1 105_554 . 150_555 60.00(2) ?
Ga1 Ga1 Ge1 105_554 . 9_555 180 ?
Ga1 Ga1 Ge1 105_554 . 105_554 0 ?
Ga1 Ga1 Ge1 105_554 . 10_555 90.00(2) ?
Ga1 Ga1 Ge1 105_554 . 106_555 90.00(4) ?
Ga1 Ga1 Ge1' 105_554 . . 135.00(2) ?
Ga1 Ga1 Ge1' 105_554 . 5_555 122.44(3) ?
Ga1 Ga1 Ge1' 105_554 . 149_545 62.88(3) ?
Ga1 Ga1 Ge1' 105_554 . 6_555 122.44(3) ?
Ga1 Ga1 Ge1' 105_554 . 150_555 62.88(3) ?
Ga1 Ga1 Ge1' 105_554 . 9_555 175.67(6) ?
Ga1 Ga1 Ge1' 105_554 . 105_554 4.86(5) ?
Ga1 Ga1 Ge1' 105_554 . 10_555 94.33(5) ?
Ga1 Ga1 Ge1' 105_554 . 106_555 94.86(6) ?
Ga1 Ga1 Ga1 10_555 . 106_555 180 ?
Ga1 Ga1 Ga1' 10_555 . . 45.000(18) ?
Ga1 Ga1 Ga1' 10_555 . 5_555 57.56(3) ?
Ga1 Ga1 Ga1' 10_555 . 149_545 117.12(3) ?
Ga1 Ga1 Ga1' 10_555 . 6_555 57.56(3) ?
Ga1 Ga1 Ga1' 10_555 . 150_555 117.12(3) ?
Ga1 Ga1 Ga1' 10_555 . 9_555 85.67(6) ?
Ga1 Ga1 Ga1' 10_555 . 105_554 85.14(5) ?
Ga1 Ga1 Ga1' 10_555 . 10_555 4.33(5) ?
Ga1 Ga1 Ga1' 10_555 . 106_555 175.14(6) ?
Ga1 Ga1 Ge1 10_555 . 2_655 135.000(18) ?
Ga1 Ga1 Ge1 10_555 . 5_555 60.000(18) ?
Ga1 Ga1 Ge1 10_555 . 149_545 120.000(13) ?
Ga1 Ga1 Ge1 10_555 . 6_555 60.000(18) ?
Ga1 Ga1 Ge1 10_555 . 150_555 120.000(13) ?
Ga1 Ga1 Ge1 10_555 . 9_555 90.00(3) ?
Ga1 Ga1 Ge1 10_555 . 105_554 90.00(2) ?
Ga1 Ga1 Ge1 10_555 . 10_555 0 ?
Ga1 Ga1 Ge1 10_555 . 106_555 180 ?
Ga1 Ga1 Ge1' 10_555 . . 45.000(18) ?
Ga1 Ga1 Ge1' 10_555 . 5_555 57.56(3) ?
Ga1 Ga1 Ge1' 10_555 . 149_545 117.12(3) ?
Ga1 Ga1 Ge1' 10_555 . 6_555 57.56(3) ?
Ga1 Ga1 Ge1' 10_555 . 150_555 117.12(3) ?
Ga1 Ga1 Ge1' 10_555 . 9_555 85.67(6) ?
Ga1 Ga1 Ge1' 10_555 . 105_554 85.14(5) ?
Ga1 Ga1 Ge1' 10_555 . 10_555 4.33(5) ?
Ga1 Ga1 Ge1' 10_555 . 106_555 175.14(6) ?
Ga1 Ga1 Ga1' 106_555 . . 135.00(2) ?
Ga1 Ga1 Ga1' 106_555 . 5_555 122.44(3) ?
Ga1 Ga1 Ga1' 106_555 . 149_545 62.88(3) ?
Ga1 Ga1 Ga1' 106_555 . 6_555 122.44(3) ?
Ga1 Ga1 Ga1' 106_555 . 150_555 62.88(3) ?
Ga1 Ga1 Ga1' 106_555 . 9_555 94.33(5) ?
Ga1 Ga1 Ga1' 106_555 . 105_554 94.86(6) ?
Ga1 Ga1 Ga1' 106_555 . 10_555 175.67(6) ?
Ga1 Ga1 Ga1' 106_555 . 106_555 4.86(5) ?
Ga1 Ga1 Ge1 106_555 . 2_655 45.00(2) ?
Ga1 Ga1 Ge1 106_555 . 5_555 120.000(13) ?
Ga1 Ga1 Ge1 106_555 . 149_545 60.00(2) ?
Ga1 Ga1 Ge1 106_555 . 6_555 120.000(13) ?
Ga1 Ga1 Ge1 106_555 . 150_555 60.00(2) ?
Ga1 Ga1 Ge1 106_555 . 9_555 90.00(2) ?
Ga1 Ga1 Ge1 106_555 . 105_554 90.00(4) ?
Ga1 Ga1 Ge1 106_555 . 10_555 180 ?
Ga1 Ga1 Ge1 106_555 . 106_555 0 ?
Ga1 Ga1 Ge1' 106_555 . . 135.00(2) ?
Ga1 Ga1 Ge1' 106_555 . 5_555 122.44(3) ?
Ga1 Ga1 Ge1' 106_555 . 149_545 62.88(3) ?
Ga1 Ga1 Ge1' 106_555 . 6_555 122.44(3) ?
Ga1 Ga1 Ge1' 106_555 . 150_555 62.88(3) ?
Ga1 Ga1 Ge1' 106_555 . 9_555 94.33(5) ?
Ga1 Ga1 Ge1' 106_555 . 105_554 94.86(6) ?
Ga1 Ga1 Ge1' 106_555 . 10_555 175.67(6) ?
Ga1 Ga1 Ge1' 106_555 . 106_555 4.86(5) ?
Ga1' Ga1 Ga1' . . 5_555 40.67(5) ?
Ga1' Ga1 Ga1' . . 149_545 130.14(5) ?
Ga1' Ga1 Ga1' . . 6_555 40.67(5) ?
Ga1' Ga1 Ga1' . . 150_555 130.14(5) ?
Ga1' Ga1 Ga1' . . 9_555 40.67(5) ?
Ga1' Ga1 Ga1' . . 105_554 130.14(5) ?
Ga1' Ga1 Ga1' . . 10_555 40.67(5) ?
Ga1' Ga1 Ga1' . . 106_555 130.14(5) ?
Ga1' Ga1 Ge1 . . 2_655 180 ?
Ga1' Ga1 Ge1 . . 5_555 45.000(18) ?
Ga1' Ga1 Ge1 . . 149_545 135.00(2) ?
Ga1' Ga1 Ge1 . . 6_555 45.000(18) ?
Ga1' Ga1 Ge1 . . 150_555 135.00(2) ?
Ga1' Ga1 Ge1 . . 9_555 45.000(18) ?
Ga1' Ga1 Ge1 . . 105_554 135.00(2) ?
Ga1' Ga1 Ge1 . . 10_555 45.000(18) ?
Ga1' Ga1 Ge1 . . 106_555 135.00(2) ?
Ga1' Ga1 Ge1' . . . 0 ?
Ga1' Ga1 Ge1' . . 5_555 40.67(5) ?
Ga1' Ga1 Ge1' . . 149_545 130.14(5) ?
Ga1' Ga1 Ge1' . . 6_555 40.67(5) ?
Ga1' Ga1 Ge1' . . 150_555 130.14(5) ?
Ga1' Ga1 Ge1' . . 9_555 40.67(5) ?
Ga1' Ga1 Ge1' . . 105_554 130.14(5) ?
Ga1' Ga1 Ge1' . . 10_555 40.67(5) ?
Ga1' Ga1 Ge1' . . 106_555 130.14(5) ?
Ga1' Ga1 Ga1' 5_555 . 149_545 170.80(7) ?
Ga1' Ga1 Ga1' 5_555 . 6_555 81.34(7) ?
Ga1' Ga1 Ga1' 5_555 . 150_555 89.47(7) ?
Ga1' Ga1 Ga1' 5_555 . 9_555 54.88(4) ?
Ga1' Ga1 Ga1' 5_555 . 105_554 119.27(4) ?
Ga1' Ga1 Ga1' 5_555 . 10_555 54.88(4) ?
Ga1' Ga1 Ga1' 5_555 . 106_555 119.27(4) ?
Ga1' Ga1 Ge1 5_555 . 2_655 139.33(5) ?
Ga1' Ga1 Ge1 5_555 . 5_555 4.33(5) ?
Ga1' Ga1 Ge1 5_555 . 149_545 175.67(6) ?
Ga1' Ga1 Ge1 5_555 . 6_555 85.67(6) ?
Ga1' Ga1 Ge1 5_555 . 150_555 94.33(5) ?
Ga1' Ga1 Ge1 5_555 . 9_555 57.56(3) ?
Ga1' Ga1 Ge1 5_555 . 105_554 122.44(3) ?
Ga1' Ga1 Ge1 5_555 . 10_555 57.56(3) ?
Ga1' Ga1 Ge1 5_555 . 106_555 122.44(3) ?
Ga1' Ga1 Ge1' 5_555 . . 40.67(5) ?
Ga1' Ga1 Ge1' 5_555 . 5_555 0 ?
Ga1' Ga1 Ge1' 5_555 . 149_545 170.80(7) ?
Ga1' Ga1 Ge1' 5_555 . 6_555 81.34(7) ?
Ga1' Ga1 Ge1' 5_555 . 150_555 89.47(7) ?
Ga1' Ga1 Ge1' 5_555 . 9_555 54.88(4) ?
Ga1' Ga1 Ge1' 5_555 . 105_554 119.27(4) ?
Ga1' Ga1 Ge1' 5_555 . 10_555 54.88(4) ?
Ga1' Ga1 Ge1' 5_555 . 106_555 119.27(4) ?
Ga1' Ga1 Ga1' 149_545 . 6_555 89.47(7) ?
Ga1' Ga1 Ga1' 149_545 . 150_555 99.73(7) ?
Ga1' Ga1 Ga1' 149_545 . 9_555 119.27(4) ?
Ga1' Ga1 Ga1' 149_545 . 105_554 65.45(4) ?
Ga1' Ga1 Ga1' 149_545 . 10_555 119.27(4) ?
Ga1' Ga1 Ga1' 149_545 . 106_555 65.45(4) ?
Ga1' Ga1 Ge1 149_545 . 2_655 49.86(5) ?
Ga1' Ga1 Ge1 149_545 . 5_555 175.14(6) ?
Ga1' Ga1 Ge1 149_545 . 149_545 4.86(5) ?
Ga1' Ga1 Ge1 149_545 . 6_555 85.14(5) ?
Ga1' Ga1 Ge1 149_545 . 150_555 94.86(6) ?
Ga1' Ga1 Ge1 149_545 . 9_555 117.12(3) ?
Ga1' Ga1 Ge1 149_545 . 105_554 62.88(3) ?
Ga1' Ga1 Ge1 149_545 . 10_555 117.12(3) ?
Ga1' Ga1 Ge1 149_545 . 106_555 62.88(3) ?
Ga1' Ga1 Ge1' 149_545 . . 130.14(5) ?
Ga1' Ga1 Ge1' 149_545 . 5_555 170.80(7) ?
Ga1' Ga1 Ge1' 149_545 . 149_545 0 ?
Ga1' Ga1 Ge1' 149_545 . 6_555 89.47(7) ?
Ga1' Ga1 Ge1' 149_545 . 150_555 99.73(7) ?
Ga1' Ga1 Ge1' 149_545 . 9_555 119.27(4) ?
Ga1' Ga1 Ge1' 149_545 . 105_554 65.45(4) ?
Ga1' Ga1 Ge1' 149_545 . 10_555 119.27(4) ?
Ga1' Ga1 Ge1' 149_545 . 106_555 65.45(4) ?
Ga1' Ga1 Ga1' 6_555 . 150_555 170.80(7) ?
Ga1' Ga1 Ga1' 6_555 . 9_555 54.88(4) ?
Ga1' Ga1 Ga1' 6_555 . 105_554 119.27(4) ?
Ga1' Ga1 Ga1' 6_555 . 10_555 54.88(4) ?
Ga1' Ga1 Ga1' 6_555 . 106_555 119.27(4) ?
Ga1' Ga1 Ge1 6_555 . 2_655 139.33(5) ?
Ga1' Ga1 Ge1 6_555 . 5_555 85.67(6) ?
Ga1' Ga1 Ge1 6_555 . 149_545 94.33(5) ?
Ga1' Ga1 Ge1 6_555 . 6_555 4.33(5) ?
Ga1' Ga1 Ge1 6_555 . 150_555 175.67(6) ?
Ga1' Ga1 Ge1 6_555 . 9_555 57.56(3) ?
Ga1' Ga1 Ge1 6_555 . 105_554 122.44(3) ?
Ga1' Ga1 Ge1 6_555 . 10_555 57.56(3) ?
Ga1' Ga1 Ge1 6_555 . 106_555 122.44(3) ?
Ga1' Ga1 Ge1' 6_555 . . 40.67(5) ?
Ga1' Ga1 Ge1' 6_555 . 5_555 81.34(7) ?
Ga1' Ga1 Ge1' 6_555 . 149_545 89.47(7) ?
Ga1' Ga1 Ge1' 6_555 . 6_555 0 ?
Ga1' Ga1 Ge1' 6_555 . 150_555 170.80(7) ?
Ga1' Ga1 Ge1' 6_555 . 9_555 54.88(4) ?
Ga1' Ga1 Ge1' 6_555 . 105_554 119.27(4) ?
Ga1' Ga1 Ge1' 6_555 . 10_555 54.88(4) ?
Ga1' Ga1 Ge1' 6_555 . 106_555 119.27(4) ?
Ga1' Ga1 Ga1' 150_555 . 9_555 119.27(4) ?
Ga1' Ga1 Ga1' 150_555 . 105_554 65.45(4) ?
Ga1' Ga1 Ga1' 150_555 . 10_555 119.27(4) ?
Ga1' Ga1 Ga1' 150_555 . 106_555 65.45(4) ?
Ga1' Ga1 Ge1 150_555 . 2_655 49.86(5) ?
Ga1' Ga1 Ge1 150_555 . 5_555 85.14(5) ?
Ga1' Ga1 Ge1 150_555 . 149_545 94.86(6) ?
Ga1' Ga1 Ge1 150_555 . 6_555 175.14(6) ?
Ga1' Ga1 Ge1 150_555 . 150_555 4.86(5) ?
Ga1' Ga1 Ge1 150_555 . 9_555 117.12(3) ?
Ga1' Ga1 Ge1 150_555 . 105_554 62.88(3) ?
Ga1' Ga1 Ge1 150_555 . 10_555 117.12(3) ?
Ga1' Ga1 Ge1 150_555 . 106_555 62.88(3) ?
Ga1' Ga1 Ge1' 150_555 . . 130.14(5) ?
Ga1' Ga1 Ge1' 150_555 . 5_555 89.47(7) ?
Ga1' Ga1 Ge1' 150_555 . 149_545 99.73(7) ?
Ga1' Ga1 Ge1' 150_555 . 6_555 170.80(7) ?
Ga1' Ga1 Ge1' 150_555 . 150_555 0 ?
Ga1' Ga1 Ge1' 150_555 . 9_555 119.27(4) ?
Ga1' Ga1 Ge1' 150_555 . 105_554 65.45(4) ?
Ga1' Ga1 Ge1' 150_555 . 10_555 119.27(4) ?
Ga1' Ga1 Ge1' 150_555 . 106_555 65.45(4) ?
Ga1' Ga1 Ga1' 9_555 . 105_554 170.80(7) ?
Ga1' Ga1 Ga1' 9_555 . 10_555 81.34(7) ?
Ga1' Ga1 Ga1' 9_555 . 106_555 89.47(7) ?
Ga1' Ga1 Ge1 9_555 . 2_655 139.33(5) ?
Ga1' Ga1 Ge1 9_555 . 5_555 57.56(3) ?
Ga1' Ga1 Ge1 9_555 . 149_545 122.44(3) ?
Ga1' Ga1 Ge1 9_555 . 6_555 57.56(3) ?
Ga1' Ga1 Ge1 9_555 . 150_555 122.44(3) ?
Ga1' Ga1 Ge1 9_555 . 9_555 4.33(5) ?
Ga1' Ga1 Ge1 9_555 . 105_554 175.67(6) ?
Ga1' Ga1 Ge1 9_555 . 10_555 85.67(6) ?
Ga1' Ga1 Ge1 9_555 . 106_555 94.33(5) ?
Ga1' Ga1 Ge1' 9_555 . . 40.67(5) ?
Ga1' Ga1 Ge1' 9_555 . 5_555 54.88(4) ?
Ga1' Ga1 Ge1' 9_555 . 149_545 119.27(4) ?
Ga1' Ga1 Ge1' 9_555 . 6_555 54.88(4) ?
Ga1' Ga1 Ge1' 9_555 . 150_555 119.27(4) ?
Ga1' Ga1 Ge1' 9_555 . 9_555 0 ?
Ga1' Ga1 Ge1' 9_555 . 105_554 170.80(7) ?
Ga1' Ga1 Ge1' 9_555 . 10_555 81.34(7) ?
Ga1' Ga1 Ge1' 9_555 . 106_555 89.47(7) ?
Ga1' Ga1 Ga1' 105_554 . 10_555 89.47(7) ?
Ga1' Ga1 Ga1' 105_554 . 106_555 99.73(7) ?
Ga1' Ga1 Ge1 105_554 . 2_655 49.86(5) ?
Ga1' Ga1 Ge1 105_554 . 5_555 117.12(3) ?
Ga1' Ga1 Ge1 105_554 . 149_545 62.88(3) ?
Ga1' Ga1 Ge1 105_554 . 6_555 117.12(3) ?
Ga1' Ga1 Ge1 105_554 . 150_555 62.88(3) ?
Ga1' Ga1 Ge1 105_554 . 9_555 175.14(6) ?
Ga1' Ga1 Ge1 105_554 . 105_554 4.86(5) ?
Ga1' Ga1 Ge1 105_554 . 10_555 85.14(5) ?
Ga1' Ga1 Ge1 105_554 . 106_555 94.86(6) ?
Ga1' Ga1 Ge1' 105_554 . . 130.14(5) ?
Ga1' Ga1 Ge1' 105_554 . 5_555 119.27(4) ?
Ga1' Ga1 Ge1' 105_554 . 149_545 65.45(4) ?
Ga1' Ga1 Ge1' 105_554 . 6_555 119.27(4) ?
Ga1' Ga1 Ge1' 105_554 . 150_555 65.45(4) ?
Ga1' Ga1 Ge1' 105_554 . 9_555 170.80(7) ?
Ga1' Ga1 Ge1' 105_554 . 105_554 0 ?
Ga1' Ga1 Ge1' 105_554 . 10_555 89.47(7) ?
Ga1' Ga1 Ge1' 105_554 . 106_555 99.73(7) ?
Ga1' Ga1 Ga1' 10_555 . 106_555 170.80(7) ?
Ga1' Ga1 Ge1 10_555 . 2_655 139.33(5) ?
Ga1' Ga1 Ge1 10_555 . 5_555 57.56(3) ?
Ga1' Ga1 Ge1 10_555 . 149_545 122.44(3) ?
Ga1' Ga1 Ge1 10_555 . 6_555 57.56(3) ?
Ga1' Ga1 Ge1 10_555 . 150_555 122.44(3) ?
Ga1' Ga1 Ge1 10_555 . 9_555 85.67(6) ?
Ga1' Ga1 Ge1 10_555 . 105_554 94.33(5) ?
Ga1' Ga1 Ge1 10_555 . 10_555 4.33(5) ?
Ga1' Ga1 Ge1 10_555 . 106_555 175.67(6) ?
Ga1' Ga1 Ge1' 10_555 . . 40.67(5) ?
Ga1' Ga1 Ge1' 10_555 . 5_555 54.88(4) ?
Ga1' Ga1 Ge1' 10_555 . 149_545 119.27(4) ?
Ga1' Ga1 Ge1' 10_555 . 6_555 54.88(4) ?
Ga1' Ga1 Ge1' 10_555 . 150_555 119.27(4) ?
Ga1' Ga1 Ge1' 10_555 . 9_555 81.34(7) ?
Ga1' Ga1 Ge1' 10_555 . 105_554 89.47(7) ?
Ga1' Ga1 Ge1' 10_555 . 10_555 0 ?
Ga1' Ga1 Ge1' 10_555 . 106_555 170.80(7) ?
Ga1' Ga1 Ge1 106_555 . 2_655 49.86(5) ?
Ga1' Ga1 Ge1 106_555 . 5_555 117.12(3) ?
Ga1' Ga1 Ge1 106_555 . 149_545 62.88(3) ?
Ga1' Ga1 Ge1 106_555 . 6_555 117.12(3) ?
Ga1' Ga1 Ge1 106_555 . 150_555 62.88(3) ?
Ga1' Ga1 Ge1 106_555 . 9_555 85.14(5) ?
Ga1' Ga1 Ge1 106_555 . 105_554 94.86(6) ?
Ga1' Ga1 Ge1 106_555 . 10_555 175.14(6) ?
Ga1' Ga1 Ge1 106_555 . 106_555 4.86(5) ?
Ga1' Ga1 Ge1' 106_555 . . 130.14(5) ?
Ga1' Ga1 Ge1' 106_555 . 5_555 119.27(4) ?
Ga1' Ga1 Ge1' 106_555 . 149_545 65.45(4) ?
Ga1' Ga1 Ge1' 106_555 . 6_555 119.27(4) ?
Ga1' Ga1 Ge1' 106_555 . 150_555 65.45(4) ?
Ga1' Ga1 Ge1' 106_555 . 9_555 89.47(7) ?
Ga1' Ga1 Ge1' 106_555 . 105_554 99.73(7) ?
Ga1' Ga1 Ge1' 106_555 . 10_555 170.80(7) ?
Ga1' Ga1 Ge1' 106_555 . 106_555 0 ?
Ge1 Ga1 Ge1 2_655 . 5_555 135.000(18) ?
Ge1 Ga1 Ge1 2_655 . 149_545 45.00(2) ?
Ge1 Ga1 Ge1 2_655 . 6_555 135.000(18) ?
Ge1 Ga1 Ge1 2_655 . 150_555 45.00(2) ?
Ge1 Ga1 Ge1 2_655 . 9_555 135.000(18) ?
Ge1 Ga1 Ge1 2_655 . 105_554 45.00(2) ?
Ge1 Ga1 Ge1 2_655 . 10_555 135.000(18) ?
Ge1 Ga1 Ge1 2_655 . 106_555 45.00(2) ?
Ge1 Ga1 Ge1' 2_655 . . 180 ?
Ge1 Ga1 Ge1' 2_655 . 5_555 139.33(5) ?
Ge1 Ga1 Ge1' 2_655 . 149_545 49.86(5) ?
Ge1 Ga1 Ge1' 2_655 . 6_555 139.33(5) ?
Ge1 Ga1 Ge1' 2_655 . 150_555 49.86(5) ?
Ge1 Ga1 Ge1' 2_655 . 9_555 139.33(5) ?
Ge1 Ga1 Ge1' 2_655 . 105_554 49.86(5) ?
Ge1 Ga1 Ge1' 2_655 . 10_555 139.33(5) ?
Ge1 Ga1 Ge1' 2_655 . 106_555 49.86(5) ?
Ge1 Ga1 Ge1 5_555 . 149_545 180 ?
Ge1 Ga1 Ge1 5_555 . 6_555 90.00(3) ?
Ge1 Ga1 Ge1 5_555 . 150_555 90.00(2) ?
Ge1 Ga1 Ge1 5_555 . 9_555 60.000(18) ?
Ge1 Ga1 Ge1 5_555 . 105_554 120.000(13) ?
Ge1 Ga1 Ge1 5_555 . 10_555 60.000(18) ?
Ge1 Ga1 Ge1 5_555 . 106_555 120.000(13) ?
Ge1 Ga1 Ge1' 5_555 . . 45.000(18) ?
Ge1 Ga1 Ge1' 5_555 . 5_555 4.33(5) ?
Ge1 Ga1 Ge1' 5_555 . 149_545 175.14(6) ?
Ge1 Ga1 Ge1' 5_555 . 6_555 85.67(6) ?
Ge1 Ga1 Ge1' 5_555 . 150_555 85.14(5) ?
Ge1 Ga1 Ge1' 5_555 . 9_555 57.56(3) ?
Ge1 Ga1 Ge1' 5_555 . 105_554 117.12(3) ?
Ge1 Ga1 Ge1' 5_555 . 10_555 57.56(3) ?
Ge1 Ga1 Ge1' 5_555 . 106_555 117.12(3) ?
Ge1 Ga1 Ge1 149_545 . 6_555 90.00(2) ?
Ge1 Ga1 Ge1 149_545 . 150_555 90.00(4) ?
Ge1 Ga1 Ge1 149_545 . 9_555 120.000(13) ?
Ge1 Ga1 Ge1 149_545 . 105_554 60.00(2) ?
Ge1 Ga1 Ge1 149_545 . 10_555 120.000(13) ?
Ge1 Ga1 Ge1 149_545 . 106_555 60.00(2) ?
Ge1 Ga1 Ge1' 149_545 . . 135.00(2) ?
Ge1 Ga1 Ge1' 149_545 . 5_555 175.67(6) ?
Ge1 Ga1 Ge1' 149_545 . 149_545 4.86(5) ?
Ge1 Ga1 Ge1' 149_545 . 6_555 94.33(5) ?
Ge1 Ga1 Ge1' 149_545 . 150_555 94.86(6) ?
Ge1 Ga1 Ge1' 149_545 . 9_555 122.44(3) ?
Ge1 Ga1 Ge1' 149_545 . 105_554 62.88(3) ?
Ge1 Ga1 Ge1' 149_545 . 10_555 122.44(3) ?
Ge1 Ga1 Ge1' 149_545 . 106_555 62.88(3) ?
Ge1 Ga1 Ge1 6_555 . 150_555 180 ?
Ge1 Ga1 Ge1 6_555 . 9_555 60.000(18) ?
Ge1 Ga1 Ge1 6_555 . 105_554 120.000(13) ?
Ge1 Ga1 Ge1 6_555 . 10_555 60.000(18) ?
Ge1 Ga1 Ge1 6_555 . 106_555 120.000(13) ?
Ge1 Ga1 Ge1' 6_555 . . 45.000(18) ?
Ge1 Ga1 Ge1' 6_555 . 5_555 85.67(6) ?
Ge1 Ga1 Ge1' 6_555 . 149_545 85.14(5) ?
Ge1 Ga1 Ge1' 6_555 . 6_555 4.33(5) ?
Ge1 Ga1 Ge1' 6_555 . 150_555 175.14(6) ?
Ge1 Ga1 Ge1' 6_555 . 9_555 57.56(3) ?
Ge1 Ga1 Ge1' 6_555 . 105_554 117.12(3) ?
Ge1 Ga1 Ge1' 6_555 . 10_555 57.56(3) ?
Ge1 Ga1 Ge1' 6_555 . 106_555 117.12(3) ?
Ge1 Ga1 Ge1 150_555 . 9_555 120.000(13) ?
Ge1 Ga1 Ge1 150_555 . 105_554 60.00(2) ?
Ge1 Ga1 Ge1 150_555 . 10_555 120.000(13) ?
Ge1 Ga1 Ge1 150_555 . 106_555 60.00(2) ?
Ge1 Ga1 Ge1' 150_555 . . 135.00(2) ?
Ge1 Ga1 Ge1' 150_555 . 5_555 94.33(5) ?
Ge1 Ga1 Ge1' 150_555 . 149_545 94.86(6) ?
Ge1 Ga1 Ge1' 150_555 . 6_555 175.67(6) ?
Ge1 Ga1 Ge1' 150_555 . 150_555 4.86(5) ?
Ge1 Ga1 Ge1' 150_555 . 9_555 122.44(3) ?
Ge1 Ga1 Ge1' 150_555 . 105_554 62.88(3) ?
Ge1 Ga1 Ge1' 150_555 . 10_555 122.44(3) ?
Ge1 Ga1 Ge1' 150_555 . 106_555 62.88(3) ?
Ge1 Ga1 Ge1 9_555 . 105_554 180 ?
Ge1 Ga1 Ge1 9_555 . 10_555 90.00(3) ?
Ge1 Ga1 Ge1 9_555 . 106_555 90.00(2) ?
Ge1 Ga1 Ge1' 9_555 . . 45.000(18) ?
Ge1 Ga1 Ge1' 9_555 . 5_555 57.56(3) ?
Ge1 Ga1 Ge1' 9_555 . 149_545 117.12(3) ?
Ge1 Ga1 Ge1' 9_555 . 6_555 57.56(3) ?
Ge1 Ga1 Ge1' 9_555 . 150_555 117.12(3) ?
Ge1 Ga1 Ge1' 9_555 . 9_555 4.33(5) ?
Ge1 Ga1 Ge1' 9_555 . 105_554 175.14(6) ?
Ge1 Ga1 Ge1' 9_555 . 10_555 85.67(6) ?
Ge1 Ga1 Ge1' 9_555 . 106_555 85.14(5) ?
Ge1 Ga1 Ge1 105_554 . 10_555 90.00(2) ?
Ge1 Ga1 Ge1 105_554 . 106_555 90.00(4) ?
Ge1 Ga1 Ge1' 105_554 . . 135.00(2) ?
Ge1 Ga1 Ge1' 105_554 . 5_555 122.44(3) ?
Ge1 Ga1 Ge1' 105_554 . 149_545 62.88(3) ?
Ge1 Ga1 Ge1' 105_554 . 6_555 122.44(3) ?
Ge1 Ga1 Ge1' 105_554 . 150_555 62.88(3) ?
Ge1 Ga1 Ge1' 105_554 . 9_555 175.67(6) ?
Ge1 Ga1 Ge1' 105_554 . 105_554 4.86(5) ?
Ge1 Ga1 Ge1' 105_554 . 10_555 94.33(5) ?
Ge1 Ga1 Ge1' 105_554 . 106_555 94.86(6) ?
Ge1 Ga1 Ge1 10_555 . 106_555 180 ?
Ge1 Ga1 Ge1' 10_555 . . 45.000(18) ?
Ge1 Ga1 Ge1' 10_555 . 5_555 57.56(3) ?
Ge1 Ga1 Ge1' 10_555 . 149_545 117.12(3) ?
Ge1 Ga1 Ge1' 10_555 . 6_555 57.56(3) ?
Ge1 Ga1 Ge1' 10_555 . 150_555 117.12(3) ?
Ge1 Ga1 Ge1' 10_555 . 9_555 85.67(6) ?
Ge1 Ga1 Ge1' 10_555 . 105_554 85.14(5) ?
Ge1 Ga1 Ge1' 10_555 . 10_555 4.33(5) ?
Ge1 Ga1 Ge1' 10_555 . 106_555 175.14(6) ?
Ge1 Ga1 Ge1' 106_555 . . 135.00(2) ?
Ge1 Ga1 Ge1' 106_555 . 5_555 122.44(3) ?
Ge1 Ga1 Ge1' 106_555 . 149_545 62.88(3) ?
Ge1 Ga1 Ge1' 106_555 . 6_555 122.44(3) ?
Ge1 Ga1 Ge1' 106_555 . 150_555 62.88(3) ?
Ge1 Ga1 Ge1' 106_555 . 9_555 94.33(5) ?
Ge1 Ga1 Ge1' 106_555 . 105_554 94.86(6) ?
Ge1 Ga1 Ge1' 106_555 . 10_555 175.67(6) ?
Ge1 Ga1 Ge1' 106_555 . 106_555 4.86(5) ?
Ge1' Ga1 Ge1' . . 5_555 40.67(5) ?
Ge1' Ga1 Ge1' . . 149_545 130.14(5) ?
Ge1' Ga1 Ge1' . . 6_555 40.67(5) ?
Ge1' Ga1 Ge1' . . 150_555 130.14(5) ?
Ge1' Ga1 Ge1' . . 9_555 40.67(5) ?
Ge1' Ga1 Ge1' . . 105_554 130.14(5) ?
Ge1' Ga1 Ge1' . . 10_555 40.67(5) ?
Ge1' Ga1 Ge1' . . 106_555 130.14(5) ?
Ge1' Ga1 Ge1' 5_555 . 149_545 170.80(7) ?
Ge1' Ga1 Ge1' 5_555 . 6_555 81.34(7) ?
Ge1' Ga1 Ge1' 5_555 . 150_555 89.47(7) ?
Ge1' Ga1 Ge1' 5_555 . 9_555 54.88(4) ?
Ge1' Ga1 Ge1' 5_555 . 105_554 119.27(4) ?
Ge1' Ga1 Ge1' 5_555 . 10_555 54.88(4) ?
Ge1' Ga1 Ge1' 5_555 . 106_555 119.27(4) ?
Ge1' Ga1 Ge1' 149_545 . 6_555 89.47(7) ?
Ge1' Ga1 Ge1' 149_545 . 150_555 99.73(7) ?
Ge1' Ga1 Ge1' 149_545 . 9_555 119.27(4) ?
Ge1' Ga1 Ge1' 149_545 . 105_554 65.45(4) ?
Ge1' Ga1 Ge1' 149_545 . 10_555 119.27(4) ?
Ge1' Ga1 Ge1' 149_545 . 106_555 65.45(4) ?
Ge1' Ga1 Ge1' 6_555 . 150_555 170.80(7) ?
Ge1' Ga1 Ge1' 6_555 . 9_555 54.88(4) ?
Ge1' Ga1 Ge1' 6_555 . 105_554 119.27(4) ?
Ge1' Ga1 Ge1' 6_555 . 10_555 54.88(4) ?
Ge1' Ga1 Ge1' 6_555 . 106_555 119.27(4) ?
Ge1' Ga1 Ge1' 150_555 . 9_555 119.27(4) ?
Ge1' Ga1 Ge1' 150_555 . 105_554 65.45(4) ?
Ge1' Ga1 Ge1' 150_555 . 10_555 119.27(4) ?
Ge1' Ga1 Ge1' 150_555 . 106_555 65.45(4) ?
Ge1' Ga1 Ge1' 9_555 . 105_554 170.80(7) ?
Ge1' Ga1 Ge1' 9_555 . 10_555 81.34(7) ?
Ge1' Ga1 Ge1' 9_555 . 106_555 89.47(7) ?
Ge1' Ga1 Ge1' 105_554 . 10_555 89.47(7) ?
Ge1' Ga1 Ge1' 105_554 . 106_555 99.73(7) ?
Ge1' Ga1 Ge1' 10_555 . 106_555 170.80(7) ?
Sm1 Ga1' Sm1 . . 49_544 178.20(13) ?
Sm1 Ga1' Sm1 . . 13_555 89.986(3) ?
Sm1 Ga1' Sm1 . . 61_545 89.986(3) ?
Sm1 Ga1' Mn1 . . . 90.90(7) ?
Sm1 Ga1' Ga1 . . . 89.10(7) ?
Sm1 Ga1' Ga1 . . 5_555 58.26(3) ?
Sm1 Ga1' Ga1 . . 149_545 116.34(9) ?
Sm1 Ga1' Ga1 . . 6_555 123.13(8) ?
Sm1 Ga1' Ga1 . . 150_555 62.11(3) ?
Sm1 Ga1' Ga1 . . 9_555 58.26(3) ?
Sm1 Ga1' Ga1 . . 105_554 116.34(9) ?
Sm1 Ga1' Ga1 . . 10_555 123.13(8) ?
Sm1 Ga1' Ga1 . . 106_555 62.11(3) ?
Sm1 Ga1' Ga1' . . 5_555 60.74(4) ?
Sm1 Ga1' Ga1' . . 149_545 119.26(9) ?
Sm1 Ga1' Ga1' . . 6_555 120.73(9) ?
Sm1 Ga1' Ga1' . . 150_555 59.27(4) ?
Sm1 Ga1' Ga1' . . 9_555 60.74(4) ?
Sm1 Ga1' Ga1' . . 105_554 119.26(9) ?
Sm1 Ga1' Ga1' . . 10_555 120.73(9) ?
Sm1 Ga1' Ga1' . . 106_555 59.27(4) ?
Sm1 Ga1' Ge1 . . . 89.10(7) ?
Sm1 Ga1' Ge1 . . 5_555 58.26(3) ?
Sm1 Ga1' Ge1 . . 149_545 116.34(9) ?
Sm1 Ga1' Ge1 . . 6_555 123.13(8) ?
Sm1 Ga1' Ge1 . . 150_555 62.11(3) ?
Sm1 Ga1' Ge1 . . 9_555 58.26(3) ?
Sm1 Ga1' Ge1 . . 105_554 116.34(9) ?
Sm1 Ga1' Ge1 . . 10_555 123.13(8) ?
Sm1 Ga1' Ge1 . . 106_555 62.11(3) ?
Sm1 Ga1' Ge1' . . 5_555 60.74(4) ?
Sm1 Ga1' Ge1' . . 149_545 119.26(9) ?
Sm1 Ga1' Ge1' . . 6_555 120.73(9) ?
Sm1 Ga1' Ge1' . . 150_555 59.27(4) ?
Sm1 Ga1' Ge1' . . 9_555 60.74(4) ?
Sm1 Ga1' Ge1' . . 105_554 119.26(9) ?
Sm1 Ga1' Ge1' . . 10_555 120.73(9) ?
Sm1 Ga1' Ge1' . . 106_555 59.27(4) ?
Sm1 Ga1' Sm1 49_544 . 13_555 89.986(3) ?
Sm1 Ga1' Sm1 49_544 . 61_545 89.986(3) ?
Sm1 Ga1' Mn1 49_544 . . 90.90(7) ?
Sm1 Ga1' Ga1 49_544 . . 89.10(7) ?
Sm1 Ga1' Ga1 49_544 . 5_555 123.13(8) ?
Sm1 Ga1' Ga1 49_544 . 149_545 62.11(3) ?
Sm1 Ga1' Ga1 49_544 . 6_555 58.26(3) ?
Sm1 Ga1' Ga1 49_544 . 150_555 116.34(9) ?
Sm1 Ga1' Ga1 49_544 . 9_555 123.13(8) ?
Sm1 Ga1' Ga1 49_544 . 105_554 62.11(3) ?
Sm1 Ga1' Ga1 49_544 . 10_555 58.26(3) ?
Sm1 Ga1' Ga1 49_544 . 106_555 116.34(9) ?
Sm1 Ga1' Ga1' 49_544 . 5_555 120.73(9) ?
Sm1 Ga1' Ga1' 49_544 . 149_545 59.27(4) ?
Sm1 Ga1' Ga1' 49_544 . 6_555 60.74(4) ?
Sm1 Ga1' Ga1' 49_544 . 150_555 119.26(9) ?
Sm1 Ga1' Ga1' 49_544 . 9_555 120.73(9) ?
Sm1 Ga1' Ga1' 49_544 . 105_554 59.27(4) ?
Sm1 Ga1' Ga1' 49_544 . 10_555 60.74(4) ?
Sm1 Ga1' Ga1' 49_544 . 106_555 119.26(9) ?
Sm1 Ga1' Ge1 49_544 . . 89.10(7) ?
Sm1 Ga1' Ge1 49_544 . 5_555 123.13(8) ?
Sm1 Ga1' Ge1 49_544 . 149_545 62.11(3) ?
Sm1 Ga1' Ge1 49_544 . 6_555 58.26(3) ?
Sm1 Ga1' Ge1 49_544 . 150_555 116.34(9) ?
Sm1 Ga1' Ge1 49_544 . 9_555 123.13(8) ?
Sm1 Ga1' Ge1 49_544 . 105_554 62.11(3) ?
Sm1 Ga1' Ge1 49_544 . 10_555 58.26(3) ?
Sm1 Ga1' Ge1 49_544 . 106_555 116.34(9) ?
Sm1 Ga1' Ge1' 49_544 . 5_555 120.73(9) ?
Sm1 Ga1' Ge1' 49_544 . 149_545 59.27(4) ?
Sm1 Ga1' Ge1' 49_544 . 6_555 60.74(4) ?
Sm1 Ga1' Ge1' 49_544 . 150_555 119.26(9) ?
Sm1 Ga1' Ge1' 49_544 . 9_555 120.73(9) ?
Sm1 Ga1' Ge1' 49_544 . 105_554 59.27(4) ?
Sm1 Ga1' Ge1' 49_544 . 10_555 60.74(4) ?
Sm1 Ga1' Ge1' 49_544 . 106_555 119.26(9) ?
Sm1 Ga1' Sm1 13_555 . 61_545 178.20(13) ?
Sm1 Ga1' Mn1 13_555 . . 90.90(7) ?
Sm1 Ga1' Ga1 13_555 . . 89.10(7) ?
Sm1 Ga1' Ga1 13_555 . 5_555 58.26(3) ?
Sm1 Ga1' Ga1 13_555 . 149_545 116.34(9) ?
Sm1 Ga1' Ga1 13_555 . 6_555 123.13(8) ?
Sm1 Ga1' Ga1 13_555 . 150_555 62.11(3) ?
Sm1 Ga1' Ga1 13_555 . 9_555 123.13(8) ?
Sm1 Ga1' Ga1 13_555 . 105_554 62.11(3) ?
Sm1 Ga1' Ga1 13_555 . 10_555 58.26(3) ?
Sm1 Ga1' Ga1 13_555 . 106_555 116.34(9) ?
Sm1 Ga1' Ga1' 13_555 . 5_555 60.74(4) ?
Sm1 Ga1' Ga1' 13_555 . 149_545 119.26(9) ?
Sm1 Ga1' Ga1' 13_555 . 6_555 120.73(9) ?
Sm1 Ga1' Ga1' 13_555 . 150_555 59.27(4) ?
Sm1 Ga1' Ga1' 13_555 . 9_555 120.73(9) ?
Sm1 Ga1' Ga1' 13_555 . 105_554 59.27(4) ?
Sm1 Ga1' Ga1' 13_555 . 10_555 60.74(4) ?
Sm1 Ga1' Ga1' 13_555 . 106_555 119.26(9) ?
Sm1 Ga1' Ge1 13_555 . . 89.10(7) ?
Sm1 Ga1' Ge1 13_555 . 5_555 58.26(3) ?
Sm1 Ga1' Ge1 13_555 . 149_545 116.34(9) ?
Sm1 Ga1' Ge1 13_555 . 6_555 123.13(8) ?
Sm1 Ga1' Ge1 13_555 . 150_555 62.11(3) ?
Sm1 Ga1' Ge1 13_555 . 9_555 123.13(8) ?
Sm1 Ga1' Ge1 13_555 . 105_554 62.11(3) ?
Sm1 Ga1' Ge1 13_555 . 10_555 58.26(3) ?
Sm1 Ga1' Ge1 13_555 . 106_555 116.34(9) ?
Sm1 Ga1' Ge1' 13_555 . 5_555 60.74(4) ?
Sm1 Ga1' Ge1' 13_555 . 149_545 119.26(9) ?
Sm1 Ga1' Ge1' 13_555 . 6_555 120.73(9) ?
Sm1 Ga1' Ge1' 13_555 . 150_555 59.27(4) ?
Sm1 Ga1' Ge1' 13_555 . 9_555 120.73(9) ?
Sm1 Ga1' Ge1' 13_555 . 105_554 59.27(4) ?
Sm1 Ga1' Ge1' 13_555 . 10_555 60.74(4) ?
Sm1 Ga1' Ge1' 13_555 . 106_555 119.26(9) ?
Sm1 Ga1' Mn1 61_545 . . 90.90(7) ?
Sm1 Ga1' Ga1 61_545 . . 89.10(7) ?
Sm1 Ga1' Ga1 61_545 . 5_555 123.13(8) ?
Sm1 Ga1' Ga1 61_545 . 149_545 62.11(3) ?
Sm1 Ga1' Ga1 61_545 . 6_555 58.26(3) ?
Sm1 Ga1' Ga1 61_545 . 150_555 116.34(9) ?
Sm1 Ga1' Ga1 61_545 . 9_555 58.26(3) ?
Sm1 Ga1' Ga1 61_545 . 105_554 116.34(9) ?
Sm1 Ga1' Ga1 61_545 . 10_555 123.13(8) ?
Sm1 Ga1' Ga1 61_545 . 106_555 62.11(3) ?
Sm1 Ga1' Ga1' 61_545 . 5_555 120.73(9) ?
Sm1 Ga1' Ga1' 61_545 . 149_545 59.27(4) ?
Sm1 Ga1' Ga1' 61_545 . 6_555 60.74(4) ?
Sm1 Ga1' Ga1' 61_545 . 150_555 119.26(9) ?
Sm1 Ga1' Ga1' 61_545 . 9_555 60.74(4) ?
Sm1 Ga1' Ga1' 61_545 . 105_554 119.26(9) ?
Sm1 Ga1' Ga1' 61_545 . 10_555 120.73(9) ?
Sm1 Ga1' Ga1' 61_545 . 106_555 59.27(4) ?
Sm1 Ga1' Ge1 61_545 . . 89.10(7) ?
Sm1 Ga1' Ge1 61_545 . 5_555 123.13(8) ?
Sm1 Ga1' Ge1 61_545 . 149_545 62.11(3) ?
Sm1 Ga1' Ge1 61_545 . 6_555 58.26(3) ?
Sm1 Ga1' Ge1 61_545 . 150_555 116.34(9) ?
Sm1 Ga1' Ge1 61_545 . 9_555 58.26(3) ?
Sm1 Ga1' Ge1 61_545 . 105_554 116.34(9) ?
Sm1 Ga1' Ge1 61_545 . 10_555 123.13(8) ?
Sm1 Ga1' Ge1 61_545 . 106_555 62.11(3) ?
Sm1 Ga1' Ge1' 61_545 . 5_555 120.73(9) ?
Sm1 Ga1' Ge1' 61_545 . 149_545 59.27(4) ?
Sm1 Ga1' Ge1' 61_545 . 6_555 60.74(4) ?
Sm1 Ga1' Ge1' 61_545 . 150_555 119.26(9) ?
Sm1 Ga1' Ge1' 61_545 . 9_555 60.74(4) ?
Sm1 Ga1' Ge1' 61_545 . 105_554 119.26(9) ?
Sm1 Ga1' Ge1' 61_545 . 10_555 120.73(9) ?
Sm1 Ga1' Ge1' 61_545 . 106_555 59.27(4) ?
Mn1 Ga1' Ga1 . . . 180 ?
Mn1 Ga1' Ga1 . . 5_555 49.33(5) ?
Mn1 Ga1' Ga1 . . 149_545 139.86(5) ?
Mn1 Ga1' Ga1 . . 6_555 49.33(5) ?
Mn1 Ga1' Ga1 . . 150_555 139.86(5) ?
Mn1 Ga1' Ga1 . . 9_555 49.33(5) ?
Mn1 Ga1' Ga1 . . 105_554 139.86(5) ?
Mn1 Ga1' Ga1 . . 10_555 49.33(5) ?
Mn1 Ga1' Ga1 . . 106_555 139.86(5) ?
Mn1 Ga1' Ga1' . . 5_555 45.00(7) ?
Mn1 Ga1' Ga1' . . 149_545 135.00(7) ?
Mn1 Ga1' Ga1' . . 6_555 45.00(7) ?
Mn1 Ga1' Ga1' . . 150_555 135.00(7) ?
Mn1 Ga1' Ga1' . . 9_555 45.00(7) ?
Mn1 Ga1' Ga1' . . 105_554 135.00(7) ?
Mn1 Ga1' Ga1' . . 10_555 45.00(7) ?
Mn1 Ga1' Ga1' . . 106_555 135.00(7) ?
Mn1 Ga1' Ge1 . . . 180 ?
Mn1 Ga1' Ge1 . . 5_555 49.33(5) ?
Mn1 Ga1' Ge1 . . 149_545 139.86(5) ?
Mn1 Ga1' Ge1 . . 6_555 49.33(5) ?
Mn1 Ga1' Ge1 . . 150_555 139.86(5) ?
Mn1 Ga1' Ge1 . . 9_555 49.33(5) ?
Mn1 Ga1' Ge1 . . 105_554 139.86(5) ?
Mn1 Ga1' Ge1 . . 10_555 49.33(5) ?
Mn1 Ga1' Ge1 . . 106_555 139.86(5) ?
Mn1 Ga1' Ge1' . . 5_555 45.00(7) ?
Mn1 Ga1' Ge1' . . 149_545 135.00(7) ?
Mn1 Ga1' Ge1' . . 6_555 45.00(7) ?
Mn1 Ga1' Ge1' . . 150_555 135.00(7) ?
Mn1 Ga1' Ge1' . . 9_555 45.00(7) ?
Mn1 Ga1' Ge1' . . 105_554 135.00(7) ?
Mn1 Ga1' Ge1' . . 10_555 45.00(7) ?
Mn1 Ga1' Ge1' . . 106_555 135.00(7) ?
Ga1 Ga1' Ga1 . . 5_555 130.67(5) ?
Ga1 Ga1' Ga1 . . 149_545 40.14(5) ?
Ga1 Ga1' Ga1 . . 6_555 130.67(5) ?
Ga1 Ga1' Ga1 . . 150_555 40.14(5) ?
Ga1 Ga1' Ga1 . . 9_555 130.67(5) ?
Ga1 Ga1' Ga1 . . 105_554 40.14(5) ?
Ga1 Ga1' Ga1 . . 10_555 130.67(5) ?
Ga1 Ga1' Ga1 . . 106_555 40.14(5) ?
Ga1 Ga1' Ga1' . . 5_555 135.00(7) ?
Ga1 Ga1' Ga1' . . 149_545 45.00(7) ?
Ga1 Ga1' Ga1' . . 6_555 135.00(7) ?
Ga1 Ga1' Ga1' . . 150_555 45.00(7) ?
Ga1 Ga1' Ga1' . . 9_555 135.00(7) ?
Ga1 Ga1' Ga1' . . 105_554 45.00(7) ?
Ga1 Ga1' Ga1' . . 10_555 135.00(7) ?
Ga1 Ga1' Ga1' . . 106_555 45.00(7) ?
Ga1 Ga1' Ge1 . . . 0 ?
Ga1 Ga1' Ge1 . . 5_555 130.67(5) ?
Ga1 Ga1' Ge1 . . 149_545 40.14(5) ?
Ga1 Ga1' Ge1 . . 6_555 130.67(5) ?
Ga1 Ga1' Ge1 . . 150_555 40.14(5) ?
Ga1 Ga1' Ge1 . . 9_555 130.67(5) ?
Ga1 Ga1' Ge1 . . 105_554 40.14(5) ?
Ga1 Ga1' Ge1 . . 10_555 130.67(5) ?
Ga1 Ga1' Ge1 . . 106_555 40.14(5) ?
Ga1 Ga1' Ge1' . . 5_555 135.00(7) ?
Ga1 Ga1' Ge1' . . 149_545 45.00(7) ?
Ga1 Ga1' Ge1' . . 6_555 135.00(7) ?
Ga1 Ga1' Ge1' . . 150_555 45.00(7) ?
Ga1 Ga1' Ge1' . . 9_555 135.00(7) ?
Ga1 Ga1' Ge1' . . 105_554 45.00(7) ?
Ga1 Ga1' Ge1' . . 10_555 135.00(7) ?
Ga1 Ga1' Ge1' . . 106_555 45.00(7) ?
Ga1 Ga1' Ga1 5_555 . 149_545 170.80(10) ?
Ga1 Ga1' Ga1 5_555 . 6_555 98.66(10) ?
Ga1 Ga1' Ga1 5_555 . 150_555 90.53(2) ?
Ga1 Ga1' Ga1 5_555 . 9_555 64.87(5) ?
Ga1 Ga1' Ga1 5_555 . 105_554 119.881(15) ?
Ga1 Ga1' Ga1 5_555 . 10_555 64.87(5) ?
Ga1 Ga1' Ga1 5_555 . 106_555 119.881(15) ?
Ga1 Ga1' Ga1' 5_555 . 5_555 4.33(5) ?
Ga1 Ga1' Ga1' 5_555 . 149_545 175.67(11) ?
Ga1 Ga1' Ga1' 5_555 . 6_555 94.33(11) ?
Ga1 Ga1' Ga1' 5_555 . 150_555 85.67(5) ?
Ga1 Ga1' Ga1' 5_555 . 9_555 62.56(6) ?
Ga1 Ga1' Ga1' 5_555 . 105_554 117.44(3) ?
Ga1 Ga1' Ga1' 5_555 . 10_555 62.56(6) ?
Ga1 Ga1' Ga1' 5_555 . 106_555 117.44(3) ?
Ga1 Ga1' Ge1 5_555 . . 130.67(5) ?
Ga1 Ga1' Ge1 5_555 . 5_555 0 ?
Ga1 Ga1' Ge1 5_555 . 149_545 170.80(10) ?
Ga1 Ga1' Ge1 5_555 . 6_555 98.66(10) ?
Ga1 Ga1' Ge1 5_555 . 150_555 90.53(2) ?
Ga1 Ga1' Ge1 5_555 . 9_555 64.87(5) ?
Ga1 Ga1' Ge1 5_555 . 105_554 119.881(15) ?
Ga1 Ga1' Ge1 5_555 . 10_555 64.87(5) ?
Ga1 Ga1' Ge1 5_555 . 106_555 119.881(15) ?
Ga1 Ga1' Ge1' 5_555 . 5_555 4.33(5) ?
Ga1 Ga1' Ge1' 5_555 . 149_545 175.67(11) ?
Ga1 Ga1' Ge1' 5_555 . 6_555 94.33(11) ?
Ga1 Ga1' Ge1' 5_555 . 150_555 85.67(5) ?
Ga1 Ga1' Ge1' 5_555 . 9_555 62.56(6) ?
Ga1 Ga1' Ge1' 5_555 . 105_554 117.44(3) ?
Ga1 Ga1' Ge1' 5_555 . 10_555 62.56(6) ?
Ga1 Ga1' Ge1' 5_555 . 106_555 117.44(3) ?
Ga1 Ga1' Ga1 149_545 . 6_555 90.53(2) ?
Ga1 Ga1' Ga1 149_545 . 150_555 80.27(9) ?
Ga1 Ga1' Ga1 149_545 . 9_555 119.881(15) ?
Ga1 Ga1' Ga1 149_545 . 105_554 54.23(6) ?
Ga1 Ga1' Ga1 149_545 . 10_555 119.881(15) ?
Ga1 Ga1' Ga1 149_545 . 106_555 54.23(6) ?
Ga1 Ga1' Ga1' 149_545 . 5_555 175.14(11) ?
Ga1 Ga1' Ga1' 149_545 . 149_545 4.86(5) ?
Ga1 Ga1' Ga1' 149_545 . 6_555 94.86(5) ?
Ga1 Ga1' Ga1' 149_545 . 150_555 85.14(10) ?
Ga1 Ga1' Ga1' 149_545 . 9_555 122.72(3) ?
Ga1 Ga1' Ga1' 149_545 . 105_554 57.28(6) ?
Ga1 Ga1' Ga1' 149_545 . 10_555 122.72(3) ?
Ga1 Ga1' Ga1' 149_545 . 106_555 57.28(6) ?
Ga1 Ga1' Ge1 149_545 . . 40.14(5) ?
Ga1 Ga1' Ge1 149_545 . 5_555 170.80(10) ?
Ga1 Ga1' Ge1 149_545 . 149_545 0 ?
Ga1 Ga1' Ge1 149_545 . 6_555 90.53(2) ?
Ga1 Ga1' Ge1 149_545 . 150_555 80.27(9) ?
Ga1 Ga1' Ge1 149_545 . 9_555 119.881(15) ?
Ga1 Ga1' Ge1 149_545 . 105_554 54.23(6) ?
Ga1 Ga1' Ge1 149_545 . 10_555 119.881(15) ?
Ga1 Ga1' Ge1 149_545 . 106_555 54.23(6) ?
Ga1 Ga1' Ge1' 149_545 . 5_555 175.14(11) ?
Ga1 Ga1' Ge1' 149_545 . 149_545 4.86(5) ?
Ga1 Ga1' Ge1' 149_545 . 6_555 94.86(5) ?
Ga1 Ga1' Ge1' 149_545 . 150_555 85.14(10) ?
Ga1 Ga1' Ge1' 149_545 . 9_555 122.72(3) ?
Ga1 Ga1' Ge1' 149_545 . 105_554 57.28(6) ?
Ga1 Ga1' Ge1' 149_545 . 10_555 122.72(3) ?
Ga1 Ga1' Ge1' 149_545 . 106_555 57.28(6) ?
Ga1 Ga1' Ga1 6_555 . 150_555 170.80(10) ?
Ga1 Ga1' Ga1 6_555 . 9_555 64.87(5) ?
Ga1 Ga1' Ga1 6_555 . 105_554 119.881(15) ?
Ga1 Ga1' Ga1 6_555 . 10_555 64.87(5) ?
Ga1 Ga1' Ga1 6_555 . 106_555 119.881(15) ?
Ga1 Ga1' Ga1' 6_555 . 5_555 94.33(11) ?
Ga1 Ga1' Ga1' 6_555 . 149_545 85.67(5) ?
Ga1 Ga1' Ga1' 6_555 . 6_555 4.33(5) ?
Ga1 Ga1' Ga1' 6_555 . 150_555 175.67(11) ?
Ga1 Ga1' Ga1' 6_555 . 9_555 62.56(6) ?
Ga1 Ga1' Ga1' 6_555 . 105_554 117.44(3) ?
Ga1 Ga1' Ga1' 6_555 . 10_555 62.56(6) ?
Ga1 Ga1' Ga1' 6_555 . 106_555 117.44(3) ?
Ga1 Ga1' Ge1 6_555 . . 130.67(5) ?
Ga1 Ga1' Ge1 6_555 . 5_555 98.66(10) ?
Ga1 Ga1' Ge1 6_555 . 149_545 90.53(2) ?
Ga1 Ga1' Ge1 6_555 . 6_555 0 ?
Ga1 Ga1' Ge1 6_555 . 150_555 170.80(10) ?
Ga1 Ga1' Ge1 6_555 . 9_555 64.87(5) ?
Ga1 Ga1' Ge1 6_555 . 105_554 119.881(15) ?
Ga1 Ga1' Ge1 6_555 . 10_555 64.87(5) ?
Ga1 Ga1' Ge1 6_555 . 106_555 119.881(15) ?
Ga1 Ga1' Ge1' 6_555 . 5_555 94.33(11) ?
Ga1 Ga1' Ge1' 6_555 . 149_545 85.67(5) ?
Ga1 Ga1' Ge1' 6_555 . 6_555 4.33(5) ?
Ga1 Ga1' Ge1' 6_555 . 150_555 175.67(11) ?
Ga1 Ga1' Ge1' 6_555 . 9_555 62.56(6) ?
Ga1 Ga1' Ge1' 6_555 . 105_554 117.44(3) ?
Ga1 Ga1' Ge1' 6_555 . 10_555 62.56(6) ?
Ga1 Ga1' Ge1' 6_555 . 106_555 117.44(3) ?
Ga1 Ga1' Ga1 150_555 . 9_555 119.881(15) ?
Ga1 Ga1' Ga1 150_555 . 105_554 54.23(6) ?
Ga1 Ga1' Ga1 150_555 . 10_555 119.881(15) ?
Ga1 Ga1' Ga1 150_555 . 106_555 54.23(6) ?
Ga1 Ga1' Ga1' 150_555 . 5_555 94.86(5) ?
Ga1 Ga1' Ga1' 150_555 . 149_545 85.14(10) ?
Ga1 Ga1' Ga1' 150_555 . 6_555 175.14(11) ?
Ga1 Ga1' Ga1' 150_555 . 150_555 4.86(5) ?
Ga1 Ga1' Ga1' 150_555 . 9_555 122.72(3) ?
Ga1 Ga1' Ga1' 150_555 . 105_554 57.28(6) ?
Ga1 Ga1' Ga1' 150_555 . 10_555 122.72(3) ?
Ga1 Ga1' Ga1' 150_555 . 106_555 57.28(6) ?
Ga1 Ga1' Ge1 150_555 . . 40.14(5) ?
Ga1 Ga1' Ge1 150_555 . 5_555 90.53(2) ?
Ga1 Ga1' Ge1 150_555 . 149_545 80.27(9) ?
Ga1 Ga1' Ge1 150_555 . 6_555 170.80(10) ?
Ga1 Ga1' Ge1 150_555 . 150_555 0 ?
Ga1 Ga1' Ge1 150_555 . 9_555 119.881(15) ?
Ga1 Ga1' Ge1 150_555 . 105_554 54.23(6) ?
Ga1 Ga1' Ge1 150_555 . 10_555 119.881(15) ?
Ga1 Ga1' Ge1 150_555 . 106_555 54.23(6) ?
Ga1 Ga1' Ge1' 150_555 . 5_555 94.86(5) ?
Ga1 Ga1' Ge1' 150_555 . 149_545 85.14(10) ?
Ga1 Ga1' Ge1' 150_555 . 6_555 175.14(11) ?
Ga1 Ga1' Ge1' 150_555 . 150_555 4.86(5) ?
Ga1 Ga1' Ge1' 150_555 . 9_555 122.72(3) ?
Ga1 Ga1' Ge1' 150_555 . 105_554 57.28(6) ?
Ga1 Ga1' Ge1' 150_555 . 10_555 122.72(3) ?
Ga1 Ga1' Ge1' 150_555 . 106_555 57.28(6) ?
Ga1 Ga1' Ga1 9_555 . 105_554 170.80(10) ?
Ga1 Ga1' Ga1 9_555 . 10_555 98.66(10) ?
Ga1 Ga1' Ga1 9_555 . 106_555 90.53(2) ?
Ga1 Ga1' Ga1' 9_555 . 5_555 62.56(6) ?
Ga1 Ga1' Ga1' 9_555 . 149_545 117.44(3) ?
Ga1 Ga1' Ga1' 9_555 . 6_555 62.56(6) ?
Ga1 Ga1' Ga1' 9_555 . 150_555 117.44(3) ?
Ga1 Ga1' Ga1' 9_555 . 9_555 4.33(5) ?
Ga1 Ga1' Ga1' 9_555 . 105_554 175.67(11) ?
Ga1 Ga1' Ga1' 9_555 . 10_555 94.33(11) ?
Ga1 Ga1' Ga1' 9_555 . 106_555 85.67(5) ?
Ga1 Ga1' Ge1 9_555 . . 130.67(5) ?
Ga1 Ga1' Ge1 9_555 . 5_555 64.87(5) ?
Ga1 Ga1' Ge1 9_555 . 149_545 119.881(15) ?
Ga1 Ga1' Ge1 9_555 . 6_555 64.87(5) ?
Ga1 Ga1' Ge1 9_555 . 150_555 119.881(15) ?
Ga1 Ga1' Ge1 9_555 . 9_555 0 ?
Ga1 Ga1' Ge1 9_555 . 105_554 170.80(10) ?
Ga1 Ga1' Ge1 9_555 . 10_555 98.66(10) ?
Ga1 Ga1' Ge1 9_555 . 106_555 90.53(2) ?
Ga1 Ga1' Ge1' 9_555 . 5_555 62.56(6) ?
Ga1 Ga1' Ge1' 9_555 . 149_545 117.44(3) ?
Ga1 Ga1' Ge1' 9_555 . 6_555 62.56(6) ?
Ga1 Ga1' Ge1' 9_555 . 150_555 117.44(3) ?
Ga1 Ga1' Ge1' 9_555 . 9_555 4.33(5) ?
Ga1 Ga1' Ge1' 9_555 . 105_554 175.67(11) ?
Ga1 Ga1' Ge1' 9_555 . 10_555 94.33(11) ?
Ga1 Ga1' Ge1' 9_555 . 106_555 85.67(5) ?
Ga1 Ga1' Ga1 105_554 . 10_555 90.53(2) ?
Ga1 Ga1' Ga1 105_554 . 106_555 80.27(9) ?
Ga1 Ga1' Ga1' 105_554 . 5_555 122.72(3) ?
Ga1 Ga1' Ga1' 105_554 . 149_545 57.28(6) ?
Ga1 Ga1' Ga1' 105_554 . 6_555 122.72(3) ?
Ga1 Ga1' Ga1' 105_554 . 150_555 57.28(6) ?
Ga1 Ga1' Ga1' 105_554 . 9_555 175.14(11) ?
Ga1 Ga1' Ga1' 105_554 . 105_554 4.86(5) ?
Ga1 Ga1' Ga1' 105_554 . 10_555 94.86(5) ?
Ga1 Ga1' Ga1' 105_554 . 106_555 85.14(10) ?
Ga1 Ga1' Ge1 105_554 . . 40.14(5) ?
Ga1 Ga1' Ge1 105_554 . 5_555 119.881(15) ?
Ga1 Ga1' Ge1 105_554 . 149_545 54.23(6) ?
Ga1 Ga1' Ge1 105_554 . 6_555 119.881(15) ?
Ga1 Ga1' Ge1 105_554 . 150_555 54.23(6) ?
Ga1 Ga1' Ge1 105_554 . 9_555 170.80(10) ?
Ga1 Ga1' Ge1 105_554 . 105_554 0 ?
Ga1 Ga1' Ge1 105_554 . 10_555 90.53(2) ?
Ga1 Ga1' Ge1 105_554 . 106_555 80.27(9) ?
Ga1 Ga1' Ge1' 105_554 . 5_555 122.72(3) ?
Ga1 Ga1' Ge1' 105_554 . 149_545 57.28(6) ?
Ga1 Ga1' Ge1' 105_554 . 6_555 122.72(3) ?
Ga1 Ga1' Ge1' 105_554 . 150_555 57.28(6) ?
Ga1 Ga1' Ge1' 105_554 . 9_555 175.14(11) ?
Ga1 Ga1' Ge1' 105_554 . 105_554 4.86(5) ?
Ga1 Ga1' Ge1' 105_554 . 10_555 94.86(5) ?
Ga1 Ga1' Ge1' 105_554 . 106_555 85.14(10) ?
Ga1 Ga1' Ga1 10_555 . 106_555 170.80(10) ?
Ga1 Ga1' Ga1' 10_555 . 5_555 62.56(6) ?
Ga1 Ga1' Ga1' 10_555 . 149_545 117.44(3) ?
Ga1 Ga1' Ga1' 10_555 . 6_555 62.56(6) ?
Ga1 Ga1' Ga1' 10_555 . 150_555 117.44(3) ?
Ga1 Ga1' Ga1' 10_555 . 9_555 94.33(11) ?
Ga1 Ga1' Ga1' 10_555 . 105_554 85.67(5) ?
Ga1 Ga1' Ga1' 10_555 . 10_555 4.33(5) ?
Ga1 Ga1' Ga1' 10_555 . 106_555 175.67(11) ?
Ga1 Ga1' Ge1 10_555 . . 130.67(5) ?
Ga1 Ga1' Ge1 10_555 . 5_555 64.87(5) ?
Ga1 Ga1' Ge1 10_555 . 149_545 119.881(15) ?
Ga1 Ga1' Ge1 10_555 . 6_555 64.87(5) ?
Ga1 Ga1' Ge1 10_555 . 150_555 119.881(15) ?
Ga1 Ga1' Ge1 10_555 . 9_555 98.66(10) ?
Ga1 Ga1' Ge1 10_555 . 105_554 90.53(2) ?
Ga1 Ga1' Ge1 10_555 . 10_555 0 ?
Ga1 Ga1' Ge1 10_555 . 106_555 170.80(10) ?
Ga1 Ga1' Ge1' 10_555 . 5_555 62.56(6) ?
Ga1 Ga1' Ge1' 10_555 . 149_545 117.44(3) ?
Ga1 Ga1' Ge1' 10_555 . 6_555 62.56(6) ?
Ga1 Ga1' Ge1' 10_555 . 150_555 117.44(3) ?
Ga1 Ga1' Ge1' 10_555 . 9_555 94.33(11) ?
Ga1 Ga1' Ge1' 10_555 . 105_554 85.67(5) ?
Ga1 Ga1' Ge1' 10_555 . 10_555 4.33(5) ?
Ga1 Ga1' Ge1' 10_555 . 106_555 175.67(11) ?
Ga1 Ga1' Ga1' 106_555 . 5_555 122.72(3) ?
Ga1 Ga1' Ga1' 106_555 . 149_545 57.28(6) ?
Ga1 Ga1' Ga1' 106_555 . 6_555 122.72(3) ?
Ga1 Ga1' Ga1' 106_555 . 150_555 57.28(6) ?
Ga1 Ga1' Ga1' 106_555 . 9_555 94.86(5) ?
Ga1 Ga1' Ga1' 106_555 . 105_554 85.14(10) ?
Ga1 Ga1' Ga1' 106_555 . 10_555 175.14(11) ?
Ga1 Ga1' Ga1' 106_555 . 106_555 4.86(5) ?
Ga1 Ga1' Ge1 106_555 . . 40.14(5) ?
Ga1 Ga1' Ge1 106_555 . 5_555 119.881(15) ?
Ga1 Ga1' Ge1 106_555 . 149_545 54.23(6) ?
Ga1 Ga1' Ge1 106_555 . 6_555 119.881(15) ?
Ga1 Ga1' Ge1 106_555 . 150_555 54.23(6) ?
Ga1 Ga1' Ge1 106_555 . 9_555 90.53(2) ?
Ga1 Ga1' Ge1 106_555 . 105_554 80.27(9) ?
Ga1 Ga1' Ge1 106_555 . 10_555 170.80(10) ?
Ga1 Ga1' Ge1 106_555 . 106_555 0 ?
Ga1 Ga1' Ge1' 106_555 . 5_555 122.72(3) ?
Ga1 Ga1' Ge1' 106_555 . 149_545 57.28(6) ?
Ga1 Ga1' Ge1' 106_555 . 6_555 122.72(3) ?
Ga1 Ga1' Ge1' 106_555 . 150_555 57.28(6) ?
Ga1 Ga1' Ge1' 106_555 . 9_555 94.86(5) ?
Ga1 Ga1' Ge1' 106_555 . 105_554 85.14(10) ?
Ga1 Ga1' Ge1' 106_555 . 10_555 175.14(11) ?
Ga1 Ga1' Ge1' 106_555 . 106_555 4.86(5) ?
Ga1' Ga1' Ga1' 5_555 . 149_545 180 ?
Ga1' Ga1' Ga1' 5_555 . 6_555 90.00(12) ?
Ga1' Ga1' Ga1' 5_555 . 150_555 90.00(7) ?
Ga1' Ga1' Ga1' 5_555 . 9_555 60.00(7) ?
Ga1' Ga1' Ga1' 5_555 . 105_554 120.00(4) ?
Ga1' Ga1' Ga1' 5_555 . 10_555 60.00(7) ?
Ga1' Ga1' Ga1' 5_555 . 106_555 120.00(4) ?
Ga1' Ga1' Ge1 5_555 . . 135.00(7) ?
Ga1' Ga1' Ge1 5_555 . 5_555 4.33(5) ?
Ga1' Ga1' Ge1 5_555 . 149_545 175.14(11) ?
Ga1' Ga1' Ge1 5_555 . 6_555 94.33(11) ?
Ga1' Ga1' Ge1 5_555 . 150_555 94.86(5) ?
Ga1' Ga1' Ge1 5_555 . 9_555 62.56(6) ?
Ga1' Ga1' Ge1 5_555 . 105_554 122.72(3) ?
Ga1' Ga1' Ge1 5_555 . 10_555 62.56(6) ?
Ga1' Ga1' Ge1 5_555 . 106_555 122.72(3) ?
Ga1' Ga1' Ge1' 5_555 . 5_555 0 ?
Ga1' Ga1' Ge1' 5_555 . 149_545 180 ?
Ga1' Ga1' Ge1' 5_555 . 6_555 90.00(12) ?
Ga1' Ga1' Ge1' 5_555 . 150_555 90.00(7) ?
Ga1' Ga1' Ge1' 5_555 . 9_555 60.00(7) ?
Ga1' Ga1' Ge1' 5_555 . 105_554 120.00(4) ?
Ga1' Ga1' Ge1' 5_555 . 10_555 60.00(7) ?
Ga1' Ga1' Ge1' 5_555 . 106_555 120.00(4) ?
Ga1' Ga1' Ga1' 149_545 . 6_555 90.00(7) ?
Ga1' Ga1' Ga1' 149_545 . 150_555 90.00(11) ?
Ga1' Ga1' Ga1' 149_545 . 9_555 120.00(4) ?
Ga1' Ga1' Ga1' 149_545 . 105_554 60.00(7) ?
Ga1' Ga1' Ga1' 149_545 . 10_555 120.00(4) ?
Ga1' Ga1' Ga1' 149_545 . 106_555 60.00(7) ?
Ga1' Ga1' Ge1 149_545 . . 45.00(7) ?
Ga1' Ga1' Ge1 149_545 . 5_555 175.67(11) ?
Ga1' Ga1' Ge1 149_545 . 149_545 4.86(5) ?
Ga1' Ga1' Ge1 149_545 . 6_555 85.67(5) ?
Ga1' Ga1' Ge1 149_545 . 150_555 85.14(10) ?
Ga1' Ga1' Ge1 149_545 . 9_555 117.44(3) ?
Ga1' Ga1' Ge1 149_545 . 105_554 57.28(6) ?
Ga1' Ga1' Ge1 149_545 . 10_555 117.44(3) ?
Ga1' Ga1' Ge1 149_545 . 106_555 57.28(6) ?
Ga1' Ga1' Ge1' 149_545 . 5_555 180 ?
Ga1' Ga1' Ge1' 149_545 . 149_545 0 ?
Ga1' Ga1' Ge1' 149_545 . 6_555 90.00(7) ?
Ga1' Ga1' Ge1' 149_545 . 150_555 90.00(11) ?
Ga1' Ga1' Ge1' 149_545 . 9_555 120.00(4) ?
Ga1' Ga1' Ge1' 149_545 . 105_554 60.00(7) ?
Ga1' Ga1' Ge1' 149_545 . 10_555 120.00(4) ?
Ga1' Ga1' Ge1' 149_545 . 106_555 60.00(7) ?
Ga1' Ga1' Ga1' 6_555 . 150_555 180 ?
Ga1' Ga1' Ga1' 6_555 . 9_555 60.00(7) ?
Ga1' Ga1' Ga1' 6_555 . 105_554 120.00(4) ?
Ga1' Ga1' Ga1' 6_555 . 10_555 60.00(7) ?
Ga1' Ga1' Ga1' 6_555 . 106_555 120.00(4) ?
Ga1' Ga1' Ge1 6_555 . . 135.00(7) ?
Ga1' Ga1' Ge1 6_555 . 5_555 94.33(11) ?
Ga1' Ga1' Ge1 6_555 . 149_545 94.86(5) ?
Ga1' Ga1' Ge1 6_555 . 6_555 4.33(5) ?
Ga1' Ga1' Ge1 6_555 . 150_555 175.14(11) ?
Ga1' Ga1' Ge1 6_555 . 9_555 62.56(6) ?
Ga1' Ga1' Ge1 6_555 . 105_554 122.72(3) ?
Ga1' Ga1' Ge1 6_555 . 10_555 62.56(6) ?
Ga1' Ga1' Ge1 6_555 . 106_555 122.72(3) ?
Ga1' Ga1' Ge1' 6_555 . 5_555 90.00(12) ?
Ga1' Ga1' Ge1' 6_555 . 149_545 90.00(7) ?
Ga1' Ga1' Ge1' 6_555 . 6_555 0 ?
Ga1' Ga1' Ge1' 6_555 . 150_555 180 ?
Ga1' Ga1' Ge1' 6_555 . 9_555 60.00(7) ?
Ga1' Ga1' Ge1' 6_555 . 105_554 120.00(4) ?
Ga1' Ga1' Ge1' 6_555 . 10_555 60.00(7) ?
Ga1' Ga1' Ge1' 6_555 . 106_555 120.00(4) ?
Ga1' Ga1' Ga1' 150_555 . 9_555 120.00(4) ?
Ga1' Ga1' Ga1' 150_555 . 105_554 60.00(7) ?
Ga1' Ga1' Ga1' 150_555 . 10_555 120.00(4) ?
Ga1' Ga1' Ga1' 150_555 . 106_555 60.00(7) ?
Ga1' Ga1' Ge1 150_555 . . 45.00(7) ?
Ga1' Ga1' Ge1 150_555 . 5_555 85.67(5) ?
Ga1' Ga1' Ge1 150_555 . 149_545 85.14(10) ?
Ga1' Ga1' Ge1 150_555 . 6_555 175.67(11) ?
Ga1' Ga1' Ge1 150_555 . 150_555 4.86(5) ?
Ga1' Ga1' Ge1 150_555 . 9_555 117.44(3) ?
Ga1' Ga1' Ge1 150_555 . 105_554 57.28(6) ?
Ga1' Ga1' Ge1 150_555 . 10_555 117.44(3) ?
Ga1' Ga1' Ge1 150_555 . 106_555 57.28(6) ?
Ga1' Ga1' Ge1' 150_555 . 5_555 90.00(7) ?
Ga1' Ga1' Ge1' 150_555 . 149_545 90.00(11) ?
Ga1' Ga1' Ge1' 150_555 . 6_555 180 ?
Ga1' Ga1' Ge1' 150_555 . 150_555 0 ?
Ga1' Ga1' Ge1' 150_555 . 9_555 120.00(4) ?
Ga1' Ga1' Ge1' 150_555 . 105_554 60.00(7) ?
Ga1' Ga1' Ge1' 150_555 . 10_555 120.00(4) ?
Ga1' Ga1' Ge1' 150_555 . 106_555 60.00(7) ?
Ga1' Ga1' Ga1' 9_555 . 105_554 180 ?
Ga1' Ga1' Ga1' 9_555 . 10_555 90.00(12) ?
Ga1' Ga1' Ga1' 9_555 . 106_555 90.00(7) ?
Ga1' Ga1' Ge1 9_555 . . 135.00(7) ?
Ga1' Ga1' Ge1 9_555 . 5_555 62.56(6) ?
Ga1' Ga1' Ge1 9_555 . 149_545 122.72(3) ?
Ga1' Ga1' Ge1 9_555 . 6_555 62.56(6) ?
Ga1' Ga1' Ge1 9_555 . 150_555 122.72(3) ?
Ga1' Ga1' Ge1 9_555 . 9_555 4.33(5) ?
Ga1' Ga1' Ge1 9_555 . 105_554 175.14(11) ?
Ga1' Ga1' Ge1 9_555 . 10_555 94.33(11) ?
Ga1' Ga1' Ge1 9_555 . 106_555 94.86(5) ?
Ga1' Ga1' Ge1' 9_555 . 5_555 60.00(7) ?
Ga1' Ga1' Ge1' 9_555 . 149_545 120.00(4) ?
Ga1' Ga1' Ge1' 9_555 . 6_555 60.00(7) ?
Ga1' Ga1' Ge1' 9_555 . 150_555 120.00(4) ?
Ga1' Ga1' Ge1' 9_555 . 9_555 0 ?
Ga1' Ga1' Ge1' 9_555 . 105_554 180 ?
Ga1' Ga1' Ge1' 9_555 . 10_555 90.00(12) ?
Ga1' Ga1' Ge1' 9_555 . 106_555 90.00(7) ?
Ga1' Ga1' Ga1' 105_554 . 10_555 90.00(7) ?
Ga1' Ga1' Ga1' 105_554 . 106_555 90.00(11) ?
Ga1' Ga1' Ge1 105_554 . . 45.00(7) ?
Ga1' Ga1' Ge1 105_554 . 5_555 117.44(3) ?
Ga1' Ga1' Ge1 105_554 . 149_545 57.28(6) ?
Ga1' Ga1' Ge1 105_554 . 6_555 117.44(3) ?
Ga1' Ga1' Ge1 105_554 . 150_555 57.28(6) ?
Ga1' Ga1' Ge1 105_554 . 9_555 175.67(11) ?
Ga1' Ga1' Ge1 105_554 . 105_554 4.86(5) ?
Ga1' Ga1' Ge1 105_554 . 10_555 85.67(5) ?
Ga1' Ga1' Ge1 105_554 . 106_555 85.14(10) ?
Ga1' Ga1' Ge1' 105_554 . 5_555 120.00(4) ?
Ga1' Ga1' Ge1' 105_554 . 149_545 60.00(7) ?
Ga1' Ga1' Ge1' 105_554 . 6_555 120.00(4) ?
Ga1' Ga1' Ge1' 105_554 . 150_555 60.00(7) ?
Ga1' Ga1' Ge1' 105_554 . 9_555 180 ?
Ga1' Ga1' Ge1' 105_554 . 105_554 0 ?
Ga1' Ga1' Ge1' 105_554 . 10_555 90.00(7) ?
Ga1' Ga1' Ge1' 105_554 . 106_555 90.00(11) ?
Ga1' Ga1' Ga1' 10_555 . 106_555 180 ?
Ga1' Ga1' Ge1 10_555 . . 135.00(7) ?
Ga1' Ga1' Ge1 10_555 . 5_555 62.56(6) ?
Ga1' Ga1' Ge1 10_555 . 149_545 122.72(3) ?
Ga1' Ga1' Ge1 10_555 . 6_555 62.56(6) ?
Ga1' Ga1' Ge1 10_555 . 150_555 122.72(3) ?
Ga1' Ga1' Ge1 10_555 . 9_555 94.33(11) ?
Ga1' Ga1' Ge1 10_555 . 105_554 94.86(5) ?
Ga1' Ga1' Ge1 10_555 . 10_555 4.33(5) ?
Ga1' Ga1' Ge1 10_555 . 106_555 175.14(11) ?
Ga1' Ga1' Ge1' 10_555 . 5_555 60.00(7) ?
Ga1' Ga1' Ge1' 10_555 . 149_545 120.00(4) ?
Ga1' Ga1' Ge1' 10_555 . 6_555 60.00(7) ?
Ga1' Ga1' Ge1' 10_555 . 150_555 120.00(4) ?
Ga1' Ga1' Ge1' 10_555 . 9_555 90.00(12) ?
Ga1' Ga1' Ge1' 10_555 . 105_554 90.00(7) ?
Ga1' Ga1' Ge1' 10_555 . 10_555 0 ?
Ga1' Ga1' Ge1' 10_555 . 106_555 180 ?
Ga1' Ga1' Ge1 106_555 . . 45.00(7) ?
Ga1' Ga1' Ge1 106_555 . 5_555 117.44(3) ?
Ga1' Ga1' Ge1 106_555 . 149_545 57.28(6) ?
Ga1' Ga1' Ge1 106_555 . 6_555 117.44(3) ?
Ga1' Ga1' Ge1 106_555 . 150_555 57.28(6) ?
Ga1' Ga1' Ge1 106_555 . 9_555 85.67(5) ?
Ga1' Ga1' Ge1 106_555 . 105_554 85.14(10) ?
Ga1' Ga1' Ge1 106_555 . 10_555 175.67(11) ?
Ga1' Ga1' Ge1 106_555 . 106_555 4.86(5) ?
Ga1' Ga1' Ge1' 106_555 . 5_555 120.00(4) ?
Ga1' Ga1' Ge1' 106_555 . 149_545 60.00(7) ?
Ga1' Ga1' Ge1' 106_555 . 6_555 120.00(4) ?
Ga1' Ga1' Ge1' 106_555 . 150_555 60.00(7) ?
Ga1' Ga1' Ge1' 106_555 . 9_555 90.00(7) ?
Ga1' Ga1' Ge1' 106_555 . 105_554 90.00(11) ?
Ga1' Ga1' Ge1' 106_555 . 10_555 180 ?
Ga1' Ga1' Ge1' 106_555 . 106_555 0 ?
Ge1 Ga1' Ge1 . . 5_555 130.67(5) ?
Ge1 Ga1' Ge1 . . 149_545 40.14(5) ?
Ge1 Ga1' Ge1 . . 6_555 130.67(5) ?
Ge1 Ga1' Ge1 . . 150_555 40.14(5) ?
Ge1 Ga1' Ge1 . . 9_555 130.67(5) ?
Ge1 Ga1' Ge1 . . 105_554 40.14(5) ?
Ge1 Ga1' Ge1 . . 10_555 130.67(5) ?
Ge1 Ga1' Ge1 . . 106_555 40.14(5) ?
Ge1 Ga1' Ge1' . . 5_555 135.00(7) ?
Ge1 Ga1' Ge1' . . 149_545 45.00(7) ?
Ge1 Ga1' Ge1' . . 6_555 135.00(7) ?
Ge1 Ga1' Ge1' . . 150_555 45.00(7) ?
Ge1 Ga1' Ge1' . . 9_555 135.00(7) ?
Ge1 Ga1' Ge1' . . 105_554 45.00(7) ?
Ge1 Ga1' Ge1' . . 10_555 135.00(7) ?
Ge1 Ga1' Ge1' . . 106_555 45.00(7) ?
Ge1 Ga1' Ge1 5_555 . 149_545 170.80(10) ?
Ge1 Ga1' Ge1 5_555 . 6_555 98.66(10) ?
Ge1 Ga1' Ge1 5_555 . 150_555 90.53(2) ?
Ge1 Ga1' Ge1 5_555 . 9_555 64.87(5) ?
Ge1 Ga1' Ge1 5_555 . 105_554 119.881(15) ?
Ge1 Ga1' Ge1 5_555 . 10_555 64.87(5) ?
Ge1 Ga1' Ge1 5_555 . 106_555 119.881(15) ?
Ge1 Ga1' Ge1' 5_555 . 5_555 4.33(5) ?
Ge1 Ga1' Ge1' 5_555 . 149_545 175.67(11) ?
Ge1 Ga1' Ge1' 5_555 . 6_555 94.33(11) ?
Ge1 Ga1' Ge1' 5_555 . 150_555 85.67(5) ?
Ge1 Ga1' Ge1' 5_555 . 9_555 62.56(6) ?
Ge1 Ga1' Ge1' 5_555 . 105_554 117.44(3) ?
Ge1 Ga1' Ge1' 5_555 . 10_555 62.56(6) ?
Ge1 Ga1' Ge1' 5_555 . 106_555 117.44(3) ?
Ge1 Ga1' Ge1 149_545 . 6_555 90.53(2) ?
Ge1 Ga1' Ge1 149_545 . 150_555 80.27(9) ?
Ge1 Ga1' Ge1 149_545 . 9_555 119.881(15) ?
Ge1 Ga1' Ge1 149_545 . 105_554 54.23(6) ?
Ge1 Ga1' Ge1 149_545 . 10_555 119.881(15) ?
Ge1 Ga1' Ge1 149_545 . 106_555 54.23(6) ?
Ge1 Ga1' Ge1' 149_545 . 5_555 175.14(11) ?
Ge1 Ga1' Ge1' 149_545 . 149_545 4.86(5) ?
Ge1 Ga1' Ge1' 149_545 . 6_555 94.86(5) ?
Ge1 Ga1' Ge1' 149_545 . 150_555 85.14(10) ?
Ge1 Ga1' Ge1' 149_545 . 9_555 122.72(3) ?
Ge1 Ga1' Ge1' 149_545 . 105_554 57.28(6) ?
Ge1 Ga1' Ge1' 149_545 . 10_555 122.72(3) ?
Ge1 Ga1' Ge1' 149_545 . 106_555 57.28(6) ?
Ge1 Ga1' Ge1 6_555 . 150_555 170.80(10) ?
Ge1 Ga1' Ge1 6_555 . 9_555 64.87(5) ?
Ge1 Ga1' Ge1 6_555 . 105_554 119.881(15) ?
Ge1 Ga1' Ge1 6_555 . 10_555 64.87(5) ?
Ge1 Ga1' Ge1 6_555 . 106_555 119.881(15) ?
Ge1 Ga1' Ge1' 6_555 . 5_555 94.33(11) ?
Ge1 Ga1' Ge1' 6_555 . 149_545 85.67(5) ?
Ge1 Ga1' Ge1' 6_555 . 6_555 4.33(5) ?
Ge1 Ga1' Ge1' 6_555 . 150_555 175.67(11) ?
Ge1 Ga1' Ge1' 6_555 . 9_555 62.56(6) ?
Ge1 Ga1' Ge1' 6_555 . 105_554 117.44(3) ?
Ge1 Ga1' Ge1' 6_555 . 10_555 62.56(6) ?
Ge1 Ga1' Ge1' 6_555 . 106_555 117.44(3) ?
Ge1 Ga1' Ge1 150_555 . 9_555 119.881(15) ?
Ge1 Ga1' Ge1 150_555 . 105_554 54.23(6) ?
Ge1 Ga1' Ge1 150_555 . 10_555 119.881(15) ?
Ge1 Ga1' Ge1 150_555 . 106_555 54.23(6) ?
Ge1 Ga1' Ge1' 150_555 . 5_555 94.86(5) ?
Ge1 Ga1' Ge1' 150_555 . 149_545 85.14(10) ?
Ge1 Ga1' Ge1' 150_555 . 6_555 175.14(11) ?
Ge1 Ga1' Ge1' 150_555 . 150_555 4.86(5) ?
Ge1 Ga1' Ge1' 150_555 . 9_555 122.72(3) ?
Ge1 Ga1' Ge1' 150_555 . 105_554 57.28(6) ?
Ge1 Ga1' Ge1' 150_555 . 10_555 122.72(3) ?
Ge1 Ga1' Ge1' 150_555 . 106_555 57.28(6) ?
Ge1 Ga1' Ge1 9_555 . 105_554 170.80(10) ?
Ge1 Ga1' Ge1 9_555 . 10_555 98.66(10) ?
Ge1 Ga1' Ge1 9_555 . 106_555 90.53(2) ?
Ge1 Ga1' Ge1' 9_555 . 5_555 62.56(6) ?
Ge1 Ga1' Ge1' 9_555 . 149_545 117.44(3) ?
Ge1 Ga1' Ge1' 9_555 . 6_555 62.56(6) ?
Ge1 Ga1' Ge1' 9_555 . 150_555 117.44(3) ?
Ge1 Ga1' Ge1' 9_555 . 9_555 4.33(5) ?
Ge1 Ga1' Ge1' 9_555 . 105_554 175.67(11) ?
Ge1 Ga1' Ge1' 9_555 . 10_555 94.33(11) ?
Ge1 Ga1' Ge1' 9_555 . 106_555 85.67(5) ?
Ge1 Ga1' Ge1 105_554 . 10_555 90.53(2) ?
Ge1 Ga1' Ge1 105_554 . 106_555 80.27(9) ?
Ge1 Ga1' Ge1' 105_554 . 5_555 122.72(3) ?
Ge1 Ga1' Ge1' 105_554 . 149_545 57.28(6) ?
Ge1 Ga1' Ge1' 105_554 . 6_555 122.72(3) ?
Ge1 Ga1' Ge1' 105_554 . 150_555 57.28(6) ?
Ge1 Ga1' Ge1' 105_554 . 9_555 175.14(11) ?
Ge1 Ga1' Ge1' 105_554 . 105_554 4.86(5) ?
Ge1 Ga1' Ge1' 105_554 . 10_555 94.86(5) ?
Ge1 Ga1' Ge1' 105_554 . 106_555 85.14(10) ?
Ge1 Ga1' Ge1 10_555 . 106_555 170.80(10) ?
Ge1 Ga1' Ge1' 10_555 . 5_555 62.56(6) ?
Ge1 Ga1' Ge1' 10_555 . 149_545 117.44(3) ?
Ge1 Ga1' Ge1' 10_555 . 6_555 62.56(6) ?
Ge1 Ga1' Ge1' 10_555 . 150_555 117.44(3) ?
Ge1 Ga1' Ge1' 10_555 . 9_555 94.33(11) ?
Ge1 Ga1' Ge1' 10_555 . 105_554 85.67(5) ?
Ge1 Ga1' Ge1' 10_555 . 10_555 4.33(5) ?
Ge1 Ga1' Ge1' 10_555 . 106_555 175.67(11) ?
Ge1 Ga1' Ge1' 106_555 . 5_555 122.72(3) ?
Ge1 Ga1' Ge1' 106_555 . 149_545 57.28(6) ?
Ge1 Ga1' Ge1' 106_555 . 6_555 122.72(3) ?
Ge1 Ga1' Ge1' 106_555 . 150_555 57.28(6) ?
Ge1 Ga1' Ge1' 106_555 . 9_555 94.86(5) ?
Ge1 Ga1' Ge1' 106_555 . 105_554 85.14(10) ?
Ge1 Ga1' Ge1' 106_555 . 10_555 175.14(11) ?
Ge1 Ga1' Ge1' 106_555 . 106_555 4.86(5) ?
Ge1' Ga1' Ge1' 5_555 . 149_545 180 ?
Ge1' Ga1' Ge1' 5_555 . 6_555 90.00(12) ?
Ge1' Ga1' Ge1' 5_555 . 150_555 90.00(7) ?
Ge1' Ga1' Ge1' 5_555 . 9_555 60.00(7) ?
Ge1' Ga1' Ge1' 5_555 . 105_554 120.00(4) ?
Ge1' Ga1' Ge1' 5_555 . 10_555 60.00(7) ?
Ge1' Ga1' Ge1' 5_555 . 106_555 120.00(4) ?
Ge1' Ga1' Ge1' 149_545 . 6_555 90.00(7) ?
Ge1' Ga1' Ge1' 149_545 . 150_555 90.00(11) ?
Ge1' Ga1' Ge1' 149_545 . 9_555 120.00(4) ?
Ge1' Ga1' Ge1' 149_545 . 105_554 60.00(7) ?
Ge1' Ga1' Ge1' 149_545 . 10_555 120.00(4) ?
Ge1' Ga1' Ge1' 149_545 . 106_555 60.00(7) ?
Ge1' Ga1' Ge1' 6_555 . 150_555 180 ?
Ge1' Ga1' Ge1' 6_555 . 9_555 60.00(7) ?
Ge1' Ga1' Ge1' 6_555 . 105_554 120.00(4) ?
Ge1' Ga1' Ge1' 6_555 . 10_555 60.00(7) ?
Ge1' Ga1' Ge1' 6_555 . 106_555 120.00(4) ?
Ge1' Ga1' Ge1' 150_555 . 9_555 120.00(4) ?
Ge1' Ga1' Ge1' 150_555 . 105_554 60.00(7) ?
Ge1' Ga1' Ge1' 150_555 . 10_555 120.00(4) ?
Ge1' Ga1' Ge1' 150_555 . 106_555 60.00(7) ?
Ge1' Ga1' Ge1' 9_555 . 105_554 180 ?
Ge1' Ga1' Ge1' 9_555 . 10_555 90.00(12) ?
Ge1' Ga1' Ge1' 9_555 . 106_555 90.00(7) ?
Ge1' Ga1' Ge1' 105_554 . 10_555 90.00(7) ?
Ge1' Ga1' Ge1' 105_554 . 106_555 90.00(11) ?
Ge1' Ga1' Ge1' 10_555 . 106_555 180 ?
Sm1 Ge1 Sm1 . . 49_544 168.84(4) ?
Sm1 Ge1 Sm1 . . 13_555 89.459(5) ?
Sm1 Ge1 Sm1 . . 61_545 89.459(5) ?
Sm1 Ge1 Mn1 . . . 84.42(2) ?
Sm1 Ge1 Ga1 . . 2_655 95.58(2) ?
Sm1 Ge1 Ga1 . . 5_555 55.503(12) ?
Sm1 Ge1 Ga1 . . 149_545 124.50(3) ?
Sm1 Ge1 Ga1 . . 6_555 115.40(3) ?
Sm1 Ge1 Ga1 . . 150_555 64.602(13) ?
Sm1 Ge1 Ga1 . . 9_555 55.503(12) ?
Sm1 Ge1 Ga1 . . 105_554 124.50(3) ?
Sm1 Ge1 Ga1 . . 10_555 115.40(3) ?
Sm1 Ge1 Ga1 . . 106_555 64.602(13) ?
Sm1 Ge1 Ga1' . . . 84.42(2) ?
Sm1 Ge1 Ga1' . . 5_555 57.84(3) ?
Sm1 Ge1 Ga1' . . 149_545 126.92(3) ?
Sm1 Ge1 Ga1' . . 6_555 112.64(4) ?
Sm1 Ge1 Ga1' . . 150_555 61.62(3) ?
Sm1 Ge1 Ga1' . . 9_555 57.84(3) ?
Sm1 Ge1 Ga1' . . 105_554 126.92(3) ?
Sm1 Ge1 Ga1' . . 10_555 112.64(4) ?
Sm1 Ge1 Ga1' . . 106_555 61.62(3) ?
Sm1 Ge1 Ge1 . . 2_655 95.58(2) ?
Sm1 Ge1 Ge1 . . 5_555 55.503(12) ?
Sm1 Ge1 Ge1 . . 149_545 124.50(3) ?
Sm1 Ge1 Ge1 . . 6_555 115.40(3) ?
Sm1 Ge1 Ge1 . . 150_555 64.602(13) ?
Sm1 Ge1 Ge1 . . 9_555 55.503(12) ?
Sm1 Ge1 Ge1 . . 105_554 124.50(3) ?
Sm1 Ge1 Ge1 . . 10_555 115.40(3) ?
Sm1 Ge1 Ge1 . . 106_555 64.602(13) ?
Sm1 Ge1 Ge1' . . . 84.42(2) ?
Sm1 Ge1 Ge1' . . 5_555 57.84(3) ?
Sm1 Ge1 Ge1' . . 149_545 126.92(3) ?
Sm1 Ge1 Ge1' . . 6_555 112.64(4) ?
Sm1 Ge1 Ge1' . . 150_555 61.62(3) ?
Sm1 Ge1 Ge1' . . 9_555 57.84(3) ?
Sm1 Ge1 Ge1' . . 105_554 126.92(3) ?
Sm1 Ge1 Ge1' . . 10_555 112.64(4) ?
Sm1 Ge1 Ge1' . . 106_555 61.62(3) ?
Sm1 Ge1 Sm1 49_544 . 13_555 89.459(5) ?
Sm1 Ge1 Sm1 49_544 . 61_545 89.459(5) ?
Sm1 Ge1 Mn1 49_544 . . 84.42(2) ?
Sm1 Ge1 Ga1 49_544 . 2_655 95.58(2) ?
Sm1 Ge1 Ga1 49_544 . 5_555 115.40(3) ?
Sm1 Ge1 Ga1 49_544 . 149_545 64.602(13) ?
Sm1 Ge1 Ga1 49_544 . 6_555 55.503(12) ?
Sm1 Ge1 Ga1 49_544 . 150_555 124.50(3) ?
Sm1 Ge1 Ga1 49_544 . 9_555 115.40(3) ?
Sm1 Ge1 Ga1 49_544 . 105_554 64.602(13) ?
Sm1 Ge1 Ga1 49_544 . 10_555 55.503(12) ?
Sm1 Ge1 Ga1 49_544 . 106_555 124.50(3) ?
Sm1 Ge1 Ga1' 49_544 . . 84.42(2) ?
Sm1 Ge1 Ga1' 49_544 . 5_555 112.64(4) ?
Sm1 Ge1 Ga1' 49_544 . 149_545 61.62(3) ?
Sm1 Ge1 Ga1' 49_544 . 6_555 57.84(3) ?
Sm1 Ge1 Ga1' 49_544 . 150_555 126.92(3) ?
Sm1 Ge1 Ga1' 49_544 . 9_555 112.64(4) ?
Sm1 Ge1 Ga1' 49_544 . 105_554 61.62(3) ?
Sm1 Ge1 Ga1' 49_544 . 10_555 57.84(3) ?
Sm1 Ge1 Ga1' 49_544 . 106_555 126.92(3) ?
Sm1 Ge1 Ge1 49_544 . 2_655 95.58(2) ?
Sm1 Ge1 Ge1 49_544 . 5_555 115.40(3) ?
Sm1 Ge1 Ge1 49_544 . 149_545 64.602(13) ?
Sm1 Ge1 Ge1 49_544 . 6_555 55.503(12) ?
Sm1 Ge1 Ge1 49_544 . 150_555 124.50(3) ?
Sm1 Ge1 Ge1 49_544 . 9_555 115.40(3) ?
Sm1 Ge1 Ge1 49_544 . 105_554 64.602(13) ?
Sm1 Ge1 Ge1 49_544 . 10_555 55.503(12) ?
Sm1 Ge1 Ge1 49_544 . 106_555 124.50(3) ?
Sm1 Ge1 Ge1' 49_544 . . 84.42(2) ?
Sm1 Ge1 Ge1' 49_544 . 5_555 112.64(4) ?
Sm1 Ge1 Ge1' 49_544 . 149_545 61.62(3) ?
Sm1 Ge1 Ge1' 49_544 . 6_555 57.84(3) ?
Sm1 Ge1 Ge1' 49_544 . 150_555 126.92(3) ?
Sm1 Ge1 Ge1' 49_544 . 9_555 112.64(4) ?
Sm1 Ge1 Ge1' 49_544 . 105_554 61.62(3) ?
Sm1 Ge1 Ge1' 49_544 . 10_555 57.84(3) ?
Sm1 Ge1 Ge1' 49_544 . 106_555 126.92(3) ?
Sm1 Ge1 Sm1 13_555 . 61_545 168.84(4) ?
Sm1 Ge1 Mn1 13_555 . . 84.42(2) ?
Sm1 Ge1 Ga1 13_555 . 2_655 95.58(2) ?
Sm1 Ge1 Ga1 13_555 . 5_555 55.503(12) ?
Sm1 Ge1 Ga1 13_555 . 149_545 124.50(3) ?
Sm1 Ge1 Ga1 13_555 . 6_555 115.40(3) ?
Sm1 Ge1 Ga1 13_555 . 150_555 64.602(13) ?
Sm1 Ge1 Ga1 13_555 . 9_555 115.40(3) ?
Sm1 Ge1 Ga1 13_555 . 105_554 64.602(13) ?
Sm1 Ge1 Ga1 13_555 . 10_555 55.503(12) ?
Sm1 Ge1 Ga1 13_555 . 106_555 124.50(3) ?
Sm1 Ge1 Ga1' 13_555 . . 84.42(2) ?
Sm1 Ge1 Ga1' 13_555 . 5_555 57.84(3) ?
Sm1 Ge1 Ga1' 13_555 . 149_545 126.92(3) ?
Sm1 Ge1 Ga1' 13_555 . 6_555 112.64(4) ?
Sm1 Ge1 Ga1' 13_555 . 150_555 61.62(3) ?
Sm1 Ge1 Ga1' 13_555 . 9_555 112.64(4) ?
Sm1 Ge1 Ga1' 13_555 . 105_554 61.62(3) ?
Sm1 Ge1 Ga1' 13_555 . 10_555 57.84(3) ?
Sm1 Ge1 Ga1' 13_555 . 106_555 126.92(3) ?
Sm1 Ge1 Ge1 13_555 . 2_655 95.58(2) ?
Sm1 Ge1 Ge1 13_555 . 5_555 55.503(12) ?
Sm1 Ge1 Ge1 13_555 . 149_545 124.50(3) ?
Sm1 Ge1 Ge1 13_555 . 6_555 115.40(3) ?
Sm1 Ge1 Ge1 13_555 . 150_555 64.602(13) ?
Sm1 Ge1 Ge1 13_555 . 9_555 115.40(3) ?
Sm1 Ge1 Ge1 13_555 . 105_554 64.602(13) ?
Sm1 Ge1 Ge1 13_555 . 10_555 55.503(12) ?
Sm1 Ge1 Ge1 13_555 . 106_555 124.50(3) ?
Sm1 Ge1 Ge1' 13_555 . . 84.42(2) ?
Sm1 Ge1 Ge1' 13_555 . 5_555 57.84(3) ?
Sm1 Ge1 Ge1' 13_555 . 149_545 126.92(3) ?
Sm1 Ge1 Ge1' 13_555 . 6_555 112.64(4) ?
Sm1 Ge1 Ge1' 13_555 . 150_555 61.62(3) ?
Sm1 Ge1 Ge1' 13_555 . 9_555 112.64(4) ?
Sm1 Ge1 Ge1' 13_555 . 105_554 61.62(3) ?
Sm1 Ge1 Ge1' 13_555 . 10_555 57.84(3) ?
Sm1 Ge1 Ge1' 13_555 . 106_555 126.92(3) ?
Sm1 Ge1 Mn1 61_545 . . 84.42(2) ?
Sm1 Ge1 Ga1 61_545 . 2_655 95.58(2) ?
Sm1 Ge1 Ga1 61_545 . 5_555 115.40(3) ?
Sm1 Ge1 Ga1 61_545 . 149_545 64.602(13) ?
Sm1 Ge1 Ga1 61_545 . 6_555 55.503(12) ?
Sm1 Ge1 Ga1 61_545 . 150_555 124.50(3) ?
Sm1 Ge1 Ga1 61_545 . 9_555 55.503(12) ?
Sm1 Ge1 Ga1 61_545 . 105_554 124.50(3) ?
Sm1 Ge1 Ga1 61_545 . 10_555 115.40(3) ?
Sm1 Ge1 Ga1 61_545 . 106_555 64.602(13) ?
Sm1 Ge1 Ga1' 61_545 . . 84.42(2) ?
Sm1 Ge1 Ga1' 61_545 . 5_555 112.64(4) ?
Sm1 Ge1 Ga1' 61_545 . 149_545 61.62(3) ?
Sm1 Ge1 Ga1' 61_545 . 6_555 57.84(3) ?
Sm1 Ge1 Ga1' 61_545 . 150_555 126.92(3) ?
Sm1 Ge1 Ga1' 61_545 . 9_555 57.84(3) ?
Sm1 Ge1 Ga1' 61_545 . 105_554 126.92(3) ?
Sm1 Ge1 Ga1' 61_545 . 10_555 112.64(4) ?
Sm1 Ge1 Ga1' 61_545 . 106_555 61.62(3) ?
Sm1 Ge1 Ge1 61_545 . 2_655 95.58(2) ?
Sm1 Ge1 Ge1 61_545 . 5_555 115.40(3) ?
Sm1 Ge1 Ge1 61_545 . 149_545 64.602(13) ?
Sm1 Ge1 Ge1 61_545 . 6_555 55.503(12) ?
Sm1 Ge1 Ge1 61_545 . 150_555 124.50(3) ?
Sm1 Ge1 Ge1 61_545 . 9_555 55.503(12) ?
Sm1 Ge1 Ge1 61_545 . 105_554 124.50(3) ?
Sm1 Ge1 Ge1 61_545 . 10_555 115.40(3) ?
Sm1 Ge1 Ge1 61_545 . 106_555 64.602(13) ?
Sm1 Ge1 Ge1' 61_545 . . 84.42(2) ?
Sm1 Ge1 Ge1' 61_545 . 5_555 112.64(4) ?
Sm1 Ge1 Ge1' 61_545 . 149_545 61.62(3) ?
Sm1 Ge1 Ge1' 61_545 . 6_555 57.84(3) ?
Sm1 Ge1 Ge1' 61_545 . 150_555 126.92(3) ?
Sm1 Ge1 Ge1' 61_545 . 9_555 57.84(3) ?
Sm1 Ge1 Ge1' 61_545 . 105_554 126.92(3) ?
Sm1 Ge1 Ge1' 61_545 . 10_555 112.64(4) ?
Sm1 Ge1 Ge1' 61_545 . 106_555 61.62(3) ?
Mn1 Ge1 Ga1 . . 2_655 180 ?
Mn1 Ge1 Ga1 . . 5_555 45.000(18) ?
Mn1 Ge1 Ga1 . . 149_545 135.00(2) ?
Mn1 Ge1 Ga1 . . 6_555 45.000(18) ?
Mn1 Ge1 Ga1 . . 150_555 135.00(2) ?
Mn1 Ge1 Ga1 . . 9_555 45.000(18) ?
Mn1 Ge1 Ga1 . . 105_554 135.00(2) ?
Mn1 Ge1 Ga1 . . 10_555 45.000(18) ?
Mn1 Ge1 Ga1 . . 106_555 135.00(2) ?
Mn1 Ge1 Ga1' . . . 0 ?
Mn1 Ge1 Ga1' . . 5_555 40.67(5) ?
Mn1 Ge1 Ga1' . . 149_545 130.14(5) ?
Mn1 Ge1 Ga1' . . 6_555 40.67(5) ?
Mn1 Ge1 Ga1' . . 150_555 130.14(5) ?
Mn1 Ge1 Ga1' . . 9_555 40.67(5) ?
Mn1 Ge1 Ga1' . . 105_554 130.14(5) ?
Mn1 Ge1 Ga1' . . 10_555 40.67(5) ?
Mn1 Ge1 Ga1' . . 106_555 130.14(5) ?
Mn1 Ge1 Ge1 . . 2_655 180 ?
Mn1 Ge1 Ge1 . . 5_555 45.000(18) ?
Mn1 Ge1 Ge1 . . 149_545 135.00(2) ?
Mn1 Ge1 Ge1 . . 6_555 45.000(18) ?
Mn1 Ge1 Ge1 . . 150_555 135.00(2) ?
Mn1 Ge1 Ge1 . . 9_555 45.000(18) ?
Mn1 Ge1 Ge1 . . 105_554 135.00(2) ?
Mn1 Ge1 Ge1 . . 10_555 45.000(18) ?
Mn1 Ge1 Ge1 . . 106_555 135.00(2) ?
Mn1 Ge1 Ge1' . . . 0 ?
Mn1 Ge1 Ge1' . . 5_555 40.67(5) ?
Mn1 Ge1 Ge1' . . 149_545 130.14(5) ?
Mn1 Ge1 Ge1' . . 6_555 40.67(5) ?
Mn1 Ge1 Ge1' . . 150_555 130.14(5) ?
Mn1 Ge1 Ge1' . . 9_555 40.67(5) ?
Mn1 Ge1 Ge1' . . 105_554 130.14(5) ?
Mn1 Ge1 Ge1' . . 10_555 40.67(5) ?
Mn1 Ge1 Ge1' . . 106_555 130.14(5) ?
Ga1 Ge1 Ga1 2_655 . 5_555 135.000(18) ?
Ga1 Ge1 Ga1 2_655 . 149_545 45.00(2) ?
Ga1 Ge1 Ga1 2_655 . 6_555 135.000(18) ?
Ga1 Ge1 Ga1 2_655 . 150_555 45.00(2) ?
Ga1 Ge1 Ga1 2_655 . 9_555 135.000(18) ?
Ga1 Ge1 Ga1 2_655 . 105_554 45.00(2) ?
Ga1 Ge1 Ga1 2_655 . 10_555 135.000(18) ?
Ga1 Ge1 Ga1 2_655 . 106_555 45.00(2) ?
Ga1 Ge1 Ga1' 2_655 . . 180 ?
Ga1 Ge1 Ga1' 2_655 . 5_555 139.33(5) ?
Ga1 Ge1 Ga1' 2_655 . 149_545 49.86(5) ?
Ga1 Ge1 Ga1' 2_655 . 6_555 139.33(5) ?
Ga1 Ge1 Ga1' 2_655 . 150_555 49.86(5) ?
Ga1 Ge1 Ga1' 2_655 . 9_555 139.33(5) ?
Ga1 Ge1 Ga1' 2_655 . 105_554 49.86(5) ?
Ga1 Ge1 Ga1' 2_655 . 10_555 139.33(5) ?
Ga1 Ge1 Ga1' 2_655 . 106_555 49.86(5) ?
Ga1 Ge1 Ge1 2_655 . 2_655 0 ?
Ga1 Ge1 Ge1 2_655 . 5_555 135.000(18) ?
Ga1 Ge1 Ge1 2_655 . 149_545 45.00(2) ?
Ga1 Ge1 Ge1 2_655 . 6_555 135.000(18) ?
Ga1 Ge1 Ge1 2_655 . 150_555 45.00(2) ?
Ga1 Ge1 Ge1 2_655 . 9_555 135.000(18) ?
Ga1 Ge1 Ge1 2_655 . 105_554 45.00(2) ?
Ga1 Ge1 Ge1 2_655 . 10_555 135.000(18) ?
Ga1 Ge1 Ge1 2_655 . 106_555 45.00(2) ?
Ga1 Ge1 Ge1' 2_655 . . 180 ?
Ga1 Ge1 Ge1' 2_655 . 5_555 139.33(5) ?
Ga1 Ge1 Ge1' 2_655 . 149_545 49.86(5) ?
Ga1 Ge1 Ge1' 2_655 . 6_555 139.33(5) ?
Ga1 Ge1 Ge1' 2_655 . 150_555 49.86(5) ?
Ga1 Ge1 Ge1' 2_655 . 9_555 139.33(5) ?
Ga1 Ge1 Ge1' 2_655 . 105_554 49.86(5) ?
Ga1 Ge1 Ge1' 2_655 . 10_555 139.33(5) ?
Ga1 Ge1 Ge1' 2_655 . 106_555 49.86(5) ?
Ga1 Ge1 Ga1 5_555 . 149_545 180 ?
Ga1 Ge1 Ga1 5_555 . 6_555 90.00(3) ?
Ga1 Ge1 Ga1 5_555 . 150_555 90.00(2) ?
Ga1 Ge1 Ga1 5_555 . 9_555 60.000(18) ?
Ga1 Ge1 Ga1 5_555 . 105_554 120.000(13) ?
Ga1 Ge1 Ga1 5_555 . 10_555 60.000(18) ?
Ga1 Ge1 Ga1 5_555 . 106_555 120.000(13) ?
Ga1 Ge1 Ga1' 5_555 . . 45.000(18) ?
Ga1 Ge1 Ga1' 5_555 . 5_555 4.33(5) ?
Ga1 Ge1 Ga1' 5_555 . 149_545 175.14(6) ?
Ga1 Ge1 Ga1' 5_555 . 6_555 85.67(6) ?
Ga1 Ge1 Ga1' 5_555 . 150_555 85.14(5) ?
Ga1 Ge1 Ga1' 5_555 . 9_555 57.56(3) ?
Ga1 Ge1 Ga1' 5_555 . 105_554 117.12(3) ?
Ga1 Ge1 Ga1' 5_555 . 10_555 57.56(3) ?
Ga1 Ge1 Ga1' 5_555 . 106_555 117.12(3) ?
Ga1 Ge1 Ge1 5_555 . 2_655 135.000(18) ?
Ga1 Ge1 Ge1 5_555 . 5_555 0 ?
Ga1 Ge1 Ge1 5_555 . 149_545 180 ?
Ga1 Ge1 Ge1 5_555 . 6_555 90.00(3) ?
Ga1 Ge1 Ge1 5_555 . 150_555 90.00(2) ?
Ga1 Ge1 Ge1 5_555 . 9_555 60.000(18) ?
Ga1 Ge1 Ge1 5_555 . 105_554 120.000(13) ?
Ga1 Ge1 Ge1 5_555 . 10_555 60.000(18) ?
Ga1 Ge1 Ge1 5_555 . 106_555 120.000(13) ?
Ga1 Ge1 Ge1' 5_555 . . 45.000(18) ?
Ga1 Ge1 Ge1' 5_555 . 5_555 4.33(5) ?
Ga1 Ge1 Ge1' 5_555 . 149_545 175.14(6) ?
Ga1 Ge1 Ge1' 5_555 . 6_555 85.67(6) ?
Ga1 Ge1 Ge1' 5_555 . 150_555 85.14(5) ?
Ga1 Ge1 Ge1' 5_555 . 9_555 57.56(3) ?
Ga1 Ge1 Ge1' 5_555 . 105_554 117.12(3) ?
Ga1 Ge1 Ge1' 5_555 . 10_555 57.56(3) ?
Ga1 Ge1 Ge1' 5_555 . 106_555 117.12(3) ?
Ga1 Ge1 Ga1 149_545 . 6_555 90.00(2) ?
Ga1 Ge1 Ga1 149_545 . 150_555 90.00(4) ?
Ga1 Ge1 Ga1 149_545 . 9_555 120.000(13) ?
Ga1 Ge1 Ga1 149_545 . 105_554 60.00(2) ?
Ga1 Ge1 Ga1 149_545 . 10_555 120.000(13) ?
Ga1 Ge1 Ga1 149_545 . 106_555 60.00(2) ?
Ga1 Ge1 Ga1' 149_545 . . 135.00(2) ?
Ga1 Ge1 Ga1' 149_545 . 5_555 175.67(6) ?
Ga1 Ge1 Ga1' 149_545 . 149_545 4.86(5) ?
Ga1 Ge1 Ga1' 149_545 . 6_555 94.33(5) ?
Ga1 Ge1 Ga1' 149_545 . 150_555 94.86(6) ?
Ga1 Ge1 Ga1' 149_545 . 9_555 122.44(3) ?
Ga1 Ge1 Ga1' 149_545 . 105_554 62.88(3) ?
Ga1 Ge1 Ga1' 149_545 . 10_555 122.44(3) ?
Ga1 Ge1 Ga1' 149_545 . 106_555 62.88(3) ?
Ga1 Ge1 Ge1 149_545 . 2_655 45.00(2) ?
Ga1 Ge1 Ge1 149_545 . 5_555 180 ?
Ga1 Ge1 Ge1 149_545 . 149_545 0 ?
Ga1 Ge1 Ge1 149_545 . 6_555 90.00(2) ?
Ga1 Ge1 Ge1 149_545 . 150_555 90.00(4) ?
Ga1 Ge1 Ge1 149_545 . 9_555 120.000(13) ?
Ga1 Ge1 Ge1 149_545 . 105_554 60.00(2) ?
Ga1 Ge1 Ge1 149_545 . 10_555 120.000(13) ?
Ga1 Ge1 Ge1 149_545 . 106_555 60.00(2) ?
Ga1 Ge1 Ge1' 149_545 . . 135.00(2) ?
Ga1 Ge1 Ge1' 149_545 . 5_555 175.67(6) ?
Ga1 Ge1 Ge1' 149_545 . 149_545 4.86(5) ?
Ga1 Ge1 Ge1' 149_545 . 6_555 94.33(5) ?
Ga1 Ge1 Ge1' 149_545 . 150_555 94.86(6) ?
Ga1 Ge1 Ge1' 149_545 . 9_555 122.44(3) ?
Ga1 Ge1 Ge1' 149_545 . 105_554 62.88(3) ?
Ga1 Ge1 Ge1' 149_545 . 10_555 122.44(3) ?
Ga1 Ge1 Ge1' 149_545 . 106_555 62.88(3) ?
Ga1 Ge1 Ga1 6_555 . 150_555 180 ?
Ga1 Ge1 Ga1 6_555 . 9_555 60.000(18) ?
Ga1 Ge1 Ga1 6_555 . 105_554 120.000(13) ?
Ga1 Ge1 Ga1 6_555 . 10_555 60.000(18) ?
Ga1 Ge1 Ga1 6_555 . 106_555 120.000(13) ?
Ga1 Ge1 Ga1' 6_555 . . 45.000(18) ?
Ga1 Ge1 Ga1' 6_555 . 5_555 85.67(6) ?
Ga1 Ge1 Ga1' 6_555 . 149_545 85.14(5) ?
Ga1 Ge1 Ga1' 6_555 . 6_555 4.33(5) ?
Ga1 Ge1 Ga1' 6_555 . 150_555 175.14(6) ?
Ga1 Ge1 Ga1' 6_555 . 9_555 57.56(3) ?
Ga1 Ge1 Ga1' 6_555 . 105_554 117.12(3) ?
Ga1 Ge1 Ga1' 6_555 . 10_555 57.56(3) ?
Ga1 Ge1 Ga1' 6_555 . 106_555 117.12(3) ?
Ga1 Ge1 Ge1 6_555 . 2_655 135.000(18) ?
Ga1 Ge1 Ge1 6_555 . 5_555 90.00(3) ?
Ga1 Ge1 Ge1 6_555 . 149_545 90.00(2) ?
Ga1 Ge1 Ge1 6_555 . 6_555 0 ?
Ga1 Ge1 Ge1 6_555 . 150_555 180 ?
Ga1 Ge1 Ge1 6_555 . 9_555 60.000(18) ?
Ga1 Ge1 Ge1 6_555 . 105_554 120.000(13) ?
Ga1 Ge1 Ge1 6_555 . 10_555 60.000(18) ?
Ga1 Ge1 Ge1 6_555 . 106_555 120.000(13) ?
Ga1 Ge1 Ge1' 6_555 . . 45.000(18) ?
Ga1 Ge1 Ge1' 6_555 . 5_555 85.67(6) ?
Ga1 Ge1 Ge1' 6_555 . 149_545 85.14(5) ?
Ga1 Ge1 Ge1' 6_555 . 6_555 4.33(5) ?
Ga1 Ge1 Ge1' 6_555 . 150_555 175.14(6) ?
Ga1 Ge1 Ge1' 6_555 . 9_555 57.56(3) ?
Ga1 Ge1 Ge1' 6_555 . 105_554 117.12(3) ?
Ga1 Ge1 Ge1' 6_555 . 10_555 57.56(3) ?
Ga1 Ge1 Ge1' 6_555 . 106_555 117.12(3) ?
Ga1 Ge1 Ga1 150_555 . 9_555 120.000(13) ?
Ga1 Ge1 Ga1 150_555 . 105_554 60.00(2) ?
Ga1 Ge1 Ga1 150_555 . 10_555 120.000(13) ?
Ga1 Ge1 Ga1 150_555 . 106_555 60.00(2) ?
Ga1 Ge1 Ga1' 150_555 . . 135.00(2) ?
Ga1 Ge1 Ga1' 150_555 . 5_555 94.33(5) ?
Ga1 Ge1 Ga1' 150_555 . 149_545 94.86(6) ?
Ga1 Ge1 Ga1' 150_555 . 6_555 175.67(6) ?
Ga1 Ge1 Ga1' 150_555 . 150_555 4.86(5) ?
Ga1 Ge1 Ga1' 150_555 . 9_555 122.44(3) ?
Ga1 Ge1 Ga1' 150_555 . 105_554 62.88(3) ?
Ga1 Ge1 Ga1' 150_555 . 10_555 122.44(3) ?
Ga1 Ge1 Ga1' 150_555 . 106_555 62.88(3) ?
Ga1 Ge1 Ge1 150_555 . 2_655 45.00(2) ?
Ga1 Ge1 Ge1 150_555 . 5_555 90.00(2) ?
Ga1 Ge1 Ge1 150_555 . 149_545 90.00(4) ?
Ga1 Ge1 Ge1 150_555 . 6_555 180 ?
Ga1 Ge1 Ge1 150_555 . 150_555 0 ?
Ga1 Ge1 Ge1 150_555 . 9_555 120.000(13) ?
Ga1 Ge1 Ge1 150_555 . 105_554 60.00(2) ?
Ga1 Ge1 Ge1 150_555 . 10_555 120.000(13) ?
Ga1 Ge1 Ge1 150_555 . 106_555 60.00(2) ?
Ga1 Ge1 Ge1' 150_555 . . 135.00(2) ?
Ga1 Ge1 Ge1' 150_555 . 5_555 94.33(5) ?
Ga1 Ge1 Ge1' 150_555 . 149_545 94.86(6) ?
Ga1 Ge1 Ge1' 150_555 . 6_555 175.67(6) ?
Ga1 Ge1 Ge1' 150_555 . 150_555 4.86(5) ?
Ga1 Ge1 Ge1' 150_555 . 9_555 122.44(3) ?
Ga1 Ge1 Ge1' 150_555 . 105_554 62.88(3) ?
Ga1 Ge1 Ge1' 150_555 . 10_555 122.44(3) ?
Ga1 Ge1 Ge1' 150_555 . 106_555 62.88(3) ?
Ga1 Ge1 Ga1 9_555 . 105_554 180 ?
Ga1 Ge1 Ga1 9_555 . 10_555 90.00(3) ?
Ga1 Ge1 Ga1 9_555 . 106_555 90.00(2) ?
Ga1 Ge1 Ga1' 9_555 . . 45.000(18) ?
Ga1 Ge1 Ga1' 9_555 . 5_555 57.56(3) ?
Ga1 Ge1 Ga1' 9_555 . 149_545 117.12(3) ?
Ga1 Ge1 Ga1' 9_555 . 6_555 57.56(3) ?
Ga1 Ge1 Ga1' 9_555 . 150_555 117.12(3) ?
Ga1 Ge1 Ga1' 9_555 . 9_555 4.33(5) ?
Ga1 Ge1 Ga1' 9_555 . 105_554 175.14(6) ?
Ga1 Ge1 Ga1' 9_555 . 10_555 85.67(6) ?
Ga1 Ge1 Ga1' 9_555 . 106_555 85.14(5) ?
Ga1 Ge1 Ge1 9_555 . 2_655 135.000(18) ?
Ga1 Ge1 Ge1 9_555 . 5_555 60.000(18) ?
Ga1 Ge1 Ge1 9_555 . 149_545 120.000(13) ?
Ga1 Ge1 Ge1 9_555 . 6_555 60.000(18) ?
Ga1 Ge1 Ge1 9_555 . 150_555 120.000(13) ?
Ga1 Ge1 Ge1 9_555 . 9_555 0 ?
Ga1 Ge1 Ge1 9_555 . 105_554 180 ?
Ga1 Ge1 Ge1 9_555 . 10_555 90.00(3) ?
Ga1 Ge1 Ge1 9_555 . 106_555 90.00(2) ?
Ga1 Ge1 Ge1' 9_555 . . 45.000(18) ?
Ga1 Ge1 Ge1' 9_555 . 5_555 57.56(3) ?
Ga1 Ge1 Ge1' 9_555 . 149_545 117.12(3) ?
Ga1 Ge1 Ge1' 9_555 . 6_555 57.56(3) ?
Ga1 Ge1 Ge1' 9_555 . 150_555 117.12(3) ?
Ga1 Ge1 Ge1' 9_555 . 9_555 4.33(5) ?
Ga1 Ge1 Ge1' 9_555 . 105_554 175.14(6) ?
Ga1 Ge1 Ge1' 9_555 . 10_555 85.67(6) ?
Ga1 Ge1 Ge1' 9_555 . 106_555 85.14(5) ?
Ga1 Ge1 Ga1 105_554 . 10_555 90.00(2) ?
Ga1 Ge1 Ga1 105_554 . 106_555 90.00(4) ?
Ga1 Ge1 Ga1' 105_554 . . 135.00(2) ?
Ga1 Ge1 Ga1' 105_554 . 5_555 122.44(3) ?
Ga1 Ge1 Ga1' 105_554 . 149_545 62.88(3) ?
Ga1 Ge1 Ga1' 105_554 . 6_555 122.44(3) ?
Ga1 Ge1 Ga1' 105_554 . 150_555 62.88(3) ?
Ga1 Ge1 Ga1' 105_554 . 9_555 175.67(6) ?
Ga1 Ge1 Ga1' 105_554 . 105_554 4.86(5) ?
Ga1 Ge1 Ga1' 105_554 . 10_555 94.33(5) ?
Ga1 Ge1 Ga1' 105_554 . 106_555 94.86(6) ?
Ga1 Ge1 Ge1 105_554 . 2_655 45.00(2) ?
Ga1 Ge1 Ge1 105_554 . 5_555 120.000(13) ?
Ga1 Ge1 Ge1 105_554 . 149_545 60.00(2) ?
Ga1 Ge1 Ge1 105_554 . 6_555 120.000(13) ?
Ga1 Ge1 Ge1 105_554 . 150_555 60.00(2) ?
Ga1 Ge1 Ge1 105_554 . 9_555 180 ?
Ga1 Ge1 Ge1 105_554 . 105_554 0 ?
Ga1 Ge1 Ge1 105_554 . 10_555 90.00(2) ?
Ga1 Ge1 Ge1 105_554 . 106_555 90.00(4) ?
Ga1 Ge1 Ge1' 105_554 . . 135.00(2) ?
Ga1 Ge1 Ge1' 105_554 . 5_555 122.44(3) ?
Ga1 Ge1 Ge1' 105_554 . 149_545 62.88(3) ?
Ga1 Ge1 Ge1' 105_554 . 6_555 122.44(3) ?
Ga1 Ge1 Ge1' 105_554 . 150_555 62.88(3) ?
Ga1 Ge1 Ge1' 105_554 . 9_555 175.67(6) ?
Ga1 Ge1 Ge1' 105_554 . 105_554 4.86(5) ?
Ga1 Ge1 Ge1' 105_554 . 10_555 94.33(5) ?
Ga1 Ge1 Ge1' 105_554 . 106_555 94.86(6) ?
Ga1 Ge1 Ga1 10_555 . 106_555 180 ?
Ga1 Ge1 Ga1' 10_555 . . 45.000(18) ?
Ga1 Ge1 Ga1' 10_555 . 5_555 57.56(3) ?
Ga1 Ge1 Ga1' 10_555 . 149_545 117.12(3) ?
Ga1 Ge1 Ga1' 10_555 . 6_555 57.56(3) ?
Ga1 Ge1 Ga1' 10_555 . 150_555 117.12(3) ?
Ga1 Ge1 Ga1' 10_555 . 9_555 85.67(6) ?
Ga1 Ge1 Ga1' 10_555 . 105_554 85.14(5) ?
Ga1 Ge1 Ga1' 10_555 . 10_555 4.33(5) ?
Ga1 Ge1 Ga1' 10_555 . 106_555 175.14(6) ?
Ga1 Ge1 Ge1 10_555 . 2_655 135.000(18) ?
Ga1 Ge1 Ge1 10_555 . 5_555 60.000(18) ?
Ga1 Ge1 Ge1 10_555 . 149_545 120.000(13) ?
Ga1 Ge1 Ge1 10_555 . 6_555 60.000(18) ?
Ga1 Ge1 Ge1 10_555 . 150_555 120.000(13) ?
Ga1 Ge1 Ge1 10_555 . 9_555 90.00(3) ?
Ga1 Ge1 Ge1 10_555 . 105_554 90.00(2) ?
Ga1 Ge1 Ge1 10_555 . 10_555 0 ?
Ga1 Ge1 Ge1 10_555 . 106_555 180 ?
Ga1 Ge1 Ge1' 10_555 . . 45.000(18) ?
Ga1 Ge1 Ge1' 10_555 . 5_555 57.56(3) ?
Ga1 Ge1 Ge1' 10_555 . 149_545 117.12(3) ?
Ga1 Ge1 Ge1' 10_555 . 6_555 57.56(3) ?
Ga1 Ge1 Ge1' 10_555 . 150_555 117.12(3) ?
Ga1 Ge1 Ge1' 10_555 . 9_555 85.67(6) ?
Ga1 Ge1 Ge1' 10_555 . 105_554 85.14(5) ?
Ga1 Ge1 Ge1' 10_555 . 10_555 4.33(5) ?
Ga1 Ge1 Ge1' 10_555 . 106_555 175.14(6) ?
Ga1 Ge1 Ga1' 106_555 . . 135.00(2) ?
Ga1 Ge1 Ga1' 106_555 . 5_555 122.44(3) ?
Ga1 Ge1 Ga1' 106_555 . 149_545 62.88(3) ?
Ga1 Ge1 Ga1' 106_555 . 6_555 122.44(3) ?
Ga1 Ge1 Ga1' 106_555 . 150_555 62.88(3) ?
Ga1 Ge1 Ga1' 106_555 . 9_555 94.33(5) ?
Ga1 Ge1 Ga1' 106_555 . 105_554 94.86(6) ?
Ga1 Ge1 Ga1' 106_555 . 10_555 175.67(6) ?
Ga1 Ge1 Ga1' 106_555 . 106_555 4.86(5) ?
Ga1 Ge1 Ge1 106_555 . 2_655 45.00(2) ?
Ga1 Ge1 Ge1 106_555 . 5_555 120.000(13) ?
Ga1 Ge1 Ge1 106_555 . 149_545 60.00(2) ?
Ga1 Ge1 Ge1 106_555 . 6_555 120.000(13) ?
Ga1 Ge1 Ge1 106_555 . 150_555 60.00(2) ?
Ga1 Ge1 Ge1 106_555 . 9_555 90.00(2) ?
Ga1 Ge1 Ge1 106_555 . 105_554 90.00(4) ?
Ga1 Ge1 Ge1 106_555 . 10_555 180 ?
Ga1 Ge1 Ge1 106_555 . 106_555 0 ?
Ga1 Ge1 Ge1' 106_555 . . 135.00(2) ?
Ga1 Ge1 Ge1' 106_555 . 5_555 122.44(3) ?
Ga1 Ge1 Ge1' 106_555 . 149_545 62.88(3) ?
Ga1 Ge1 Ge1' 106_555 . 6_555 122.44(3) ?
Ga1 Ge1 Ge1' 106_555 . 150_555 62.88(3) ?
Ga1 Ge1 Ge1' 106_555 . 9_555 94.33(5) ?
Ga1 Ge1 Ge1' 106_555 . 105_554 94.86(6) ?
Ga1 Ge1 Ge1' 106_555 . 10_555 175.67(6) ?
Ga1 Ge1 Ge1' 106_555 . 106_555 4.86(5) ?
Ga1' Ge1 Ga1' . . 5_555 40.67(5) ?
Ga1' Ge1 Ga1' . . 149_545 130.14(5) ?
Ga1' Ge1 Ga1' . . 6_555 40.67(5) ?
Ga1' Ge1 Ga1' . . 150_555 130.14(5) ?
Ga1' Ge1 Ga1' . . 9_555 40.67(5) ?
Ga1' Ge1 Ga1' . . 105_554 130.14(5) ?
Ga1' Ge1 Ga1' . . 10_555 40.67(5) ?
Ga1' Ge1 Ga1' . . 106_555 130.14(5) ?
Ga1' Ge1 Ge1 . . 2_655 180 ?
Ga1' Ge1 Ge1 . . 5_555 45.000(18) ?
Ga1' Ge1 Ge1 . . 149_545 135.00(2) ?
Ga1' Ge1 Ge1 . . 6_555 45.000(18) ?
Ga1' Ge1 Ge1 . . 150_555 135.00(2) ?
Ga1' Ge1 Ge1 . . 9_555 45.000(18) ?
Ga1' Ge1 Ge1 . . 105_554 135.00(2) ?
Ga1' Ge1 Ge1 . . 10_555 45.000(18) ?
Ga1' Ge1 Ge1 . . 106_555 135.00(2) ?
Ga1' Ge1 Ge1' . . . 0 ?
Ga1' Ge1 Ge1' . . 5_555 40.67(5) ?
Ga1' Ge1 Ge1' . . 149_545 130.14(5) ?
Ga1' Ge1 Ge1' . . 6_555 40.67(5) ?
Ga1' Ge1 Ge1' . . 150_555 130.14(5) ?
Ga1' Ge1 Ge1' . . 9_555 40.67(5) ?
Ga1' Ge1 Ge1' . . 105_554 130.14(5) ?
Ga1' Ge1 Ge1' . . 10_555 40.67(5) ?
Ga1' Ge1 Ge1' . . 106_555 130.14(5) ?
Ga1' Ge1 Ga1' 5_555 . 149_545 170.80(7) ?
Ga1' Ge1 Ga1' 5_555 . 6_555 81.34(7) ?
Ga1' Ge1 Ga1' 5_555 . 150_555 89.47(7) ?
Ga1' Ge1 Ga1' 5_555 . 9_555 54.88(4) ?
Ga1' Ge1 Ga1' 5_555 . 105_554 119.27(4) ?
Ga1' Ge1 Ga1' 5_555 . 10_555 54.88(4) ?
Ga1' Ge1 Ga1' 5_555 . 106_555 119.27(4) ?
Ga1' Ge1 Ge1 5_555 . 2_655 139.33(5) ?
Ga1' Ge1 Ge1 5_555 . 5_555 4.33(5) ?
Ga1' Ge1 Ge1 5_555 . 149_545 175.67(6) ?
Ga1' Ge1 Ge1 5_555 . 6_555 85.67(6) ?
Ga1' Ge1 Ge1 5_555 . 150_555 94.33(5) ?
Ga1' Ge1 Ge1 5_555 . 9_555 57.56(3) ?
Ga1' Ge1 Ge1 5_555 . 105_554 122.44(3) ?
Ga1' Ge1 Ge1 5_555 . 10_555 57.56(3) ?
Ga1' Ge1 Ge1 5_555 . 106_555 122.44(3) ?
Ga1' Ge1 Ge1' 5_555 . . 40.67(5) ?
Ga1' Ge1 Ge1' 5_555 . 5_555 0 ?
Ga1' Ge1 Ge1' 5_555 . 149_545 170.80(7) ?
Ga1' Ge1 Ge1' 5_555 . 6_555 81.34(7) ?
Ga1' Ge1 Ge1' 5_555 . 150_555 89.47(7) ?
Ga1' Ge1 Ge1' 5_555 . 9_555 54.88(4) ?
Ga1' Ge1 Ge1' 5_555 . 105_554 119.27(4) ?
Ga1' Ge1 Ge1' 5_555 . 10_555 54.88(4) ?
Ga1' Ge1 Ge1' 5_555 . 106_555 119.27(4) ?
Ga1' Ge1 Ga1' 149_545 . 6_555 89.47(7) ?
Ga1' Ge1 Ga1' 149_545 . 150_555 99.73(7) ?
Ga1' Ge1 Ga1' 149_545 . 9_555 119.27(4) ?
Ga1' Ge1 Ga1' 149_545 . 105_554 65.45(4) ?
Ga1' Ge1 Ga1' 149_545 . 10_555 119.27(4) ?
Ga1' Ge1 Ga1' 149_545 . 106_555 65.45(4) ?
Ga1' Ge1 Ge1 149_545 . 2_655 49.86(5) ?
Ga1' Ge1 Ge1 149_545 . 5_555 175.14(6) ?
Ga1' Ge1 Ge1 149_545 . 149_545 4.86(5) ?
Ga1' Ge1 Ge1 149_545 . 6_555 85.14(5) ?
Ga1' Ge1 Ge1 149_545 . 150_555 94.86(6) ?
Ga1' Ge1 Ge1 149_545 . 9_555 117.12(3) ?
Ga1' Ge1 Ge1 149_545 . 105_554 62.88(3) ?
Ga1' Ge1 Ge1 149_545 . 10_555 117.12(3) ?
Ga1' Ge1 Ge1 149_545 . 106_555 62.88(3) ?
Ga1' Ge1 Ge1' 149_545 . . 130.14(5) ?
Ga1' Ge1 Ge1' 149_545 . 5_555 170.80(7) ?
Ga1' Ge1 Ge1' 149_545 . 149_545 0 ?
Ga1' Ge1 Ge1' 149_545 . 6_555 89.47(7) ?
Ga1' Ge1 Ge1' 149_545 . 150_555 99.73(7) ?
Ga1' Ge1 Ge1' 149_545 . 9_555 119.27(4) ?
Ga1' Ge1 Ge1' 149_545 . 105_554 65.45(4) ?
Ga1' Ge1 Ge1' 149_545 . 10_555 119.27(4) ?
Ga1' Ge1 Ge1' 149_545 . 106_555 65.45(4) ?
Ga1' Ge1 Ga1' 6_555 . 150_555 170.80(7) ?
Ga1' Ge1 Ga1' 6_555 . 9_555 54.88(4) ?
Ga1' Ge1 Ga1' 6_555 . 105_554 119.27(4) ?
Ga1' Ge1 Ga1' 6_555 . 10_555 54.88(4) ?
Ga1' Ge1 Ga1' 6_555 . 106_555 119.27(4) ?
Ga1' Ge1 Ge1 6_555 . 2_655 139.33(5) ?
Ga1' Ge1 Ge1 6_555 . 5_555 85.67(6) ?
Ga1' Ge1 Ge1 6_555 . 149_545 94.33(5) ?
Ga1' Ge1 Ge1 6_555 . 6_555 4.33(5) ?
Ga1' Ge1 Ge1 6_555 . 150_555 175.67(6) ?
Ga1' Ge1 Ge1 6_555 . 9_555 57.56(3) ?
Ga1' Ge1 Ge1 6_555 . 105_554 122.44(3) ?
Ga1' Ge1 Ge1 6_555 . 10_555 57.56(3) ?
Ga1' Ge1 Ge1 6_555 . 106_555 122.44(3) ?
Ga1' Ge1 Ge1' 6_555 . . 40.67(5) ?
Ga1' Ge1 Ge1' 6_555 . 5_555 81.34(7) ?
Ga1' Ge1 Ge1' 6_555 . 149_545 89.47(7) ?
Ga1' Ge1 Ge1' 6_555 . 6_555 0 ?
Ga1' Ge1 Ge1' 6_555 . 150_555 170.80(7) ?
Ga1' Ge1 Ge1' 6_555 . 9_555 54.88(4) ?
Ga1' Ge1 Ge1' 6_555 . 105_554 119.27(4) ?
Ga1' Ge1 Ge1' 6_555 . 10_555 54.88(4) ?
Ga1' Ge1 Ge1' 6_555 . 106_555 119.27(4) ?
Ga1' Ge1 Ga1' 150_555 . 9_555 119.27(4) ?
Ga1' Ge1 Ga1' 150_555 . 105_554 65.45(4) ?
Ga1' Ge1 Ga1' 150_555 . 10_555 119.27(4) ?
Ga1' Ge1 Ga1' 150_555 . 106_555 65.45(4) ?
Ga1' Ge1 Ge1 150_555 . 2_655 49.86(5) ?
Ga1' Ge1 Ge1 150_555 . 5_555 85.14(5) ?
Ga1' Ge1 Ge1 150_555 . 149_545 94.86(6) ?
Ga1' Ge1 Ge1 150_555 . 6_555 175.14(6) ?
Ga1' Ge1 Ge1 150_555 . 150_555 4.86(5) ?
Ga1' Ge1 Ge1 150_555 . 9_555 117.12(3) ?
Ga1' Ge1 Ge1 150_555 . 105_554 62.88(3) ?
Ga1' Ge1 Ge1 150_555 . 10_555 117.12(3) ?
Ga1' Ge1 Ge1 150_555 . 106_555 62.88(3) ?
Ga1' Ge1 Ge1' 150_555 . . 130.14(5) ?
Ga1' Ge1 Ge1' 150_555 . 5_555 89.47(7) ?
Ga1' Ge1 Ge1' 150_555 . 149_545 99.73(7) ?
Ga1' Ge1 Ge1' 150_555 . 6_555 170.80(7) ?
Ga1' Ge1 Ge1' 150_555 . 150_555 0 ?
Ga1' Ge1 Ge1' 150_555 . 9_555 119.27(4) ?
Ga1' Ge1 Ge1' 150_555 . 105_554 65.45(4) ?
Ga1' Ge1 Ge1' 150_555 . 10_555 119.27(4) ?
Ga1' Ge1 Ge1' 150_555 . 106_555 65.45(4) ?
Ga1' Ge1 Ga1' 9_555 . 105_554 170.80(7) ?
Ga1' Ge1 Ga1' 9_555 . 10_555 81.34(7) ?
Ga1' Ge1 Ga1' 9_555 . 106_555 89.47(7) ?
Ga1' Ge1 Ge1 9_555 . 2_655 139.33(5) ?
Ga1' Ge1 Ge1 9_555 . 5_555 57.56(3) ?
Ga1' Ge1 Ge1 9_555 . 149_545 122.44(3) ?
Ga1' Ge1 Ge1 9_555 . 6_555 57.56(3) ?
Ga1' Ge1 Ge1 9_555 . 150_555 122.44(3) ?
Ga1' Ge1 Ge1 9_555 . 9_555 4.33(5) ?
Ga1' Ge1 Ge1 9_555 . 105_554 175.67(6) ?
Ga1' Ge1 Ge1 9_555 . 10_555 85.67(6) ?
Ga1' Ge1 Ge1 9_555 . 106_555 94.33(5) ?
Ga1' Ge1 Ge1' 9_555 . . 40.67(5) ?
Ga1' Ge1 Ge1' 9_555 . 5_555 54.88(4) ?
Ga1' Ge1 Ge1' 9_555 . 149_545 119.27(4) ?
Ga1' Ge1 Ge1' 9_555 . 6_555 54.88(4) ?
Ga1' Ge1 Ge1' 9_555 . 150_555 119.27(4) ?
Ga1' Ge1 Ge1' 9_555 . 9_555 0 ?
Ga1' Ge1 Ge1' 9_555 . 105_554 170.80(7) ?
Ga1' Ge1 Ge1' 9_555 . 10_555 81.34(7) ?
Ga1' Ge1 Ge1' 9_555 . 106_555 89.47(7) ?
Ga1' Ge1 Ga1' 105_554 . 10_555 89.47(7) ?
Ga1' Ge1 Ga1' 105_554 . 106_555 99.73(7) ?
Ga1' Ge1 Ge1 105_554 . 2_655 49.86(5) ?
Ga1' Ge1 Ge1 105_554 . 5_555 117.12(3) ?
Ga1' Ge1 Ge1 105_554 . 149_545 62.88(3) ?
Ga1' Ge1 Ge1 105_554 . 6_555 117.12(3) ?
Ga1' Ge1 Ge1 105_554 . 150_555 62.88(3) ?
Ga1' Ge1 Ge1 105_554 . 9_555 175.14(6) ?
Ga1' Ge1 Ge1 105_554 . 105_554 4.86(5) ?
Ga1' Ge1 Ge1 105_554 . 10_555 85.14(5) ?
Ga1' Ge1 Ge1 105_554 . 106_555 94.86(6) ?
Ga1' Ge1 Ge1' 105_554 . . 130.14(5) ?
Ga1' Ge1 Ge1' 105_554 . 5_555 119.27(4) ?
Ga1' Ge1 Ge1' 105_554 . 149_545 65.45(4) ?
Ga1' Ge1 Ge1' 105_554 . 6_555 119.27(4) ?
Ga1' Ge1 Ge1' 105_554 . 150_555 65.45(4) ?
Ga1' Ge1 Ge1' 105_554 . 9_555 170.80(7) ?
Ga1' Ge1 Ge1' 105_554 . 105_554 0 ?
Ga1' Ge1 Ge1' 105_554 . 10_555 89.47(7) ?
Ga1' Ge1 Ge1' 105_554 . 106_555 99.73(7) ?
Ga1' Ge1 Ga1' 10_555 . 106_555 170.80(7) ?
Ga1' Ge1 Ge1 10_555 . 2_655 139.33(5) ?
Ga1' Ge1 Ge1 10_555 . 5_555 57.56(3) ?
Ga1' Ge1 Ge1 10_555 . 149_545 122.44(3) ?
Ga1' Ge1 Ge1 10_555 . 6_555 57.56(3) ?
Ga1' Ge1 Ge1 10_555 . 150_555 122.44(3) ?
Ga1' Ge1 Ge1 10_555 . 9_555 85.67(6) ?
Ga1' Ge1 Ge1 10_555 . 105_554 94.33(5) ?
Ga1' Ge1 Ge1 10_555 . 10_555 4.33(5) ?
Ga1' Ge1 Ge1 10_555 . 106_555 175.67(6) ?
Ga1' Ge1 Ge1' 10_555 . . 40.67(5) ?
Ga1' Ge1 Ge1' 10_555 . 5_555 54.88(4) ?
Ga1' Ge1 Ge1' 10_555 . 149_545 119.27(4) ?
Ga1' Ge1 Ge1' 10_555 . 6_555 54.88(4) ?
Ga1' Ge1 Ge1' 10_555 . 150_555 119.27(4) ?
Ga1' Ge1 Ge1' 10_555 . 9_555 81.34(7) ?
Ga1' Ge1 Ge1' 10_555 . 105_554 89.47(7) ?
Ga1' Ge1 Ge1' 10_555 . 10_555 0 ?
Ga1' Ge1 Ge1' 10_555 . 106_555 170.80(7) ?
Ga1' Ge1 Ge1 106_555 . 2_655 49.86(5) ?
Ga1' Ge1 Ge1 106_555 . 5_555 117.12(3) ?
Ga1' Ge1 Ge1 106_555 . 149_545 62.88(3) ?
Ga1' Ge1 Ge1 106_555 . 6_555 117.12(3) ?
Ga1' Ge1 Ge1 106_555 . 150_555 62.88(3) ?
Ga1' Ge1 Ge1 106_555 . 9_555 85.14(5) ?
Ga1' Ge1 Ge1 106_555 . 105_554 94.86(6) ?
Ga1' Ge1 Ge1 106_555 . 10_555 175.14(6) ?
Ga1' Ge1 Ge1 106_555 . 106_555 4.86(5) ?
Ga1' Ge1 Ge1' 106_555 . . 130.14(5) ?
Ga1' Ge1 Ge1' 106_555 . 5_555 119.27(4) ?
Ga1' Ge1 Ge1' 106_555 . 149_545 65.45(4) ?
Ga1' Ge1 Ge1' 106_555 . 6_555 119.27(4) ?
Ga1' Ge1 Ge1' 106_555 . 150_555 65.45(4) ?
Ga1' Ge1 Ge1' 106_555 . 9_555 89.47(7) ?
Ga1' Ge1 Ge1' 106_555 . 105_554 99.73(7) ?
Ga1' Ge1 Ge1' 106_555 . 10_555 170.80(7) ?
Ga1' Ge1 Ge1' 106_555 . 106_555 0 ?
Ge1 Ge1 Ge1 2_655 . 5_555 135.000(18) ?
Ge1 Ge1 Ge1 2_655 . 149_545 45.00(2) ?
Ge1 Ge1 Ge1 2_655 . 6_555 135.000(18) ?
Ge1 Ge1 Ge1 2_655 . 150_555 45.00(2) ?
Ge1 Ge1 Ge1 2_655 . 9_555 135.000(18) ?
Ge1 Ge1 Ge1 2_655 . 105_554 45.00(2) ?
Ge1 Ge1 Ge1 2_655 . 10_555 135.000(18) ?
Ge1 Ge1 Ge1 2_655 . 106_555 45.00(2) ?
Ge1 Ge1 Ge1' 2_655 . . 180 ?
Ge1 Ge1 Ge1' 2_655 . 5_555 139.33(5) ?
Ge1 Ge1 Ge1' 2_655 . 149_545 49.86(5) ?
Ge1 Ge1 Ge1' 2_655 . 6_555 139.33(5) ?
Ge1 Ge1 Ge1' 2_655 . 150_555 49.86(5) ?
Ge1 Ge1 Ge1' 2_655 . 9_555 139.33(5) ?
Ge1 Ge1 Ge1' 2_655 . 105_554 49.86(5) ?
Ge1 Ge1 Ge1' 2_655 . 10_555 139.33(5) ?
Ge1 Ge1 Ge1' 2_655 . 106_555 49.86(5) ?
Ge1 Ge1 Ge1 5_555 . 149_545 180 ?
Ge1 Ge1 Ge1 5_555 . 6_555 90.00(3) ?
Ge1 Ge1 Ge1 5_555 . 150_555 90.00(2) ?
Ge1 Ge1 Ge1 5_555 . 9_555 60.000(18) ?
Ge1 Ge1 Ge1 5_555 . 105_554 120.000(13) ?
Ge1 Ge1 Ge1 5_555 . 10_555 60.000(18) ?
Ge1 Ge1 Ge1 5_555 . 106_555 120.000(13) ?
Ge1 Ge1 Ge1' 5_555 . . 45.000(18) ?
Ge1 Ge1 Ge1' 5_555 . 5_555 4.33(5) ?
Ge1 Ge1 Ge1' 5_555 . 149_545 175.14(6) ?
Ge1 Ge1 Ge1' 5_555 . 6_555 85.67(6) ?
Ge1 Ge1 Ge1' 5_555 . 150_555 85.14(5) ?
Ge1 Ge1 Ge1' 5_555 . 9_555 57.56(3) ?
Ge1 Ge1 Ge1' 5_555 . 105_554 117.12(3) ?
Ge1 Ge1 Ge1' 5_555 . 10_555 57.56(3) ?
Ge1 Ge1 Ge1' 5_555 . 106_555 117.12(3) ?
Ge1 Ge1 Ge1 149_545 . 6_555 90.00(2) ?
Ge1 Ge1 Ge1 149_545 . 150_555 90.00(4) ?
Ge1 Ge1 Ge1 149_545 . 9_555 120.000(13) ?
Ge1 Ge1 Ge1 149_545 . 105_554 60.00(2) ?
Ge1 Ge1 Ge1 149_545 . 10_555 120.000(13) ?
Ge1 Ge1 Ge1 149_545 . 106_555 60.00(2) ?
Ge1 Ge1 Ge1' 149_545 . . 135.00(2) ?
Ge1 Ge1 Ge1' 149_545 . 5_555 175.67(6) ?
Ge1 Ge1 Ge1' 149_545 . 149_545 4.86(5) ?
Ge1 Ge1 Ge1' 149_545 . 6_555 94.33(5) ?
Ge1 Ge1 Ge1' 149_545 . 150_555 94.86(6) ?
Ge1 Ge1 Ge1' 149_545 . 9_555 122.44(3) ?
Ge1 Ge1 Ge1' 149_545 . 105_554 62.88(3) ?
Ge1 Ge1 Ge1' 149_545 . 10_555 122.44(3) ?
Ge1 Ge1 Ge1' 149_545 . 106_555 62.88(3) ?
Ge1 Ge1 Ge1 6_555 . 150_555 180 ?
Ge1 Ge1 Ge1 6_555 . 9_555 60.000(18) ?
Ge1 Ge1 Ge1 6_555 . 105_554 120.000(13) ?
Ge1 Ge1 Ge1 6_555 . 10_555 60.000(18) ?
Ge1 Ge1 Ge1 6_555 . 106_555 120.000(13) ?
Ge1 Ge1 Ge1' 6_555 . . 45.000(18) ?
Ge1 Ge1 Ge1' 6_555 . 5_555 85.67(6) ?
Ge1 Ge1 Ge1' 6_555 . 149_545 85.14(5) ?
Ge1 Ge1 Ge1' 6_555 . 6_555 4.33(5) ?
Ge1 Ge1 Ge1' 6_555 . 150_555 175.14(6) ?
Ge1 Ge1 Ge1' 6_555 . 9_555 57.56(3) ?
Ge1 Ge1 Ge1' 6_555 . 105_554 117.12(3) ?
Ge1 Ge1 Ge1' 6_555 . 10_555 57.56(3) ?
Ge1 Ge1 Ge1' 6_555 . 106_555 117.12(3) ?
Ge1 Ge1 Ge1 150_555 . 9_555 120.000(13) ?
Ge1 Ge1 Ge1 150_555 . 105_554 60.00(2) ?
Ge1 Ge1 Ge1 150_555 . 10_555 120.000(13) ?
Ge1 Ge1 Ge1 150_555 . 106_555 60.00(2) ?
Ge1 Ge1 Ge1' 150_555 . . 135.00(2) ?
Ge1 Ge1 Ge1' 150_555 . 5_555 94.33(5) ?
Ge1 Ge1 Ge1' 150_555 . 149_545 94.86(6) ?
Ge1 Ge1 Ge1' 150_555 . 6_555 175.67(6) ?
Ge1 Ge1 Ge1' 150_555 . 150_555 4.86(5) ?
Ge1 Ge1 Ge1' 150_555 . 9_555 122.44(3) ?
Ge1 Ge1 Ge1' 150_555 . 105_554 62.88(3) ?
Ge1 Ge1 Ge1' 150_555 . 10_555 122.44(3) ?
Ge1 Ge1 Ge1' 150_555 . 106_555 62.88(3) ?
Ge1 Ge1 Ge1 9_555 . 105_554 180 ?
Ge1 Ge1 Ge1 9_555 . 10_555 90.00(3) ?
Ge1 Ge1 Ge1 9_555 . 106_555 90.00(2) ?
Ge1 Ge1 Ge1' 9_555 . . 45.000(18) ?
Ge1 Ge1 Ge1' 9_555 . 5_555 57.56(3) ?
Ge1 Ge1 Ge1' 9_555 . 149_545 117.12(3) ?
Ge1 Ge1 Ge1' 9_555 . 6_555 57.56(3) ?
Ge1 Ge1 Ge1' 9_555 . 150_555 117.12(3) ?
Ge1 Ge1 Ge1' 9_555 . 9_555 4.33(5) ?
Ge1 Ge1 Ge1' 9_555 . 105_554 175.14(6) ?
Ge1 Ge1 Ge1' 9_555 . 10_555 85.67(6) ?
Ge1 Ge1 Ge1' 9_555 . 106_555 85.14(5) ?
Ge1 Ge1 Ge1 105_554 . 10_555 90.00(2) ?
Ge1 Ge1 Ge1 105_554 . 106_555 90.00(4) ?
Ge1 Ge1 Ge1' 105_554 . . 135.00(2) ?
Ge1 Ge1 Ge1' 105_554 . 5_555 122.44(3) ?
Ge1 Ge1 Ge1' 105_554 . 149_545 62.88(3) ?
Ge1 Ge1 Ge1' 105_554 . 6_555 122.44(3) ?
Ge1 Ge1 Ge1' 105_554 . 150_555 62.88(3) ?
Ge1 Ge1 Ge1' 105_554 . 9_555 175.67(6) ?
Ge1 Ge1 Ge1' 105_554 . 105_554 4.86(5) ?
Ge1 Ge1 Ge1' 105_554 . 10_555 94.33(5) ?
Ge1 Ge1 Ge1' 105_554 . 106_555 94.86(6) ?
Ge1 Ge1 Ge1 10_555 . 106_555 180 ?
Ge1 Ge1 Ge1' 10_555 . . 45.000(18) ?
Ge1 Ge1 Ge1' 10_555 . 5_555 57.56(3) ?
Ge1 Ge1 Ge1' 10_555 . 149_545 117.12(3) ?
Ge1 Ge1 Ge1' 10_555 . 6_555 57.56(3) ?
Ge1 Ge1 Ge1' 10_555 . 150_555 117.12(3) ?
Ge1 Ge1 Ge1' 10_555 . 9_555 85.67(6) ?
Ge1 Ge1 Ge1' 10_555 . 105_554 85.14(5) ?
Ge1 Ge1 Ge1' 10_555 . 10_555 4.33(5) ?
Ge1 Ge1 Ge1' 10_555 . 106_555 175.14(6) ?
Ge1 Ge1 Ge1' 106_555 . . 135.00(2) ?
Ge1 Ge1 Ge1' 106_555 . 5_555 122.44(3) ?
Ge1 Ge1 Ge1' 106_555 . 149_545 62.88(3) ?
Ge1 Ge1 Ge1' 106_555 . 6_555 122.44(3) ?
Ge1 Ge1 Ge1' 106_555 . 150_555 62.88(3) ?
Ge1 Ge1 Ge1' 106_555 . 9_555 94.33(5) ?
Ge1 Ge1 Ge1' 106_555 . 105_554 94.86(6) ?
Ge1 Ge1 Ge1' 106_555 . 10_555 175.67(6) ?
Ge1 Ge1 Ge1' 106_555 . 106_555 4.86(5) ?
Ge1' Ge1 Ge1' . . 5_555 40.67(5) ?
Ge1' Ge1 Ge1' . . 149_545 130.14(5) ?
Ge1' Ge1 Ge1' . . 6_555 40.67(5) ?
Ge1' Ge1 Ge1' . . 150_555 130.14(5) ?
Ge1' Ge1 Ge1' . . 9_555 40.67(5) ?
Ge1' Ge1 Ge1' . . 105_554 130.14(5) ?
Ge1' Ge1 Ge1' . . 10_555 40.67(5) ?
Ge1' Ge1 Ge1' . . 106_555 130.14(5) ?
Ge1' Ge1 Ge1' 5_555 . 149_545 170.80(7) ?
Ge1' Ge1 Ge1' 5_555 . 6_555 81.34(7) ?
Ge1' Ge1 Ge1' 5_555 . 150_555 89.47(7) ?
Ge1' Ge1 Ge1' 5_555 . 9_555 54.88(4) ?
Ge1' Ge1 Ge1' 5_555 . 105_554 119.27(4) ?
Ge1' Ge1 Ge1' 5_555 . 10_555 54.88(4) ?
Ge1' Ge1 Ge1' 5_555 . 106_555 119.27(4) ?
Ge1' Ge1 Ge1' 149_545 . 6_555 89.47(7) ?
Ge1' Ge1 Ge1' 149_545 . 150_555 99.73(7) ?
Ge1' Ge1 Ge1' 149_545 . 9_555 119.27(4) ?
Ge1' Ge1 Ge1' 149_545 . 105_554 65.45(4) ?
Ge1' Ge1 Ge1' 149_545 . 10_555 119.27(4) ?
Ge1' Ge1 Ge1' 149_545 . 106_555 65.45(4) ?
Ge1' Ge1 Ge1' 6_555 . 150_555 170.80(7) ?
Ge1' Ge1 Ge1' 6_555 . 9_555 54.88(4) ?
Ge1' Ge1 Ge1' 6_555 . 105_554 119.27(4) ?
Ge1' Ge1 Ge1' 6_555 . 10_555 54.88(4) ?
Ge1' Ge1 Ge1' 6_555 . 106_555 119.27(4) ?
Ge1' Ge1 Ge1' 150_555 . 9_555 119.27(4) ?
Ge1' Ge1 Ge1' 150_555 . 105_554 65.45(4) ?
Ge1' Ge1 Ge1' 150_555 . 10_555 119.27(4) ?
Ge1' Ge1 Ge1' 150_555 . 106_555 65.45(4) ?
Ge1' Ge1 Ge1' 9_555 . 105_554 170.80(7) ?
Ge1' Ge1 Ge1' 9_555 . 10_555 81.34(7) ?
Ge1' Ge1 Ge1' 9_555 . 106_555 89.47(7) ?
Ge1' Ge1 Ge1' 105_554 . 10_555 89.47(7) ?
Ge1' Ge1 Ge1' 105_554 . 106_555 99.73(7) ?
Ge1' Ge1 Ge1' 10_555 . 106_555 170.80(7) ?
Sm1 Ge1' Sm1 . . 49_544 178.20(13) ?
Sm1 Ge1' Sm1 . . 13_555 89.986(3) ?
Sm1 Ge1' Sm1 . . 61_545 89.986(3) ?
Sm1 Ge1' Mn1 . . . 90.90(7) ?
Sm1 Ge1' Ga1 . . . 89.10(7) ?
Sm1 Ge1' Ga1 . . 5_555 58.26(3) ?
Sm1 Ge1' Ga1 . . 149_545 116.34(9) ?
Sm1 Ge1' Ga1 . . 6_555 123.13(8) ?
Sm1 Ge1' Ga1 . . 150_555 62.11(3) ?
Sm1 Ge1' Ga1 . . 9_555 58.26(3) ?
Sm1 Ge1' Ga1 . . 105_554 116.34(9) ?
Sm1 Ge1' Ga1 . . 10_555 123.13(8) ?
Sm1 Ge1' Ga1 . . 106_555 62.11(3) ?
Sm1 Ge1' Ga1' . . 5_555 60.74(4) ?
Sm1 Ge1' Ga1' . . 149_545 119.26(9) ?
Sm1 Ge1' Ga1' . . 6_555 120.73(9) ?
Sm1 Ge1' Ga1' . . 150_555 59.27(4) ?
Sm1 Ge1' Ga1' . . 9_555 60.74(4) ?
Sm1 Ge1' Ga1' . . 105_554 119.26(9) ?
Sm1 Ge1' Ga1' . . 10_555 120.73(9) ?
Sm1 Ge1' Ga1' . . 106_555 59.27(4) ?
Sm1 Ge1' Ge1 . . . 89.10(7) ?
Sm1 Ge1' Ge1 . . 5_555 58.26(3) ?
Sm1 Ge1' Ge1 . . 149_545 116.34(9) ?
Sm1 Ge1' Ge1 . . 6_555 123.13(8) ?
Sm1 Ge1' Ge1 . . 150_555 62.11(3) ?
Sm1 Ge1' Ge1 . . 9_555 58.26(3) ?
Sm1 Ge1' Ge1 . . 105_554 116.34(9) ?
Sm1 Ge1' Ge1 . . 10_555 123.13(8) ?
Sm1 Ge1' Ge1 . . 106_555 62.11(3) ?
Sm1 Ge1' Ge1' . . 5_555 60.74(4) ?
Sm1 Ge1' Ge1' . . 149_545 119.26(9) ?
Sm1 Ge1' Ge1' . . 6_555 120.73(9) ?
Sm1 Ge1' Ge1' . . 150_555 59.27(4) ?
Sm1 Ge1' Ge1' . . 9_555 60.74(4) ?
Sm1 Ge1' Ge1' . . 105_554 119.26(9) ?
Sm1 Ge1' Ge1' . . 10_555 120.73(9) ?
Sm1 Ge1' Ge1' . . 106_555 59.27(4) ?
Sm1 Ge1' Sm1 49_544 . 13_555 89.986(3) ?
Sm1 Ge1' Sm1 49_544 . 61_545 89.986(3) ?
Sm1 Ge1' Mn1 49_544 . . 90.90(7) ?
Sm1 Ge1' Ga1 49_544 . . 89.10(7) ?
Sm1 Ge1' Ga1 49_544 . 5_555 123.13(8) ?
Sm1 Ge1' Ga1 49_544 . 149_545 62.11(3) ?
Sm1 Ge1' Ga1 49_544 . 6_555 58.26(3) ?
Sm1 Ge1' Ga1 49_544 . 150_555 116.34(9) ?
Sm1 Ge1' Ga1 49_544 . 9_555 123.13(8) ?
Sm1 Ge1' Ga1 49_544 . 105_554 62.11(3) ?
Sm1 Ge1' Ga1 49_544 . 10_555 58.26(3) ?
Sm1 Ge1' Ga1 49_544 . 106_555 116.34(9) ?
Sm1 Ge1' Ga1' 49_544 . 5_555 120.73(9) ?
Sm1 Ge1' Ga1' 49_544 . 149_545 59.27(4) ?
Sm1 Ge1' Ga1' 49_544 . 6_555 60.74(4) ?
Sm1 Ge1' Ga1' 49_544 . 150_555 119.26(9) ?
Sm1 Ge1' Ga1' 49_544 . 9_555 120.73(9) ?
Sm1 Ge1' Ga1' 49_544 . 105_554 59.27(4) ?
Sm1 Ge1' Ga1' 49_544 . 10_555 60.74(4) ?
Sm1 Ge1' Ga1' 49_544 . 106_555 119.26(9) ?
Sm1 Ge1' Ge1 49_544 . . 89.10(7) ?
Sm1 Ge1' Ge1 49_544 . 5_555 123.13(8) ?
Sm1 Ge1' Ge1 49_544 . 149_545 62.11(3) ?
Sm1 Ge1' Ge1 49_544 . 6_555 58.26(3) ?
Sm1 Ge1' Ge1 49_544 . 150_555 116.34(9) ?
Sm1 Ge1' Ge1 49_544 . 9_555 123.13(8) ?
Sm1 Ge1' Ge1 49_544 . 105_554 62.11(3) ?
Sm1 Ge1' Ge1 49_544 . 10_555 58.26(3) ?
Sm1 Ge1' Ge1 49_544 . 106_555 116.34(9) ?
Sm1 Ge1' Ge1' 49_544 . 5_555 120.73(9) ?
Sm1 Ge1' Ge1' 49_544 . 149_545 59.27(4) ?
Sm1 Ge1' Ge1' 49_544 . 6_555 60.74(4) ?
Sm1 Ge1' Ge1' 49_544 . 150_555 119.26(9) ?
Sm1 Ge1' Ge1' 49_544 . 9_555 120.73(9) ?
Sm1 Ge1' Ge1' 49_544 . 105_554 59.27(4) ?
Sm1 Ge1' Ge1' 49_544 . 10_555 60.74(4) ?
Sm1 Ge1' Ge1' 49_544 . 106_555 119.26(9) ?
Sm1 Ge1' Sm1 13_555 . 61_545 178.20(13) ?
Sm1 Ge1' Mn1 13_555 . . 90.90(7) ?
Sm1 Ge1' Ga1 13_555 . . 89.10(7) ?
Sm1 Ge1' Ga1 13_555 . 5_555 58.26(3) ?
Sm1 Ge1' Ga1 13_555 . 149_545 116.34(9) ?
Sm1 Ge1' Ga1 13_555 . 6_555 123.13(8) ?
Sm1 Ge1' Ga1 13_555 . 150_555 62.11(3) ?
Sm1 Ge1' Ga1 13_555 . 9_555 123.13(8) ?
Sm1 Ge1' Ga1 13_555 . 105_554 62.11(3) ?
Sm1 Ge1' Ga1 13_555 . 10_555 58.26(3) ?
Sm1 Ge1' Ga1 13_555 . 106_555 116.34(9) ?
Sm1 Ge1' Ga1' 13_555 . 5_555 60.74(4) ?
Sm1 Ge1' Ga1' 13_555 . 149_545 119.26(9) ?
Sm1 Ge1' Ga1' 13_555 . 6_555 120.73(9) ?
Sm1 Ge1' Ga1' 13_555 . 150_555 59.27(4) ?
Sm1 Ge1' Ga1' 13_555 . 9_555 120.73(9) ?
Sm1 Ge1' Ga1' 13_555 . 105_554 59.27(4) ?
Sm1 Ge1' Ga1' 13_555 . 10_555 60.74(4) ?
Sm1 Ge1' Ga1' 13_555 . 106_555 119.26(9) ?
Sm1 Ge1' Ge1 13_555 . . 89.10(7) ?
Sm1 Ge1' Ge1 13_555 . 5_555 58.26(3) ?
Sm1 Ge1' Ge1 13_555 . 149_545 116.34(9) ?
Sm1 Ge1' Ge1 13_555 . 6_555 123.13(8) ?
Sm1 Ge1' Ge1 13_555 . 150_555 62.11(3) ?
Sm1 Ge1' Ge1 13_555 . 9_555 123.13(8) ?
Sm1 Ge1' Ge1 13_555 . 105_554 62.11(3) ?
Sm1 Ge1' Ge1 13_555 . 10_555 58.26(3) ?
Sm1 Ge1' Ge1 13_555 . 106_555 116.34(9) ?
Sm1 Ge1' Ge1' 13_555 . 5_555 60.74(4) ?
Sm1 Ge1' Ge1' 13_555 . 149_545 119.26(9) ?
Sm1 Ge1' Ge1' 13_555 . 6_555 120.73(9) ?
Sm1 Ge1' Ge1' 13_555 . 150_555 59.27(4) ?
Sm1 Ge1' Ge1' 13_555 . 9_555 120.73(9) ?
Sm1 Ge1' Ge1' 13_555 . 105_554 59.27(4) ?
Sm1 Ge1' Ge1' 13_555 . 10_555 60.74(4) ?
Sm1 Ge1' Ge1' 13_555 . 106_555 119.26(9) ?
Sm1 Ge1' Mn1 61_545 . . 90.90(7) ?
Sm1 Ge1' Ga1 61_545 . . 89.10(7) ?
Sm1 Ge1' Ga1 61_545 . 5_555 123.13(8) ?
Sm1 Ge1' Ga1 61_545 . 149_545 62.11(3) ?
Sm1 Ge1' Ga1 61_545 . 6_555 58.26(3) ?
Sm1 Ge1' Ga1 61_545 . 150_555 116.34(9) ?
Sm1 Ge1' Ga1 61_545 . 9_555 58.26(3) ?
Sm1 Ge1' Ga1 61_545 . 105_554 116.34(9) ?
Sm1 Ge1' Ga1 61_545 . 10_555 123.13(8) ?
Sm1 Ge1' Ga1 61_545 . 106_555 62.11(3) ?
Sm1 Ge1' Ga1' 61_545 . 5_555 120.73(9) ?
Sm1 Ge1' Ga1' 61_545 . 149_545 59.27(4) ?
Sm1 Ge1' Ga1' 61_545 . 6_555 60.74(4) ?
Sm1 Ge1' Ga1' 61_545 . 150_555 119.26(9) ?
Sm1 Ge1' Ga1' 61_545 . 9_555 60.74(4) ?
Sm1 Ge1' Ga1' 61_545 . 105_554 119.26(9) ?
Sm1 Ge1' Ga1' 61_545 . 10_555 120.73(9) ?
Sm1 Ge1' Ga1' 61_545 . 106_555 59.27(4) ?
Sm1 Ge1' Ge1 61_545 . . 89.10(7) ?
Sm1 Ge1' Ge1 61_545 . 5_555 123.13(8) ?
Sm1 Ge1' Ge1 61_545 . 149_545 62.11(3) ?
Sm1 Ge1' Ge1 61_545 . 6_555 58.26(3) ?
Sm1 Ge1' Ge1 61_545 . 150_555 116.34(9) ?
Sm1 Ge1' Ge1 61_545 . 9_555 58.26(3) ?
Sm1 Ge1' Ge1 61_545 . 105_554 116.34(9) ?
Sm1 Ge1' Ge1 61_545 . 10_555 123.13(8) ?
Sm1 Ge1' Ge1 61_545 . 106_555 62.11(3) ?
Sm1 Ge1' Ge1' 61_545 . 5_555 120.73(9) ?
Sm1 Ge1' Ge1' 61_545 . 149_545 59.27(4) ?
Sm1 Ge1' Ge1' 61_545 . 6_555 60.74(4) ?
Sm1 Ge1' Ge1' 61_545 . 150_555 119.26(9) ?
Sm1 Ge1' Ge1' 61_545 . 9_555 60.74(4) ?
Sm1 Ge1' Ge1' 61_545 . 105_554 119.26(9) ?
Sm1 Ge1' Ge1' 61_545 . 10_555 120.73(9) ?
Sm1 Ge1' Ge1' 61_545 . 106_555 59.27(4) ?
Mn1 Ge1' Ga1 . . . 180 ?
Mn1 Ge1' Ga1 . . 5_555 49.33(5) ?
Mn1 Ge1' Ga1 . . 149_545 139.86(5) ?
Mn1 Ge1' Ga1 . . 6_555 49.33(5) ?
Mn1 Ge1' Ga1 . . 150_555 139.86(5) ?
Mn1 Ge1' Ga1 . . 9_555 49.33(5) ?
Mn1 Ge1' Ga1 . . 105_554 139.86(5) ?
Mn1 Ge1' Ga1 . . 10_555 49.33(5) ?
Mn1 Ge1' Ga1 . . 106_555 139.86(5) ?
Mn1 Ge1' Ga1' . . 5_555 45.00(7) ?
Mn1 Ge1' Ga1' . . 149_545 135.00(7) ?
Mn1 Ge1' Ga1' . . 6_555 45.00(7) ?
Mn1 Ge1' Ga1' . . 150_555 135.00(7) ?
Mn1 Ge1' Ga1' . . 9_555 45.00(7) ?
Mn1 Ge1' Ga1' . . 105_554 135.00(7) ?
Mn1 Ge1' Ga1' . . 10_555 45.00(7) ?
Mn1 Ge1' Ga1' . . 106_555 135.00(7) ?
Mn1 Ge1' Ge1 . . . 180 ?
Mn1 Ge1' Ge1 . . 5_555 49.33(5) ?
Mn1 Ge1' Ge1 . . 149_545 139.86(5) ?
Mn1 Ge1' Ge1 . . 6_555 49.33(5) ?
Mn1 Ge1' Ge1 . . 150_555 139.86(5) ?
Mn1 Ge1' Ge1 . . 9_555 49.33(5) ?
Mn1 Ge1' Ge1 . . 105_554 139.86(5) ?
Mn1 Ge1' Ge1 . . 10_555 49.33(5) ?
Mn1 Ge1' Ge1 . . 106_555 139.86(5) ?
Mn1 Ge1' Ge1' . . 5_555 45.00(7) ?
Mn1 Ge1' Ge1' . . 149_545 135.00(7) ?
Mn1 Ge1' Ge1' . . 6_555 45.00(7) ?
Mn1 Ge1' Ge1' . . 150_555 135.00(7) ?
Mn1 Ge1' Ge1' . . 9_555 45.00(7) ?
Mn1 Ge1' Ge1' . . 105_554 135.00(7) ?
Mn1 Ge1' Ge1' . . 10_555 45.00(7) ?
Mn1 Ge1' Ge1' . . 106_555 135.00(7) ?
Ga1 Ge1' Ga1 . . 5_555 130.67(5) ?
Ga1 Ge1' Ga1 . . 149_545 40.14(5) ?
Ga1 Ge1' Ga1 . . 6_555 130.67(5) ?
Ga1 Ge1' Ga1 . . 150_555 40.14(5) ?
Ga1 Ge1' Ga1 . . 9_555 130.67(5) ?
Ga1 Ge1' Ga1 . . 105_554 40.14(5) ?
Ga1 Ge1' Ga1 . . 10_555 130.67(5) ?
Ga1 Ge1' Ga1 . . 106_555 40.14(5) ?
Ga1 Ge1' Ga1' . . 5_555 135.00(7) ?
Ga1 Ge1' Ga1' . . 149_545 45.00(7) ?
Ga1 Ge1' Ga1' . . 6_555 135.00(7) ?
Ga1 Ge1' Ga1' . . 150_555 45.00(7) ?
Ga1 Ge1' Ga1' . . 9_555 135.00(7) ?
Ga1 Ge1' Ga1' . . 105_554 45.00(7) ?
Ga1 Ge1' Ga1' . . 10_555 135.00(7) ?
Ga1 Ge1' Ga1' . . 106_555 45.00(7) ?
Ga1 Ge1' Ge1 . . . 0 ?
Ga1 Ge1' Ge1 . . 5_555 130.67(5) ?
Ga1 Ge1' Ge1 . . 149_545 40.14(5) ?
Ga1 Ge1' Ge1 . . 6_555 130.67(5) ?
Ga1 Ge1' Ge1 . . 150_555 40.14(5) ?
Ga1 Ge1' Ge1 . . 9_555 130.67(5) ?
Ga1 Ge1' Ge1 . . 105_554 40.14(5) ?
Ga1 Ge1' Ge1 . . 10_555 130.67(5) ?
Ga1 Ge1' Ge1 . . 106_555 40.14(5) ?
Ga1 Ge1' Ge1' . . 5_555 135.00(7) ?
Ga1 Ge1' Ge1' . . 149_545 45.00(7) ?
Ga1 Ge1' Ge1' . . 6_555 135.00(7) ?
Ga1 Ge1' Ge1' . . 150_555 45.00(7) ?
Ga1 Ge1' Ge1' . . 9_555 135.00(7) ?
Ga1 Ge1' Ge1' . . 105_554 45.00(7) ?
Ga1 Ge1' Ge1' . . 10_555 135.00(7) ?
Ga1 Ge1' Ge1' . . 106_555 45.00(7) ?
Ga1 Ge1' Ga1 5_555 . 149_545 170.80(10) ?
Ga1 Ge1' Ga1 5_555 . 6_555 98.66(10) ?
Ga1 Ge1' Ga1 5_555 . 150_555 90.53(2) ?
Ga1 Ge1' Ga1 5_555 . 9_555 64.87(5) ?
Ga1 Ge1' Ga1 5_555 . 105_554 119.881(15) ?
Ga1 Ge1' Ga1 5_555 . 10_555 64.87(5) ?
Ga1 Ge1' Ga1 5_555 . 106_555 119.881(15) ?
Ga1 Ge1' Ga1' 5_555 . 5_555 4.33(5) ?
Ga1 Ge1' Ga1' 5_555 . 149_545 175.67(11) ?
Ga1 Ge1' Ga1' 5_555 . 6_555 94.33(11) ?
Ga1 Ge1' Ga1' 5_555 . 150_555 85.67(5) ?
Ga1 Ge1' Ga1' 5_555 . 9_555 62.56(6) ?
Ga1 Ge1' Ga1' 5_555 . 105_554 117.44(3) ?
Ga1 Ge1' Ga1' 5_555 . 10_555 62.56(6) ?
Ga1 Ge1' Ga1' 5_555 . 106_555 117.44(3) ?
Ga1 Ge1' Ge1 5_555 . . 130.67(5) ?
Ga1 Ge1' Ge1 5_555 . 5_555 0 ?
Ga1 Ge1' Ge1 5_555 . 149_545 170.80(10) ?
Ga1 Ge1' Ge1 5_555 . 6_555 98.66(10) ?
Ga1 Ge1' Ge1 5_555 . 150_555 90.53(2) ?
Ga1 Ge1' Ge1 5_555 . 9_555 64.87(5) ?
Ga1 Ge1' Ge1 5_555 . 105_554 119.881(15) ?
Ga1 Ge1' Ge1 5_555 . 10_555 64.87(5) ?
Ga1 Ge1' Ge1 5_555 . 106_555 119.881(15) ?
Ga1 Ge1' Ge1' 5_555 . 5_555 4.33(5) ?
Ga1 Ge1' Ge1' 5_555 . 149_545 175.67(11) ?
Ga1 Ge1' Ge1' 5_555 . 6_555 94.33(11) ?
Ga1 Ge1' Ge1' 5_555 . 150_555 85.67(5) ?
Ga1 Ge1' Ge1' 5_555 . 9_555 62.56(6) ?
Ga1 Ge1' Ge1' 5_555 . 105_554 117.44(3) ?
Ga1 Ge1' Ge1' 5_555 . 10_555 62.56(6) ?
Ga1 Ge1' Ge1' 5_555 . 106_555 117.44(3) ?
Ga1 Ge1' Ga1 149_545 . 6_555 90.53(2) ?
Ga1 Ge1' Ga1 149_545 . 150_555 80.27(9) ?
Ga1 Ge1' Ga1 149_545 . 9_555 119.881(15) ?
Ga1 Ge1' Ga1 149_545 . 105_554 54.23(6) ?
Ga1 Ge1' Ga1 149_545 . 10_555 119.881(15) ?
Ga1 Ge1' Ga1 149_545 . 106_555 54.23(6) ?
Ga1 Ge1' Ga1' 149_545 . 5_555 175.14(11) ?
Ga1 Ge1' Ga1' 149_545 . 149_545 4.86(5) ?
Ga1 Ge1' Ga1' 149_545 . 6_555 94.86(5) ?
Ga1 Ge1' Ga1' 149_545 . 150_555 85.14(10) ?
Ga1 Ge1' Ga1' 149_545 . 9_555 122.72(3) ?
Ga1 Ge1' Ga1' 149_545 . 105_554 57.28(6) ?
Ga1 Ge1' Ga1' 149_545 . 10_555 122.72(3) ?
Ga1 Ge1' Ga1' 149_545 . 106_555 57.28(6) ?
Ga1 Ge1' Ge1 149_545 . . 40.14(5) ?
Ga1 Ge1' Ge1 149_545 . 5_555 170.80(10) ?
Ga1 Ge1' Ge1 149_545 . 149_545 0 ?
Ga1 Ge1' Ge1 149_545 . 6_555 90.53(2) ?
Ga1 Ge1' Ge1 149_545 . 150_555 80.27(9) ?
Ga1 Ge1' Ge1 149_545 . 9_555 119.881(15) ?
Ga1 Ge1' Ge1 149_545 . 105_554 54.23(6) ?
Ga1 Ge1' Ge1 149_545 . 10_555 119.881(15) ?
Ga1 Ge1' Ge1 149_545 . 106_555 54.23(6) ?
Ga1 Ge1' Ge1' 149_545 . 5_555 175.14(11) ?
Ga1 Ge1' Ge1' 149_545 . 149_545 4.86(5) ?
Ga1 Ge1' Ge1' 149_545 . 6_555 94.86(5) ?
Ga1 Ge1' Ge1' 149_545 . 150_555 85.14(10) ?
Ga1 Ge1' Ge1' 149_545 . 9_555 122.72(3) ?
Ga1 Ge1' Ge1' 149_545 . 105_554 57.28(6) ?
Ga1 Ge1' Ge1' 149_545 . 10_555 122.72(3) ?
Ga1 Ge1' Ge1' 149_545 . 106_555 57.28(6) ?
Ga1 Ge1' Ga1 6_555 . 150_555 170.80(10) ?
Ga1 Ge1' Ga1 6_555 . 9_555 64.87(5) ?
Ga1 Ge1' Ga1 6_555 . 105_554 119.881(15) ?
Ga1 Ge1' Ga1 6_555 . 10_555 64.87(5) ?
Ga1 Ge1' Ga1 6_555 . 106_555 119.881(15) ?
Ga1 Ge1' Ga1' 6_555 . 5_555 94.33(11) ?
Ga1 Ge1' Ga1' 6_555 . 149_545 85.67(5) ?
Ga1 Ge1' Ga1' 6_555 . 6_555 4.33(5) ?
Ga1 Ge1' Ga1' 6_555 . 150_555 175.67(11) ?
Ga1 Ge1' Ga1' 6_555 . 9_555 62.56(6) ?
Ga1 Ge1' Ga1' 6_555 . 105_554 117.44(3) ?
Ga1 Ge1' Ga1' 6_555 . 10_555 62.56(6) ?
Ga1 Ge1' Ga1' 6_555 . 106_555 117.44(3) ?
Ga1 Ge1' Ge1 6_555 . . 130.67(5) ?
Ga1 Ge1' Ge1 6_555 . 5_555 98.66(10) ?
Ga1 Ge1' Ge1 6_555 . 149_545 90.53(2) ?
Ga1 Ge1' Ge1 6_555 . 6_555 0 ?
Ga1 Ge1' Ge1 6_555 . 150_555 170.80(10) ?
Ga1 Ge1' Ge1 6_555 . 9_555 64.87(5) ?
Ga1 Ge1' Ge1 6_555 . 105_554 119.881(15) ?
Ga1 Ge1' Ge1 6_555 . 10_555 64.87(5) ?
Ga1 Ge1' Ge1 6_555 . 106_555 119.881(15) ?
Ga1 Ge1' Ge1' 6_555 . 5_555 94.33(11) ?
Ga1 Ge1' Ge1' 6_555 . 149_545 85.67(5) ?
Ga1 Ge1' Ge1' 6_555 . 6_555 4.33(5) ?
Ga1 Ge1' Ge1' 6_555 . 150_555 175.67(11) ?
Ga1 Ge1' Ge1' 6_555 . 9_555 62.56(6) ?
Ga1 Ge1' Ge1' 6_555 . 105_554 117.44(3) ?
Ga1 Ge1' Ge1' 6_555 . 10_555 62.56(6) ?
Ga1 Ge1' Ge1' 6_555 . 106_555 117.44(3) ?
Ga1 Ge1' Ga1 150_555 . 9_555 119.881(15) ?
Ga1 Ge1' Ga1 150_555 . 105_554 54.23(6) ?
Ga1 Ge1' Ga1 150_555 . 10_555 119.881(15) ?
Ga1 Ge1' Ga1 150_555 . 106_555 54.23(6) ?
Ga1 Ge1' Ga1' 150_555 . 5_555 94.86(5) ?
Ga1 Ge1' Ga1' 150_555 . 149_545 85.14(10) ?
Ga1 Ge1' Ga1' 150_555 . 6_555 175.14(11) ?
Ga1 Ge1' Ga1' 150_555 . 150_555 4.86(5) ?
Ga1 Ge1' Ga1' 150_555 . 9_555 122.72(3) ?
Ga1 Ge1' Ga1' 150_555 . 105_554 57.28(6) ?
Ga1 Ge1' Ga1' 150_555 . 10_555 122.72(3) ?
Ga1 Ge1' Ga1' 150_555 . 106_555 57.28(6) ?
Ga1 Ge1' Ge1 150_555 . . 40.14(5) ?
Ga1 Ge1' Ge1 150_555 . 5_555 90.53(2) ?
Ga1 Ge1' Ge1 150_555 . 149_545 80.27(9) ?
Ga1 Ge1' Ge1 150_555 . 6_555 170.80(10) ?
Ga1 Ge1' Ge1 150_555 . 150_555 0 ?
Ga1 Ge1' Ge1 150_555 . 9_555 119.881(15) ?
Ga1 Ge1' Ge1 150_555 . 105_554 54.23(6) ?
Ga1 Ge1' Ge1 150_555 . 10_555 119.881(15) ?
Ga1 Ge1' Ge1 150_555 . 106_555 54.23(6) ?
Ga1 Ge1' Ge1' 150_555 . 5_555 94.86(5) ?
Ga1 Ge1' Ge1' 150_555 . 149_545 85.14(10) ?
Ga1 Ge1' Ge1' 150_555 . 6_555 175.14(11) ?
Ga1 Ge1' Ge1' 150_555 . 150_555 4.86(5) ?
Ga1 Ge1' Ge1' 150_555 . 9_555 122.72(3) ?
Ga1 Ge1' Ge1' 150_555 . 105_554 57.28(6) ?
Ga1 Ge1' Ge1' 150_555 . 10_555 122.72(3) ?
Ga1 Ge1' Ge1' 150_555 . 106_555 57.28(6) ?
Ga1 Ge1' Ga1 9_555 . 105_554 170.80(10) ?
Ga1 Ge1' Ga1 9_555 . 10_555 98.66(10) ?
Ga1 Ge1' Ga1 9_555 . 106_555 90.53(2) ?
Ga1 Ge1' Ga1' 9_555 . 5_555 62.56(6) ?
Ga1 Ge1' Ga1' 9_555 . 149_545 117.44(3) ?
Ga1 Ge1' Ga1' 9_555 . 6_555 62.56(6) ?
Ga1 Ge1' Ga1' 9_555 . 150_555 117.44(3) ?
Ga1 Ge1' Ga1' 9_555 . 9_555 4.33(5) ?
Ga1 Ge1' Ga1' 9_555 . 105_554 175.67(11) ?
Ga1 Ge1' Ga1' 9_555 . 10_555 94.33(11) ?
Ga1 Ge1' Ga1' 9_555 . 106_555 85.67(5) ?
Ga1 Ge1' Ge1 9_555 . . 130.67(5) ?
Ga1 Ge1' Ge1 9_555 . 5_555 64.87(5) ?
Ga1 Ge1' Ge1 9_555 . 149_545 119.881(15) ?
Ga1 Ge1' Ge1 9_555 . 6_555 64.87(5) ?
Ga1 Ge1' Ge1 9_555 . 150_555 119.881(15) ?
Ga1 Ge1' Ge1 9_555 . 9_555 0 ?
Ga1 Ge1' Ge1 9_555 . 105_554 170.80(10) ?
Ga1 Ge1' Ge1 9_555 . 10_555 98.66(10) ?
Ga1 Ge1' Ge1 9_555 . 106_555 90.53(2) ?
Ga1 Ge1' Ge1' 9_555 . 5_555 62.56(6) ?
Ga1 Ge1' Ge1' 9_555 . 149_545 117.44(3) ?
Ga1 Ge1' Ge1' 9_555 . 6_555 62.56(6) ?
Ga1 Ge1' Ge1' 9_555 . 150_555 117.44(3) ?
Ga1 Ge1' Ge1' 9_555 . 9_555 4.33(5) ?
Ga1 Ge1' Ge1' 9_555 . 105_554 175.67(11) ?
Ga1 Ge1' Ge1' 9_555 . 10_555 94.33(11) ?
Ga1 Ge1' Ge1' 9_555 . 106_555 85.67(5) ?
Ga1 Ge1' Ga1 105_554 . 10_555 90.53(2) ?
Ga1 Ge1' Ga1 105_554 . 106_555 80.27(9) ?
Ga1 Ge1' Ga1' 105_554 . 5_555 122.72(3) ?
Ga1 Ge1' Ga1' 105_554 . 149_545 57.28(6) ?
Ga1 Ge1' Ga1' 105_554 . 6_555 122.72(3) ?
Ga1 Ge1' Ga1' 105_554 . 150_555 57.28(6) ?
Ga1 Ge1' Ga1' 105_554 . 9_555 175.14(11) ?
Ga1 Ge1' Ga1' 105_554 . 105_554 4.86(5) ?
Ga1 Ge1' Ga1' 105_554 . 10_555 94.86(5) ?
Ga1 Ge1' Ga1' 105_554 . 106_555 85.14(10) ?
Ga1 Ge1' Ge1 105_554 . . 40.14(5) ?
Ga1 Ge1' Ge1 105_554 . 5_555 119.881(15) ?
Ga1 Ge1' Ge1 105_554 . 149_545 54.23(6) ?
Ga1 Ge1' Ge1 105_554 . 6_555 119.881(15) ?
Ga1 Ge1' Ge1 105_554 . 150_555 54.23(6) ?
Ga1 Ge1' Ge1 105_554 . 9_555 170.80(10) ?
Ga1 Ge1' Ge1 105_554 . 105_554 0 ?
Ga1 Ge1' Ge1 105_554 . 10_555 90.53(2) ?
Ga1 Ge1' Ge1 105_554 . 106_555 80.27(9) ?
Ga1 Ge1' Ge1' 105_554 . 5_555 122.72(3) ?
Ga1 Ge1' Ge1' 105_554 . 149_545 57.28(6) ?
Ga1 Ge1' Ge1' 105_554 . 6_555 122.72(3) ?
Ga1 Ge1' Ge1' 105_554 . 150_555 57.28(6) ?
Ga1 Ge1' Ge1' 105_554 . 9_555 175.14(11) ?
Ga1 Ge1' Ge1' 105_554 . 105_554 4.86(5) ?
Ga1 Ge1' Ge1' 105_554 . 10_555 94.86(5) ?
Ga1 Ge1' Ge1' 105_554 . 106_555 85.14(10) ?
Ga1 Ge1' Ga1 10_555 . 106_555 170.80(10) ?
Ga1 Ge1' Ga1' 10_555 . 5_555 62.56(6) ?
Ga1 Ge1' Ga1' 10_555 . 149_545 117.44(3) ?
Ga1 Ge1' Ga1' 10_555 . 6_555 62.56(6) ?
Ga1 Ge1' Ga1' 10_555 . 150_555 117.44(3) ?
Ga1 Ge1' Ga1' 10_555 . 9_555 94.33(11) ?
Ga1 Ge1' Ga1' 10_555 . 105_554 85.67(5) ?
Ga1 Ge1' Ga1' 10_555 . 10_555 4.33(5) ?
Ga1 Ge1' Ga1' 10_555 . 106_555 175.67(11) ?
Ga1 Ge1' Ge1 10_555 . . 130.67(5) ?
Ga1 Ge1' Ge1 10_555 . 5_555 64.87(5) ?
Ga1 Ge1' Ge1 10_555 . 149_545 119.881(15) ?
Ga1 Ge1' Ge1 10_555 . 6_555 64.87(5) ?
Ga1 Ge1' Ge1 10_555 . 150_555 119.881(15) ?
Ga1 Ge1' Ge1 10_555 . 9_555 98.66(10) ?
Ga1 Ge1' Ge1 10_555 . 105_554 90.53(2) ?
Ga1 Ge1' Ge1 10_555 . 10_555 0 ?
Ga1 Ge1' Ge1 10_555 . 106_555 170.80(10) ?
Ga1 Ge1' Ge1' 10_555 . 5_555 62.56(6) ?
Ga1 Ge1' Ge1' 10_555 . 149_545 117.44(3) ?
Ga1 Ge1' Ge1' 10_555 . 6_555 62.56(6) ?
Ga1 Ge1' Ge1' 10_555 . 150_555 117.44(3) ?
Ga1 Ge1' Ge1' 10_555 . 9_555 94.33(11) ?
Ga1 Ge1' Ge1' 10_555 . 105_554 85.67(5) ?
Ga1 Ge1' Ge1' 10_555 . 10_555 4.33(5) ?
Ga1 Ge1' Ge1' 10_555 . 106_555 175.67(11) ?
Ga1 Ge1' Ga1' 106_555 . 5_555 122.72(3) ?
Ga1 Ge1' Ga1' 106_555 . 149_545 57.28(6) ?
Ga1 Ge1' Ga1' 106_555 . 6_555 122.72(3) ?
Ga1 Ge1' Ga1' 106_555 . 150_555 57.28(6) ?
Ga1 Ge1' Ga1' 106_555 . 9_555 94.86(5) ?
Ga1 Ge1' Ga1' 106_555 . 105_554 85.14(10) ?
Ga1 Ge1' Ga1' 106_555 . 10_555 175.14(11) ?
Ga1 Ge1' Ga1' 106_555 . 106_555 4.86(5) ?
Ga1 Ge1' Ge1 106_555 . . 40.14(5) ?
Ga1 Ge1' Ge1 106_555 . 5_555 119.881(15) ?
Ga1 Ge1' Ge1 106_555 . 149_545 54.23(6) ?
Ga1 Ge1' Ge1 106_555 . 6_555 119.881(15) ?
Ga1 Ge1' Ge1 106_555 . 150_555 54.23(6) ?
Ga1 Ge1' Ge1 106_555 . 9_555 90.53(2) ?
Ga1 Ge1' Ge1 106_555 . 105_554 80.27(9) ?
Ga1 Ge1' Ge1 106_555 . 10_555 170.80(10) ?
Ga1 Ge1' Ge1 106_555 . 106_555 0 ?
Ga1 Ge1' Ge1' 106_555 . 5_555 122.72(3) ?
Ga1 Ge1' Ge1' 106_555 . 149_545 57.28(6) ?
Ga1 Ge1' Ge1' 106_555 . 6_555 122.72(3) ?
Ga1 Ge1' Ge1' 106_555 . 150_555 57.28(6) ?
Ga1 Ge1' Ge1' 106_555 . 9_555 94.86(5) ?
Ga1 Ge1' Ge1' 106_555 . 105_554 85.14(10) ?
Ga1 Ge1' Ge1' 106_555 . 10_555 175.14(11) ?
Ga1 Ge1' Ge1' 106_555 . 106_555 4.86(5) ?
Ga1' Ge1' Ga1' 5_555 . 149_545 180 ?
Ga1' Ge1' Ga1' 5_555 . 6_555 90.00(12) ?
Ga1' Ge1' Ga1' 5_555 . 150_555 90.00(7) ?
Ga1' Ge1' Ga1' 5_555 . 9_555 60.00(7) ?
Ga1' Ge1' Ga1' 5_555 . 105_554 120.00(4) ?
Ga1' Ge1' Ga1' 5_555 . 10_555 60.00(7) ?
Ga1' Ge1' Ga1' 5_555 . 106_555 120.00(4) ?
Ga1' Ge1' Ge1 5_555 . . 135.00(7) ?
Ga1' Ge1' Ge1 5_555 . 5_555 4.33(5) ?
Ga1' Ge1' Ge1 5_555 . 149_545 175.14(11) ?
Ga1' Ge1' Ge1 5_555 . 6_555 94.33(11) ?
Ga1' Ge1' Ge1 5_555 . 150_555 94.86(5) ?
Ga1' Ge1' Ge1 5_555 . 9_555 62.56(6) ?
Ga1' Ge1' Ge1 5_555 . 105_554 122.72(3) ?
Ga1' Ge1' Ge1 5_555 . 10_555 62.56(6) ?
Ga1' Ge1' Ge1 5_555 . 106_555 122.72(3) ?
Ga1' Ge1' Ge1' 5_555 . 5_555 0 ?
Ga1' Ge1' Ge1' 5_555 . 149_545 180 ?
Ga1' Ge1' Ge1' 5_555 . 6_555 90.00(12) ?
Ga1' Ge1' Ge1' 5_555 . 150_555 90.00(7) ?
Ga1' Ge1' Ge1' 5_555 . 9_555 60.00(7) ?
Ga1' Ge1' Ge1' 5_555 . 105_554 120.00(4) ?
Ga1' Ge1' Ge1' 5_555 . 10_555 60.00(7) ?
Ga1' Ge1' Ge1' 5_555 . 106_555 120.00(4) ?
Ga1' Ge1' Ga1' 149_545 . 6_555 90.00(7) ?
Ga1' Ge1' Ga1' 149_545 . 150_555 90.00(11) ?
Ga1' Ge1' Ga1' 149_545 . 9_555 120.00(4) ?
Ga1' Ge1' Ga1' 149_545 . 105_554 60.00(7) ?
Ga1' Ge1' Ga1' 149_545 . 10_555 120.00(4) ?
Ga1' Ge1' Ga1' 149_545 . 106_555 60.00(7) ?
Ga1' Ge1' Ge1 149_545 . . 45.00(7) ?
Ga1' Ge1' Ge1 149_545 . 5_555 175.67(11) ?
Ga1' Ge1' Ge1 149_545 . 149_545 4.86(5) ?
Ga1' Ge1' Ge1 149_545 . 6_555 85.67(5) ?
Ga1' Ge1' Ge1 149_545 . 150_555 85.14(10) ?
Ga1' Ge1' Ge1 149_545 . 9_555 117.44(3) ?
Ga1' Ge1' Ge1 149_545 . 105_554 57.28(6) ?
Ga1' Ge1' Ge1 149_545 . 10_555 117.44(3) ?
Ga1' Ge1' Ge1 149_545 . 106_555 57.28(6) ?
Ga1' Ge1' Ge1' 149_545 . 5_555 180 ?
Ga1' Ge1' Ge1' 149_545 . 149_545 0 ?
Ga1' Ge1' Ge1' 149_545 . 6_555 90.00(7) ?
Ga1' Ge1' Ge1' 149_545 . 150_555 90.00(11) ?
Ga1' Ge1' Ge1' 149_545 . 9_555 120.00(4) ?
Ga1' Ge1' Ge1' 149_545 . 105_554 60.00(7) ?
Ga1' Ge1' Ge1' 149_545 . 10_555 120.00(4) ?
Ga1' Ge1' Ge1' 149_545 . 106_555 60.00(7) ?
Ga1' Ge1' Ga1' 6_555 . 150_555 180 ?
Ga1' Ge1' Ga1' 6_555 . 9_555 60.00(7) ?
Ga1' Ge1' Ga1' 6_555 . 105_554 120.00(4) ?
Ga1' Ge1' Ga1' 6_555 . 10_555 60.00(7) ?
Ga1' Ge1' Ga1' 6_555 . 106_555 120.00(4) ?
Ga1' Ge1' Ge1 6_555 . . 135.00(7) ?
Ga1' Ge1' Ge1 6_555 . 5_555 94.33(11) ?
Ga1' Ge1' Ge1 6_555 . 149_545 94.86(5) ?
Ga1' Ge1' Ge1 6_555 . 6_555 4.33(5) ?
Ga1' Ge1' Ge1 6_555 . 150_555 175.14(11) ?
Ga1' Ge1' Ge1 6_555 . 9_555 62.56(6) ?
Ga1' Ge1' Ge1 6_555 . 105_554 122.72(3) ?
Ga1' Ge1' Ge1 6_555 . 10_555 62.56(6) ?
Ga1' Ge1' Ge1 6_555 . 106_555 122.72(3) ?
Ga1' Ge1' Ge1' 6_555 . 5_555 90.00(12) ?
Ga1' Ge1' Ge1' 6_555 . 149_545 90.00(7) ?
Ga1' Ge1' Ge1' 6_555 . 6_555 0 ?
Ga1' Ge1' Ge1' 6_555 . 150_555 180 ?
Ga1' Ge1' Ge1' 6_555 . 9_555 60.00(7) ?
Ga1' Ge1' Ge1' 6_555 . 105_554 120.00(4) ?
Ga1' Ge1' Ge1' 6_555 . 10_555 60.00(7) ?
Ga1' Ge1' Ge1' 6_555 . 106_555 120.00(4) ?
Ga1' Ge1' Ga1' 150_555 . 9_555 120.00(4) ?
Ga1' Ge1' Ga1' 150_555 . 105_554 60.00(7) ?
Ga1' Ge1' Ga1' 150_555 . 10_555 120.00(4) ?
Ga1' Ge1' Ga1' 150_555 . 106_555 60.00(7) ?
Ga1' Ge1' Ge1 150_555 . . 45.00(7) ?
Ga1' Ge1' Ge1 150_555 . 5_555 85.67(5) ?
Ga1' Ge1' Ge1 150_555 . 149_545 85.14(10) ?
Ga1' Ge1' Ge1 150_555 . 6_555 175.67(11) ?
Ga1' Ge1' Ge1 150_555 . 150_555 4.86(5) ?
Ga1' Ge1' Ge1 150_555 . 9_555 117.44(3) ?
Ga1' Ge1' Ge1 150_555 . 105_554 57.28(6) ?
Ga1' Ge1' Ge1 150_555 . 10_555 117.44(3) ?
Ga1' Ge1' Ge1 150_555 . 106_555 57.28(6) ?
Ga1' Ge1' Ge1' 150_555 . 5_555 90.00(7) ?
Ga1' Ge1' Ge1' 150_555 . 149_545 90.00(11) ?
Ga1' Ge1' Ge1' 150_555 . 6_555 180 ?
Ga1' Ge1' Ge1' 150_555 . 150_555 0 ?
Ga1' Ge1' Ge1' 150_555 . 9_555 120.00(4) ?
Ga1' Ge1' Ge1' 150_555 . 105_554 60.00(7) ?
Ga1' Ge1' Ge1' 150_555 . 10_555 120.00(4) ?
Ga1' Ge1' Ge1' 150_555 . 106_555 60.00(7) ?
Ga1' Ge1' Ga1' 9_555 . 105_554 180 ?
Ga1' Ge1' Ga1' 9_555 . 10_555 90.00(12) ?
Ga1' Ge1' Ga1' 9_555 . 106_555 90.00(7) ?
Ga1' Ge1' Ge1 9_555 . . 135.00(7) ?
Ga1' Ge1' Ge1 9_555 . 5_555 62.56(6) ?
Ga1' Ge1' Ge1 9_555 . 149_545 122.72(3) ?
Ga1' Ge1' Ge1 9_555 . 6_555 62.56(6) ?
Ga1' Ge1' Ge1 9_555 . 150_555 122.72(3) ?
Ga1' Ge1' Ge1 9_555 . 9_555 4.33(5) ?
Ga1' Ge1' Ge1 9_555 . 105_554 175.14(11) ?
Ga1' Ge1' Ge1 9_555 . 10_555 94.33(11) ?
Ga1' Ge1' Ge1 9_555 . 106_555 94.86(5) ?
Ga1' Ge1' Ge1' 9_555 . 5_555 60.00(7) ?
Ga1' Ge1' Ge1' 9_555 . 149_545 120.00(4) ?
Ga1' Ge1' Ge1' 9_555 . 6_555 60.00(7) ?
Ga1' Ge1' Ge1' 9_555 . 150_555 120.00(4) ?
Ga1' Ge1' Ge1' 9_555 . 9_555 0 ?
Ga1' Ge1' Ge1' 9_555 . 105_554 180 ?
Ga1' Ge1' Ge1' 9_555 . 10_555 90.00(12) ?
Ga1' Ge1' Ge1' 9_555 . 106_555 90.00(7) ?
Ga1' Ge1' Ga1' 105_554 . 10_555 90.00(7) ?
Ga1' Ge1' Ga1' 105_554 . 106_555 90.00(11) ?
Ga1' Ge1' Ge1 105_554 . . 45.00(7) ?
Ga1' Ge1' Ge1 105_554 . 5_555 117.44(3) ?
Ga1' Ge1' Ge1 105_554 . 149_545 57.28(6) ?
Ga1' Ge1' Ge1 105_554 . 6_555 117.44(3) ?
Ga1' Ge1' Ge1 105_554 . 150_555 57.28(6) ?
Ga1' Ge1' Ge1 105_554 . 9_555 175.67(11) ?
Ga1' Ge1' Ge1 105_554 . 105_554 4.86(5) ?
Ga1' Ge1' Ge1 105_554 . 10_555 85.67(5) ?
Ga1' Ge1' Ge1 105_554 . 106_555 85.14(10) ?
Ga1' Ge1' Ge1' 105_554 . 5_555 120.00(4) ?
Ga1' Ge1' Ge1' 105_554 . 149_545 60.00(7) ?
Ga1' Ge1' Ge1' 105_554 . 6_555 120.00(4) ?
Ga1' Ge1' Ge1' 105_554 . 150_555 60.00(7) ?
Ga1' Ge1' Ge1' 105_554 . 9_555 180 ?
Ga1' Ge1' Ge1' 105_554 . 105_554 0 ?
Ga1' Ge1' Ge1' 105_554 . 10_555 90.00(7) ?
Ga1' Ge1' Ge1' 105_554 . 106_555 90.00(11) ?
Ga1' Ge1' Ga1' 10_555 . 106_555 180 ?
Ga1' Ge1' Ge1 10_555 . . 135.00(7) ?
Ga1' Ge1' Ge1 10_555 . 5_555 62.56(6) ?
Ga1' Ge1' Ge1 10_555 . 149_545 122.72(3) ?
Ga1' Ge1' Ge1 10_555 . 6_555 62.56(6) ?
Ga1' Ge1' Ge1 10_555 . 150_555 122.72(3) ?
Ga1' Ge1' Ge1 10_555 . 9_555 94.33(11) ?
Ga1' Ge1' Ge1 10_555 . 105_554 94.86(5) ?
Ga1' Ge1' Ge1 10_555 . 10_555 4.33(5) ?
Ga1' Ge1' Ge1 10_555 . 106_555 175.14(11) ?
Ga1' Ge1' Ge1' 10_555 . 5_555 60.00(7) ?
Ga1' Ge1' Ge1' 10_555 . 149_545 120.00(4) ?
Ga1' Ge1' Ge1' 10_555 . 6_555 60.00(7) ?
Ga1' Ge1' Ge1' 10_555 . 150_555 120.00(4) ?
Ga1' Ge1' Ge1' 10_555 . 9_555 90.00(12) ?
Ga1' Ge1' Ge1' 10_555 . 105_554 90.00(7) ?
Ga1' Ge1' Ge1' 10_555 . 10_555 0 ?
Ga1' Ge1' Ge1' 10_555 . 106_555 180 ?
Ga1' Ge1' Ge1 106_555 . . 45.00(7) ?
Ga1' Ge1' Ge1 106_555 . 5_555 117.44(3) ?
Ga1' Ge1' Ge1 106_555 . 149_545 57.28(6) ?
Ga1' Ge1' Ge1 106_555 . 6_555 117.44(3) ?
Ga1' Ge1' Ge1 106_555 . 150_555 57.28(6) ?
Ga1' Ge1' Ge1 106_555 . 9_555 85.67(5) ?
Ga1' Ge1' Ge1 106_555 . 105_554 85.14(10) ?
Ga1' Ge1' Ge1 106_555 . 10_555 175.67(11) ?
Ga1' Ge1' Ge1 106_555 . 106_555 4.86(5) ?
Ga1' Ge1' Ge1' 106_555 . 5_555 120.00(4) ?
Ga1' Ge1' Ge1' 106_555 . 149_545 60.00(7) ?
Ga1' Ge1' Ge1' 106_555 . 6_555 120.00(4) ?
Ga1' Ge1' Ge1' 106_555 . 150_555 60.00(7) ?
Ga1' Ge1' Ge1' 106_555 . 9_555 90.00(7) ?
Ga1' Ge1' Ge1' 106_555 . 105_554 90.00(11) ?
Ga1' Ge1' Ge1' 106_555 . 10_555 180 ?
Ga1' Ge1' Ge1' 106_555 . 106_555 0 ?
Ge1 Ge1' Ge1 . . 5_555 130.67(5) ?
Ge1 Ge1' Ge1 . . 149_545 40.14(5) ?
Ge1 Ge1' Ge1 . . 6_555 130.67(5) ?
Ge1 Ge1' Ge1 . . 150_555 40.14(5) ?
Ge1 Ge1' Ge1 . . 9_555 130.67(5) ?
Ge1 Ge1' Ge1 . . 105_554 40.14(5) ?
Ge1 Ge1' Ge1 . . 10_555 130.67(5) ?
Ge1 Ge1' Ge1 . . 106_555 40.14(5) ?
Ge1 Ge1' Ge1' . . 5_555 135.00(7) ?
Ge1 Ge1' Ge1' . . 149_545 45.00(7) ?
Ge1 Ge1' Ge1' . . 6_555 135.00(7) ?
Ge1 Ge1' Ge1' . . 150_555 45.00(7) ?
Ge1 Ge1' Ge1' . . 9_555 135.00(7) ?
Ge1 Ge1' Ge1' . . 105_554 45.00(7) ?
Ge1 Ge1' Ge1' . . 10_555 135.00(7) ?
Ge1 Ge1' Ge1' . . 106_555 45.00(7) ?
Ge1 Ge1' Ge1 5_555 . 149_545 170.80(10) ?
Ge1 Ge1' Ge1 5_555 . 6_555 98.66(10) ?
Ge1 Ge1' Ge1 5_555 . 150_555 90.53(2) ?
Ge1 Ge1' Ge1 5_555 . 9_555 64.87(5) ?
Ge1 Ge1' Ge1 5_555 . 105_554 119.881(15) ?
Ge1 Ge1' Ge1 5_555 . 10_555 64.87(5) ?
Ge1 Ge1' Ge1 5_555 . 106_555 119.881(15) ?
Ge1 Ge1' Ge1' 5_555 . 5_555 4.33(5) ?
Ge1 Ge1' Ge1' 5_555 . 149_545 175.67(11) ?
Ge1 Ge1' Ge1' 5_555 . 6_555 94.33(11) ?
Ge1 Ge1' Ge1' 5_555 . 150_555 85.67(5) ?
Ge1 Ge1' Ge1' 5_555 . 9_555 62.56(6) ?
Ge1 Ge1' Ge1' 5_555 . 105_554 117.44(3) ?
Ge1 Ge1' Ge1' 5_555 . 10_555 62.56(6) ?
Ge1 Ge1' Ge1' 5_555 . 106_555 117.44(3) ?
Ge1 Ge1' Ge1 149_545 . 6_555 90.53(2) ?
Ge1 Ge1' Ge1 149_545 . 150_555 80.27(9) ?
Ge1 Ge1' Ge1 149_545 . 9_555 119.881(15) ?
Ge1 Ge1' Ge1 149_545 . 105_554 54.23(6) ?
Ge1 Ge1' Ge1 149_545 . 10_555 119.881(15) ?
Ge1 Ge1' Ge1 149_545 . 106_555 54.23(6) ?
Ge1 Ge1' Ge1' 149_545 . 5_555 175.14(11) ?
Ge1 Ge1' Ge1' 149_545 . 149_545 4.86(5) ?
Ge1 Ge1' Ge1' 149_545 . 6_555 94.86(5) ?
Ge1 Ge1' Ge1' 149_545 . 150_555 85.14(10) ?
Ge1 Ge1' Ge1' 149_545 . 9_555 122.72(3) ?
Ge1 Ge1' Ge1' 149_545 . 105_554 57.28(6) ?
Ge1 Ge1' Ge1' 149_545 . 10_555 122.72(3) ?
Ge1 Ge1' Ge1' 149_545 . 106_555 57.28(6) ?
Ge1 Ge1' Ge1 6_555 . 150_555 170.80(10) ?
Ge1 Ge1' Ge1 6_555 . 9_555 64.87(5) ?
Ge1 Ge1' Ge1 6_555 . 105_554 119.881(15) ?
Ge1 Ge1' Ge1 6_555 . 10_555 64.87(5) ?
Ge1 Ge1' Ge1 6_555 . 106_555 119.881(15) ?
Ge1 Ge1' Ge1' 6_555 . 5_555 94.33(11) ?
Ge1 Ge1' Ge1' 6_555 . 149_545 85.67(5) ?
Ge1 Ge1' Ge1' 6_555 . 6_555 4.33(5) ?
Ge1 Ge1' Ge1' 6_555 . 150_555 175.67(11) ?
Ge1 Ge1' Ge1' 6_555 . 9_555 62.56(6) ?
Ge1 Ge1' Ge1' 6_555 . 105_554 117.44(3) ?
Ge1 Ge1' Ge1' 6_555 . 10_555 62.56(6) ?
Ge1 Ge1' Ge1' 6_555 . 106_555 117.44(3) ?
Ge1 Ge1' Ge1 150_555 . 9_555 119.881(15) ?
Ge1 Ge1' Ge1 150_555 . 105_554 54.23(6) ?
Ge1 Ge1' Ge1 150_555 . 10_555 119.881(15) ?
Ge1 Ge1' Ge1 150_555 . 106_555 54.23(6) ?
Ge1 Ge1' Ge1' 150_555 . 5_555 94.86(5) ?
Ge1 Ge1' Ge1' 150_555 . 149_545 85.14(10) ?
Ge1 Ge1' Ge1' 150_555 . 6_555 175.14(11) ?
Ge1 Ge1' Ge1' 150_555 . 150_555 4.86(5) ?
Ge1 Ge1' Ge1' 150_555 . 9_555 122.72(3) ?
Ge1 Ge1' Ge1' 150_555 . 105_554 57.28(6) ?
Ge1 Ge1' Ge1' 150_555 . 10_555 122.72(3) ?
Ge1 Ge1' Ge1' 150_555 . 106_555 57.28(6) ?
Ge1 Ge1' Ge1 9_555 . 105_554 170.80(10) ?
Ge1 Ge1' Ge1 9_555 . 10_555 98.66(10) ?
Ge1 Ge1' Ge1 9_555 . 106_555 90.53(2) ?
Ge1 Ge1' Ge1' 9_555 . 5_555 62.56(6) ?
Ge1 Ge1' Ge1' 9_555 . 149_545 117.44(3) ?
Ge1 Ge1' Ge1' 9_555 . 6_555 62.56(6) ?
Ge1 Ge1' Ge1' 9_555 . 150_555 117.44(3) ?
Ge1 Ge1' Ge1' 9_555 . 9_555 4.33(5) ?
Ge1 Ge1' Ge1' 9_555 . 105_554 175.67(11) ?
Ge1 Ge1' Ge1' 9_555 . 10_555 94.33(11) ?
Ge1 Ge1' Ge1' 9_555 . 106_555 85.67(5) ?
Ge1 Ge1' Ge1 105_554 . 10_555 90.53(2) ?
Ge1 Ge1' Ge1 105_554 . 106_555 80.27(9) ?
Ge1 Ge1' Ge1' 105_554 . 5_555 122.72(3) ?
Ge1 Ge1' Ge1' 105_554 . 149_545 57.28(6) ?
Ge1 Ge1' Ge1' 105_554 . 6_555 122.72(3) ?
Ge1 Ge1' Ge1' 105_554 . 150_555 57.28(6) ?
Ge1 Ge1' Ge1' 105_554 . 9_555 175.14(11) ?
Ge1 Ge1' Ge1' 105_554 . 105_554 4.86(5) ?
Ge1 Ge1' Ge1' 105_554 . 10_555 94.86(5) ?
Ge1 Ge1' Ge1' 105_554 . 106_555 85.14(10) ?
Ge1 Ge1' Ge1 10_555 . 106_555 170.80(10) ?
Ge1 Ge1' Ge1' 10_555 . 5_555 62.56(6) ?
Ge1 Ge1' Ge1' 10_555 . 149_545 117.44(3) ?
Ge1 Ge1' Ge1' 10_555 . 6_555 62.56(6) ?
Ge1 Ge1' Ge1' 10_555 . 150_555 117.44(3) ?
Ge1 Ge1' Ge1' 10_555 . 9_555 94.33(11) ?
Ge1 Ge1' Ge1' 10_555 . 105_554 85.67(5) ?
Ge1 Ge1' Ge1' 10_555 . 10_555 4.33(5) ?
Ge1 Ge1' Ge1' 10_555 . 106_555 175.67(11) ?
Ge1 Ge1' Ge1' 106_555 . 5_555 122.72(3) ?
Ge1 Ge1' Ge1' 106_555 . 149_545 57.28(6) ?
Ge1 Ge1' Ge1' 106_555 . 6_555 122.72(3) ?
Ge1 Ge1' Ge1' 106_555 . 150_555 57.28(6) ?
Ge1 Ge1' Ge1' 106_555 . 9_555 94.86(5) ?
Ge1 Ge1' Ge1' 106_555 . 105_554 85.14(10) ?
Ge1 Ge1' Ge1' 106_555 . 10_555 175.14(11) ?
Ge1 Ge1' Ge1' 106_555 . 106_555 4.86(5) ?
Ge1' Ge1' Ge1' 5_555 . 149_545 180 ?
Ge1' Ge1' Ge1' 5_555 . 6_555 90.00(12) ?
Ge1' Ge1' Ge1' 5_555 . 150_555 90.00(7) ?
Ge1' Ge1' Ge1' 5_555 . 9_555 60.00(7) ?
Ge1' Ge1' Ge1' 5_555 . 105_554 120.00(4) ?
Ge1' Ge1' Ge1' 5_555 . 10_555 60.00(7) ?
Ge1' Ge1' Ge1' 5_555 . 106_555 120.00(4) ?
Ge1' Ge1' Ge1' 149_545 . 6_555 90.00(7) ?
Ge1' Ge1' Ge1' 149_545 . 150_555 90.00(11) ?
Ge1' Ge1' Ge1' 149_545 . 9_555 120.00(4) ?
Ge1' Ge1' Ge1' 149_545 . 105_554 60.00(7) ?
Ge1' Ge1' Ge1' 149_545 . 10_555 120.00(4) ?
Ge1' Ge1' Ge1' 149_545 . 106_555 60.00(7) ?
Ge1' Ge1' Ge1' 6_555 . 150_555 180 ?
Ge1' Ge1' Ge1' 6_555 . 9_555 60.00(7) ?
Ge1' Ge1' Ge1' 6_555 . 105_554 120.00(4) ?
Ge1' Ge1' Ge1' 6_555 . 10_555 60.00(7) ?
Ge1' Ge1' Ge1' 6_555 . 106_555 120.00(4) ?
Ge1' Ge1' Ge1' 150_555 . 9_555 120.00(4) ?
Ge1' Ge1' Ge1' 150_555 . 105_554 60.00(7) ?
Ge1' Ge1' Ge1' 150_555 . 10_555 120.00(4) ?
Ge1' Ge1' Ge1' 150_555 . 106_555 60.00(7) ?
Ge1' Ge1' Ge1' 9_555 . 105_554 180 ?
Ge1' Ge1' Ge1' 9_555 . 10_555 90.00(12) ?
Ge1' Ge1' Ge1' 9_555 . 106_555 90.00(7) ?
Ge1' Ge1' Ge1' 105_554 . 10_555 90.00(7) ?
Ge1' Ge1' Ge1' 105_554 . 106_555 90.00(11) ?
Ge1' Ge1' Ge1' 10_555 . 106_555 180 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 11. STRUCTURE-FACTOR LIST


_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Sm4MnGa86Ge34T293K
_database_code_depnum_ccdc_archive 'CCDC 2302495'
loop_
_audit_author_name
_audit_author_address
'Roman Khalaniya'
;Lomonosov Moscow State University
Russia
;
_audit_update_record             
;
2023-12-07 deposited with the CCDC.	2023-12-13 downloaded from the CCDC.
;
#=======================================================================

_audit_creation_method           'Jana2006 Version : 15/02/2021'

#=======================================================================

# 4. CHECKCIF RESPONSE 

# start Validation Reply Form

#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        Sm4MnGa8.6Ge3.4
_chemical_name_common            ?
_chemical_formula_moiety         'Sm4 Mn Ga8.6 Ge3.4'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'Ga8.6 Ge3.4 Mn1 Sm4'
_chemical_formula_weight         1502.8
_chemical_melting_point          ?
_chemical_compound_source        ?
_chemical_absolute_configuration .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'I m -3 m'
_symmetry_space_group_name_Hall  '-I 4;2;3'
_symmetry_Int_Tables_number      229

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -x,y,-z
4 x,-y,-z
5 z,x,y
6 z,-x,-y
7 -z,-x,y
8 -z,x,-y
9 y,z,x
10 -y,z,-x
11 y,-z,-x
12 -y,-z,x
13 y,x,-z
14 -y,-x,-z
15 y,-x,z
16 -y,x,z
17 x,z,-y
18 -x,z,y
19 -x,-z,-y
20 x,-z,y
21 z,y,-x
22 z,-y,x
23 -z,y,x
24 -z,-y,-x
25 -x,-y,-z
26 x,y,-z
27 x,-y,z
28 -x,y,z
29 -z,-x,-y
30 -z,x,y
31 z,x,-y
32 z,-x,y
33 -y,-z,-x
34 y,-z,x
35 -y,z,x
36 y,z,-x
37 -y,-x,z
38 y,x,z
39 -y,x,-z
40 y,-x,-z
41 -x,-z,y
42 x,-z,-y
43 x,z,y
44 -x,z,-y
45 -z,-y,x
46 -z,y,-x
47 z,-y,-x
48 z,y,x
49 x+1/2,y+1/2,z+1/2
50 -x+1/2,-y+1/2,z+1/2
51 -x+1/2,y+1/2,-z+1/2
52 x+1/2,-y+1/2,-z+1/2
53 z+1/2,x+1/2,y+1/2
54 z+1/2,-x+1/2,-y+1/2
55 -z+1/2,-x+1/2,y+1/2
56 -z+1/2,x+1/2,-y+1/2
57 y+1/2,z+1/2,x+1/2
58 -y+1/2,z+1/2,-x+1/2
59 y+1/2,-z+1/2,-x+1/2
60 -y+1/2,-z+1/2,x+1/2
61 y+1/2,x+1/2,-z+1/2
62 -y+1/2,-x+1/2,-z+1/2
63 y+1/2,-x+1/2,z+1/2
64 -y+1/2,x+1/2,z+1/2
65 x+1/2,z+1/2,-y+1/2
66 -x+1/2,z+1/2,y+1/2
67 -x+1/2,-z+1/2,-y+1/2
68 x+1/2,-z+1/2,y+1/2
69 z+1/2,y+1/2,-x+1/2
70 z+1/2,-y+1/2,x+1/2
71 -z+1/2,y+1/2,x+1/2
72 -z+1/2,-y+1/2,-x+1/2
73 -x+1/2,-y+1/2,-z+1/2
74 x+1/2,y+1/2,-z+1/2
75 x+1/2,-y+1/2,z+1/2
76 -x+1/2,y+1/2,z+1/2
77 -z+1/2,-x+1/2,-y+1/2
78 -z+1/2,x+1/2,y+1/2
79 z+1/2,x+1/2,-y+1/2
80 z+1/2,-x+1/2,y+1/2
81 -y+1/2,-z+1/2,-x+1/2
82 y+1/2,-z+1/2,x+1/2
83 -y+1/2,z+1/2,x+1/2
84 y+1/2,z+1/2,-x+1/2
85 -y+1/2,-x+1/2,z+1/2
86 y+1/2,x+1/2,z+1/2
87 -y+1/2,x+1/2,-z+1/2
88 y+1/2,-x+1/2,-z+1/2
89 -x+1/2,-z+1/2,y+1/2
90 x+1/2,-z+1/2,-y+1/2
91 x+1/2,z+1/2,y+1/2
92 -x+1/2,z+1/2,-y+1/2
93 -z+1/2,-y+1/2,x+1/2
94 -z+1/2,y+1/2,-x+1/2
95 z+1/2,-y+1/2,-x+1/2
96 z+1/2,y+1/2,x+1/2

_cell_length_a                   8.66770(10)
_cell_length_b                   8.66770(10)
_cell_length_c                   8.66770(10)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     651.196(13)

loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z            2

_cell_measurement_reflns_used    9227
_cell_measurement_theta_min      3.37
_cell_measurement_theta_max      33.55
_cell_measurement_temperature    293
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    7.6641
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             1297

_exptl_absorpt_coefficient_mu    43.757
_exptl_crystal_description       'rectangular cuboid'
_exptl_crystal_size_max          0.4
_exptl_crystal_size_mid          0.3
_exptl_crystal_size_min          0.2
_exptl_crystal_size_rad          ?
_exptl_crystal_colour            grey
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   
;
CrysAlisPro 1.171.41.123a (Rigaku Oxford Diffraction, 2022)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_correction_T_min  0.072
_exptl_absorpt_correction_T_max  1
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?

_diffrn_ambient_temperature      293
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_power             ?
_diffrn_source_voltage           ?
_diffrn_source_current           ?
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  mirror
_diffrn_measurement_device       ?
_diffrn_measurement_device_type  
'XtaLAB Synergy, Single source at home/near, HyPix'
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_measurement_method       'ω scans'
_diffrn_measurement_specimen_support ?

_diffrn_reflns_number            12575
_diffrn_reflns_theta_min         3.32
_diffrn_reflns_theta_max         33.58
_diffrn_reflns_theta_full        33.58
_diffrn_measured_fraction_theta_max 0.99
_diffrn_measured_fraction_theta_full 0.99
_diffrn_reflns_av_R_equivalents  0.079
_diffrn_reflns_av_unetI/netI     0.0087
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_reduction_process ?

_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?

_diffrn_radiation_probe          X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

_reflns_number_total             157
_reflns_number_gt                149
_reflns_threshold_expression     I>2σ(I)

_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0255
_refine_ls_wR_factor_gt          0.0292
_refine_ls_R_factor_all          0.0266
_refine_ls_wR_factor_ref         0.0294
_refine_ls_goodness_of_fit_ref   1.08
_refine_ls_goodness_of_fit_gt    1.10
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         157
_refine_ls_number_parameters     19
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.000625F²)
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0223
_refine_ls_shift/su_mean         0.0023
_refine_diff_density_max         1.63
_refine_diff_density_min         -1.88
_refine_ls_extinction_method     
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef       870(40)
_refine_ls_extinction_expression ?
_refine_ls_abs_structure_details ?
_refine_ls_abs_structure_Flack   ?
_refine_ls_abs_structure_Rogers  ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga 0.2307 1.6083 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Ge 0.1547 1.8001 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.3368 0.7283 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Sm -0.1638 3.4418 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       'CrysAlisPro 1.171.41.123a (Rigaku OD, 2022)'
_computing_cell_refinement       'CrysAlisPro 1.171.41.123a (Rigaku OD, 2022)'
_computing_data_reduction        'CrysAlisPro 1.171.41.123a (Rigaku OD, 2022)'
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?

loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?

loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?

loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sm1 Sm 0.25 0.25 0.25 Uani 0.0104(5) 8 1 d . . .
Mn1 Mn 0 0 0 Uani 0.0089(3) 2 1 d . . .
Ga1 Ga 0.5 0 0.25 Uani 0.0126(4) 12 0.7167 d . . .
Ge1 Ge 0.5 0 0.25 Uani 0.0126(4) 12 0.2833 d . . .
Ga2 Ga 0.2917(3) 0 0 Uani 0.0116(4) 12 0.7167 d . . .
Ge2 Ge 0.2917(3) 0 0 Uani 0.0116(4) 12 0.2833 d . . .


loop_
_jana_atom_site_ADP_C_label
_jana_atom_site_ADP_C_type_symbol
_jana_atom_site_ADP_C_111
_jana_atom_site_ADP_C_112
_jana_atom_site_ADP_C_113
_jana_atom_site_ADP_C_122
_jana_atom_site_ADP_C_123
_jana_atom_site_ADP_C_133
_jana_atom_site_ADP_C_222
_jana_atom_site_ADP_C_223
_jana_atom_site_ADP_C_233
_jana_atom_site_ADP_C_333
Sm1 Sm 0 0 0 0 0 0 0 0 0 0
Ga1 Ga 0 0 0.00032(11) 0 0 0 0 -0.00032(11) 0 0
Ge1 Ge 0 0 0.00032(11) 0 0 0 0 -0.00032(11) 0 0
Ga2 Ga 0.0010(4) 0 0 -0.00057(17) 0 -0.00057(17) 0 0 0 0
Ge2 Ge 0.0010(4) 0 0 -0.00057(17) 0 -0.00057(17) 0 0 0 0

loop_
_jana_atom_site_ADP_D_label
_jana_atom_site_ADP_D_type_symbol
_jana_atom_site_ADP_D_1111
_jana_atom_site_ADP_D_1112
_jana_atom_site_ADP_D_1113
_jana_atom_site_ADP_D_1122
_jana_atom_site_ADP_D_1123
_jana_atom_site_ADP_D_1133
_jana_atom_site_ADP_D_1222
_jana_atom_site_ADP_D_1223
_jana_atom_site_ADP_D_1233
_jana_atom_site_ADP_D_1333
_jana_atom_site_ADP_D_2222
_jana_atom_site_ADP_D_2223
_jana_atom_site_ADP_D_2233
_jana_atom_site_ADP_D_2333
_jana_atom_site_ADP_D_3333
Sm1 Sm 0.0006(2) 0 0 0.00014(7) -0.00005(2) 0.00014(7) 0 -0.00005(2)
-0.00005(2) 0 0.0006(2) 0 0.00014(7) 0 0.0006(2)
Ga1 Ga 0.0009(3) 0 0 0 0 0 0 0 0 0 0.0009(3) 0 0 0 0
Ge1 Ge 0.0009(3) 0 0 0 0 0 0 0 0 0 0.0009(3) 0 0 0 0
Ga2 Ga 0 0 0 0.00019(9) 0 0.00019(9) 0 0 0 0 0.0005(3) 0 0 0 0.0005(3)
Ge2 Ge 0 0 0 0.00019(9) 0 0.00019(9) 0 0 0 0 0.0005(3) 0 0 0 0.0005(3)


loop_
_jana_atom_site_ADP_E_label
_jana_atom_site_ADP_E_type_symbol
_jana_atom_site_ADP_E_11111
_jana_atom_site_ADP_E_11112
_jana_atom_site_ADP_E_11113
_jana_atom_site_ADP_E_11122
_jana_atom_site_ADP_E_11123
_jana_atom_site_ADP_E_11133
_jana_atom_site_ADP_E_11222
_jana_atom_site_ADP_E_11223
_jana_atom_site_ADP_E_11233
_jana_atom_site_ADP_E_11333
_jana_atom_site_ADP_E_12222
_jana_atom_site_ADP_E_12223
_jana_atom_site_ADP_E_12233
_jana_atom_site_ADP_E_12333
_jana_atom_site_ADP_E_13333
_jana_atom_site_ADP_E_22222
_jana_atom_site_ADP_E_22223
_jana_atom_site_ADP_E_22233
_jana_atom_site_ADP_E_22333
_jana_atom_site_ADP_E_23333
_jana_atom_site_ADP_E_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_F_label
_jana_atom_site_ADP_F_type_symbol
_jana_atom_site_ADP_F_111111
_jana_atom_site_ADP_F_111112
_jana_atom_site_ADP_F_111113
_jana_atom_site_ADP_F_111122
_jana_atom_site_ADP_F_111123
_jana_atom_site_ADP_F_111133
_jana_atom_site_ADP_F_111222
_jana_atom_site_ADP_F_111223
_jana_atom_site_ADP_F_111233
_jana_atom_site_ADP_F_111333
_jana_atom_site_ADP_F_112222
_jana_atom_site_ADP_F_112223
_jana_atom_site_ADP_F_112233
_jana_atom_site_ADP_F_112333
_jana_atom_site_ADP_F_113333
_jana_atom_site_ADP_F_122222
_jana_atom_site_ADP_F_122223
_jana_atom_site_ADP_F_122233
_jana_atom_site_ADP_F_122333
_jana_atom_site_ADP_F_123333
_jana_atom_site_ADP_F_133333
_jana_atom_site_ADP_F_222222
_jana_atom_site_ADP_F_222223
_jana_atom_site_ADP_F_222233
_jana_atom_site_ADP_F_222333
_jana_atom_site_ADP_F_223333
_jana_atom_site_ADP_F_233333
_jana_atom_site_ADP_F_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sm1 Mn1 . . 3.75322(5) ?
Sm1 Mn1 . 49_555 3.75322(5) ?
Sm1 Ga1 . . 3.06449(5) ?
Sm1 Ga1 . 51_555 3.06449(5) ?
Sm1 Ga1 . 5_555 3.06449(5) ?
Sm1 Ga1 . 55_555 3.06449(5) ?
Sm1 Ga1 . 9_555 3.06449(5) ?
Sm1 Ga1 . 59_555 3.06449(5) ?
Sm1 Ge1 . . 3.06449(5) ?
Sm1 Ge1 . 51_555 3.06449(5) ?
Sm1 Ge1 . 5_555 3.06449(5) ?
Sm1 Ge1 . 55_555 3.06449(5) ?
Sm1 Ge1 . 9_555 3.06449(5) ?
Sm1 Ge1 . 59_555 3.06449(5) ?
Sm1 Ga2 . . 3.0857(3) ?
Sm1 Ga2 . 50_555 3.0857(3) ?
Sm1 Ga2 . 5_555 3.0857(3) ?
Sm1 Ga2 . 54_555 3.0857(3) ?
Sm1 Ga2 . 9_555 3.0857(3) ?
Sm1 Ga2 . 58_555 3.0857(3) ?
Sm1 Ge2 . . 3.0857(3) ?
Sm1 Ge2 . 50_555 3.0857(3) ?
Sm1 Ge2 . 5_555 3.0857(3) ?
Sm1 Ge2 . 54_555 3.0857(3) ?
Sm1 Ge2 . 9_555 3.0857(3) ?
Sm1 Ge2 . 58_555 3.0857(3) ?
Mn1 Ga2 . . 2.528(2) ?
Mn1 Ga2 . 2_555 2.528(2) ?
Mn1 Ga2 . 5_555 2.528(2) ?
Mn1 Ga2 . 6_555 2.528(2) ?
Mn1 Ga2 . 9_555 2.528(2) ?
Mn1 Ga2 . 10_555 2.528(2) ?
Mn1 Ge2 . . 2.528(2) ?
Mn1 Ge2 . 2_555 2.528(2) ?
Mn1 Ge2 . 5_555 2.528(2) ?
Mn1 Ge2 . 6_555 2.528(2) ?
Mn1 Ge2 . 9_555 2.528(2) ?
Mn1 Ge2 . 10_555 2.528(2) ?
Ga1 Ga1 . 53_545 3.06449(5) ?
Ga1 Ga1 . 55_555 3.06449(5) ?
Ga1 Ga1 . 57_544 3.06449(5) ?
Ga1 Ga1 . 59_555 3.06449(5) ?
Ga1 Ge1 . 53_545 3.06449(5) ?
Ga1 Ge1 . 55_555 3.06449(5) ?
Ga1 Ge1 . 57_544 3.06449(5) ?
Ga1 Ge1 . 59_555 3.06449(5) ?
Ga1 Ga2 . . 2.8206(15) ?
Ga1 Ga2 . 2_655 2.8206(15) ?
Ga1 Ga2 . 53_545 2.8206(15) ?
Ga1 Ga2 . 54_555 2.8206(15) ?
Ga1 Ge2 . . 2.8206(15) ?
Ga1 Ge2 . 2_655 2.8206(15) ?
Ga1 Ge2 . 53_545 2.8206(15) ?
Ga1 Ge2 . 54_555 2.8206(15) ?
Ge1 Ge1 . 53_545 3.06449(5) ?
Ge1 Ge1 . 55_555 3.06449(5) ?
Ge1 Ge1 . 57_544 3.06449(5) ?
Ge1 Ge1 . 59_555 3.06449(5) ?
Ge1 Ga2 . . 2.8206(15) ?
Ge1 Ga2 . 2_655 2.8206(15) ?
Ge1 Ga2 . 53_545 2.8206(15) ?
Ge1 Ga2 . 54_555 2.8206(15) ?
Ge1 Ge2 . . 2.8206(15) ?
Ge1 Ge2 . 2_655 2.8206(15) ?
Ge1 Ge2 . 53_545 2.8206(15) ?
Ge1 Ge2 . 54_555 2.8206(15) ?
Ga2 Ga2 . 2_655 3.611(3) ?
Ga2 Ga2 . 5_555 3.575(2) ?
Ga2 Ga2 . 6_555 3.575(2) ?
Ga2 Ga2 . 9_555 3.575(2) ?
Ga2 Ga2 . 10_555 3.575(2) ?
Ga2 Ge2 . 2_655 3.611(3) ?
Ga2 Ge2 . 5_555 3.575(2) ?
Ga2 Ge2 . 6_555 3.575(2) ?
Ga2 Ge2 . 9_555 3.575(2) ?
Ga2 Ge2 . 10_555 3.575(2) ?
Ge2 Ge2 . 2_655 3.611(3) ?
Ge2 Ge2 . 5_555 3.575(2) ?
Ge2 Ge2 . 6_555 3.575(2) ?
Ge2 Ge2 . 9_555 3.575(2) ?
Ge2 Ge2 . 10_555 3.575(2) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Mn1 Sm1 Mn1 . . 49_555 180 ?
Mn1 Sm1 Ga1 . . . 90.0000(8) ?
Mn1 Sm1 Ga1 . . 51_555 90.0000(8) ?
Mn1 Sm1 Ga1 . . 5_555 90.0000(8) ?
Mn1 Sm1 Ga1 . . 55_555 90.0000(8) ?
Mn1 Sm1 Ga1 . . 9_555 90.0000(8) ?
Mn1 Sm1 Ga1 . . 59_555 90.0000(8) ?
Mn1 Sm1 Ge1 . . . 90.0000(8) ?
Mn1 Sm1 Ge1 . . 51_555 90.0000(8) ?
Mn1 Sm1 Ge1 . . 5_555 90.0000(8) ?
Mn1 Sm1 Ge1 . . 55_555 90.0000(8) ?
Mn1 Sm1 Ge1 . . 9_555 90.0000(8) ?
Mn1 Sm1 Ge1 . . 59_555 90.0000(8) ?
Mn1 Sm1 Ga2 . . . 41.99(4) ?
Mn1 Sm1 Ga2 . . 50_555 138.01(4) ?
Mn1 Sm1 Ga2 . . 5_555 41.99(4) ?
Mn1 Sm1 Ga2 . . 54_555 138.01(4) ?
Mn1 Sm1 Ga2 . . 9_555 41.99(4) ?
Mn1 Sm1 Ga2 . . 58_555 138.01(4) ?
Mn1 Sm1 Ge2 . . . 41.99(4) ?
Mn1 Sm1 Ge2 . . 50_555 138.01(4) ?
Mn1 Sm1 Ge2 . . 5_555 41.99(4) ?
Mn1 Sm1 Ge2 . . 54_555 138.01(4) ?
Mn1 Sm1 Ge2 . . 9_555 41.99(4) ?
Mn1 Sm1 Ge2 . . 58_555 138.01(4) ?
Mn1 Sm1 Ga1 49_555 . . 90.0000(8) ?
Mn1 Sm1 Ga1 49_555 . 51_555 90.0000(8) ?
Mn1 Sm1 Ga1 49_555 . 5_555 90.0000(8) ?
Mn1 Sm1 Ga1 49_555 . 55_555 90.0000(8) ?
Mn1 Sm1 Ga1 49_555 . 9_555 90.0000(8) ?
Mn1 Sm1 Ga1 49_555 . 59_555 90.0000(8) ?
Mn1 Sm1 Ge1 49_555 . . 90.0000(8) ?
Mn1 Sm1 Ge1 49_555 . 51_555 90.0000(8) ?
Mn1 Sm1 Ge1 49_555 . 5_555 90.0000(8) ?
Mn1 Sm1 Ge1 49_555 . 55_555 90.0000(8) ?
Mn1 Sm1 Ge1 49_555 . 9_555 90.0000(8) ?
Mn1 Sm1 Ge1 49_555 . 59_555 90.0000(8) ?
Mn1 Sm1 Ga2 49_555 . . 138.01(4) ?
Mn1 Sm1 Ga2 49_555 . 50_555 41.99(4) ?
Mn1 Sm1 Ga2 49_555 . 5_555 138.01(4) ?
Mn1 Sm1 Ga2 49_555 . 54_555 41.99(4) ?
Mn1 Sm1 Ga2 49_555 . 9_555 138.01(4) ?
Mn1 Sm1 Ga2 49_555 . 58_555 41.99(4) ?
Mn1 Sm1 Ge2 49_555 . . 138.01(4) ?
Mn1 Sm1 Ge2 49_555 . 50_555 41.99(4) ?
Mn1 Sm1 Ge2 49_555 . 5_555 138.01(4) ?
Mn1 Sm1 Ge2 49_555 . 54_555 41.99(4) ?
Mn1 Sm1 Ge2 49_555 . 9_555 138.01(4) ?
Mn1 Sm1 Ge2 49_555 . 58_555 41.99(4) ?
Ga1 Sm1 Ga1 . . 51_555 180 ?
Ga1 Sm1 Ga1 . . 5_555 120.0000(5) ?
Ga1 Sm1 Ga1 . . 55_555 60.0000(5) ?
Ga1 Sm1 Ga1 . . 9_555 120.0000(5) ?
Ga1 Sm1 Ga1 . . 59_555 60.0000(5) ?
Ga1 Sm1 Ge1 . . . 0 ?
Ga1 Sm1 Ge1 . . 51_555 180 ?
Ga1 Sm1 Ge1 . . 5_555 120.0000(5) ?
Ga1 Sm1 Ge1 . . 55_555 60.0000(5) ?
Ga1 Sm1 Ge1 . . 9_555 120.0000(5) ?
Ga1 Sm1 Ge1 . . 59_555 60.0000(5) ?
Ga1 Sm1 Ga2 . . . 54.59(3) ?
Ga1 Sm1 Ga2 . . 50_555 125.41(3) ?
Ga1 Sm1 Ga2 . . 5_555 125.41(3) ?
Ga1 Sm1 Ga2 . . 54_555 54.59(3) ?
Ga1 Sm1 Ga2 . . 9_555 90.0000(9) ?
Ga1 Sm1 Ga2 . . 58_555 90.0000(9) ?
Ga1 Sm1 Ge2 . . . 54.59(3) ?
Ga1 Sm1 Ge2 . . 50_555 125.41(3) ?
Ga1 Sm1 Ge2 . . 5_555 125.41(3) ?
Ga1 Sm1 Ge2 . . 54_555 54.59(3) ?
Ga1 Sm1 Ge2 . . 9_555 90.0000(9) ?
Ga1 Sm1 Ge2 . . 58_555 90.0000(9) ?
Ga1 Sm1 Ga1 51_555 . 5_555 60.0000(5) ?
Ga1 Sm1 Ga1 51_555 . 55_555 120.0000(5) ?
Ga1 Sm1 Ga1 51_555 . 9_555 60.0000(5) ?
Ga1 Sm1 Ga1 51_555 . 59_555 120.0000(5) ?
Ga1 Sm1 Ge1 51_555 . . 180 ?
Ga1 Sm1 Ge1 51_555 . 51_555 0 ?
Ga1 Sm1 Ge1 51_555 . 5_555 60.0000(5) ?
Ga1 Sm1 Ge1 51_555 . 55_555 120.0000(5) ?
Ga1 Sm1 Ge1 51_555 . 9_555 60.0000(5) ?
Ga1 Sm1 Ge1 51_555 . 59_555 120.0000(5) ?
Ga1 Sm1 Ga2 51_555 . . 125.41(3) ?
Ga1 Sm1 Ga2 51_555 . 50_555 54.59(3) ?
Ga1 Sm1 Ga2 51_555 . 5_555 54.59(3) ?
Ga1 Sm1 Ga2 51_555 . 54_555 125.41(3) ?
Ga1 Sm1 Ga2 51_555 . 9_555 90.0000(9) ?
Ga1 Sm1 Ga2 51_555 . 58_555 90.0000(9) ?
Ga1 Sm1 Ge2 51_555 . . 125.41(3) ?
Ga1 Sm1 Ge2 51_555 . 50_555 54.59(3) ?
Ga1 Sm1 Ge2 51_555 . 5_555 54.59(3) ?
Ga1 Sm1 Ge2 51_555 . 54_555 125.41(3) ?
Ga1 Sm1 Ge2 51_555 . 9_555 90.0000(9) ?
Ga1 Sm1 Ge2 51_555 . 58_555 90.0000(9) ?
Ga1 Sm1 Ga1 5_555 . 55_555 180 ?
Ga1 Sm1 Ga1 5_555 . 9_555 120.0000(5) ?
Ga1 Sm1 Ga1 5_555 . 59_555 60.0000(5) ?
Ga1 Sm1 Ge1 5_555 . . 120.0000(5) ?
Ga1 Sm1 Ge1 5_555 . 51_555 60.0000(5) ?
Ga1 Sm1 Ge1 5_555 . 5_555 0 ?
Ga1 Sm1 Ge1 5_555 . 55_555 180 ?
Ga1 Sm1 Ge1 5_555 . 9_555 120.0000(5) ?
Ga1 Sm1 Ge1 5_555 . 59_555 60.0000(5) ?
Ga1 Sm1 Ga2 5_555 . . 90.0000(9) ?
Ga1 Sm1 Ga2 5_555 . 50_555 90.0000(9) ?
Ga1 Sm1 Ga2 5_555 . 5_555 54.59(3) ?
Ga1 Sm1 Ga2 5_555 . 54_555 125.41(3) ?
Ga1 Sm1 Ga2 5_555 . 9_555 125.41(3) ?
Ga1 Sm1 Ga2 5_555 . 58_555 54.59(3) ?
Ga1 Sm1 Ge2 5_555 . . 90.0000(9) ?
Ga1 Sm1 Ge2 5_555 . 50_555 90.0000(9) ?
Ga1 Sm1 Ge2 5_555 . 5_555 54.59(3) ?
Ga1 Sm1 Ge2 5_555 . 54_555 125.41(3) ?
Ga1 Sm1 Ge2 5_555 . 9_555 125.41(3) ?
Ga1 Sm1 Ge2 5_555 . 58_555 54.59(3) ?
Ga1 Sm1 Ga1 55_555 . 9_555 60.0000(5) ?
Ga1 Sm1 Ga1 55_555 . 59_555 120.0000(5) ?
Ga1 Sm1 Ge1 55_555 . . 60.0000(5) ?
Ga1 Sm1 Ge1 55_555 . 51_555 120.0000(5) ?
Ga1 Sm1 Ge1 55_555 . 5_555 180 ?
Ga1 Sm1 Ge1 55_555 . 55_555 0 ?
Ga1 Sm1 Ge1 55_555 . 9_555 60.0000(5) ?
Ga1 Sm1 Ge1 55_555 . 59_555 120.0000(5) ?
Ga1 Sm1 Ga2 55_555 . . 90.0000(9) ?
Ga1 Sm1 Ga2 55_555 . 50_555 90.0000(9) ?
Ga1 Sm1 Ga2 55_555 . 5_555 125.41(3) ?
Ga1 Sm1 Ga2 55_555 . 54_555 54.59(3) ?
Ga1 Sm1 Ga2 55_555 . 9_555 54.59(3) ?
Ga1 Sm1 Ga2 55_555 . 58_555 125.41(3) ?
Ga1 Sm1 Ge2 55_555 . . 90.0000(9) ?
Ga1 Sm1 Ge2 55_555 . 50_555 90.0000(9) ?
Ga1 Sm1 Ge2 55_555 . 5_555 125.41(3) ?
Ga1 Sm1 Ge2 55_555 . 54_555 54.59(3) ?
Ga1 Sm1 Ge2 55_555 . 9_555 54.59(3) ?
Ga1 Sm1 Ge2 55_555 . 58_555 125.41(3) ?
Ga1 Sm1 Ga1 9_555 . 59_555 180 ?
Ga1 Sm1 Ge1 9_555 . . 120.0000(5) ?
Ga1 Sm1 Ge1 9_555 . 51_555 60.0000(5) ?
Ga1 Sm1 Ge1 9_555 . 5_555 120.0000(5) ?
Ga1 Sm1 Ge1 9_555 . 55_555 60.0000(5) ?
Ga1 Sm1 Ge1 9_555 . 9_555 0 ?
Ga1 Sm1 Ge1 9_555 . 59_555 180 ?
Ga1 Sm1 Ga2 9_555 . . 125.41(3) ?
Ga1 Sm1 Ga2 9_555 . 50_555 54.59(3) ?
Ga1 Sm1 Ga2 9_555 . 5_555 90.0000(9) ?
Ga1 Sm1 Ga2 9_555 . 54_555 90.0000(9) ?
Ga1 Sm1 Ga2 9_555 . 9_555 54.59(3) ?
Ga1 Sm1 Ga2 9_555 . 58_555 125.41(3) ?
Ga1 Sm1 Ge2 9_555 . . 125.41(3) ?
Ga1 Sm1 Ge2 9_555 . 50_555 54.59(3) ?
Ga1 Sm1 Ge2 9_555 . 5_555 90.0000(9) ?
Ga1 Sm1 Ge2 9_555 . 54_555 90.0000(9) ?
Ga1 Sm1 Ge2 9_555 . 9_555 54.59(3) ?
Ga1 Sm1 Ge2 9_555 . 58_555 125.41(3) ?
Ga1 Sm1 Ge1 59_555 . . 60.0000(5) ?
Ga1 Sm1 Ge1 59_555 . 51_555 120.0000(5) ?
Ga1 Sm1 Ge1 59_555 . 5_555 60.0000(5) ?
Ga1 Sm1 Ge1 59_555 . 55_555 120.0000(5) ?
Ga1 Sm1 Ge1 59_555 . 9_555 180 ?
Ga1 Sm1 Ge1 59_555 . 59_555 0 ?
Ga1 Sm1 Ga2 59_555 . . 54.59(3) ?
Ga1 Sm1 Ga2 59_555 . 50_555 125.41(3) ?
Ga1 Sm1 Ga2 59_555 . 5_555 90.0000(9) ?
Ga1 Sm1 Ga2 59_555 . 54_555 90.0000(9) ?
Ga1 Sm1 Ga2 59_555 . 9_555 125.41(3) ?
Ga1 Sm1 Ga2 59_555 . 58_555 54.59(3) ?
Ga1 Sm1 Ge2 59_555 . . 54.59(3) ?
Ga1 Sm1 Ge2 59_555 . 50_555 125.41(3) ?
Ga1 Sm1 Ge2 59_555 . 5_555 90.0000(9) ?
Ga1 Sm1 Ge2 59_555 . 54_555 90.0000(9) ?
Ga1 Sm1 Ge2 59_555 . 9_555 125.41(3) ?
Ga1 Sm1 Ge2 59_555 . 58_555 54.59(3) ?
Ge1 Sm1 Ge1 . . 51_555 180 ?
Ge1 Sm1 Ge1 . . 5_555 120.0000(5) ?
Ge1 Sm1 Ge1 . . 55_555 60.0000(5) ?
Ge1 Sm1 Ge1 . . 9_555 120.0000(5) ?
Ge1 Sm1 Ge1 . . 59_555 60.0000(5) ?
Ge1 Sm1 Ga2 . . . 54.59(3) ?
Ge1 Sm1 Ga2 . . 50_555 125.41(3) ?
Ge1 Sm1 Ga2 . . 5_555 125.41(3) ?
Ge1 Sm1 Ga2 . . 54_555 54.59(3) ?
Ge1 Sm1 Ga2 . . 9_555 90.0000(9) ?
Ge1 Sm1 Ga2 . . 58_555 90.0000(9) ?
Ge1 Sm1 Ge2 . . . 54.59(3) ?
Ge1 Sm1 Ge2 . . 50_555 125.41(3) ?
Ge1 Sm1 Ge2 . . 5_555 125.41(3) ?
Ge1 Sm1 Ge2 . . 54_555 54.59(3) ?
Ge1 Sm1 Ge2 . . 9_555 90.0000(9) ?
Ge1 Sm1 Ge2 . . 58_555 90.0000(9) ?
Ge1 Sm1 Ge1 51_555 . 5_555 60.0000(5) ?
Ge1 Sm1 Ge1 51_555 . 55_555 120.0000(5) ?
Ge1 Sm1 Ge1 51_555 . 9_555 60.0000(5) ?
Ge1 Sm1 Ge1 51_555 . 59_555 120.0000(5) ?
Ge1 Sm1 Ga2 51_555 . . 125.41(3) ?
Ge1 Sm1 Ga2 51_555 . 50_555 54.59(3) ?
Ge1 Sm1 Ga2 51_555 . 5_555 54.59(3) ?
Ge1 Sm1 Ga2 51_555 . 54_555 125.41(3) ?
Ge1 Sm1 Ga2 51_555 . 9_555 90.0000(9) ?
Ge1 Sm1 Ga2 51_555 . 58_555 90.0000(9) ?
Ge1 Sm1 Ge2 51_555 . . 125.41(3) ?
Ge1 Sm1 Ge2 51_555 . 50_555 54.59(3) ?
Ge1 Sm1 Ge2 51_555 . 5_555 54.59(3) ?
Ge1 Sm1 Ge2 51_555 . 54_555 125.41(3) ?
Ge1 Sm1 Ge2 51_555 . 9_555 90.0000(9) ?
Ge1 Sm1 Ge2 51_555 . 58_555 90.0000(9) ?
Ge1 Sm1 Ge1 5_555 . 55_555 180 ?
Ge1 Sm1 Ge1 5_555 . 9_555 120.0000(5) ?
Ge1 Sm1 Ge1 5_555 . 59_555 60.0000(5) ?
Ge1 Sm1 Ga2 5_555 . . 90.0000(9) ?
Ge1 Sm1 Ga2 5_555 . 50_555 90.0000(9) ?
Ge1 Sm1 Ga2 5_555 . 5_555 54.59(3) ?
Ge1 Sm1 Ga2 5_555 . 54_555 125.41(3) ?
Ge1 Sm1 Ga2 5_555 . 9_555 125.41(3) ?
Ge1 Sm1 Ga2 5_555 . 58_555 54.59(3) ?
Ge1 Sm1 Ge2 5_555 . . 90.0000(9) ?
Ge1 Sm1 Ge2 5_555 . 50_555 90.0000(9) ?
Ge1 Sm1 Ge2 5_555 . 5_555 54.59(3) ?
Ge1 Sm1 Ge2 5_555 . 54_555 125.41(3) ?
Ge1 Sm1 Ge2 5_555 . 9_555 125.41(3) ?
Ge1 Sm1 Ge2 5_555 . 58_555 54.59(3) ?
Ge1 Sm1 Ge1 55_555 . 9_555 60.0000(5) ?
Ge1 Sm1 Ge1 55_555 . 59_555 120.0000(5) ?
Ge1 Sm1 Ga2 55_555 . . 90.0000(9) ?
Ge1 Sm1 Ga2 55_555 . 50_555 90.0000(9) ?
Ge1 Sm1 Ga2 55_555 . 5_555 125.41(3) ?
Ge1 Sm1 Ga2 55_555 . 54_555 54.59(3) ?
Ge1 Sm1 Ga2 55_555 . 9_555 54.59(3) ?
Ge1 Sm1 Ga2 55_555 . 58_555 125.41(3) ?
Ge1 Sm1 Ge2 55_555 . . 90.0000(9) ?
Ge1 Sm1 Ge2 55_555 . 50_555 90.0000(9) ?
Ge1 Sm1 Ge2 55_555 . 5_555 125.41(3) ?
Ge1 Sm1 Ge2 55_555 . 54_555 54.59(3) ?
Ge1 Sm1 Ge2 55_555 . 9_555 54.59(3) ?
Ge1 Sm1 Ge2 55_555 . 58_555 125.41(3) ?
Ge1 Sm1 Ge1 9_555 . 59_555 180 ?
Ge1 Sm1 Ga2 9_555 . . 125.41(3) ?
Ge1 Sm1 Ga2 9_555 . 50_555 54.59(3) ?
Ge1 Sm1 Ga2 9_555 . 5_555 90.0000(9) ?
Ge1 Sm1 Ga2 9_555 . 54_555 90.0000(9) ?
Ge1 Sm1 Ga2 9_555 . 9_555 54.59(3) ?
Ge1 Sm1 Ga2 9_555 . 58_555 125.41(3) ?
Ge1 Sm1 Ge2 9_555 . . 125.41(3) ?
Ge1 Sm1 Ge2 9_555 . 50_555 54.59(3) ?
Ge1 Sm1 Ge2 9_555 . 5_555 90.0000(9) ?
Ge1 Sm1 Ge2 9_555 . 54_555 90.0000(9) ?
Ge1 Sm1 Ge2 9_555 . 9_555 54.59(3) ?
Ge1 Sm1 Ge2 9_555 . 58_555 125.41(3) ?
Ge1 Sm1 Ga2 59_555 . . 54.59(3) ?
Ge1 Sm1 Ga2 59_555 . 50_555 125.41(3) ?
Ge1 Sm1 Ga2 59_555 . 5_555 90.0000(9) ?
Ge1 Sm1 Ga2 59_555 . 54_555 90.0000(9) ?
Ge1 Sm1 Ga2 59_555 . 9_555 125.41(3) ?
Ge1 Sm1 Ga2 59_555 . 58_555 54.59(3) ?
Ge1 Sm1 Ge2 59_555 . . 54.59(3) ?
Ge1 Sm1 Ge2 59_555 . 50_555 125.41(3) ?
Ge1 Sm1 Ge2 59_555 . 5_555 90.0000(9) ?
Ge1 Sm1 Ge2 59_555 . 54_555 90.0000(9) ?
Ge1 Sm1 Ge2 59_555 . 9_555 125.41(3) ?
Ge1 Sm1 Ge2 59_555 . 58_555 54.59(3) ?
Ga2 Sm1 Ga2 . . 50_555 180 ?
Ga2 Sm1 Ga2 . . 5_555 70.81(5) ?
Ga2 Sm1 Ga2 . . 54_555 109.19(5) ?
Ga2 Sm1 Ga2 . . 9_555 70.81(5) ?
Ga2 Sm1 Ga2 . . 58_555 109.19(5) ?
Ga2 Sm1 Ge2 . . . 0 ?
Ga2 Sm1 Ge2 . . 50_555 180 ?
Ga2 Sm1 Ge2 . . 5_555 70.81(5) ?
Ga2 Sm1 Ge2 . . 54_555 109.19(5) ?
Ga2 Sm1 Ge2 . . 9_555 70.81(5) ?
Ga2 Sm1 Ge2 . . 58_555 109.19(5) ?
Ga2 Sm1 Ga2 50_555 . 5_555 109.19(5) ?
Ga2 Sm1 Ga2 50_555 . 54_555 70.81(5) ?
Ga2 Sm1 Ga2 50_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ga2 50_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ge2 50_555 . . 180 ?
Ga2 Sm1 Ge2 50_555 . 50_555 0 ?
Ga2 Sm1 Ge2 50_555 . 5_555 109.19(5) ?
Ga2 Sm1 Ge2 50_555 . 54_555 70.81(5) ?
Ga2 Sm1 Ge2 50_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ge2 50_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ga2 5_555 . 54_555 180 ?
Ga2 Sm1 Ga2 5_555 . 9_555 70.81(5) ?
Ga2 Sm1 Ga2 5_555 . 58_555 109.19(5) ?
Ga2 Sm1 Ge2 5_555 . . 70.81(5) ?
Ga2 Sm1 Ge2 5_555 . 50_555 109.19(5) ?
Ga2 Sm1 Ge2 5_555 . 5_555 0 ?
Ga2 Sm1 Ge2 5_555 . 54_555 180 ?
Ga2 Sm1 Ge2 5_555 . 9_555 70.81(5) ?
Ga2 Sm1 Ge2 5_555 . 58_555 109.19(5) ?
Ga2 Sm1 Ga2 54_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ga2 54_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ge2 54_555 . . 109.19(5) ?
Ga2 Sm1 Ge2 54_555 . 50_555 70.81(5) ?
Ga2 Sm1 Ge2 54_555 . 5_555 180 ?
Ga2 Sm1 Ge2 54_555 . 54_555 0 ?
Ga2 Sm1 Ge2 54_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ge2 54_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ga2 9_555 . 58_555 180 ?
Ga2 Sm1 Ge2 9_555 . . 70.81(5) ?
Ga2 Sm1 Ge2 9_555 . 50_555 109.19(5) ?
Ga2 Sm1 Ge2 9_555 . 5_555 70.81(5) ?
Ga2 Sm1 Ge2 9_555 . 54_555 109.19(5) ?
Ga2 Sm1 Ge2 9_555 . 9_555 0 ?
Ga2 Sm1 Ge2 9_555 . 58_555 180 ?
Ga2 Sm1 Ge2 58_555 . . 109.19(5) ?
Ga2 Sm1 Ge2 58_555 . 50_555 70.81(5) ?
Ga2 Sm1 Ge2 58_555 . 5_555 109.19(5) ?
Ga2 Sm1 Ge2 58_555 . 54_555 70.81(5) ?
Ga2 Sm1 Ge2 58_555 . 9_555 180 ?
Ga2 Sm1 Ge2 58_555 . 58_555 0 ?
Ge2 Sm1 Ge2 . . 50_555 180 ?
Ge2 Sm1 Ge2 . . 5_555 70.81(5) ?
Ge2 Sm1 Ge2 . . 54_555 109.19(5) ?
Ge2 Sm1 Ge2 . . 9_555 70.81(5) ?
Ge2 Sm1 Ge2 . . 58_555 109.19(5) ?
Ge2 Sm1 Ge2 50_555 . 5_555 109.19(5) ?
Ge2 Sm1 Ge2 50_555 . 54_555 70.81(5) ?
Ge2 Sm1 Ge2 50_555 . 9_555 109.19(5) ?
Ge2 Sm1 Ge2 50_555 . 58_555 70.81(5) ?
Ge2 Sm1 Ge2 5_555 . 54_555 180 ?
Ge2 Sm1 Ge2 5_555 . 9_555 70.81(5) ?
Ge2 Sm1 Ge2 5_555 . 58_555 109.19(5) ?
Ge2 Sm1 Ge2 54_555 . 9_555 109.19(5) ?
Ge2 Sm1 Ge2 54_555 . 58_555 70.81(5) ?
Ge2 Sm1 Ge2 9_555 . 58_555 180 ?
Sm1 Mn1 Sm1 . . 49_444 180 ?
Sm1 Mn1 Sm1 . . 2_555 109.4712(8) ?
Sm1 Mn1 Sm1 . . 50_554 70.5288(8) ?
Sm1 Mn1 Sm1 . . 3_555 109.4712(8) ?
Sm1 Mn1 Sm1 . . 51_545 70.5288(8) ?
Sm1 Mn1 Sm1 . . 4_555 109.4712(8) ?
Sm1 Mn1 Sm1 . . 52_455 70.5288(8) ?
Sm1 Mn1 Ga2 . . . 54.7356(4) ?
Sm1 Mn1 Ga2 . . 2_555 125.2644(4) ?
Sm1 Mn1 Ga2 . . 5_555 54.7356(4) ?
Sm1 Mn1 Ga2 . . 6_555 125.2644(4) ?
Sm1 Mn1 Ga2 . . 9_555 54.7356(4) ?
Sm1 Mn1 Ga2 . . 10_555 125.2644(4) ?
Sm1 Mn1 Ge2 . . . 54.7356(4) ?
Sm1 Mn1 Ge2 . . 2_555 125.2644(4) ?
Sm1 Mn1 Ge2 . . 5_555 54.7356(4) ?
Sm1 Mn1 Ge2 . . 6_555 125.2644(4) ?
Sm1 Mn1 Ge2 . . 9_555 54.7356(4) ?
Sm1 Mn1 Ge2 . . 10_555 125.2644(4) ?
Sm1 Mn1 Sm1 49_444 . 2_555 70.5288(8) ?
Sm1 Mn1 Sm1 49_444 . 50_554 109.4712(8) ?
Sm1 Mn1 Sm1 49_444 . 3_555 70.5288(8) ?
Sm1 Mn1 Sm1 49_444 . 51_545 109.4712(8) ?
Sm1 Mn1 Sm1 49_444 . 4_555 70.5288(8) ?
Sm1 Mn1 Sm1 49_444 . 52_455 109.4712(8) ?
Sm1 Mn1 Ga2 49_444 . . 125.2644(4) ?
Sm1 Mn1 Ga2 49_444 . 2_555 54.7356(4) ?
Sm1 Mn1 Ga2 49_444 . 5_555 125.2644(4) ?
Sm1 Mn1 Ga2 49_444 . 6_555 54.7356(4) ?
Sm1 Mn1 Ga2 49_444 . 9_555 125.2644(4) ?
Sm1 Mn1 Ga2 49_444 . 10_555 54.7356(4) ?
Sm1 Mn1 Ge2 49_444 . . 125.2644(4) ?
Sm1 Mn1 Ge2 49_444 . 2_555 54.7356(4) ?
Sm1 Mn1 Ge2 49_444 . 5_555 125.2644(4) ?
Sm1 Mn1 Ge2 49_444 . 6_555 54.7356(4) ?
Sm1 Mn1 Ge2 49_444 . 9_555 125.2644(4) ?
Sm1 Mn1 Ge2 49_444 . 10_555 54.7356(4) ?
Sm1 Mn1 Sm1 2_555 . 50_554 180 ?
Sm1 Mn1 Sm1 2_555 . 3_555 109.4712(8) ?
Sm1 Mn1 Sm1 2_555 . 51_545 70.5288(8) ?
Sm1 Mn1 Sm1 2_555 . 4_555 109.4712(8) ?
Sm1 Mn1 Sm1 2_555 . 52_455 70.5288(8) ?
Sm1 Mn1 Ga2 2_555 . . 125.2644(4) ?
Sm1 Mn1 Ga2 2_555 . 2_555 54.7356(4) ?
Sm1 Mn1 Ga2 2_555 . 5_555 125.2644(4) ?
Sm1 Mn1 Ga2 2_555 . 6_555 54.7356(4) ?
Sm1 Mn1 Ga2 2_555 . 9_555 54.7356(4) ?
Sm1 Mn1 Ga2 2_555 . 10_555 125.2644(4) ?
Sm1 Mn1 Ge2 2_555 . . 125.2644(4) ?
Sm1 Mn1 Ge2 2_555 . 2_555 54.7356(4) ?
Sm1 Mn1 Ge2 2_555 . 5_555 125.2644(4) ?
Sm1 Mn1 Ge2 2_555 . 6_555 54.7356(4) ?
Sm1 Mn1 Ge2 2_555 . 9_555 54.7356(4) ?
Sm1 Mn1 Ge2 2_555 . 10_555 125.2644(4) ?
Sm1 Mn1 Sm1 50_554 . 3_555 70.5288(8) ?
Sm1 Mn1 Sm1 50_554 . 51_545 109.4712(8) ?
Sm1 Mn1 Sm1 50_554 . 4_555 70.5288(8) ?
Sm1 Mn1 Sm1 50_554 . 52_455 109.4712(8) ?
Sm1 Mn1 Ga2 50_554 . . 54.7356(4) ?
Sm1 Mn1 Ga2 50_554 . 2_555 125.2644(4) ?
Sm1 Mn1 Ga2 50_554 . 5_555 54.7356(4) ?
Sm1 Mn1 Ga2 50_554 . 6_555 125.2644(4) ?
Sm1 Mn1 Ga2 50_554 . 9_555 125.2644(4) ?
Sm1 Mn1 Ga2 50_554 . 10_555 54.7356(4) ?
Sm1 Mn1 Ge2 50_554 . . 54.7356(4) ?
Sm1 Mn1 Ge2 50_554 . 2_555 125.2644(4) ?
Sm1 Mn1 Ge2 50_554 . 5_555 54.7356(4) ?
Sm1 Mn1 Ge2 50_554 . 6_555 125.2644(4) ?
Sm1 Mn1 Ge2 50_554 . 9_555 125.2644(4) ?
Sm1 Mn1 Ge2 50_554 . 10_555 54.7356(4) ?
Sm1 Mn1 Sm1 3_555 . 51_545 180 ?
Sm1 Mn1 Sm1 3_555 . 4_555 109.4712(8) ?
Sm1 Mn1 Sm1 3_555 . 52_455 70.5288(8) ?
Sm1 Mn1 Ga2 3_555 . . 125.2644(4) ?
Sm1 Mn1 Ga2 3_555 . 2_555 54.7356(4) ?
Sm1 Mn1 Ga2 3_555 . 5_555 54.7356(4) ?
Sm1 Mn1 Ga2 3_555 . 6_555 125.2644(4) ?
Sm1 Mn1 Ga2 3_555 . 9_555 125.2644(4) ?
Sm1 Mn1 Ga2 3_555 . 10_555 54.7356(4) ?
Sm1 Mn1 Ge2 3_555 . . 125.2644(4) ?
Sm1 Mn1 Ge2 3_555 . 2_555 54.7356(4) ?
Sm1 Mn1 Ge2 3_555 . 5_555 54.7356(4) ?
Sm1 Mn1 Ge2 3_555 . 6_555 125.2644(4) ?
Sm1 Mn1 Ge2 3_555 . 9_555 125.2644(4) ?
Sm1 Mn1 Ge2 3_555 . 10_555 54.7356(4) ?
Sm1 Mn1 Sm1 51_545 . 4_555 70.5288(8) ?
Sm1 Mn1 Sm1 51_545 . 52_455 109.4712(8) ?
Sm1 Mn1 Ga2 51_545 . . 54.7356(4) ?
Sm1 Mn1 Ga2 51_545 . 2_555 125.2644(4) ?
Sm1 Mn1 Ga2 51_545 . 5_555 125.2644(4) ?
Sm1 Mn1 Ga2 51_545 . 6_555 54.7356(4) ?
Sm1 Mn1 Ga2 51_545 . 9_555 54.7356(4) ?
Sm1 Mn1 Ga2 51_545 . 10_555 125.2644(4) ?
Sm1 Mn1 Ge2 51_545 . . 54.7356(4) ?
Sm1 Mn1 Ge2 51_545 . 2_555 125.2644(4) ?
Sm1 Mn1 Ge2 51_545 . 5_555 125.2644(4) ?
Sm1 Mn1 Ge2 51_545 . 6_555 54.7356(4) ?
Sm1 Mn1 Ge2 51_545 . 9_555 54.7356(4) ?
Sm1 Mn1 Ge2 51_545 . 10_555 125.2644(4) ?
Sm1 Mn1 Sm1 4_555 . 52_455 180 ?
Sm1 Mn1 Ga2 4_555 . . 54.7356(4) ?
Sm1 Mn1 Ga2 4_555 . 2_555 125.2644(4) ?
Sm1 Mn1 Ga2 4_555 . 5_555 125.2644(4) ?
Sm1 Mn1 Ga2 4_555 . 6_555 54.7356(4) ?
Sm1 Mn1 Ga2 4_555 . 9_555 125.2644(4) ?
Sm1 Mn1 Ga2 4_555 . 10_555 54.7356(4) ?
Sm1 Mn1 Ge2 4_555 . . 54.7356(4) ?
Sm1 Mn1 Ge2 4_555 . 2_555 125.2644(4) ?
Sm1 Mn1 Ge2 4_555 . 5_555 125.2644(4) ?
Sm1 Mn1 Ge2 4_555 . 6_555 54.7356(4) ?
Sm1 Mn1 Ge2 4_555 . 9_555 125.2644(4) ?
Sm1 Mn1 Ge2 4_555 . 10_555 54.7356(4) ?
Sm1 Mn1 Ga2 52_455 . . 125.2644(4) ?
Sm1 Mn1 Ga2 52_455 . 2_555 54.7356(4) ?
Sm1 Mn1 Ga2 52_455 . 5_555 54.7356(4) ?
Sm1 Mn1 Ga2 52_455 . 6_555 125.2644(4) ?
Sm1 Mn1 Ga2 52_455 . 9_555 54.7356(4) ?
Sm1 Mn1 Ga2 52_455 . 10_555 125.2644(4) ?
Sm1 Mn1 Ge2 52_455 . . 125.2644(4) ?
Sm1 Mn1 Ge2 52_455 . 2_555 54.7356(4) ?
Sm1 Mn1 Ge2 52_455 . 5_555 54.7356(4) ?
Sm1 Mn1 Ge2 52_455 . 6_555 125.2644(4) ?
Sm1 Mn1 Ge2 52_455 . 9_555 54.7356(4) ?
Sm1 Mn1 Ge2 52_455 . 10_555 125.2644(4) ?
Ga2 Mn1 Ga2 . . 2_555 180 ?
Ga2 Mn1 Ga2 . . 5_555 90 ?
Ga2 Mn1 Ga2 . . 6_555 90 ?
Ga2 Mn1 Ga2 . . 9_555 90 ?
Ga2 Mn1 Ga2 . . 10_555 90 ?
Ga2 Mn1 Ge2 . . . 0 ?
Ga2 Mn1 Ge2 . . 2_555 180 ?
Ga2 Mn1 Ge2 . . 5_555 90 ?
Ga2 Mn1 Ge2 . . 6_555 90 ?
Ga2 Mn1 Ge2 . . 9_555 90 ?
Ga2 Mn1 Ge2 . . 10_555 90 ?
Ga2 Mn1 Ga2 2_555 . 5_555 90 ?
Ga2 Mn1 Ga2 2_555 . 6_555 90 ?
Ga2 Mn1 Ga2 2_555 . 9_555 90 ?
Ga2 Mn1 Ga2 2_555 . 10_555 90 ?
Ga2 Mn1 Ge2 2_555 . . 180 ?
Ga2 Mn1 Ge2 2_555 . 2_555 0 ?
Ga2 Mn1 Ge2 2_555 . 5_555 90 ?
Ga2 Mn1 Ge2 2_555 . 6_555 90 ?
Ga2 Mn1 Ge2 2_555 . 9_555 90 ?
Ga2 Mn1 Ge2 2_555 . 10_555 90 ?
Ga2 Mn1 Ga2 5_555 . 6_555 180 ?
Ga2 Mn1 Ga2 5_555 . 9_555 90 ?
Ga2 Mn1 Ga2 5_555 . 10_555 90 ?
Ga2 Mn1 Ge2 5_555 . . 90 ?
Ga2 Mn1 Ge2 5_555 . 2_555 90 ?
Ga2 Mn1 Ge2 5_555 . 5_555 0 ?
Ga2 Mn1 Ge2 5_555 . 6_555 180 ?
Ga2 Mn1 Ge2 5_555 . 9_555 90 ?
Ga2 Mn1 Ge2 5_555 . 10_555 90 ?
Ga2 Mn1 Ga2 6_555 . 9_555 90 ?
Ga2 Mn1 Ga2 6_555 . 10_555 90 ?
Ga2 Mn1 Ge2 6_555 . . 90 ?
Ga2 Mn1 Ge2 6_555 . 2_555 90 ?
Ga2 Mn1 Ge2 6_555 . 5_555 180 ?
Ga2 Mn1 Ge2 6_555 . 6_555 0 ?
Ga2 Mn1 Ge2 6_555 . 9_555 90 ?
Ga2 Mn1 Ge2 6_555 . 10_555 90 ?
Ga2 Mn1 Ga2 9_555 . 10_555 180 ?
Ga2 Mn1 Ge2 9_555 . . 90 ?
Ga2 Mn1 Ge2 9_555 . 2_555 90 ?
Ga2 Mn1 Ge2 9_555 . 5_555 90 ?
Ga2 Mn1 Ge2 9_555 . 6_555 90 ?
Ga2 Mn1 Ge2 9_555 . 9_555 0 ?
Ga2 Mn1 Ge2 9_555 . 10_555 180 ?
Ga2 Mn1 Ge2 10_555 . . 90 ?
Ga2 Mn1 Ge2 10_555 . 2_555 90 ?
Ga2 Mn1 Ge2 10_555 . 5_555 90 ?
Ga2 Mn1 Ge2 10_555 . 6_555 90 ?
Ga2 Mn1 Ge2 10_555 . 9_555 180 ?
Ga2 Mn1 Ge2 10_555 . 10_555 0 ?
Ge2 Mn1 Ge2 . . 2_555 180 ?
Ge2 Mn1 Ge2 . . 5_555 90 ?
Ge2 Mn1 Ge2 . . 6_555 90 ?
Ge2 Mn1 Ge2 . . 9_555 90 ?
Ge2 Mn1 Ge2 . . 10_555 90 ?
Ge2 Mn1 Ge2 2_555 . 5_555 90 ?
Ge2 Mn1 Ge2 2_555 . 6_555 90 ?
Ge2 Mn1 Ge2 2_555 . 9_555 90 ?
Ge2 Mn1 Ge2 2_555 . 10_555 90 ?
Ge2 Mn1 Ge2 5_555 . 6_555 180 ?
Ge2 Mn1 Ge2 5_555 . 9_555 90 ?
Ge2 Mn1 Ge2 5_555 . 10_555 90 ?
Ge2 Mn1 Ge2 6_555 . 9_555 90 ?
Ge2 Mn1 Ge2 6_555 . 10_555 90 ?
Ge2 Mn1 Ge2 9_555 . 10_555 180 ?
Sm1 Ga1 Sm1 . . 2_655 180 ?
Sm1 Ga1 Sm1 . . 51_545 90.0000(9) ?
Sm1 Ga1 Sm1 . . 52_555 90.0000(9) ?
Sm1 Ga1 Ga1 . . 53_545 120.0000(5) ?
Sm1 Ga1 Ga1 . . 55_555 60.0000(5) ?
Sm1 Ga1 Ga1 . . 57_544 120.0000(5) ?
Sm1 Ga1 Ga1 . . 59_555 60.0000(5) ?
Sm1 Ga1 Ge1 . . 53_545 120.0000(5) ?
Sm1 Ga1 Ge1 . . 55_555 60.0000(5) ?
Sm1 Ga1 Ge1 . . 57_544 120.0000(5) ?
Sm1 Ga1 Ge1 . . 59_555 60.0000(5) ?
Sm1 Ga1 Ga2 . . . 63.09(2) ?
Sm1 Ga1 Ga2 . . 2_655 116.91(2) ?
Sm1 Ga1 Ga2 . . 53_545 116.91(2) ?
Sm1 Ga1 Ga2 . . 54_555 63.09(2) ?
Sm1 Ga1 Ge2 . . . 63.09(2) ?
Sm1 Ga1 Ge2 . . 2_655 116.91(2) ?
Sm1 Ga1 Ge2 . . 53_545 116.91(2) ?
Sm1 Ga1 Ge2 . . 54_555 63.09(2) ?
Sm1 Ga1 Sm1 2_655 . 51_545 90.0000(9) ?
Sm1 Ga1 Sm1 2_655 . 52_555 90.0000(9) ?
Sm1 Ga1 Ga1 2_655 . 53_545 60.0000(5) ?
Sm1 Ga1 Ga1 2_655 . 55_555 120.0000(5) ?
Sm1 Ga1 Ga1 2_655 . 57_544 60.0000(5) ?
Sm1 Ga1 Ga1 2_655 . 59_555 120.0000(5) ?
Sm1 Ga1 Ge1 2_655 . 53_545 60.0000(5) ?
Sm1 Ga1 Ge1 2_655 . 55_555 120.0000(5) ?
Sm1 Ga1 Ge1 2_655 . 57_544 60.0000(5) ?
Sm1 Ga1 Ge1 2_655 . 59_555 120.0000(5) ?
Sm1 Ga1 Ga2 2_655 . . 116.91(2) ?
Sm1 Ga1 Ga2 2_655 . 2_655 63.09(2) ?
Sm1 Ga1 Ga2 2_655 . 53_545 63.09(2) ?
Sm1 Ga1 Ga2 2_655 . 54_555 116.91(2) ?
Sm1 Ga1 Ge2 2_655 . . 116.91(2) ?
Sm1 Ga1 Ge2 2_655 . 2_655 63.09(2) ?
Sm1 Ga1 Ge2 2_655 . 53_545 63.09(2) ?
Sm1 Ga1 Ge2 2_655 . 54_555 116.91(2) ?
Sm1 Ga1 Sm1 51_545 . 52_555 180 ?
Sm1 Ga1 Ga1 51_545 . 53_545 120.0000(5) ?
Sm1 Ga1 Ga1 51_545 . 55_555 60.0000(5) ?
Sm1 Ga1 Ga1 51_545 . 57_544 60.0000(5) ?
Sm1 Ga1 Ga1 51_545 . 59_555 120.0000(5) ?
Sm1 Ga1 Ge1 51_545 . 53_545 120.0000(5) ?
Sm1 Ga1 Ge1 51_545 . 55_555 60.0000(5) ?
Sm1 Ga1 Ge1 51_545 . 57_544 60.0000(5) ?
Sm1 Ga1 Ge1 51_545 . 59_555 120.0000(5) ?
Sm1 Ga1 Ga2 51_545 . . 63.09(2) ?
Sm1 Ga1 Ga2 51_545 . 2_655 116.91(2) ?
Sm1 Ga1 Ga2 51_545 . 53_545 63.09(2) ?
Sm1 Ga1 Ga2 51_545 . 54_555 116.91(2) ?
Sm1 Ga1 Ge2 51_545 . . 63.09(2) ?
Sm1 Ga1 Ge2 51_545 . 2_655 116.91(2) ?
Sm1 Ga1 Ge2 51_545 . 53_545 63.09(2) ?
Sm1 Ga1 Ge2 51_545 . 54_555 116.91(2) ?
Sm1 Ga1 Ga1 52_555 . 53_545 60.0000(5) ?
Sm1 Ga1 Ga1 52_555 . 55_555 120.0000(5) ?
Sm1 Ga1 Ga1 52_555 . 57_544 120.0000(5) ?
Sm1 Ga1 Ga1 52_555 . 59_555 60.0000(5) ?
Sm1 Ga1 Ge1 52_555 . 53_545 60.0000(5) ?
Sm1 Ga1 Ge1 52_555 . 55_555 120.0000(5) ?
Sm1 Ga1 Ge1 52_555 . 57_544 120.0000(5) ?
Sm1 Ga1 Ge1 52_555 . 59_555 60.0000(5) ?
Sm1 Ga1 Ga2 52_555 . . 116.91(2) ?
Sm1 Ga1 Ga2 52_555 . 2_655 63.09(2) ?
Sm1 Ga1 Ga2 52_555 . 53_545 116.91(2) ?
Sm1 Ga1 Ga2 52_555 . 54_555 63.09(2) ?
Sm1 Ga1 Ge2 52_555 . . 116.91(2) ?
Sm1 Ga1 Ge2 52_555 . 2_655 63.09(2) ?
Sm1 Ga1 Ge2 52_555 . 53_545 116.91(2) ?
Sm1 Ga1 Ge2 52_555 . 54_555 63.09(2) ?
Ga1 Ga1 Ga1 53_545 . 55_555 90.0000(9) ?
Ga1 Ga1 Ga1 53_545 . 57_544 120.0000(5) ?
Ga1 Ga1 Ga1 53_545 . 59_555 120.0000(5) ?
Ga1 Ga1 Ge1 53_545 . 53_545 0 ?
Ga1 Ga1 Ge1 53_545 . 55_555 90.0000(9) ?
Ga1 Ga1 Ge1 53_545 . 57_544 120.0000(5) ?
Ga1 Ga1 Ge1 53_545 . 59_555 120.0000(5) ?
Ga1 Ga1 Ga2 53_545 . . 174.80(4) ?
Ga1 Ga1 Ga2 53_545 . 2_655 95.20(4) ?
Ga1 Ga1 Ga2 53_545 . 53_545 57.10(2) ?
Ga1 Ga1 Ga2 53_545 . 54_555 57.10(2) ?
Ga1 Ga1 Ge2 53_545 . . 174.80(4) ?
Ga1 Ga1 Ge2 53_545 . 2_655 95.20(4) ?
Ga1 Ga1 Ge2 53_545 . 53_545 57.10(2) ?
Ga1 Ga1 Ge2 53_545 . 54_555 57.10(2) ?
Ga1 Ga1 Ga1 55_555 . 57_544 120.0000(5) ?
Ga1 Ga1 Ga1 55_555 . 59_555 120.0000(5) ?
Ga1 Ga1 Ge1 55_555 . 53_545 90.0000(9) ?
Ga1 Ga1 Ge1 55_555 . 55_555 0 ?
Ga1 Ga1 Ge1 55_555 . 57_544 120.0000(5) ?
Ga1 Ga1 Ge1 55_555 . 59_555 120.0000(5) ?
Ga1 Ga1 Ga2 55_555 . . 95.20(4) ?
Ga1 Ga1 Ga2 55_555 . 2_655 174.80(4) ?
Ga1 Ga1 Ga2 55_555 . 53_545 57.10(2) ?
Ga1 Ga1 Ga2 55_555 . 54_555 57.10(2) ?
Ga1 Ga1 Ge2 55_555 . . 95.20(4) ?
Ga1 Ga1 Ge2 55_555 . 2_655 174.80(4) ?
Ga1 Ga1 Ge2 55_555 . 53_545 57.10(2) ?
Ga1 Ga1 Ge2 55_555 . 54_555 57.10(2) ?
Ga1 Ga1 Ga1 57_544 . 59_555 90.0000(9) ?
Ga1 Ga1 Ge1 57_544 . 53_545 120.0000(5) ?
Ga1 Ga1 Ge1 57_544 . 55_555 120.0000(5) ?
Ga1 Ga1 Ge1 57_544 . 57_544 0 ?
Ga1 Ga1 Ge1 57_544 . 59_555 90.0000(9) ?
Ga1 Ga1 Ga2 57_544 . . 57.10(2) ?
Ga1 Ga1 Ga2 57_544 . 2_655 57.10(2) ?
Ga1 Ga1 Ga2 57_544 . 53_545 95.20(4) ?
Ga1 Ga1 Ga2 57_544 . 54_555 174.80(4) ?
Ga1 Ga1 Ge2 57_544 . . 57.10(2) ?
Ga1 Ga1 Ge2 57_544 . 2_655 57.10(2) ?
Ga1 Ga1 Ge2 57_544 . 53_545 95.20(4) ?
Ga1 Ga1 Ge2 57_544 . 54_555 174.80(4) ?
Ga1 Ga1 Ge1 59_555 . 53_545 120.0000(5) ?
Ga1 Ga1 Ge1 59_555 . 55_555 120.0000(5) ?
Ga1 Ga1 Ge1 59_555 . 57_544 90.0000(9) ?
Ga1 Ga1 Ge1 59_555 . 59_555 0 ?
Ga1 Ga1 Ga2 59_555 . . 57.10(2) ?
Ga1 Ga1 Ga2 59_555 . 2_655 57.10(2) ?
Ga1 Ga1 Ga2 59_555 . 53_545 174.80(4) ?
Ga1 Ga1 Ga2 59_555 . 54_555 95.20(4) ?
Ga1 Ga1 Ge2 59_555 . . 57.10(2) ?
Ga1 Ga1 Ge2 59_555 . 2_655 57.10(2) ?
Ga1 Ga1 Ge2 59_555 . 53_545 174.80(4) ?
Ga1 Ga1 Ge2 59_555 . 54_555 95.20(4) ?
Ge1 Ga1 Ge1 53_545 . 55_555 90.0000(9) ?
Ge1 Ga1 Ge1 53_545 . 57_544 120.0000(5) ?
Ge1 Ga1 Ge1 53_545 . 59_555 120.0000(5) ?
Ge1 Ga1 Ga2 53_545 . . 174.80(4) ?
Ge1 Ga1 Ga2 53_545 . 2_655 95.20(4) ?
Ge1 Ga1 Ga2 53_545 . 53_545 57.10(2) ?
Ge1 Ga1 Ga2 53_545 . 54_555 57.10(2) ?
Ge1 Ga1 Ge2 53_545 . . 174.80(4) ?
Ge1 Ga1 Ge2 53_545 . 2_655 95.20(4) ?
Ge1 Ga1 Ge2 53_545 . 53_545 57.10(2) ?
Ge1 Ga1 Ge2 53_545 . 54_555 57.10(2) ?
Ge1 Ga1 Ge1 55_555 . 57_544 120.0000(5) ?
Ge1 Ga1 Ge1 55_555 . 59_555 120.0000(5) ?
Ge1 Ga1 Ga2 55_555 . . 95.20(4) ?
Ge1 Ga1 Ga2 55_555 . 2_655 174.80(4) ?
Ge1 Ga1 Ga2 55_555 . 53_545 57.10(2) ?
Ge1 Ga1 Ga2 55_555 . 54_555 57.10(2) ?
Ge1 Ga1 Ge2 55_555 . . 95.20(4) ?
Ge1 Ga1 Ge2 55_555 . 2_655 174.80(4) ?
Ge1 Ga1 Ge2 55_555 . 53_545 57.10(2) ?
Ge1 Ga1 Ge2 55_555 . 54_555 57.10(2) ?
Ge1 Ga1 Ge1 57_544 . 59_555 90.0000(9) ?
Ge1 Ga1 Ga2 57_544 . . 57.10(2) ?
Ge1 Ga1 Ga2 57_544 . 2_655 57.10(2) ?
Ge1 Ga1 Ga2 57_544 . 53_545 95.20(4) ?
Ge1 Ga1 Ga2 57_544 . 54_555 174.80(4) ?
Ge1 Ga1 Ge2 57_544 . . 57.10(2) ?
Ge1 Ga1 Ge2 57_544 . 2_655 57.10(2) ?
Ge1 Ga1 Ge2 57_544 . 53_545 95.20(4) ?
Ge1 Ga1 Ge2 57_544 . 54_555 174.80(4) ?
Ge1 Ga1 Ga2 59_555 . . 57.10(2) ?
Ge1 Ga1 Ga2 59_555 . 2_655 57.10(2) ?
Ge1 Ga1 Ga2 59_555 . 53_545 174.80(4) ?
Ge1 Ga1 Ga2 59_555 . 54_555 95.20(4) ?
Ge1 Ga1 Ge2 59_555 . . 57.10(2) ?
Ge1 Ga1 Ge2 59_555 . 2_655 57.10(2) ?
Ge1 Ga1 Ge2 59_555 . 53_545 174.80(4) ?
Ge1 Ga1 Ge2 59_555 . 54_555 95.20(4) ?
Ga2 Ga1 Ga2 . . 2_655 79.61(5) ?
Ga2 Ga1 Ga2 . . 53_545 126.17(3) ?
Ga2 Ga1 Ga2 . . 54_555 126.17(3) ?
Ga2 Ga1 Ge2 . . . 0 ?
Ga2 Ga1 Ge2 . . 2_655 79.61(5) ?
Ga2 Ga1 Ge2 . . 53_545 126.17(3) ?
Ga2 Ga1 Ge2 . . 54_555 126.17(3) ?
Ga2 Ga1 Ga2 2_655 . 53_545 126.17(3) ?
Ga2 Ga1 Ga2 2_655 . 54_555 126.17(3) ?
Ga2 Ga1 Ge2 2_655 . . 79.61(5) ?
Ga2 Ga1 Ge2 2_655 . 2_655 0 ?
Ga2 Ga1 Ge2 2_655 . 53_545 126.17(3) ?
Ga2 Ga1 Ge2 2_655 . 54_555 126.17(3) ?
Ga2 Ga1 Ga2 53_545 . 54_555 79.61(5) ?
Ga2 Ga1 Ge2 53_545 . . 126.17(3) ?
Ga2 Ga1 Ge2 53_545 . 2_655 126.17(3) ?
Ga2 Ga1 Ge2 53_545 . 53_545 0 ?
Ga2 Ga1 Ge2 53_545 . 54_555 79.61(5) ?
Ga2 Ga1 Ge2 54_555 . . 126.17(3) ?
Ga2 Ga1 Ge2 54_555 . 2_655 126.17(3) ?
Ga2 Ga1 Ge2 54_555 . 53_545 79.61(5) ?
Ga2 Ga1 Ge2 54_555 . 54_555 0 ?
Ge2 Ga1 Ge2 . . 2_655 79.61(5) ?
Ge2 Ga1 Ge2 . . 53_545 126.17(3) ?
Ge2 Ga1 Ge2 . . 54_555 126.17(3) ?
Ge2 Ga1 Ge2 2_655 . 53_545 126.17(3) ?
Ge2 Ga1 Ge2 2_655 . 54_555 126.17(3) ?
Ge2 Ga1 Ge2 53_545 . 54_555 79.61(5) ?
Sm1 Ge1 Sm1 . . 2_655 180 ?
Sm1 Ge1 Sm1 . . 51_545 90.0000(9) ?
Sm1 Ge1 Sm1 . . 52_555 90.0000(9) ?
Sm1 Ge1 Ga1 . . 53_545 120.0000(5) ?
Sm1 Ge1 Ga1 . . 55_555 60.0000(5) ?
Sm1 Ge1 Ga1 . . 57_544 120.0000(5) ?
Sm1 Ge1 Ga1 . . 59_555 60.0000(5) ?
Sm1 Ge1 Ge1 . . 53_545 120.0000(5) ?
Sm1 Ge1 Ge1 . . 55_555 60.0000(5) ?
Sm1 Ge1 Ge1 . . 57_544 120.0000(5) ?
Sm1 Ge1 Ge1 . . 59_555 60.0000(5) ?
Sm1 Ge1 Ga2 . . . 63.09(2) ?
Sm1 Ge1 Ga2 . . 2_655 116.91(2) ?
Sm1 Ge1 Ga2 . . 53_545 116.91(2) ?
Sm1 Ge1 Ga2 . . 54_555 63.09(2) ?
Sm1 Ge1 Ge2 . . . 63.09(2) ?
Sm1 Ge1 Ge2 . . 2_655 116.91(2) ?
Sm1 Ge1 Ge2 . . 53_545 116.91(2) ?
Sm1 Ge1 Ge2 . . 54_555 63.09(2) ?
Sm1 Ge1 Sm1 2_655 . 51_545 90.0000(9) ?
Sm1 Ge1 Sm1 2_655 . 52_555 90.0000(9) ?
Sm1 Ge1 Ga1 2_655 . 53_545 60.0000(5) ?
Sm1 Ge1 Ga1 2_655 . 55_555 120.0000(5) ?
Sm1 Ge1 Ga1 2_655 . 57_544 60.0000(5) ?
Sm1 Ge1 Ga1 2_655 . 59_555 120.0000(5) ?
Sm1 Ge1 Ge1 2_655 . 53_545 60.0000(5) ?
Sm1 Ge1 Ge1 2_655 . 55_555 120.0000(5) ?
Sm1 Ge1 Ge1 2_655 . 57_544 60.0000(5) ?
Sm1 Ge1 Ge1 2_655 . 59_555 120.0000(5) ?
Sm1 Ge1 Ga2 2_655 . . 116.91(2) ?
Sm1 Ge1 Ga2 2_655 . 2_655 63.09(2) ?
Sm1 Ge1 Ga2 2_655 . 53_545 63.09(2) ?
Sm1 Ge1 Ga2 2_655 . 54_555 116.91(2) ?
Sm1 Ge1 Ge2 2_655 . . 116.91(2) ?
Sm1 Ge1 Ge2 2_655 . 2_655 63.09(2) ?
Sm1 Ge1 Ge2 2_655 . 53_545 63.09(2) ?
Sm1 Ge1 Ge2 2_655 . 54_555 116.91(2) ?
Sm1 Ge1 Sm1 51_545 . 52_555 180 ?
Sm1 Ge1 Ga1 51_545 . 53_545 120.0000(5) ?
Sm1 Ge1 Ga1 51_545 . 55_555 60.0000(5) ?
Sm1 Ge1 Ga1 51_545 . 57_544 60.0000(5) ?
Sm1 Ge1 Ga1 51_545 . 59_555 120.0000(5) ?
Sm1 Ge1 Ge1 51_545 . 53_545 120.0000(5) ?
Sm1 Ge1 Ge1 51_545 . 55_555 60.0000(5) ?
Sm1 Ge1 Ge1 51_545 . 57_544 60.0000(5) ?
Sm1 Ge1 Ge1 51_545 . 59_555 120.0000(5) ?
Sm1 Ge1 Ga2 51_545 . . 63.09(2) ?
Sm1 Ge1 Ga2 51_545 . 2_655 116.91(2) ?
Sm1 Ge1 Ga2 51_545 . 53_545 63.09(2) ?
Sm1 Ge1 Ga2 51_545 . 54_555 116.91(2) ?
Sm1 Ge1 Ge2 51_545 . . 63.09(2) ?
Sm1 Ge1 Ge2 51_545 . 2_655 116.91(2) ?
Sm1 Ge1 Ge2 51_545 . 53_545 63.09(2) ?
Sm1 Ge1 Ge2 51_545 . 54_555 116.91(2) ?
Sm1 Ge1 Ga1 52_555 . 53_545 60.0000(5) ?
Sm1 Ge1 Ga1 52_555 . 55_555 120.0000(5) ?
Sm1 Ge1 Ga1 52_555 . 57_544 120.0000(5) ?
Sm1 Ge1 Ga1 52_555 . 59_555 60.0000(5) ?
Sm1 Ge1 Ge1 52_555 . 53_545 60.0000(5) ?
Sm1 Ge1 Ge1 52_555 . 55_555 120.0000(5) ?
Sm1 Ge1 Ge1 52_555 . 57_544 120.0000(5) ?
Sm1 Ge1 Ge1 52_555 . 59_555 60.0000(5) ?
Sm1 Ge1 Ga2 52_555 . . 116.91(2) ?
Sm1 Ge1 Ga2 52_555 . 2_655 63.09(2) ?
Sm1 Ge1 Ga2 52_555 . 53_545 116.91(2) ?
Sm1 Ge1 Ga2 52_555 . 54_555 63.09(2) ?
Sm1 Ge1 Ge2 52_555 . . 116.91(2) ?
Sm1 Ge1 Ge2 52_555 . 2_655 63.09(2) ?
Sm1 Ge1 Ge2 52_555 . 53_545 116.91(2) ?
Sm1 Ge1 Ge2 52_555 . 54_555 63.09(2) ?
Ga1 Ge1 Ga1 53_545 . 55_555 90.0000(9) ?
Ga1 Ge1 Ga1 53_545 . 57_544 120.0000(5) ?
Ga1 Ge1 Ga1 53_545 . 59_555 120.0000(5) ?
Ga1 Ge1 Ge1 53_545 . 53_545 0 ?
Ga1 Ge1 Ge1 53_545 . 55_555 90.0000(9) ?
Ga1 Ge1 Ge1 53_545 . 57_544 120.0000(5) ?
Ga1 Ge1 Ge1 53_545 . 59_555 120.0000(5) ?
Ga1 Ge1 Ga2 53_545 . . 174.80(4) ?
Ga1 Ge1 Ga2 53_545 . 2_655 95.20(4) ?
Ga1 Ge1 Ga2 53_545 . 53_545 57.10(2) ?
Ga1 Ge1 Ga2 53_545 . 54_555 57.10(2) ?
Ga1 Ge1 Ge2 53_545 . . 174.80(4) ?
Ga1 Ge1 Ge2 53_545 . 2_655 95.20(4) ?
Ga1 Ge1 Ge2 53_545 . 53_545 57.10(2) ?
Ga1 Ge1 Ge2 53_545 . 54_555 57.10(2) ?
Ga1 Ge1 Ga1 55_555 . 57_544 120.0000(5) ?
Ga1 Ge1 Ga1 55_555 . 59_555 120.0000(5) ?
Ga1 Ge1 Ge1 55_555 . 53_545 90.0000(9) ?
Ga1 Ge1 Ge1 55_555 . 55_555 0 ?
Ga1 Ge1 Ge1 55_555 . 57_544 120.0000(5) ?
Ga1 Ge1 Ge1 55_555 . 59_555 120.0000(5) ?
Ga1 Ge1 Ga2 55_555 . . 95.20(4) ?
Ga1 Ge1 Ga2 55_555 . 2_655 174.80(4) ?
Ga1 Ge1 Ga2 55_555 . 53_545 57.10(2) ?
Ga1 Ge1 Ga2 55_555 . 54_555 57.10(2) ?
Ga1 Ge1 Ge2 55_555 . . 95.20(4) ?
Ga1 Ge1 Ge2 55_555 . 2_655 174.80(4) ?
Ga1 Ge1 Ge2 55_555 . 53_545 57.10(2) ?
Ga1 Ge1 Ge2 55_555 . 54_555 57.10(2) ?
Ga1 Ge1 Ga1 57_544 . 59_555 90.0000(9) ?
Ga1 Ge1 Ge1 57_544 . 53_545 120.0000(5) ?
Ga1 Ge1 Ge1 57_544 . 55_555 120.0000(5) ?
Ga1 Ge1 Ge1 57_544 . 57_544 0 ?
Ga1 Ge1 Ge1 57_544 . 59_555 90.0000(9) ?
Ga1 Ge1 Ga2 57_544 . . 57.10(2) ?
Ga1 Ge1 Ga2 57_544 . 2_655 57.10(2) ?
Ga1 Ge1 Ga2 57_544 . 53_545 95.20(4) ?
Ga1 Ge1 Ga2 57_544 . 54_555 174.80(4) ?
Ga1 Ge1 Ge2 57_544 . . 57.10(2) ?
Ga1 Ge1 Ge2 57_544 . 2_655 57.10(2) ?
Ga1 Ge1 Ge2 57_544 . 53_545 95.20(4) ?
Ga1 Ge1 Ge2 57_544 . 54_555 174.80(4) ?
Ga1 Ge1 Ge1 59_555 . 53_545 120.0000(5) ?
Ga1 Ge1 Ge1 59_555 . 55_555 120.0000(5) ?
Ga1 Ge1 Ge1 59_555 . 57_544 90.0000(9) ?
Ga1 Ge1 Ge1 59_555 . 59_555 0 ?
Ga1 Ge1 Ga2 59_555 . . 57.10(2) ?
Ga1 Ge1 Ga2 59_555 . 2_655 57.10(2) ?
Ga1 Ge1 Ga2 59_555 . 53_545 174.80(4) ?
Ga1 Ge1 Ga2 59_555 . 54_555 95.20(4) ?
Ga1 Ge1 Ge2 59_555 . . 57.10(2) ?
Ga1 Ge1 Ge2 59_555 . 2_655 57.10(2) ?
Ga1 Ge1 Ge2 59_555 . 53_545 174.80(4) ?
Ga1 Ge1 Ge2 59_555 . 54_555 95.20(4) ?
Ge1 Ge1 Ge1 53_545 . 55_555 90.0000(9) ?
Ge1 Ge1 Ge1 53_545 . 57_544 120.0000(5) ?
Ge1 Ge1 Ge1 53_545 . 59_555 120.0000(5) ?
Ge1 Ge1 Ga2 53_545 . . 174.80(4) ?
Ge1 Ge1 Ga2 53_545 . 2_655 95.20(4) ?
Ge1 Ge1 Ga2 53_545 . 53_545 57.10(2) ?
Ge1 Ge1 Ga2 53_545 . 54_555 57.10(2) ?
Ge1 Ge1 Ge2 53_545 . . 174.80(4) ?
Ge1 Ge1 Ge2 53_545 . 2_655 95.20(4) ?
Ge1 Ge1 Ge2 53_545 . 53_545 57.10(2) ?
Ge1 Ge1 Ge2 53_545 . 54_555 57.10(2) ?
Ge1 Ge1 Ge1 55_555 . 57_544 120.0000(5) ?
Ge1 Ge1 Ge1 55_555 . 59_555 120.0000(5) ?
Ge1 Ge1 Ga2 55_555 . . 95.20(4) ?
Ge1 Ge1 Ga2 55_555 . 2_655 174.80(4) ?
Ge1 Ge1 Ga2 55_555 . 53_545 57.10(2) ?
Ge1 Ge1 Ga2 55_555 . 54_555 57.10(2) ?
Ge1 Ge1 Ge2 55_555 . . 95.20(4) ?
Ge1 Ge1 Ge2 55_555 . 2_655 174.80(4) ?
Ge1 Ge1 Ge2 55_555 . 53_545 57.10(2) ?
Ge1 Ge1 Ge2 55_555 . 54_555 57.10(2) ?
Ge1 Ge1 Ge1 57_544 . 59_555 90.0000(9) ?
Ge1 Ge1 Ga2 57_544 . . 57.10(2) ?
Ge1 Ge1 Ga2 57_544 . 2_655 57.10(2) ?
Ge1 Ge1 Ga2 57_544 . 53_545 95.20(4) ?
Ge1 Ge1 Ga2 57_544 . 54_555 174.80(4) ?
Ge1 Ge1 Ge2 57_544 . . 57.10(2) ?
Ge1 Ge1 Ge2 57_544 . 2_655 57.10(2) ?
Ge1 Ge1 Ge2 57_544 . 53_545 95.20(4) ?
Ge1 Ge1 Ge2 57_544 . 54_555 174.80(4) ?
Ge1 Ge1 Ga2 59_555 . . 57.10(2) ?
Ge1 Ge1 Ga2 59_555 . 2_655 57.10(2) ?
Ge1 Ge1 Ga2 59_555 . 53_545 174.80(4) ?
Ge1 Ge1 Ga2 59_555 . 54_555 95.20(4) ?
Ge1 Ge1 Ge2 59_555 . . 57.10(2) ?
Ge1 Ge1 Ge2 59_555 . 2_655 57.10(2) ?
Ge1 Ge1 Ge2 59_555 . 53_545 174.80(4) ?
Ge1 Ge1 Ge2 59_555 . 54_555 95.20(4) ?
Ga2 Ge1 Ga2 . . 2_655 79.61(5) ?
Ga2 Ge1 Ga2 . . 53_545 126.17(3) ?
Ga2 Ge1 Ga2 . . 54_555 126.17(3) ?
Ga2 Ge1 Ge2 . . . 0 ?
Ga2 Ge1 Ge2 . . 2_655 79.61(5) ?
Ga2 Ge1 Ge2 . . 53_545 126.17(3) ?
Ga2 Ge1 Ge2 . . 54_555 126.17(3) ?
Ga2 Ge1 Ga2 2_655 . 53_545 126.17(3) ?
Ga2 Ge1 Ga2 2_655 . 54_555 126.17(3) ?
Ga2 Ge1 Ge2 2_655 . . 79.61(5) ?
Ga2 Ge1 Ge2 2_655 . 2_655 0 ?
Ga2 Ge1 Ge2 2_655 . 53_545 126.17(3) ?
Ga2 Ge1 Ge2 2_655 . 54_555 126.17(3) ?
Ga2 Ge1 Ga2 53_545 . 54_555 79.61(5) ?
Ga2 Ge1 Ge2 53_545 . . 126.17(3) ?
Ga2 Ge1 Ge2 53_545 . 2_655 126.17(3) ?
Ga2 Ge1 Ge2 53_545 . 53_545 0 ?
Ga2 Ge1 Ge2 53_545 . 54_555 79.61(5) ?
Ga2 Ge1 Ge2 54_555 . . 126.17(3) ?
Ga2 Ge1 Ge2 54_555 . 2_655 126.17(3) ?
Ga2 Ge1 Ge2 54_555 . 53_545 79.61(5) ?
Ga2 Ge1 Ge2 54_555 . 54_555 0 ?
Ge2 Ge1 Ge2 . . 2_655 79.61(5) ?
Ge2 Ge1 Ge2 . . 53_545 126.17(3) ?
Ge2 Ge1 Ge2 . . 54_555 126.17(3) ?
Ge2 Ge1 Ge2 2_655 . 53_545 126.17(3) ?
Ge2 Ge1 Ge2 2_655 . 54_555 126.17(3) ?
Ge2 Ge1 Ge2 53_545 . 54_555 79.61(5) ?
Sm1 Ga2 Sm1 . . 50_554 89.214(10) ?
Sm1 Ga2 Sm1 . . 51_545 89.214(10) ?
Sm1 Ga2 Sm1 . . 4_555 166.55(9) ?
Sm1 Ga2 Mn1 . . . 83.28(4) ?
Sm1 Ga2 Ga1 . . . 62.319(12) ?
Sm1 Ga2 Ga1 . . 3_655 127.91(5) ?
Sm1 Ga2 Ga1 . . 57_544 127.91(5) ?
Sm1 Ga2 Ga1 . . 59_555 62.319(12) ?
Sm1 Ga2 Ge1 . . . 62.319(12) ?
Sm1 Ga2 Ge1 . . 3_655 127.91(5) ?
Sm1 Ga2 Ge1 . . 57_544 127.91(5) ?
Sm1 Ga2 Ge1 . . 59_555 62.319(12) ?
Sm1 Ga2 Ga2 . . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 . . 5_555 54.59(3) ?
Sm1 Ga2 Ga2 . . 6_555 114.44(6) ?
Sm1 Ga2 Ga2 . . 9_555 54.59(3) ?
Sm1 Ga2 Ga2 . . 10_555 114.44(6) ?
Sm1 Ga2 Ge2 . . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 . . 5_555 54.59(3) ?
Sm1 Ga2 Ge2 . . 6_555 114.44(6) ?
Sm1 Ga2 Ge2 . . 9_555 54.59(3) ?
Sm1 Ga2 Ge2 . . 10_555 114.44(6) ?
Sm1 Ga2 Sm1 50_554 . 51_545 166.55(9) ?
Sm1 Ga2 Sm1 50_554 . 4_555 89.214(10) ?
Sm1 Ga2 Mn1 50_554 . . 83.28(4) ?
Sm1 Ga2 Ga1 50_554 . . 127.91(5) ?
Sm1 Ga2 Ga1 50_554 . 3_655 62.319(12) ?
Sm1 Ga2 Ga1 50_554 . 57_544 127.91(5) ?
Sm1 Ga2 Ga1 50_554 . 59_555 62.319(12) ?
Sm1 Ga2 Ge1 50_554 . . 127.91(5) ?
Sm1 Ga2 Ge1 50_554 . 3_655 62.319(12) ?
Sm1 Ga2 Ge1 50_554 . 57_544 127.91(5) ?
Sm1 Ga2 Ge1 50_554 . 59_555 62.319(12) ?
Sm1 Ga2 Ga2 50_554 . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 50_554 . 5_555 54.59(3) ?
Sm1 Ga2 Ga2 50_554 . 6_555 114.44(6) ?
Sm1 Ga2 Ga2 50_554 . 9_555 114.44(6) ?
Sm1 Ga2 Ga2 50_554 . 10_555 54.59(3) ?
Sm1 Ga2 Ge2 50_554 . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 50_554 . 5_555 54.59(3) ?
Sm1 Ga2 Ge2 50_554 . 6_555 114.44(6) ?
Sm1 Ga2 Ge2 50_554 . 9_555 114.44(6) ?
Sm1 Ga2 Ge2 50_554 . 10_555 54.59(3) ?
Sm1 Ga2 Sm1 51_545 . 4_555 89.214(10) ?
Sm1 Ga2 Mn1 51_545 . . 83.28(4) ?
Sm1 Ga2 Ga1 51_545 . . 62.319(12) ?
Sm1 Ga2 Ga1 51_545 . 3_655 127.91(5) ?
Sm1 Ga2 Ga1 51_545 . 57_544 62.319(12) ?
Sm1 Ga2 Ga1 51_545 . 59_555 127.91(5) ?
Sm1 Ga2 Ge1 51_545 . . 62.319(12) ?
Sm1 Ga2 Ge1 51_545 . 3_655 127.91(5) ?
Sm1 Ga2 Ge1 51_545 . 57_544 62.319(12) ?
Sm1 Ga2 Ge1 51_545 . 59_555 127.91(5) ?
Sm1 Ga2 Ga2 51_545 . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 51_545 . 5_555 114.44(6) ?
Sm1 Ga2 Ga2 51_545 . 6_555 54.59(3) ?
Sm1 Ga2 Ga2 51_545 . 9_555 54.59(3) ?
Sm1 Ga2 Ga2 51_545 . 10_555 114.44(6) ?
Sm1 Ga2 Ge2 51_545 . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 51_545 . 5_555 114.44(6) ?
Sm1 Ga2 Ge2 51_545 . 6_555 54.59(3) ?
Sm1 Ga2 Ge2 51_545 . 9_555 54.59(3) ?
Sm1 Ga2 Ge2 51_545 . 10_555 114.44(6) ?
Sm1 Ga2 Mn1 4_555 . . 83.28(4) ?
Sm1 Ga2 Ga1 4_555 . . 127.91(5) ?
Sm1 Ga2 Ga1 4_555 . 3_655 62.319(12) ?
Sm1 Ga2 Ga1 4_555 . 57_544 62.319(12) ?
Sm1 Ga2 Ga1 4_555 . 59_555 127.91(5) ?
Sm1 Ga2 Ge1 4_555 . . 127.91(5) ?
Sm1 Ga2 Ge1 4_555 . 3_655 62.319(12) ?
Sm1 Ga2 Ge1 4_555 . 57_544 62.319(12) ?
Sm1 Ga2 Ge1 4_555 . 59_555 127.91(5) ?
Sm1 Ga2 Ga2 4_555 . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 4_555 . 5_555 114.44(6) ?
Sm1 Ga2 Ga2 4_555 . 6_555 54.59(3) ?
Sm1 Ga2 Ga2 4_555 . 9_555 114.44(6) ?
Sm1 Ga2 Ga2 4_555 . 10_555 54.59(3) ?
Sm1 Ga2 Ge2 4_555 . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 4_555 . 5_555 114.44(6) ?
Sm1 Ga2 Ge2 4_555 . 6_555 54.59(3) ?
Sm1 Ga2 Ge2 4_555 . 9_555 114.44(6) ?
Sm1 Ga2 Ge2 4_555 . 10_555 54.59(3) ?
Mn1 Ga2 Ga1 . . . 129.80(4) ?
Mn1 Ga2 Ga1 . . 3_655 129.80(4) ?
Mn1 Ga2 Ga1 . . 57_544 129.80(4) ?
Mn1 Ga2 Ga1 . . 59_555 129.80(4) ?
Mn1 Ga2 Ge1 . . . 129.80(4) ?
Mn1 Ga2 Ge1 . . 3_655 129.80(4) ?
Mn1 Ga2 Ge1 . . 57_544 129.80(4) ?
Mn1 Ga2 Ge1 . . 59_555 129.80(4) ?
Mn1 Ga2 Ga2 . . 2_655 180 ?
Mn1 Ga2 Ga2 . . 5_555 45.00(4) ?
Mn1 Ga2 Ga2 . . 6_555 45.00(4) ?
Mn1 Ga2 Ga2 . . 9_555 45.00(4) ?
Mn1 Ga2 Ga2 . . 10_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 2_655 180 ?
Mn1 Ga2 Ge2 . . 5_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 6_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 9_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 10_555 45.00(4) ?
Ga1 Ga2 Ga1 . . 3_655 100.39(7) ?
Ga1 Ga2 Ga1 . . 57_544 65.81(4) ?
Ga1 Ga2 Ga1 . . 59_555 65.81(4) ?
Ga1 Ga2 Ge1 . . . 0 ?
Ga1 Ga2 Ge1 . . 3_655 100.39(7) ?
Ga1 Ga2 Ge1 . . 57_544 65.81(4) ?
Ga1 Ga2 Ge1 . . 59_555 65.81(4) ?
Ga1 Ga2 Ga2 . . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 . . 5_555 116.914(16) ?
Ga1 Ga2 Ga2 . . 6_555 116.914(16) ?
Ga1 Ga2 Ga2 . . 9_555 84.80(3) ?
Ga1 Ga2 Ga2 . . 10_555 174.80(7) ?
Ga1 Ga2 Ge2 . . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 . . 5_555 116.914(16) ?
Ga1 Ga2 Ge2 . . 6_555 116.914(16) ?
Ga1 Ga2 Ge2 . . 9_555 84.80(3) ?
Ga1 Ga2 Ge2 . . 10_555 174.80(7) ?
Ga1 Ga2 Ga1 3_655 . 57_544 65.81(4) ?
Ga1 Ga2 Ga1 3_655 . 59_555 65.81(4) ?
Ga1 Ga2 Ge1 3_655 . . 100.39(7) ?
Ga1 Ga2 Ge1 3_655 . 3_655 0 ?
Ga1 Ga2 Ge1 3_655 . 57_544 65.81(4) ?
Ga1 Ga2 Ge1 3_655 . 59_555 65.81(4) ?
Ga1 Ga2 Ga2 3_655 . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 3_655 . 5_555 116.914(16) ?
Ga1 Ga2 Ga2 3_655 . 6_555 116.914(16) ?
Ga1 Ga2 Ga2 3_655 . 9_555 174.80(7) ?
Ga1 Ga2 Ga2 3_655 . 10_555 84.80(3) ?
Ga1 Ga2 Ge2 3_655 . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 3_655 . 5_555 116.914(16) ?
Ga1 Ga2 Ge2 3_655 . 6_555 116.914(16) ?
Ga1 Ga2 Ge2 3_655 . 9_555 174.80(7) ?
Ga1 Ga2 Ge2 3_655 . 10_555 84.80(3) ?
Ga1 Ga2 Ga1 57_544 . 59_555 100.39(7) ?
Ga1 Ga2 Ge1 57_544 . . 65.81(4) ?
Ga1 Ga2 Ge1 57_544 . 3_655 65.81(4) ?
Ga1 Ga2 Ge1 57_544 . 57_544 0 ?
Ga1 Ga2 Ge1 57_544 . 59_555 100.39(7) ?
Ga1 Ga2 Ga2 57_544 . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 57_544 . 5_555 174.80(7) ?
Ga1 Ga2 Ga2 57_544 . 6_555 84.80(3) ?
Ga1 Ga2 Ga2 57_544 . 9_555 116.914(16) ?
Ga1 Ga2 Ga2 57_544 . 10_555 116.914(16) ?
Ga1 Ga2 Ge2 57_544 . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 57_544 . 5_555 174.80(7) ?
Ga1 Ga2 Ge2 57_544 . 6_555 84.80(3) ?
Ga1 Ga2 Ge2 57_544 . 9_555 116.914(16) ?
Ga1 Ga2 Ge2 57_544 . 10_555 116.914(16) ?
Ga1 Ga2 Ge1 59_555 . . 65.81(4) ?
Ga1 Ga2 Ge1 59_555 . 3_655 65.81(4) ?
Ga1 Ga2 Ge1 59_555 . 57_544 100.39(7) ?
Ga1 Ga2 Ge1 59_555 . 59_555 0 ?
Ga1 Ga2 Ga2 59_555 . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 59_555 . 5_555 84.80(3) ?
Ga1 Ga2 Ga2 59_555 . 6_555 174.80(7) ?
Ga1 Ga2 Ga2 59_555 . 9_555 116.914(16) ?
Ga1 Ga2 Ga2 59_555 . 10_555 116.914(16) ?
Ga1 Ga2 Ge2 59_555 . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 59_555 . 5_555 84.80(3) ?
Ga1 Ga2 Ge2 59_555 . 6_555 174.80(7) ?
Ga1 Ga2 Ge2 59_555 . 9_555 116.914(16) ?
Ga1 Ga2 Ge2 59_555 . 10_555 116.914(16) ?
Ge1 Ga2 Ge1 . . 3_655 100.39(7) ?
Ge1 Ga2 Ge1 . . 57_544 65.81(4) ?
Ge1 Ga2 Ge1 . . 59_555 65.81(4) ?
Ge1 Ga2 Ga2 . . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 . . 5_555 116.914(16) ?
Ge1 Ga2 Ga2 . . 6_555 116.914(16) ?
Ge1 Ga2 Ga2 . . 9_555 84.80(3) ?
Ge1 Ga2 Ga2 . . 10_555 174.80(7) ?
Ge1 Ga2 Ge2 . . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 . . 5_555 116.914(16) ?
Ge1 Ga2 Ge2 . . 6_555 116.914(16) ?
Ge1 Ga2 Ge2 . . 9_555 84.80(3) ?
Ge1 Ga2 Ge2 . . 10_555 174.80(7) ?
Ge1 Ga2 Ge1 3_655 . 57_544 65.81(4) ?
Ge1 Ga2 Ge1 3_655 . 59_555 65.81(4) ?
Ge1 Ga2 Ga2 3_655 . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 3_655 . 5_555 116.914(16) ?
Ge1 Ga2 Ga2 3_655 . 6_555 116.914(16) ?
Ge1 Ga2 Ga2 3_655 . 9_555 174.80(7) ?
Ge1 Ga2 Ga2 3_655 . 10_555 84.80(3) ?
Ge1 Ga2 Ge2 3_655 . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 3_655 . 5_555 116.914(16) ?
Ge1 Ga2 Ge2 3_655 . 6_555 116.914(16) ?
Ge1 Ga2 Ge2 3_655 . 9_555 174.80(7) ?
Ge1 Ga2 Ge2 3_655 . 10_555 84.80(3) ?
Ge1 Ga2 Ge1 57_544 . 59_555 100.39(7) ?
Ge1 Ga2 Ga2 57_544 . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 57_544 . 5_555 174.80(7) ?
Ge1 Ga2 Ga2 57_544 . 6_555 84.80(3) ?
Ge1 Ga2 Ga2 57_544 . 9_555 116.914(16) ?
Ge1 Ga2 Ga2 57_544 . 10_555 116.914(16) ?
Ge1 Ga2 Ge2 57_544 . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 57_544 . 5_555 174.80(7) ?
Ge1 Ga2 Ge2 57_544 . 6_555 84.80(3) ?
Ge1 Ga2 Ge2 57_544 . 9_555 116.914(16) ?
Ge1 Ga2 Ge2 57_544 . 10_555 116.914(16) ?
Ge1 Ga2 Ga2 59_555 . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 59_555 . 5_555 84.80(3) ?
Ge1 Ga2 Ga2 59_555 . 6_555 174.80(7) ?
Ge1 Ga2 Ga2 59_555 . 9_555 116.914(16) ?
Ge1 Ga2 Ga2 59_555 . 10_555 116.914(16) ?
Ge1 Ga2 Ge2 59_555 . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 59_555 . 5_555 84.80(3) ?
Ge1 Ga2 Ge2 59_555 . 6_555 174.80(7) ?
Ge1 Ga2 Ge2 59_555 . 9_555 116.914(16) ?
Ge1 Ga2 Ge2 59_555 . 10_555 116.914(16) ?
Ga2 Ga2 Ga2 2_655 . 5_555 135.00(4) ?
Ga2 Ga2 Ga2 2_655 . 6_555 135.00(4) ?
Ga2 Ga2 Ga2 2_655 . 9_555 135.00(4) ?
Ga2 Ga2 Ga2 2_655 . 10_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 2_655 0 ?
Ga2 Ga2 Ge2 2_655 . 5_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 6_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 9_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 10_555 135.00(4) ?
Ga2 Ga2 Ga2 5_555 . 6_555 90.00(7) ?
Ga2 Ga2 Ga2 5_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ga2 5_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ge2 5_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 5_555 . 5_555 0 ?
Ga2 Ga2 Ge2 5_555 . 6_555 90.00(7) ?
Ga2 Ga2 Ge2 5_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ge2 5_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ga2 6_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ga2 6_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ge2 6_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 6_555 . 5_555 90.00(7) ?
Ga2 Ga2 Ge2 6_555 . 6_555 0 ?
Ga2 Ga2 Ge2 6_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ge2 6_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ga2 9_555 . 10_555 90.00(7) ?
Ga2 Ga2 Ge2 9_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 9_555 . 5_555 60.00(4) ?
Ga2 Ga2 Ge2 9_555 . 6_555 60.00(4) ?
Ga2 Ga2 Ge2 9_555 . 9_555 0 ?
Ga2 Ga2 Ge2 9_555 . 10_555 90.00(7) ?
Ga2 Ga2 Ge2 10_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 10_555 . 5_555 60.00(4) ?
Ga2 Ga2 Ge2 10_555 . 6_555 60.00(4) ?
Ga2 Ga2 Ge2 10_555 . 9_555 90.00(7) ?
Ga2 Ga2 Ge2 10_555 . 10_555 0 ?
Ge2 Ga2 Ge2 2_655 . 5_555 135.00(4) ?
Ge2 Ga2 Ge2 2_655 . 6_555 135.00(4) ?
Ge2 Ga2 Ge2 2_655 . 9_555 135.00(4) ?
Ge2 Ga2 Ge2 2_655 . 10_555 135.00(4) ?
Ge2 Ga2 Ge2 5_555 . 6_555 90.00(7) ?
Ge2 Ga2 Ge2 5_555 . 9_555 60.00(4) ?
Ge2 Ga2 Ge2 5_555 . 10_555 60.00(4) ?
Ge2 Ga2 Ge2 6_555 . 9_555 60.00(4) ?
Ge2 Ga2 Ge2 6_555 . 10_555 60.00(4) ?
Ge2 Ga2 Ge2 9_555 . 10_555 90.00(7) ?
Sm1 Ge2 Sm1 . . 50_554 89.214(10) ?
Sm1 Ge2 Sm1 . . 51_545 89.214(10) ?
Sm1 Ge2 Sm1 . . 4_555 166.55(9) ?
Sm1 Ge2 Mn1 . . . 83.28(4) ?
Sm1 Ge2 Ga1 . . . 62.319(12) ?
Sm1 Ge2 Ga1 . . 3_655 127.91(5) ?
Sm1 Ge2 Ga1 . . 57_544 127.91(5) ?
Sm1 Ge2 Ga1 . . 59_555 62.319(12) ?
Sm1 Ge2 Ge1 . . . 62.319(12) ?
Sm1 Ge2 Ge1 . . 3_655 127.91(5) ?
Sm1 Ge2 Ge1 . . 57_544 127.91(5) ?
Sm1 Ge2 Ge1 . . 59_555 62.319(12) ?
Sm1 Ge2 Ga2 . . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 . . 5_555 54.59(3) ?
Sm1 Ge2 Ga2 . . 6_555 114.44(6) ?
Sm1 Ge2 Ga2 . . 9_555 54.59(3) ?
Sm1 Ge2 Ga2 . . 10_555 114.44(6) ?
Sm1 Ge2 Ge2 . . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 . . 5_555 54.59(3) ?
Sm1 Ge2 Ge2 . . 6_555 114.44(6) ?
Sm1 Ge2 Ge2 . . 9_555 54.59(3) ?
Sm1 Ge2 Ge2 . . 10_555 114.44(6) ?
Sm1 Ge2 Sm1 50_554 . 51_545 166.55(9) ?
Sm1 Ge2 Sm1 50_554 . 4_555 89.214(10) ?
Sm1 Ge2 Mn1 50_554 . . 83.28(4) ?
Sm1 Ge2 Ga1 50_554 . . 127.91(5) ?
Sm1 Ge2 Ga1 50_554 . 3_655 62.319(12) ?
Sm1 Ge2 Ga1 50_554 . 57_544 127.91(5) ?
Sm1 Ge2 Ga1 50_554 . 59_555 62.319(12) ?
Sm1 Ge2 Ge1 50_554 . . 127.91(5) ?
Sm1 Ge2 Ge1 50_554 . 3_655 62.319(12) ?
Sm1 Ge2 Ge1 50_554 . 57_544 127.91(5) ?
Sm1 Ge2 Ge1 50_554 . 59_555 62.319(12) ?
Sm1 Ge2 Ga2 50_554 . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 50_554 . 5_555 54.59(3) ?
Sm1 Ge2 Ga2 50_554 . 6_555 114.44(6) ?
Sm1 Ge2 Ga2 50_554 . 9_555 114.44(6) ?
Sm1 Ge2 Ga2 50_554 . 10_555 54.59(3) ?
Sm1 Ge2 Ge2 50_554 . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 50_554 . 5_555 54.59(3) ?
Sm1 Ge2 Ge2 50_554 . 6_555 114.44(6) ?
Sm1 Ge2 Ge2 50_554 . 9_555 114.44(6) ?
Sm1 Ge2 Ge2 50_554 . 10_555 54.59(3) ?
Sm1 Ge2 Sm1 51_545 . 4_555 89.214(10) ?
Sm1 Ge2 Mn1 51_545 . . 83.28(4) ?
Sm1 Ge2 Ga1 51_545 . . 62.319(12) ?
Sm1 Ge2 Ga1 51_545 . 3_655 127.91(5) ?
Sm1 Ge2 Ga1 51_545 . 57_544 62.319(12) ?
Sm1 Ge2 Ga1 51_545 . 59_555 127.91(5) ?
Sm1 Ge2 Ge1 51_545 . . 62.319(12) ?
Sm1 Ge2 Ge1 51_545 . 3_655 127.91(5) ?
Sm1 Ge2 Ge1 51_545 . 57_544 62.319(12) ?
Sm1 Ge2 Ge1 51_545 . 59_555 127.91(5) ?
Sm1 Ge2 Ga2 51_545 . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 51_545 . 5_555 114.44(6) ?
Sm1 Ge2 Ga2 51_545 . 6_555 54.59(3) ?
Sm1 Ge2 Ga2 51_545 . 9_555 54.59(3) ?
Sm1 Ge2 Ga2 51_545 . 10_555 114.44(6) ?
Sm1 Ge2 Ge2 51_545 . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 51_545 . 5_555 114.44(6) ?
Sm1 Ge2 Ge2 51_545 . 6_555 54.59(3) ?
Sm1 Ge2 Ge2 51_545 . 9_555 54.59(3) ?
Sm1 Ge2 Ge2 51_545 . 10_555 114.44(6) ?
Sm1 Ge2 Mn1 4_555 . . 83.28(4) ?
Sm1 Ge2 Ga1 4_555 . . 127.91(5) ?
Sm1 Ge2 Ga1 4_555 . 3_655 62.319(12) ?
Sm1 Ge2 Ga1 4_555 . 57_544 62.319(12) ?
Sm1 Ge2 Ga1 4_555 . 59_555 127.91(5) ?
Sm1 Ge2 Ge1 4_555 . . 127.91(5) ?
Sm1 Ge2 Ge1 4_555 . 3_655 62.319(12) ?
Sm1 Ge2 Ge1 4_555 . 57_544 62.319(12) ?
Sm1 Ge2 Ge1 4_555 . 59_555 127.91(5) ?
Sm1 Ge2 Ga2 4_555 . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 4_555 . 5_555 114.44(6) ?
Sm1 Ge2 Ga2 4_555 . 6_555 54.59(3) ?
Sm1 Ge2 Ga2 4_555 . 9_555 114.44(6) ?
Sm1 Ge2 Ga2 4_555 . 10_555 54.59(3) ?
Sm1 Ge2 Ge2 4_555 . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 4_555 . 5_555 114.44(6) ?
Sm1 Ge2 Ge2 4_555 . 6_555 54.59(3) ?
Sm1 Ge2 Ge2 4_555 . 9_555 114.44(6) ?
Sm1 Ge2 Ge2 4_555 . 10_555 54.59(3) ?
Mn1 Ge2 Ga1 . . . 129.80(4) ?
Mn1 Ge2 Ga1 . . 3_655 129.80(4) ?
Mn1 Ge2 Ga1 . . 57_544 129.80(4) ?
Mn1 Ge2 Ga1 . . 59_555 129.80(4) ?
Mn1 Ge2 Ge1 . . . 129.80(4) ?
Mn1 Ge2 Ge1 . . 3_655 129.80(4) ?
Mn1 Ge2 Ge1 . . 57_544 129.80(4) ?
Mn1 Ge2 Ge1 . . 59_555 129.80(4) ?
Mn1 Ge2 Ga2 . . 2_655 180 ?
Mn1 Ge2 Ga2 . . 5_555 45.00(4) ?
Mn1 Ge2 Ga2 . . 6_555 45.00(4) ?
Mn1 Ge2 Ga2 . . 9_555 45.00(4) ?
Mn1 Ge2 Ga2 . . 10_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 2_655 180 ?
Mn1 Ge2 Ge2 . . 5_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 6_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 9_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 10_555 45.00(4) ?
Ga1 Ge2 Ga1 . . 3_655 100.39(7) ?
Ga1 Ge2 Ga1 . . 57_544 65.81(4) ?
Ga1 Ge2 Ga1 . . 59_555 65.81(4) ?
Ga1 Ge2 Ge1 . . . 0 ?
Ga1 Ge2 Ge1 . . 3_655 100.39(7) ?
Ga1 Ge2 Ge1 . . 57_544 65.81(4) ?
Ga1 Ge2 Ge1 . . 59_555 65.81(4) ?
Ga1 Ge2 Ga2 . . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 . . 5_555 116.914(16) ?
Ga1 Ge2 Ga2 . . 6_555 116.914(16) ?
Ga1 Ge2 Ga2 . . 9_555 84.80(3) ?
Ga1 Ge2 Ga2 . . 10_555 174.80(7) ?
Ga1 Ge2 Ge2 . . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 . . 5_555 116.914(16) ?
Ga1 Ge2 Ge2 . . 6_555 116.914(16) ?
Ga1 Ge2 Ge2 . . 9_555 84.80(3) ?
Ga1 Ge2 Ge2 . . 10_555 174.80(7) ?
Ga1 Ge2 Ga1 3_655 . 57_544 65.81(4) ?
Ga1 Ge2 Ga1 3_655 . 59_555 65.81(4) ?
Ga1 Ge2 Ge1 3_655 . . 100.39(7) ?
Ga1 Ge2 Ge1 3_655 . 3_655 0 ?
Ga1 Ge2 Ge1 3_655 . 57_544 65.81(4) ?
Ga1 Ge2 Ge1 3_655 . 59_555 65.81(4) ?
Ga1 Ge2 Ga2 3_655 . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 3_655 . 5_555 116.914(16) ?
Ga1 Ge2 Ga2 3_655 . 6_555 116.914(16) ?
Ga1 Ge2 Ga2 3_655 . 9_555 174.80(7) ?
Ga1 Ge2 Ga2 3_655 . 10_555 84.80(3) ?
Ga1 Ge2 Ge2 3_655 . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 3_655 . 5_555 116.914(16) ?
Ga1 Ge2 Ge2 3_655 . 6_555 116.914(16) ?
Ga1 Ge2 Ge2 3_655 . 9_555 174.80(7) ?
Ga1 Ge2 Ge2 3_655 . 10_555 84.80(3) ?
Ga1 Ge2 Ga1 57_544 . 59_555 100.39(7) ?
Ga1 Ge2 Ge1 57_544 . . 65.81(4) ?
Ga1 Ge2 Ge1 57_544 . 3_655 65.81(4) ?
Ga1 Ge2 Ge1 57_544 . 57_544 0 ?
Ga1 Ge2 Ge1 57_544 . 59_555 100.39(7) ?
Ga1 Ge2 Ga2 57_544 . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 57_544 . 5_555 174.80(7) ?
Ga1 Ge2 Ga2 57_544 . 6_555 84.80(3) ?
Ga1 Ge2 Ga2 57_544 . 9_555 116.914(16) ?
Ga1 Ge2 Ga2 57_544 . 10_555 116.914(16) ?
Ga1 Ge2 Ge2 57_544 . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 57_544 . 5_555 174.80(7) ?
Ga1 Ge2 Ge2 57_544 . 6_555 84.80(3) ?
Ga1 Ge2 Ge2 57_544 . 9_555 116.914(16) ?
Ga1 Ge2 Ge2 57_544 . 10_555 116.914(16) ?
Ga1 Ge2 Ge1 59_555 . . 65.81(4) ?
Ga1 Ge2 Ge1 59_555 . 3_655 65.81(4) ?
Ga1 Ge2 Ge1 59_555 . 57_544 100.39(7) ?
Ga1 Ge2 Ge1 59_555 . 59_555 0 ?
Ga1 Ge2 Ga2 59_555 . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 59_555 . 5_555 84.80(3) ?
Ga1 Ge2 Ga2 59_555 . 6_555 174.80(7) ?
Ga1 Ge2 Ga2 59_555 . 9_555 116.914(16) ?
Ga1 Ge2 Ga2 59_555 . 10_555 116.914(16) ?
Ga1 Ge2 Ge2 59_555 . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 59_555 . 5_555 84.80(3) ?
Ga1 Ge2 Ge2 59_555 . 6_555 174.80(7) ?
Ga1 Ge2 Ge2 59_555 . 9_555 116.914(16) ?
Ga1 Ge2 Ge2 59_555 . 10_555 116.914(16) ?
Ge1 Ge2 Ge1 . . 3_655 100.39(7) ?
Ge1 Ge2 Ge1 . . 57_544 65.81(4) ?
Ge1 Ge2 Ge1 . . 59_555 65.81(4) ?
Ge1 Ge2 Ga2 . . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 . . 5_555 116.914(16) ?
Ge1 Ge2 Ga2 . . 6_555 116.914(16) ?
Ge1 Ge2 Ga2 . . 9_555 84.80(3) ?
Ge1 Ge2 Ga2 . . 10_555 174.80(7) ?
Ge1 Ge2 Ge2 . . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 . . 5_555 116.914(16) ?
Ge1 Ge2 Ge2 . . 6_555 116.914(16) ?
Ge1 Ge2 Ge2 . . 9_555 84.80(3) ?
Ge1 Ge2 Ge2 . . 10_555 174.80(7) ?
Ge1 Ge2 Ge1 3_655 . 57_544 65.81(4) ?
Ge1 Ge2 Ge1 3_655 . 59_555 65.81(4) ?
Ge1 Ge2 Ga2 3_655 . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 3_655 . 5_555 116.914(16) ?
Ge1 Ge2 Ga2 3_655 . 6_555 116.914(16) ?
Ge1 Ge2 Ga2 3_655 . 9_555 174.80(7) ?
Ge1 Ge2 Ga2 3_655 . 10_555 84.80(3) ?
Ge1 Ge2 Ge2 3_655 . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 3_655 . 5_555 116.914(16) ?
Ge1 Ge2 Ge2 3_655 . 6_555 116.914(16) ?
Ge1 Ge2 Ge2 3_655 . 9_555 174.80(7) ?
Ge1 Ge2 Ge2 3_655 . 10_555 84.80(3) ?
Ge1 Ge2 Ge1 57_544 . 59_555 100.39(7) ?
Ge1 Ge2 Ga2 57_544 . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 57_544 . 5_555 174.80(7) ?
Ge1 Ge2 Ga2 57_544 . 6_555 84.80(3) ?
Ge1 Ge2 Ga2 57_544 . 9_555 116.914(16) ?
Ge1 Ge2 Ga2 57_544 . 10_555 116.914(16) ?
Ge1 Ge2 Ge2 57_544 . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 57_544 . 5_555 174.80(7) ?
Ge1 Ge2 Ge2 57_544 . 6_555 84.80(3) ?
Ge1 Ge2 Ge2 57_544 . 9_555 116.914(16) ?
Ge1 Ge2 Ge2 57_544 . 10_555 116.914(16) ?
Ge1 Ge2 Ga2 59_555 . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 59_555 . 5_555 84.80(3) ?
Ge1 Ge2 Ga2 59_555 . 6_555 174.80(7) ?
Ge1 Ge2 Ga2 59_555 . 9_555 116.914(16) ?
Ge1 Ge2 Ga2 59_555 . 10_555 116.914(16) ?
Ge1 Ge2 Ge2 59_555 . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 59_555 . 5_555 84.80(3) ?
Ge1 Ge2 Ge2 59_555 . 6_555 174.80(7) ?
Ge1 Ge2 Ge2 59_555 . 9_555 116.914(16) ?
Ge1 Ge2 Ge2 59_555 . 10_555 116.914(16) ?
Ga2 Ge2 Ga2 2_655 . 5_555 135.00(4) ?
Ga2 Ge2 Ga2 2_655 . 6_555 135.00(4) ?
Ga2 Ge2 Ga2 2_655 . 9_555 135.00(4) ?
Ga2 Ge2 Ga2 2_655 . 10_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 2_655 0 ?
Ga2 Ge2 Ge2 2_655 . 5_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 6_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 9_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 10_555 135.00(4) ?
Ga2 Ge2 Ga2 5_555 . 6_555 90.00(7) ?
Ga2 Ge2 Ga2 5_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ga2 5_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ge2 5_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 5_555 . 5_555 0 ?
Ga2 Ge2 Ge2 5_555 . 6_555 90.00(7) ?
Ga2 Ge2 Ge2 5_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ge2 5_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ga2 6_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ga2 6_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ge2 6_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 6_555 . 5_555 90.00(7) ?
Ga2 Ge2 Ge2 6_555 . 6_555 0 ?
Ga2 Ge2 Ge2 6_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ge2 6_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ga2 9_555 . 10_555 90.00(7) ?
Ga2 Ge2 Ge2 9_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 9_555 . 5_555 60.00(4) ?
Ga2 Ge2 Ge2 9_555 . 6_555 60.00(4) ?
Ga2 Ge2 Ge2 9_555 . 9_555 0 ?
Ga2 Ge2 Ge2 9_555 . 10_555 90.00(7) ?
Ga2 Ge2 Ge2 10_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 10_555 . 5_555 60.00(4) ?
Ga2 Ge2 Ge2 10_555 . 6_555 60.00(4) ?
Ga2 Ge2 Ge2 10_555 . 9_555 90.00(7) ?
Ga2 Ge2 Ge2 10_555 . 10_555 0 ?
Ge2 Ge2 Ge2 2_655 . 5_555 135.00(4) ?
Ge2 Ge2 Ge2 2_655 . 6_555 135.00(4) ?
Ge2 Ge2 Ge2 2_655 . 9_555 135.00(4) ?
Ge2 Ge2 Ge2 2_655 . 10_555 135.00(4) ?
Ge2 Ge2 Ge2 5_555 . 6_555 90.00(7) ?
Ge2 Ge2 Ge2 5_555 . 9_555 60.00(4) ?
Ge2 Ge2 Ge2 5_555 . 10_555 60.00(4) ?
Ge2 Ge2 Ge2 6_555 . 9_555 60.00(4) ?
Ge2 Ge2 Ge2 6_555 . 10_555 60.00(4) ?
Ge2 Ge2 Ge2 9_555 . 10_555 90.00(7) ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 11. STRUCTURE-FACTOR LIST


_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Sm2Mn074Ga51Ge09anharmonic
_database_code_depnum_ccdc_archive 'CCDC 2302494'
loop_
_audit_author_name
_audit_author_address
'Roman Khalaniya'
;Lomonosov Moscow State University
Russia
;
_audit_update_record             
;
2023-12-07 deposited with the CCDC.	2023-12-13 downloaded from the CCDC.
;
#=======================================================================

_audit_creation_method           'Jana2006 Version : 15/02/2021'

#=======================================================================

# 4. CHECKCIF RESPONSE 

# start Validation Reply Form

#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        Sm2Mn0.74Ga5.1Ge0.9
_chemical_name_common            ?
_chemical_formula_moiety         'Sm2 Mn0.742 Ga5.1 Ge0.9'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'Ga5.1 Ge0.9 Mn0.742 Sm2'
_chemical_formula_weight         762.3
_chemical_melting_point          ?
_chemical_compound_source        ?
_chemical_absolute_configuration .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'F m -3 m'
_symmetry_space_group_name_Hall  '-F 4;2;3'
_symmetry_Int_Tables_number      225

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -x,y,-z
4 x,-y,-z
5 z,x,y
6 z,-x,-y
7 -z,-x,y
8 -z,x,-y
9 y,z,x
10 -y,z,-x
11 y,-z,-x
12 -y,-z,x
13 y,x,-z
14 -y,-x,-z
15 y,-x,z
16 -y,x,z
17 x,z,-y
18 -x,z,y
19 -x,-z,-y
20 x,-z,y
21 z,y,-x
22 z,-y,x
23 -z,y,x
24 -z,-y,-x
25 -x,-y,-z
26 x,y,-z
27 x,-y,z
28 -x,y,z
29 -z,-x,-y
30 -z,x,y
31 z,x,-y
32 z,-x,y
33 -y,-z,-x
34 y,-z,x
35 -y,z,x
36 y,z,-x
37 -y,-x,z
38 y,x,z
39 -y,x,-z
40 y,-x,-z
41 -x,-z,y
42 x,-z,-y
43 x,z,y
44 -x,z,-y
45 -z,-y,x
46 -z,y,-x
47 z,-y,-x
48 z,y,x
49 x,y+1/2,z+1/2
50 -x,-y+1/2,z+1/2
51 -x,y+1/2,-z+1/2
52 x,-y+1/2,-z+1/2
53 z,x+1/2,y+1/2
54 z,-x+1/2,-y+1/2
55 -z,-x+1/2,y+1/2
56 -z,x+1/2,-y+1/2
57 y,z+1/2,x+1/2
58 -y,z+1/2,-x+1/2
59 y,-z+1/2,-x+1/2
60 -y,-z+1/2,x+1/2
61 y,x+1/2,-z+1/2
62 -y,-x+1/2,-z+1/2
63 y,-x+1/2,z+1/2
64 -y,x+1/2,z+1/2
65 x,z+1/2,-y+1/2
66 -x,z+1/2,y+1/2
67 -x,-z+1/2,-y+1/2
68 x,-z+1/2,y+1/2
69 z,y+1/2,-x+1/2
70 z,-y+1/2,x+1/2
71 -z,y+1/2,x+1/2
72 -z,-y+1/2,-x+1/2
73 -x,-y+1/2,-z+1/2
74 x,y+1/2,-z+1/2
75 x,-y+1/2,z+1/2
76 -x,y+1/2,z+1/2
77 -z,-x+1/2,-y+1/2
78 -z,x+1/2,y+1/2
79 z,x+1/2,-y+1/2
80 z,-x+1/2,y+1/2
81 -y,-z+1/2,-x+1/2
82 y,-z+1/2,x+1/2
83 -y,z+1/2,x+1/2
84 y,z+1/2,-x+1/2
85 -y,-x+1/2,z+1/2
86 y,x+1/2,z+1/2
87 -y,x+1/2,-z+1/2
88 y,-x+1/2,-z+1/2
89 -x,-z+1/2,y+1/2
90 x,-z+1/2,-y+1/2
91 x,z+1/2,y+1/2
92 -x,z+1/2,-y+1/2
93 -z,-y+1/2,x+1/2
94 -z,y+1/2,-x+1/2
95 z,-y+1/2,-x+1/2
96 z,y+1/2,x+1/2
97 x+1/2,y,z+1/2
98 -x+1/2,-y,z+1/2
99 -x+1/2,y,-z+1/2
100 x+1/2,-y,-z+1/2
101 z+1/2,x,y+1/2
102 z+1/2,-x,-y+1/2
103 -z+1/2,-x,y+1/2
104 -z+1/2,x,-y+1/2
105 y+1/2,z,x+1/2
106 -y+1/2,z,-x+1/2
107 y+1/2,-z,-x+1/2
108 -y+1/2,-z,x+1/2
109 y+1/2,x,-z+1/2
110 -y+1/2,-x,-z+1/2
111 y+1/2,-x,z+1/2
112 -y+1/2,x,z+1/2
113 x+1/2,z,-y+1/2
114 -x+1/2,z,y+1/2
115 -x+1/2,-z,-y+1/2
116 x+1/2,-z,y+1/2
117 z+1/2,y,-x+1/2
118 z+1/2,-y,x+1/2
119 -z+1/2,y,x+1/2
120 -z+1/2,-y,-x+1/2
121 -x+1/2,-y,-z+1/2
122 x+1/2,y,-z+1/2
123 x+1/2,-y,z+1/2
124 -x+1/2,y,z+1/2
125 -z+1/2,-x,-y+1/2
126 -z+1/2,x,y+1/2
127 z+1/2,x,-y+1/2
128 z+1/2,-x,y+1/2
129 -y+1/2,-z,-x+1/2
130 y+1/2,-z,x+1/2
131 -y+1/2,z,x+1/2
132 y+1/2,z,-x+1/2
133 -y+1/2,-x,z+1/2
134 y+1/2,x,z+1/2
135 -y+1/2,x,-z+1/2
136 y+1/2,-x,-z+1/2
137 -x+1/2,-z,y+1/2
138 x+1/2,-z,-y+1/2
139 x+1/2,z,y+1/2
140 -x+1/2,z,-y+1/2
141 -z+1/2,-y,x+1/2
142 -z+1/2,y,-x+1/2
143 z+1/2,-y,-x+1/2
144 z+1/2,y,x+1/2
145 x+1/2,y+1/2,z
146 -x+1/2,-y+1/2,z
147 -x+1/2,y+1/2,-z
148 x+1/2,-y+1/2,-z
149 z+1/2,x+1/2,y
150 z+1/2,-x+1/2,-y
151 -z+1/2,-x+1/2,y
152 -z+1/2,x+1/2,-y
153 y+1/2,z+1/2,x
154 -y+1/2,z+1/2,-x
155 y+1/2,-z+1/2,-x
156 -y+1/2,-z+1/2,x
157 y+1/2,x+1/2,-z
158 -y+1/2,-x+1/2,-z
159 y+1/2,-x+1/2,z
160 -y+1/2,x+1/2,z
161 x+1/2,z+1/2,-y
162 -x+1/2,z+1/2,y
163 -x+1/2,-z+1/2,-y
164 x+1/2,-z+1/2,y
165 z+1/2,y+1/2,-x
166 z+1/2,-y+1/2,x
167 -z+1/2,y+1/2,x
168 -z+1/2,-y+1/2,-x
169 -x+1/2,-y+1/2,-z
170 x+1/2,y+1/2,-z
171 x+1/2,-y+1/2,z
172 -x+1/2,y+1/2,z
173 -z+1/2,-x+1/2,-y
174 -z+1/2,x+1/2,y
175 z+1/2,x+1/2,-y
176 z+1/2,-x+1/2,y
177 -y+1/2,-z+1/2,-x
178 y+1/2,-z+1/2,x
179 -y+1/2,z+1/2,x
180 y+1/2,z+1/2,-x
181 -y+1/2,-x+1/2,z
182 y+1/2,x+1/2,z
183 -y+1/2,x+1/2,-z
184 y+1/2,-x+1/2,-z
185 -x+1/2,-z+1/2,y
186 x+1/2,-z+1/2,-y
187 x+1/2,z+1/2,y
188 -x+1/2,z+1/2,-y
189 -z+1/2,-y+1/2,x
190 -z+1/2,y+1/2,-x
191 z+1/2,-y+1/2,-x
192 z+1/2,y+1/2,x

_cell_length_a                   8.7126(3)
_cell_length_b                   8.7126(3)
_cell_length_c                   8.7126(3)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     661.37(4)

loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z            4

_cell_measurement_reflns_used    2654
_cell_measurement_theta_min      4.68
_cell_measurement_theta_max      55.47
_cell_measurement_temperature    100
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    7.6561
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             1318


_exptl_absorpt_coefficient_mu    43.138
_exptl_crystal_description       'rectangular cuboid'
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.1
_exptl_crystal_size_rad          ?
_exptl_crystal_colour            grey
_exptl_absorpt_correction_type   multi-scan,gaussian
_exptl_absorpt_process_details   
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_absorpt_correction_T_min  0.0047
_exptl_absorpt_correction_T_max  0.0242
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?

_diffrn_ambient_temperature      100
_diffrn_source                   ?
_diffrn_source_power             ?
_diffrn_source_voltage           ?
_diffrn_source_current           ?
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_detector                 ?
_diffrn_detector_area_resol_mean ?
_diffrn_measurement_method       'Bruker CCD'
_diffrn_measurement_specimen_support ?

_diffrn_reflns_number            3772
_diffrn_reflns_theta_min         4.05
_diffrn_reflns_theta_max         56.29
_diffrn_reflns_theta_full        56.29
_diffrn_measured_fraction_theta_max 0.98
_diffrn_measured_fraction_theta_full 0.98
_diffrn_reflns_av_R_equivalents  0.0774
_diffrn_reflns_av_unetI/netI     0.0341
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_reduction_process ?

_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?

_diffrn_radiation_probe          X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

_reflns_number_total             268
_reflns_number_gt                222
_reflns_threshold_expression     I>2σ(I)

_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0215
_refine_ls_wR_factor_gt          0.0235
_refine_ls_R_factor_all          0.0296
_refine_ls_wR_factor_ref         0.0248
_refine_ls_goodness_of_fit_ref   1.04
_refine_ls_goodness_of_fit_gt    1.09
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         268
_refine_ls_number_parameters     15
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.0001F²)
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0024
_refine_ls_shift/su_mean         0.0011
_refine_diff_density_max         1.79
_refine_diff_density_min         -2.20
_refine_ls_extinction_method     
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef       206(19)
_refine_ls_extinction_expression ?
_refine_ls_abs_structure_details ?
_refine_ls_abs_structure_Flack   ?
_refine_ls_abs_structure_Rogers  ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga 0.2307 1.6083 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Ge 0.1547 1.8001 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.3368 0.7283 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Sm -0.1638 3.4418 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?

loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?

loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?

loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sm1 Sm 0.25 0.25 0.25 Uani 0.00819(16) 8 1 d . . .
Mn1 Mn 0 0 0 Uani 0.0088(2) 4 0.742(9) d . . .
Ga1 Ga 0.2760(2) 0 0 Uani 0.0163(3) 24 0.85 d . . .
Ge1 Ge 0.2760(2) 0 0 Uani 0.0163(3) 24 0.15 d . . .


loop_
_jana_atom_site_ADP_C_label
_jana_atom_site_ADP_C_type_symbol
_jana_atom_site_ADP_C_111
_jana_atom_site_ADP_C_112
_jana_atom_site_ADP_C_113
_jana_atom_site_ADP_C_122
_jana_atom_site_ADP_C_123
_jana_atom_site_ADP_C_133
_jana_atom_site_ADP_C_222
_jana_atom_site_ADP_C_223
_jana_atom_site_ADP_C_233
_jana_atom_site_ADP_C_333
Sm1 Sm 0 0 0 0 -0.00004(3) 0 0 0 0 0
Ga1 Ga -0.0030(8) 0 0 0 0 0 0 0 0 0
Ge1 Ge -0.0030(8) 0 0 0 0 0 0 0 0 0

loop_
_jana_atom_site_ADP_D_label
_jana_atom_site_ADP_D_type_symbol
_jana_atom_site_ADP_D_1111
_jana_atom_site_ADP_D_1112
_jana_atom_site_ADP_D_1113
_jana_atom_site_ADP_D_1122
_jana_atom_site_ADP_D_1123
_jana_atom_site_ADP_D_1133
_jana_atom_site_ADP_D_1222
_jana_atom_site_ADP_D_1223
_jana_atom_site_ADP_D_1233
_jana_atom_site_ADP_D_1333
_jana_atom_site_ADP_D_2222
_jana_atom_site_ADP_D_2223
_jana_atom_site_ADP_D_2233
_jana_atom_site_ADP_D_2333
_jana_atom_site_ADP_D_3333
Sm1 Sm 0.00015(4) 0 0 0.000066(12) 0 0.000066(12) 0 0 0 0 0.00015(4) 0
0.000066(12) 0 0.00015(4)
Ga1 Ga 0.0006(3) 0 0 0 0 0 0 0 0 0 0 0 0.00010(3) 0 0
Ge1 Ge 0.0006(3) 0 0 0 0 0 0 0 0 0 0 0 0.00010(3) 0 0

loop_
_jana_atom_site_ADP_E_label
_jana_atom_site_ADP_E_type_symbol
_jana_atom_site_ADP_E_11111
_jana_atom_site_ADP_E_11112
_jana_atom_site_ADP_E_11113
_jana_atom_site_ADP_E_11122
_jana_atom_site_ADP_E_11123
_jana_atom_site_ADP_E_11133
_jana_atom_site_ADP_E_11222
_jana_atom_site_ADP_E_11223
_jana_atom_site_ADP_E_11233
_jana_atom_site_ADP_E_11333
_jana_atom_site_ADP_E_12222
_jana_atom_site_ADP_E_12223
_jana_atom_site_ADP_E_12233
_jana_atom_site_ADP_E_12333
_jana_atom_site_ADP_E_13333
_jana_atom_site_ADP_E_22222
_jana_atom_site_ADP_E_22223
_jana_atom_site_ADP_E_22233
_jana_atom_site_ADP_E_22333
_jana_atom_site_ADP_E_23333
_jana_atom_site_ADP_E_33333
Ga1 Ga 0.0025(3) 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0
Ge1 Ge 0.0025(3) 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

loop_
_jana_atom_site_ADP_F_label
_jana_atom_site_ADP_F_type_symbol
_jana_atom_site_ADP_F_111111
_jana_atom_site_ADP_F_111112
_jana_atom_site_ADP_F_111113
_jana_atom_site_ADP_F_111122
_jana_atom_site_ADP_F_111123
_jana_atom_site_ADP_F_111133
_jana_atom_site_ADP_F_111222
_jana_atom_site_ADP_F_111223
_jana_atom_site_ADP_F_111233
_jana_atom_site_ADP_F_111333
_jana_atom_site_ADP_F_112222
_jana_atom_site_ADP_F_112223
_jana_atom_site_ADP_F_112233
_jana_atom_site_ADP_F_112333
_jana_atom_site_ADP_F_113333
_jana_atom_site_ADP_F_122222
_jana_atom_site_ADP_F_122223
_jana_atom_site_ADP_F_122233
_jana_atom_site_ADP_F_122333
_jana_atom_site_ADP_F_123333
_jana_atom_site_ADP_F_133333
_jana_atom_site_ADP_F_222222
_jana_atom_site_ADP_F_222223
_jana_atom_site_ADP_F_222233
_jana_atom_site_ADP_F_222333
_jana_atom_site_ADP_F_223333
_jana_atom_site_ADP_F_233333
_jana_atom_site_ADP_F_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sm1 Mn1 . . 3.77267(15) ?
Sm1 Mn1 . 49_555 3.77267(15) ?
Sm1 Mn1 . 97_555 3.77267(15) ?
Sm1 Mn1 . 145_555 3.77267(15) ?
Sm1 Ga1 . . 3.0887(2) ?
Sm1 Ga1 . 49_555 3.0887(2) ?
Sm1 Ga1 . 98_555 3.0887(2) ?
Sm1 Ga1 . 146_555 3.0887(2) ?
Sm1 Ga1 . 5_555 3.0887(2) ?
Sm1 Ga1 . 101_555 3.0887(2) ?
Sm1 Ga1 . 54_555 3.0887(2) ?
Sm1 Ga1 . 150_555 3.0887(2) ?
Sm1 Ga1 . 9_555 3.0887(2) ?
Sm1 Ga1 . 153_555 3.0887(2) ?
Sm1 Ga1 . 58_555 3.0887(2) ?
Sm1 Ga1 . 106_555 3.0887(2) ?
Sm1 Ge1 . . 3.0887(2) ?
Sm1 Ge1 . 49_555 3.0887(2) ?
Sm1 Ge1 . 98_555 3.0887(2) ?
Sm1 Ge1 . 146_555 3.0887(2) ?
Sm1 Ge1 . 5_555 3.0887(2) ?
Sm1 Ge1 . 101_555 3.0887(2) ?
Sm1 Ge1 . 54_555 3.0887(2) ?
Sm1 Ge1 . 150_555 3.0887(2) ?
Sm1 Ge1 . 9_555 3.0887(2) ?
Sm1 Ge1 . 153_555 3.0887(2) ?
Sm1 Ge1 . 58_555 3.0887(2) ?
Sm1 Ge1 . 106_555 3.0887(2) ?
Mn1 Ga1 . . 2.4045(18) ?
Mn1 Ga1 . 2_555 2.4045(18) ?
Mn1 Ga1 . 5_555 2.4045(18) ?
Mn1 Ga1 . 6_555 2.4045(18) ?
Mn1 Ga1 . 9_555 2.4045(18) ?
Mn1 Ga1 . 10_555 2.4045(18) ?
Mn1 Ge1 . . 2.4045(18) ?
Mn1 Ge1 . 2_555 2.4045(18) ?
Mn1 Ge1 . 5_555 2.4045(18) ?
Mn1 Ge1 . 6_555 2.4045(18) ?
Mn1 Ge1 . 9_555 2.4045(18) ?
Mn1 Ge1 . 10_555 2.4045(18) ?
Ga1 Ga1 . 5_555 3.4005(18) ?
Ga1 Ga1 . 149_545 2.7602(18) ?
Ga1 Ga1 . 6_555 3.4005(18) ?
Ga1 Ga1 . 150_555 2.7602(18) ?
Ga1 Ga1 . 9_555 3.4005(18) ?
Ga1 Ga1 . 105_554 2.7602(18) ?
Ga1 Ga1 . 10_555 3.4005(18) ?
Ga1 Ga1 . 106_555 2.7602(18) ?
Ga1 Ge1 . 5_555 3.4005(18) ?
Ga1 Ge1 . 149_545 2.7602(18) ?
Ga1 Ge1 . 6_555 3.4005(18) ?
Ga1 Ge1 . 150_555 2.7602(18) ?
Ga1 Ge1 . 9_555 3.4005(18) ?
Ga1 Ge1 . 105_554 2.7602(18) ?
Ga1 Ge1 . 10_555 3.4005(18) ?
Ga1 Ge1 . 106_555 2.7602(18) ?
Ge1 Ge1 . 5_555 3.4005(18) ?
Ge1 Ge1 . 149_545 2.7602(18) ?
Ge1 Ge1 . 6_555 3.4005(18) ?
Ge1 Ge1 . 150_555 2.7602(18) ?
Ge1 Ge1 . 9_555 3.4005(18) ?
Ge1 Ge1 . 105_554 2.7602(18) ?
Ge1 Ge1 . 10_555 3.4005(18) ?
Ge1 Ge1 . 106_555 2.7602(18) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Mn1 Sm1 Mn1 . . 49_555 109.471(2) ?
Mn1 Sm1 Mn1 . . 97_555 109.471(2) ?
Mn1 Sm1 Mn1 . . 145_555 109.471(2) ?
Mn1 Sm1 Ga1 . . . 39.47(3) ?
Mn1 Sm1 Ga1 . . 49_555 148.94(3) ?
Mn1 Sm1 Ga1 . . 98_555 87.575(19) ?
Mn1 Sm1 Ga1 . . 146_555 87.575(19) ?
Mn1 Sm1 Ga1 . . 5_555 39.47(3) ?
Mn1 Sm1 Ga1 . . 101_555 148.94(3) ?
Mn1 Sm1 Ga1 . . 54_555 87.575(19) ?
Mn1 Sm1 Ga1 . . 150_555 87.575(19) ?
Mn1 Sm1 Ga1 . . 9_555 39.47(3) ?
Mn1 Sm1 Ga1 . . 153_555 148.94(3) ?
Mn1 Sm1 Ga1 . . 58_555 87.575(19) ?
Mn1 Sm1 Ga1 . . 106_555 87.575(19) ?
Mn1 Sm1 Ge1 . . . 39.47(3) ?
Mn1 Sm1 Ge1 . . 49_555 148.94(3) ?
Mn1 Sm1 Ge1 . . 98_555 87.575(19) ?
Mn1 Sm1 Ge1 . . 146_555 87.575(19) ?
Mn1 Sm1 Ge1 . . 5_555 39.47(3) ?
Mn1 Sm1 Ge1 . . 101_555 148.94(3) ?
Mn1 Sm1 Ge1 . . 54_555 87.575(19) ?
Mn1 Sm1 Ge1 . . 150_555 87.575(19) ?
Mn1 Sm1 Ge1 . . 9_555 39.47(3) ?
Mn1 Sm1 Ge1 . . 153_555 148.94(3) ?
Mn1 Sm1 Ge1 . . 58_555 87.575(19) ?
Mn1 Sm1 Ge1 . . 106_555 87.575(19) ?
Mn1 Sm1 Mn1 49_555 . 97_555 109.471(2) ?
Mn1 Sm1 Mn1 49_555 . 145_555 109.471(2) ?
Mn1 Sm1 Ga1 49_555 . . 148.94(3) ?
Mn1 Sm1 Ga1 49_555 . 49_555 39.47(3) ?
Mn1 Sm1 Ga1 49_555 . 98_555 87.575(19) ?
Mn1 Sm1 Ga1 49_555 . 146_555 87.575(19) ?
Mn1 Sm1 Ga1 49_555 . 5_555 87.575(19) ?
Mn1 Sm1 Ga1 49_555 . 101_555 87.575(19) ?
Mn1 Sm1 Ga1 49_555 . 54_555 39.47(3) ?
Mn1 Sm1 Ga1 49_555 . 150_555 148.94(3) ?
Mn1 Sm1 Ga1 49_555 . 9_555 87.575(19) ?
Mn1 Sm1 Ga1 49_555 . 153_555 87.575(19) ?
Mn1 Sm1 Ga1 49_555 . 58_555 39.47(3) ?
Mn1 Sm1 Ga1 49_555 . 106_555 148.94(3) ?
Mn1 Sm1 Ge1 49_555 . . 148.94(3) ?
Mn1 Sm1 Ge1 49_555 . 49_555 39.47(3) ?
Mn1 Sm1 Ge1 49_555 . 98_555 87.575(19) ?
Mn1 Sm1 Ge1 49_555 . 146_555 87.575(19) ?
Mn1 Sm1 Ge1 49_555 . 5_555 87.575(19) ?
Mn1 Sm1 Ge1 49_555 . 101_555 87.575(19) ?
Mn1 Sm1 Ge1 49_555 . 54_555 39.47(3) ?
Mn1 Sm1 Ge1 49_555 . 150_555 148.94(3) ?
Mn1 Sm1 Ge1 49_555 . 9_555 87.575(19) ?
Mn1 Sm1 Ge1 49_555 . 153_555 87.575(19) ?
Mn1 Sm1 Ge1 49_555 . 58_555 39.47(3) ?
Mn1 Sm1 Ge1 49_555 . 106_555 148.94(3) ?
Mn1 Sm1 Mn1 97_555 . 145_555 109.471(2) ?
Mn1 Sm1 Ga1 97_555 . . 87.575(19) ?
Mn1 Sm1 Ga1 97_555 . 49_555 87.575(19) ?
Mn1 Sm1 Ga1 97_555 . 98_555 39.47(3) ?
Mn1 Sm1 Ga1 97_555 . 146_555 148.94(3) ?
Mn1 Sm1 Ga1 97_555 . 5_555 148.94(3) ?
Mn1 Sm1 Ga1 97_555 . 101_555 39.47(3) ?
Mn1 Sm1 Ga1 97_555 . 54_555 87.575(19) ?
Mn1 Sm1 Ga1 97_555 . 150_555 87.575(19) ?
Mn1 Sm1 Ga1 97_555 . 9_555 87.575(19) ?
Mn1 Sm1 Ga1 97_555 . 153_555 87.575(19) ?
Mn1 Sm1 Ga1 97_555 . 58_555 148.94(3) ?
Mn1 Sm1 Ga1 97_555 . 106_555 39.47(3) ?
Mn1 Sm1 Ge1 97_555 . . 87.575(19) ?
Mn1 Sm1 Ge1 97_555 . 49_555 87.575(19) ?
Mn1 Sm1 Ge1 97_555 . 98_555 39.47(3) ?
Mn1 Sm1 Ge1 97_555 . 146_555 148.94(3) ?
Mn1 Sm1 Ge1 97_555 . 5_555 148.94(3) ?
Mn1 Sm1 Ge1 97_555 . 101_555 39.47(3) ?
Mn1 Sm1 Ge1 97_555 . 54_555 87.575(19) ?
Mn1 Sm1 Ge1 97_555 . 150_555 87.575(19) ?
Mn1 Sm1 Ge1 97_555 . 9_555 87.575(19) ?
Mn1 Sm1 Ge1 97_555 . 153_555 87.575(19) ?
Mn1 Sm1 Ge1 97_555 . 58_555 148.94(3) ?
Mn1 Sm1 Ge1 97_555 . 106_555 39.47(3) ?
Mn1 Sm1 Ga1 145_555 . . 87.575(19) ?
Mn1 Sm1 Ga1 145_555 . 49_555 87.575(19) ?
Mn1 Sm1 Ga1 145_555 . 98_555 148.94(3) ?
Mn1 Sm1 Ga1 145_555 . 146_555 39.47(3) ?
Mn1 Sm1 Ga1 145_555 . 5_555 87.575(19) ?
Mn1 Sm1 Ga1 145_555 . 101_555 87.575(19) ?
Mn1 Sm1 Ga1 145_555 . 54_555 148.94(3) ?
Mn1 Sm1 Ga1 145_555 . 150_555 39.47(3) ?
Mn1 Sm1 Ga1 145_555 . 9_555 148.94(3) ?
Mn1 Sm1 Ga1 145_555 . 153_555 39.47(3) ?
Mn1 Sm1 Ga1 145_555 . 58_555 87.575(19) ?
Mn1 Sm1 Ga1 145_555 . 106_555 87.575(19) ?
Mn1 Sm1 Ge1 145_555 . . 87.575(19) ?
Mn1 Sm1 Ge1 145_555 . 49_555 87.575(19) ?
Mn1 Sm1 Ge1 145_555 . 98_555 148.94(3) ?
Mn1 Sm1 Ge1 145_555 . 146_555 39.47(3) ?
Mn1 Sm1 Ge1 145_555 . 5_555 87.575(19) ?
Mn1 Sm1 Ge1 145_555 . 101_555 87.575(19) ?
Mn1 Sm1 Ge1 145_555 . 54_555 148.94(3) ?
Mn1 Sm1 Ge1 145_555 . 150_555 39.47(3) ?
Mn1 Sm1 Ge1 145_555 . 9_555 148.94(3) ?
Mn1 Sm1 Ge1 145_555 . 153_555 39.47(3) ?
Mn1 Sm1 Ge1 145_555 . 58_555 87.575(19) ?
Mn1 Sm1 Ge1 145_555 . 106_555 87.575(19) ?
Ga1 Sm1 Ga1 . . 49_555 171.59(5) ?
Ga1 Sm1 Ga1 . . 98_555 90.308(4) ?
Ga1 Sm1 Ga1 . . 146_555 90.308(4) ?
Ga1 Sm1 Ga1 . . 5_555 66.80(4) ?
Ga1 Sm1 Ga1 . . 101_555 119.82(4) ?
Ga1 Sm1 Ga1 . . 54_555 119.82(4) ?
Ga1 Sm1 Ga1 . . 150_555 53.08(4) ?
Ga1 Sm1 Ga1 . . 9_555 66.80(4) ?
Ga1 Sm1 Ga1 . . 153_555 119.82(4) ?
Ga1 Sm1 Ga1 . . 58_555 119.82(4) ?
Ga1 Sm1 Ga1 . . 106_555 53.08(4) ?
Ga1 Sm1 Ge1 . . . 0 ?
Ga1 Sm1 Ge1 . . 49_555 171.59(5) ?
Ga1 Sm1 Ge1 . . 98_555 90.308(4) ?
Ga1 Sm1 Ge1 . . 146_555 90.308(4) ?
Ga1 Sm1 Ge1 . . 5_555 66.80(4) ?
Ga1 Sm1 Ge1 . . 101_555 119.82(4) ?
Ga1 Sm1 Ge1 . . 54_555 119.82(4) ?
Ga1 Sm1 Ge1 . . 150_555 53.08(4) ?
Ga1 Sm1 Ge1 . . 9_555 66.80(4) ?
Ga1 Sm1 Ge1 . . 153_555 119.82(4) ?
Ga1 Sm1 Ge1 . . 58_555 119.82(4) ?
Ga1 Sm1 Ge1 . . 106_555 53.08(4) ?
Ga1 Sm1 Ga1 49_555 . 98_555 90.308(4) ?
Ga1 Sm1 Ga1 49_555 . 146_555 90.308(4) ?
Ga1 Sm1 Ga1 49_555 . 5_555 119.82(4) ?
Ga1 Sm1 Ga1 49_555 . 101_555 53.08(4) ?
Ga1 Sm1 Ga1 49_555 . 54_555 66.80(4) ?
Ga1 Sm1 Ga1 49_555 . 150_555 119.82(4) ?
Ga1 Sm1 Ga1 49_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ga1 49_555 . 153_555 53.08(4) ?
Ga1 Sm1 Ga1 49_555 . 58_555 66.80(4) ?
Ga1 Sm1 Ga1 49_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ge1 49_555 . . 171.59(5) ?
Ga1 Sm1 Ge1 49_555 . 49_555 0 ?
Ga1 Sm1 Ge1 49_555 . 98_555 90.308(4) ?
Ga1 Sm1 Ge1 49_555 . 146_555 90.308(4) ?
Ga1 Sm1 Ge1 49_555 . 5_555 119.82(4) ?
Ga1 Sm1 Ge1 49_555 . 101_555 53.08(4) ?
Ga1 Sm1 Ge1 49_555 . 54_555 66.80(4) ?
Ga1 Sm1 Ge1 49_555 . 150_555 119.82(4) ?
Ga1 Sm1 Ge1 49_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ge1 49_555 . 153_555 53.08(4) ?
Ga1 Sm1 Ge1 49_555 . 58_555 66.80(4) ?
Ga1 Sm1 Ge1 49_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ga1 98_555 . 146_555 171.59(5) ?
Ga1 Sm1 Ga1 98_555 . 5_555 119.82(4) ?
Ga1 Sm1 Ga1 98_555 . 101_555 66.80(4) ?
Ga1 Sm1 Ga1 98_555 . 54_555 53.08(4) ?
Ga1 Sm1 Ga1 98_555 . 150_555 119.82(4) ?
Ga1 Sm1 Ga1 98_555 . 9_555 53.08(4) ?
Ga1 Sm1 Ga1 98_555 . 153_555 119.82(4) ?
Ga1 Sm1 Ga1 98_555 . 58_555 119.82(4) ?
Ga1 Sm1 Ga1 98_555 . 106_555 66.80(4) ?
Ga1 Sm1 Ge1 98_555 . . 90.308(4) ?
Ga1 Sm1 Ge1 98_555 . 49_555 90.308(4) ?
Ga1 Sm1 Ge1 98_555 . 98_555 0 ?
Ga1 Sm1 Ge1 98_555 . 146_555 171.59(5) ?
Ga1 Sm1 Ge1 98_555 . 5_555 119.82(4) ?
Ga1 Sm1 Ge1 98_555 . 101_555 66.80(4) ?
Ga1 Sm1 Ge1 98_555 . 54_555 53.08(4) ?
Ga1 Sm1 Ge1 98_555 . 150_555 119.82(4) ?
Ga1 Sm1 Ge1 98_555 . 9_555 53.08(4) ?
Ga1 Sm1 Ge1 98_555 . 153_555 119.82(4) ?
Ga1 Sm1 Ge1 98_555 . 58_555 119.82(4) ?
Ga1 Sm1 Ge1 98_555 . 106_555 66.80(4) ?
Ga1 Sm1 Ga1 146_555 . 5_555 53.08(4) ?
Ga1 Sm1 Ga1 146_555 . 101_555 119.82(4) ?
Ga1 Sm1 Ga1 146_555 . 54_555 119.82(4) ?
Ga1 Sm1 Ga1 146_555 . 150_555 66.80(4) ?
Ga1 Sm1 Ga1 146_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ga1 146_555 . 153_555 66.80(4) ?
Ga1 Sm1 Ga1 146_555 . 58_555 53.08(4) ?
Ga1 Sm1 Ga1 146_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ge1 146_555 . . 90.308(4) ?
Ga1 Sm1 Ge1 146_555 . 49_555 90.308(4) ?
Ga1 Sm1 Ge1 146_555 . 98_555 171.59(5) ?
Ga1 Sm1 Ge1 146_555 . 146_555 0 ?
Ga1 Sm1 Ge1 146_555 . 5_555 53.08(4) ?
Ga1 Sm1 Ge1 146_555 . 101_555 119.82(4) ?
Ga1 Sm1 Ge1 146_555 . 54_555 119.82(4) ?
Ga1 Sm1 Ge1 146_555 . 150_555 66.80(4) ?
Ga1 Sm1 Ge1 146_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ge1 146_555 . 153_555 66.80(4) ?
Ga1 Sm1 Ge1 146_555 . 58_555 53.08(4) ?
Ga1 Sm1 Ge1 146_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ga1 5_555 . 101_555 171.59(5) ?
Ga1 Sm1 Ga1 5_555 . 54_555 90.308(4) ?
Ga1 Sm1 Ga1 5_555 . 150_555 90.308(4) ?
Ga1 Sm1 Ga1 5_555 . 9_555 66.80(4) ?
Ga1 Sm1 Ga1 5_555 . 153_555 119.82(4) ?
Ga1 Sm1 Ga1 5_555 . 58_555 53.08(4) ?
Ga1 Sm1 Ga1 5_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ge1 5_555 . . 66.80(4) ?
Ga1 Sm1 Ge1 5_555 . 49_555 119.82(4) ?
Ga1 Sm1 Ge1 5_555 . 98_555 119.82(4) ?
Ga1 Sm1 Ge1 5_555 . 146_555 53.08(4) ?
Ga1 Sm1 Ge1 5_555 . 5_555 0 ?
Ga1 Sm1 Ge1 5_555 . 101_555 171.59(5) ?
Ga1 Sm1 Ge1 5_555 . 54_555 90.308(4) ?
Ga1 Sm1 Ge1 5_555 . 150_555 90.308(4) ?
Ga1 Sm1 Ge1 5_555 . 9_555 66.80(4) ?
Ga1 Sm1 Ge1 5_555 . 153_555 119.82(4) ?
Ga1 Sm1 Ge1 5_555 . 58_555 53.08(4) ?
Ga1 Sm1 Ge1 5_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ga1 101_555 . 54_555 90.308(4) ?
Ga1 Sm1 Ga1 101_555 . 150_555 90.308(4) ?
Ga1 Sm1 Ga1 101_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ga1 101_555 . 153_555 53.08(4) ?
Ga1 Sm1 Ga1 101_555 . 58_555 119.82(4) ?
Ga1 Sm1 Ga1 101_555 . 106_555 66.80(4) ?
Ga1 Sm1 Ge1 101_555 . . 119.82(4) ?
Ga1 Sm1 Ge1 101_555 . 49_555 53.08(4) ?
Ga1 Sm1 Ge1 101_555 . 98_555 66.80(4) ?
Ga1 Sm1 Ge1 101_555 . 146_555 119.82(4) ?
Ga1 Sm1 Ge1 101_555 . 5_555 171.59(5) ?
Ga1 Sm1 Ge1 101_555 . 101_555 0 ?
Ga1 Sm1 Ge1 101_555 . 54_555 90.308(4) ?
Ga1 Sm1 Ge1 101_555 . 150_555 90.308(4) ?
Ga1 Sm1 Ge1 101_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ge1 101_555 . 153_555 53.08(4) ?
Ga1 Sm1 Ge1 101_555 . 58_555 119.82(4) ?
Ga1 Sm1 Ge1 101_555 . 106_555 66.80(4) ?
Ga1 Sm1 Ga1 54_555 . 150_555 171.59(5) ?
Ga1 Sm1 Ga1 54_555 . 9_555 53.08(4) ?
Ga1 Sm1 Ga1 54_555 . 153_555 119.82(4) ?
Ga1 Sm1 Ga1 54_555 . 58_555 66.80(4) ?
Ga1 Sm1 Ga1 54_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ge1 54_555 . . 119.82(4) ?
Ga1 Sm1 Ge1 54_555 . 49_555 66.80(4) ?
Ga1 Sm1 Ge1 54_555 . 98_555 53.08(4) ?
Ga1 Sm1 Ge1 54_555 . 146_555 119.82(4) ?
Ga1 Sm1 Ge1 54_555 . 5_555 90.308(4) ?
Ga1 Sm1 Ge1 54_555 . 101_555 90.308(4) ?
Ga1 Sm1 Ge1 54_555 . 54_555 0 ?
Ga1 Sm1 Ge1 54_555 . 150_555 171.59(5) ?
Ga1 Sm1 Ge1 54_555 . 9_555 53.08(4) ?
Ga1 Sm1 Ge1 54_555 . 153_555 119.82(4) ?
Ga1 Sm1 Ge1 54_555 . 58_555 66.80(4) ?
Ga1 Sm1 Ge1 54_555 . 106_555 119.82(4) ?
Ga1 Sm1 Ga1 150_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ga1 150_555 . 153_555 66.80(4) ?
Ga1 Sm1 Ga1 150_555 . 58_555 119.82(4) ?
Ga1 Sm1 Ga1 150_555 . 106_555 53.08(4) ?
Ga1 Sm1 Ge1 150_555 . . 53.08(4) ?
Ga1 Sm1 Ge1 150_555 . 49_555 119.82(4) ?
Ga1 Sm1 Ge1 150_555 . 98_555 119.82(4) ?
Ga1 Sm1 Ge1 150_555 . 146_555 66.80(4) ?
Ga1 Sm1 Ge1 150_555 . 5_555 90.308(4) ?
Ga1 Sm1 Ge1 150_555 . 101_555 90.308(4) ?
Ga1 Sm1 Ge1 150_555 . 54_555 171.59(5) ?
Ga1 Sm1 Ge1 150_555 . 150_555 0 ?
Ga1 Sm1 Ge1 150_555 . 9_555 119.82(4) ?
Ga1 Sm1 Ge1 150_555 . 153_555 66.80(4) ?
Ga1 Sm1 Ge1 150_555 . 58_555 119.82(4) ?
Ga1 Sm1 Ge1 150_555 . 106_555 53.08(4) ?
Ga1 Sm1 Ga1 9_555 . 153_555 171.59(5) ?
Ga1 Sm1 Ga1 9_555 . 58_555 90.308(4) ?
Ga1 Sm1 Ga1 9_555 . 106_555 90.308(4) ?
Ga1 Sm1 Ge1 9_555 . . 66.80(4) ?
Ga1 Sm1 Ge1 9_555 . 49_555 119.82(4) ?
Ga1 Sm1 Ge1 9_555 . 98_555 53.08(4) ?
Ga1 Sm1 Ge1 9_555 . 146_555 119.82(4) ?
Ga1 Sm1 Ge1 9_555 . 5_555 66.80(4) ?
Ga1 Sm1 Ge1 9_555 . 101_555 119.82(4) ?
Ga1 Sm1 Ge1 9_555 . 54_555 53.08(4) ?
Ga1 Sm1 Ge1 9_555 . 150_555 119.82(4) ?
Ga1 Sm1 Ge1 9_555 . 9_555 0 ?
Ga1 Sm1 Ge1 9_555 . 153_555 171.59(5) ?
Ga1 Sm1 Ge1 9_555 . 58_555 90.308(4) ?
Ga1 Sm1 Ge1 9_555 . 106_555 90.308(4) ?
Ga1 Sm1 Ga1 153_555 . 58_555 90.308(4) ?
Ga1 Sm1 Ga1 153_555 . 106_555 90.308(4) ?
Ga1 Sm1 Ge1 153_555 . . 119.82(4) ?
Ga1 Sm1 Ge1 153_555 . 49_555 53.08(4) ?
Ga1 Sm1 Ge1 153_555 . 98_555 119.82(4) ?
Ga1 Sm1 Ge1 153_555 . 146_555 66.80(4) ?
Ga1 Sm1 Ge1 153_555 . 5_555 119.82(4) ?
Ga1 Sm1 Ge1 153_555 . 101_555 53.08(4) ?
Ga1 Sm1 Ge1 153_555 . 54_555 119.82(4) ?
Ga1 Sm1 Ge1 153_555 . 150_555 66.80(4) ?
Ga1 Sm1 Ge1 153_555 . 9_555 171.59(5) ?
Ga1 Sm1 Ge1 153_555 . 153_555 0 ?
Ga1 Sm1 Ge1 153_555 . 58_555 90.308(4) ?
Ga1 Sm1 Ge1 153_555 . 106_555 90.308(4) ?
Ga1 Sm1 Ga1 58_555 . 106_555 171.59(5) ?
Ga1 Sm1 Ge1 58_555 . . 119.82(4) ?
Ga1 Sm1 Ge1 58_555 . 49_555 66.80(4) ?
Ga1 Sm1 Ge1 58_555 . 98_555 119.82(4) ?
Ga1 Sm1 Ge1 58_555 . 146_555 53.08(4) ?
Ga1 Sm1 Ge1 58_555 . 5_555 53.08(4) ?
Ga1 Sm1 Ge1 58_555 . 101_555 119.82(4) ?
Ga1 Sm1 Ge1 58_555 . 54_555 66.80(4) ?
Ga1 Sm1 Ge1 58_555 . 150_555 119.82(4) ?
Ga1 Sm1 Ge1 58_555 . 9_555 90.308(4) ?
Ga1 Sm1 Ge1 58_555 . 153_555 90.308(4) ?
Ga1 Sm1 Ge1 58_555 . 58_555 0 ?
Ga1 Sm1 Ge1 58_555 . 106_555 171.59(5) ?
Ga1 Sm1 Ge1 106_555 . . 53.08(4) ?
Ga1 Sm1 Ge1 106_555 . 49_555 119.82(4) ?
Ga1 Sm1 Ge1 106_555 . 98_555 66.80(4) ?
Ga1 Sm1 Ge1 106_555 . 146_555 119.82(4) ?
Ga1 Sm1 Ge1 106_555 . 5_555 119.82(4) ?
Ga1 Sm1 Ge1 106_555 . 101_555 66.80(4) ?
Ga1 Sm1 Ge1 106_555 . 54_555 119.82(4) ?
Ga1 Sm1 Ge1 106_555 . 150_555 53.08(4) ?
Ga1 Sm1 Ge1 106_555 . 9_555 90.308(4) ?
Ga1 Sm1 Ge1 106_555 . 153_555 90.308(4) ?
Ga1 Sm1 Ge1 106_555 . 58_555 171.59(5) ?
Ga1 Sm1 Ge1 106_555 . 106_555 0 ?
Ge1 Sm1 Ge1 . . 49_555 171.59(5) ?
Ge1 Sm1 Ge1 . . 98_555 90.308(4) ?
Ge1 Sm1 Ge1 . . 146_555 90.308(4) ?
Ge1 Sm1 Ge1 . . 5_555 66.80(4) ?
Ge1 Sm1 Ge1 . . 101_555 119.82(4) ?
Ge1 Sm1 Ge1 . . 54_555 119.82(4) ?
Ge1 Sm1 Ge1 . . 150_555 53.08(4) ?
Ge1 Sm1 Ge1 . . 9_555 66.80(4) ?
Ge1 Sm1 Ge1 . . 153_555 119.82(4) ?
Ge1 Sm1 Ge1 . . 58_555 119.82(4) ?
Ge1 Sm1 Ge1 . . 106_555 53.08(4) ?
Ge1 Sm1 Ge1 49_555 . 98_555 90.308(4) ?
Ge1 Sm1 Ge1 49_555 . 146_555 90.308(4) ?
Ge1 Sm1 Ge1 49_555 . 5_555 119.82(4) ?
Ge1 Sm1 Ge1 49_555 . 101_555 53.08(4) ?
Ge1 Sm1 Ge1 49_555 . 54_555 66.80(4) ?
Ge1 Sm1 Ge1 49_555 . 150_555 119.82(4) ?
Ge1 Sm1 Ge1 49_555 . 9_555 119.82(4) ?
Ge1 Sm1 Ge1 49_555 . 153_555 53.08(4) ?
Ge1 Sm1 Ge1 49_555 . 58_555 66.80(4) ?
Ge1 Sm1 Ge1 49_555 . 106_555 119.82(4) ?
Ge1 Sm1 Ge1 98_555 . 146_555 171.59(5) ?
Ge1 Sm1 Ge1 98_555 . 5_555 119.82(4) ?
Ge1 Sm1 Ge1 98_555 . 101_555 66.80(4) ?
Ge1 Sm1 Ge1 98_555 . 54_555 53.08(4) ?
Ge1 Sm1 Ge1 98_555 . 150_555 119.82(4) ?
Ge1 Sm1 Ge1 98_555 . 9_555 53.08(4) ?
Ge1 Sm1 Ge1 98_555 . 153_555 119.82(4) ?
Ge1 Sm1 Ge1 98_555 . 58_555 119.82(4) ?
Ge1 Sm1 Ge1 98_555 . 106_555 66.80(4) ?
Ge1 Sm1 Ge1 146_555 . 5_555 53.08(4) ?
Ge1 Sm1 Ge1 146_555 . 101_555 119.82(4) ?
Ge1 Sm1 Ge1 146_555 . 54_555 119.82(4) ?
Ge1 Sm1 Ge1 146_555 . 150_555 66.80(4) ?
Ge1 Sm1 Ge1 146_555 . 9_555 119.82(4) ?
Ge1 Sm1 Ge1 146_555 . 153_555 66.80(4) ?
Ge1 Sm1 Ge1 146_555 . 58_555 53.08(4) ?
Ge1 Sm1 Ge1 146_555 . 106_555 119.82(4) ?
Ge1 Sm1 Ge1 5_555 . 101_555 171.59(5) ?
Ge1 Sm1 Ge1 5_555 . 54_555 90.308(4) ?
Ge1 Sm1 Ge1 5_555 . 150_555 90.308(4) ?
Ge1 Sm1 Ge1 5_555 . 9_555 66.80(4) ?
Ge1 Sm1 Ge1 5_555 . 153_555 119.82(4) ?
Ge1 Sm1 Ge1 5_555 . 58_555 53.08(4) ?
Ge1 Sm1 Ge1 5_555 . 106_555 119.82(4) ?
Ge1 Sm1 Ge1 101_555 . 54_555 90.308(4) ?
Ge1 Sm1 Ge1 101_555 . 150_555 90.308(4) ?
Ge1 Sm1 Ge1 101_555 . 9_555 119.82(4) ?
Ge1 Sm1 Ge1 101_555 . 153_555 53.08(4) ?
Ge1 Sm1 Ge1 101_555 . 58_555 119.82(4) ?
Ge1 Sm1 Ge1 101_555 . 106_555 66.80(4) ?
Ge1 Sm1 Ge1 54_555 . 150_555 171.59(5) ?
Ge1 Sm1 Ge1 54_555 . 9_555 53.08(4) ?
Ge1 Sm1 Ge1 54_555 . 153_555 119.82(4) ?
Ge1 Sm1 Ge1 54_555 . 58_555 66.80(4) ?
Ge1 Sm1 Ge1 54_555 . 106_555 119.82(4) ?
Ge1 Sm1 Ge1 150_555 . 9_555 119.82(4) ?
Ge1 Sm1 Ge1 150_555 . 153_555 66.80(4) ?
Ge1 Sm1 Ge1 150_555 . 58_555 119.82(4) ?
Ge1 Sm1 Ge1 150_555 . 106_555 53.08(4) ?
Ge1 Sm1 Ge1 9_555 . 153_555 171.59(5) ?
Ge1 Sm1 Ge1 9_555 . 58_555 90.308(4) ?
Ge1 Sm1 Ge1 9_555 . 106_555 90.308(4) ?
Ge1 Sm1 Ge1 153_555 . 58_555 90.308(4) ?
Ge1 Sm1 Ge1 153_555 . 106_555 90.308(4) ?
Ge1 Sm1 Ge1 58_555 . 106_555 171.59(5) ?
Sm1 Mn1 Sm1 . . 49_544 109.471(2) ?
Sm1 Mn1 Sm1 . . 97_454 109.471(2) ?
Sm1 Mn1 Sm1 . . 145_445 109.471(2) ?
Sm1 Mn1 Sm1 . . 13_555 70.529(2) ?
Sm1 Mn1 Sm1 . . 61_545 70.529(2) ?
Sm1 Mn1 Sm1 . . 109_455 70.529(2) ?
Sm1 Mn1 Sm1 . . 157_445 180 ?
Sm1 Mn1 Ga1 . . . 54.7356(11) ?
Sm1 Mn1 Ga1 . . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 . . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 . . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 . . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 . . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 . . . 54.7356(11) ?
Sm1 Mn1 Ge1 . . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 . . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 . . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 . . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 . . 10_555 125.2644(11) ?
Sm1 Mn1 Sm1 49_544 . 97_454 109.471(2) ?
Sm1 Mn1 Sm1 49_544 . 145_445 109.471(2) ?
Sm1 Mn1 Sm1 49_544 . 13_555 70.529(2) ?
Sm1 Mn1 Sm1 49_544 . 61_545 70.529(2) ?
Sm1 Mn1 Sm1 49_544 . 109_455 180 ?
Sm1 Mn1 Sm1 49_544 . 157_445 70.529(2) ?
Sm1 Mn1 Ga1 49_544 . . 54.7356(11) ?
Sm1 Mn1 Ga1 49_544 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 49_544 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 49_544 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 49_544 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 49_544 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 49_544 . . 54.7356(11) ?
Sm1 Mn1 Ge1 49_544 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 49_544 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 49_544 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 49_544 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 49_544 . 10_555 54.7356(11) ?
Sm1 Mn1 Sm1 97_454 . 145_445 109.471(2) ?
Sm1 Mn1 Sm1 97_454 . 13_555 70.529(2) ?
Sm1 Mn1 Sm1 97_454 . 61_545 180 ?
Sm1 Mn1 Sm1 97_454 . 109_455 70.529(2) ?
Sm1 Mn1 Sm1 97_454 . 157_445 70.529(2) ?
Sm1 Mn1 Ga1 97_454 . . 125.2644(11) ?
Sm1 Mn1 Ga1 97_454 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 97_454 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 97_454 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 97_454 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 97_454 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 97_454 . . 125.2644(11) ?
Sm1 Mn1 Ge1 97_454 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 97_454 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 97_454 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 97_454 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 97_454 . 10_555 54.7356(11) ?
Sm1 Mn1 Sm1 145_445 . 13_555 180 ?
Sm1 Mn1 Sm1 145_445 . 61_545 70.529(2) ?
Sm1 Mn1 Sm1 145_445 . 109_455 70.529(2) ?
Sm1 Mn1 Sm1 145_445 . 157_445 70.529(2) ?
Sm1 Mn1 Ga1 145_445 . . 125.2644(11) ?
Sm1 Mn1 Ga1 145_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 145_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 145_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 145_445 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 145_445 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 145_445 . . 125.2644(11) ?
Sm1 Mn1 Ge1 145_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 145_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 145_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 145_445 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 145_445 . 10_555 125.2644(11) ?
Sm1 Mn1 Sm1 13_555 . 61_545 109.471(2) ?
Sm1 Mn1 Sm1 13_555 . 109_455 109.471(2) ?
Sm1 Mn1 Sm1 13_555 . 157_445 109.471(2) ?
Sm1 Mn1 Ga1 13_555 . . 54.7356(11) ?
Sm1 Mn1 Ga1 13_555 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 13_555 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 13_555 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 13_555 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 13_555 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 13_555 . . 54.7356(11) ?
Sm1 Mn1 Ge1 13_555 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 13_555 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 13_555 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 13_555 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 13_555 . 10_555 54.7356(11) ?
Sm1 Mn1 Sm1 61_545 . 109_455 109.471(2) ?
Sm1 Mn1 Sm1 61_545 . 157_445 109.471(2) ?
Sm1 Mn1 Ga1 61_545 . . 54.7356(11) ?
Sm1 Mn1 Ga1 61_545 . 2_555 125.2644(11) ?
Sm1 Mn1 Ga1 61_545 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 61_545 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 61_545 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 61_545 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 61_545 . . 54.7356(11) ?
Sm1 Mn1 Ge1 61_545 . 2_555 125.2644(11) ?
Sm1 Mn1 Ge1 61_545 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 61_545 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 61_545 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 61_545 . 10_555 125.2644(11) ?
Sm1 Mn1 Sm1 109_455 . 157_445 109.471(2) ?
Sm1 Mn1 Ga1 109_455 . . 125.2644(11) ?
Sm1 Mn1 Ga1 109_455 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 109_455 . 5_555 54.7356(11) ?
Sm1 Mn1 Ga1 109_455 . 6_555 125.2644(11) ?
Sm1 Mn1 Ga1 109_455 . 9_555 54.7356(11) ?
Sm1 Mn1 Ga1 109_455 . 10_555 125.2644(11) ?
Sm1 Mn1 Ge1 109_455 . . 125.2644(11) ?
Sm1 Mn1 Ge1 109_455 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 109_455 . 5_555 54.7356(11) ?
Sm1 Mn1 Ge1 109_455 . 6_555 125.2644(11) ?
Sm1 Mn1 Ge1 109_455 . 9_555 54.7356(11) ?
Sm1 Mn1 Ge1 109_455 . 10_555 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . . 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ga1 157_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ga1 157_445 . 9_555 125.2644(11) ?
Sm1 Mn1 Ga1 157_445 . 10_555 54.7356(11) ?
Sm1 Mn1 Ge1 157_445 . . 125.2644(11) ?
Sm1 Mn1 Ge1 157_445 . 2_555 54.7356(11) ?
Sm1 Mn1 Ge1 157_445 . 5_555 125.2644(11) ?
Sm1 Mn1 Ge1 157_445 . 6_555 54.7356(11) ?
Sm1 Mn1 Ge1 157_445 . 9_555 125.2644(11) ?
Sm1 Mn1 Ge1 157_445 . 10_555 54.7356(11) ?
Ga1 Mn1 Ga1 . . 2_555 180 ?
Ga1 Mn1 Ga1 . . 5_555 90 ?
Ga1 Mn1 Ga1 . . 6_555 90 ?
Ga1 Mn1 Ga1 . . 9_555 90 ?
Ga1 Mn1 Ga1 . . 10_555 90 ?
Ga1 Mn1 Ge1 . . . 0 ?
Ga1 Mn1 Ge1 . . 2_555 180 ?
Ga1 Mn1 Ge1 . . 5_555 90 ?
Ga1 Mn1 Ge1 . . 6_555 90 ?
Ga1 Mn1 Ge1 . . 9_555 90 ?
Ga1 Mn1 Ge1 . . 10_555 90 ?
Ga1 Mn1 Ga1 2_555 . 5_555 90 ?
Ga1 Mn1 Ga1 2_555 . 6_555 90 ?
Ga1 Mn1 Ga1 2_555 . 9_555 90 ?
Ga1 Mn1 Ga1 2_555 . 10_555 90 ?
Ga1 Mn1 Ge1 2_555 . . 180 ?
Ga1 Mn1 Ge1 2_555 . 2_555 0 ?
Ga1 Mn1 Ge1 2_555 . 5_555 90 ?
Ga1 Mn1 Ge1 2_555 . 6_555 90 ?
Ga1 Mn1 Ge1 2_555 . 9_555 90 ?
Ga1 Mn1 Ge1 2_555 . 10_555 90 ?
Ga1 Mn1 Ga1 5_555 . 6_555 180 ?
Ga1 Mn1 Ga1 5_555 . 9_555 90 ?
Ga1 Mn1 Ga1 5_555 . 10_555 90 ?
Ga1 Mn1 Ge1 5_555 . . 90 ?
Ga1 Mn1 Ge1 5_555 . 2_555 90 ?
Ga1 Mn1 Ge1 5_555 . 5_555 0 ?
Ga1 Mn1 Ge1 5_555 . 6_555 180 ?
Ga1 Mn1 Ge1 5_555 . 9_555 90 ?
Ga1 Mn1 Ge1 5_555 . 10_555 90 ?
Ga1 Mn1 Ga1 6_555 . 9_555 90 ?
Ga1 Mn1 Ga1 6_555 . 10_555 90 ?
Ga1 Mn1 Ge1 6_555 . . 90 ?
Ga1 Mn1 Ge1 6_555 . 2_555 90 ?
Ga1 Mn1 Ge1 6_555 . 5_555 180 ?
Ga1 Mn1 Ge1 6_555 . 6_555 0 ?
Ga1 Mn1 Ge1 6_555 . 9_555 90 ?
Ga1 Mn1 Ge1 6_555 . 10_555 90 ?
Ga1 Mn1 Ga1 9_555 . 10_555 180 ?
Ga1 Mn1 Ge1 9_555 . . 90 ?
Ga1 Mn1 Ge1 9_555 . 2_555 90 ?
Ga1 Mn1 Ge1 9_555 . 5_555 90 ?
Ga1 Mn1 Ge1 9_555 . 6_555 90 ?
Ga1 Mn1 Ge1 9_555 . 9_555 0 ?
Ga1 Mn1 Ge1 9_555 . 10_555 180 ?
Ga1 Mn1 Ge1 10_555 . . 90 ?
Ga1 Mn1 Ge1 10_555 . 2_555 90 ?
Ga1 Mn1 Ge1 10_555 . 5_555 90 ?
Ga1 Mn1 Ge1 10_555 . 6_555 90 ?
Ga1 Mn1 Ge1 10_555 . 9_555 180 ?
Ga1 Mn1 Ge1 10_555 . 10_555 0 ?
Ge1 Mn1 Ge1 . . 2_555 180 ?
Ge1 Mn1 Ge1 . . 5_555 90 ?
Ge1 Mn1 Ge1 . . 6_555 90 ?
Ge1 Mn1 Ge1 . . 9_555 90 ?
Ge1 Mn1 Ge1 . . 10_555 90 ?
Ge1 Mn1 Ge1 2_555 . 5_555 90 ?
Ge1 Mn1 Ge1 2_555 . 6_555 90 ?
Ge1 Mn1 Ge1 2_555 . 9_555 90 ?
Ge1 Mn1 Ge1 2_555 . 10_555 90 ?
Ge1 Mn1 Ge1 5_555 . 6_555 180 ?
Ge1 Mn1 Ge1 5_555 . 9_555 90 ?
Ge1 Mn1 Ge1 5_555 . 10_555 90 ?
Ge1 Mn1 Ge1 6_555 . 9_555 90 ?
Ge1 Mn1 Ge1 6_555 . 10_555 90 ?
Ge1 Mn1 Ge1 9_555 . 10_555 180 ?
Sm1 Ga1 Sm1 . . 49_544 171.59(7) ?
Sm1 Ga1 Sm1 . . 13_555 89.692(6) ?
Sm1 Ga1 Sm1 . . 61_545 89.692(6) ?
Sm1 Ga1 Mn1 . . . 85.80(3) ?
Sm1 Ga1 Ga1 . . 5_555 56.600(19) ?
Sm1 Ga1 Ga1 . . 149_545 123.40(4) ?
Sm1 Ga1 Ga1 . . 6_555 116.54(4) ?
Sm1 Ga1 Ga1 . . 150_555 63.46(2) ?
Sm1 Ga1 Ga1 . . 9_555 56.600(19) ?
Sm1 Ga1 Ga1 . . 105_554 123.40(4) ?
Sm1 Ga1 Ga1 . . 10_555 116.54(4) ?
Sm1 Ga1 Ga1 . . 106_555 63.46(2) ?
Sm1 Ga1 Ge1 . . 5_555 56.600(19) ?
Sm1 Ga1 Ge1 . . 149_545 123.40(4) ?
Sm1 Ga1 Ge1 . . 6_555 116.54(4) ?
Sm1 Ga1 Ge1 . . 150_555 63.46(2) ?
Sm1 Ga1 Ge1 . . 9_555 56.600(19) ?
Sm1 Ga1 Ge1 . . 105_554 123.40(4) ?
Sm1 Ga1 Ge1 . . 10_555 116.54(4) ?
Sm1 Ga1 Ge1 . . 106_555 63.46(2) ?
Sm1 Ga1 Sm1 49_544 . 13_555 89.692(6) ?
Sm1 Ga1 Sm1 49_544 . 61_545 89.692(6) ?
Sm1 Ga1 Mn1 49_544 . . 85.80(3) ?
Sm1 Ga1 Ga1 49_544 . 5_555 116.54(4) ?
Sm1 Ga1 Ga1 49_544 . 149_545 63.46(2) ?
Sm1 Ga1 Ga1 49_544 . 6_555 56.600(19) ?
Sm1 Ga1 Ga1 49_544 . 150_555 123.40(4) ?
Sm1 Ga1 Ga1 49_544 . 9_555 116.54(4) ?
Sm1 Ga1 Ga1 49_544 . 105_554 63.46(2) ?
Sm1 Ga1 Ga1 49_544 . 10_555 56.600(19) ?
Sm1 Ga1 Ga1 49_544 . 106_555 123.40(4) ?
Sm1 Ga1 Ge1 49_544 . 5_555 116.54(4) ?
Sm1 Ga1 Ge1 49_544 . 149_545 63.46(2) ?
Sm1 Ga1 Ge1 49_544 . 6_555 56.600(19) ?
Sm1 Ga1 Ge1 49_544 . 150_555 123.40(4) ?
Sm1 Ga1 Ge1 49_544 . 9_555 116.54(4) ?
Sm1 Ga1 Ge1 49_544 . 105_554 63.46(2) ?
Sm1 Ga1 Ge1 49_544 . 10_555 56.600(19) ?
Sm1 Ga1 Ge1 49_544 . 106_555 123.40(4) ?
Sm1 Ga1 Sm1 13_555 . 61_545 171.59(7) ?
Sm1 Ga1 Mn1 13_555 . . 85.80(3) ?
Sm1 Ga1 Ga1 13_555 . 5_555 56.600(19) ?
Sm1 Ga1 Ga1 13_555 . 149_545 123.40(4) ?
Sm1 Ga1 Ga1 13_555 . 6_555 116.54(4) ?
Sm1 Ga1 Ga1 13_555 . 150_555 63.46(2) ?
Sm1 Ga1 Ga1 13_555 . 9_555 116.54(4) ?
Sm1 Ga1 Ga1 13_555 . 105_554 63.46(2) ?
Sm1 Ga1 Ga1 13_555 . 10_555 56.600(19) ?
Sm1 Ga1 Ga1 13_555 . 106_555 123.40(4) ?
Sm1 Ga1 Ge1 13_555 . 5_555 56.600(19) ?
Sm1 Ga1 Ge1 13_555 . 149_545 123.40(4) ?
Sm1 Ga1 Ge1 13_555 . 6_555 116.54(4) ?
Sm1 Ga1 Ge1 13_555 . 150_555 63.46(2) ?
Sm1 Ga1 Ge1 13_555 . 9_555 116.54(4) ?
Sm1 Ga1 Ge1 13_555 . 105_554 63.46(2) ?
Sm1 Ga1 Ge1 13_555 . 10_555 56.600(19) ?
Sm1 Ga1 Ge1 13_555 . 106_555 123.40(4) ?
Sm1 Ga1 Mn1 61_545 . . 85.80(3) ?
Sm1 Ga1 Ga1 61_545 . 5_555 116.54(4) ?
Sm1 Ga1 Ga1 61_545 . 149_545 63.46(2) ?
Sm1 Ga1 Ga1 61_545 . 6_555 56.600(19) ?
Sm1 Ga1 Ga1 61_545 . 150_555 123.40(4) ?
Sm1 Ga1 Ga1 61_545 . 9_555 56.600(19) ?
Sm1 Ga1 Ga1 61_545 . 105_554 123.40(4) ?
Sm1 Ga1 Ga1 61_545 . 10_555 116.54(4) ?
Sm1 Ga1 Ga1 61_545 . 106_555 63.46(2) ?
Sm1 Ga1 Ge1 61_545 . 5_555 116.54(4) ?
Sm1 Ga1 Ge1 61_545 . 149_545 63.46(2) ?
Sm1 Ga1 Ge1 61_545 . 6_555 56.600(19) ?
Sm1 Ga1 Ge1 61_545 . 150_555 123.40(4) ?
Sm1 Ga1 Ge1 61_545 . 9_555 56.600(19) ?
Sm1 Ga1 Ge1 61_545 . 105_554 123.40(4) ?
Sm1 Ga1 Ge1 61_545 . 10_555 116.54(4) ?
Sm1 Ga1 Ge1 61_545 . 106_555 63.46(2) ?
Mn1 Ga1 Ga1 . . 5_555 45.00(3) ?
Mn1 Ga1 Ga1 . . 149_545 135.00(4) ?
Mn1 Ga1 Ga1 . . 6_555 45.00(3) ?
Mn1 Ga1 Ga1 . . 150_555 135.00(4) ?
Mn1 Ga1 Ga1 . . 9_555 45.00(3) ?
Mn1 Ga1 Ga1 . . 105_554 135.00(4) ?
Mn1 Ga1 Ga1 . . 10_555 45.00(3) ?
Mn1 Ga1 Ga1 . . 106_555 135.00(4) ?
Mn1 Ga1 Ge1 . . 5_555 45.00(3) ?
Mn1 Ga1 Ge1 . . 149_545 135.00(4) ?
Mn1 Ga1 Ge1 . . 6_555 45.00(3) ?
Mn1 Ga1 Ge1 . . 150_555 135.00(4) ?
Mn1 Ga1 Ge1 . . 9_555 45.00(3) ?
Mn1 Ga1 Ge1 . . 105_554 135.00(4) ?
Mn1 Ga1 Ge1 . . 10_555 45.00(3) ?
Mn1 Ga1 Ge1 . . 106_555 135.00(4) ?
Ga1 Ga1 Ga1 5_555 . 149_545 180 ?
Ga1 Ga1 Ga1 5_555 . 6_555 90.00(5) ?
Ga1 Ga1 Ga1 5_555 . 150_555 90.00(3) ?
Ga1 Ga1 Ga1 5_555 . 9_555 60.00(3) ?
Ga1 Ga1 Ga1 5_555 . 105_554 120.00(2) ?
Ga1 Ga1 Ga1 5_555 . 10_555 60.00(3) ?
Ga1 Ga1 Ga1 5_555 . 106_555 120.00(2) ?
Ga1 Ga1 Ge1 5_555 . 5_555 0 ?
Ga1 Ga1 Ge1 5_555 . 149_545 180 ?
Ga1 Ga1 Ge1 5_555 . 6_555 90.00(5) ?
Ga1 Ga1 Ge1 5_555 . 150_555 90.00(3) ?
Ga1 Ga1 Ge1 5_555 . 9_555 60.00(3) ?
Ga1 Ga1 Ge1 5_555 . 105_554 120.00(2) ?
Ga1 Ga1 Ge1 5_555 . 10_555 60.00(3) ?
Ga1 Ga1 Ge1 5_555 . 106_555 120.00(2) ?
Ga1 Ga1 Ga1 149_545 . 6_555 90.00(3) ?
Ga1 Ga1 Ga1 149_545 . 150_555 90.00(7) ?
Ga1 Ga1 Ga1 149_545 . 9_555 120.00(2) ?
Ga1 Ga1 Ga1 149_545 . 105_554 60.00(4) ?
Ga1 Ga1 Ga1 149_545 . 10_555 120.00(2) ?
Ga1 Ga1 Ga1 149_545 . 106_555 60.00(4) ?
Ga1 Ga1 Ge1 149_545 . 5_555 180 ?
Ga1 Ga1 Ge1 149_545 . 149_545 0 ?
Ga1 Ga1 Ge1 149_545 . 6_555 90.00(3) ?
Ga1 Ga1 Ge1 149_545 . 150_555 90.00(7) ?
Ga1 Ga1 Ge1 149_545 . 9_555 120.00(2) ?
Ga1 Ga1 Ge1 149_545 . 105_554 60.00(4) ?
Ga1 Ga1 Ge1 149_545 . 10_555 120.00(2) ?
Ga1 Ga1 Ge1 149_545 . 106_555 60.00(4) ?
Ga1 Ga1 Ga1 6_555 . 150_555 180 ?
Ga1 Ga1 Ga1 6_555 . 9_555 60.00(3) ?
Ga1 Ga1 Ga1 6_555 . 105_554 120.00(2) ?
Ga1 Ga1 Ga1 6_555 . 10_555 60.00(3) ?
Ga1 Ga1 Ga1 6_555 . 106_555 120.00(2) ?
Ga1 Ga1 Ge1 6_555 . 5_555 90.00(5) ?
Ga1 Ga1 Ge1 6_555 . 149_545 90.00(3) ?
Ga1 Ga1 Ge1 6_555 . 6_555 0 ?
Ga1 Ga1 Ge1 6_555 . 150_555 180 ?
Ga1 Ga1 Ge1 6_555 . 9_555 60.00(3) ?
Ga1 Ga1 Ge1 6_555 . 105_554 120.00(2) ?
Ga1 Ga1 Ge1 6_555 . 10_555 60.00(3) ?
Ga1 Ga1 Ge1 6_555 . 106_555 120.00(2) ?
Ga1 Ga1 Ga1 150_555 . 9_555 120.00(2) ?
Ga1 Ga1 Ga1 150_555 . 105_554 60.00(4) ?
Ga1 Ga1 Ga1 150_555 . 10_555 120.00(2) ?
Ga1 Ga1 Ga1 150_555 . 106_555 60.00(4) ?
Ga1 Ga1 Ge1 150_555 . 5_555 90.00(3) ?
Ga1 Ga1 Ge1 150_555 . 149_545 90.00(7) ?
Ga1 Ga1 Ge1 150_555 . 6_555 180 ?
Ga1 Ga1 Ge1 150_555 . 150_555 0 ?
Ga1 Ga1 Ge1 150_555 . 9_555 120.00(2) ?
Ga1 Ga1 Ge1 150_555 . 105_554 60.00(4) ?
Ga1 Ga1 Ge1 150_555 . 10_555 120.00(2) ?
Ga1 Ga1 Ge1 150_555 . 106_555 60.00(4) ?
Ga1 Ga1 Ga1 9_555 . 105_554 180 ?
Ga1 Ga1 Ga1 9_555 . 10_555 90.00(5) ?
Ga1 Ga1 Ga1 9_555 . 106_555 90.00(3) ?
Ga1 Ga1 Ge1 9_555 . 5_555 60.00(3) ?
Ga1 Ga1 Ge1 9_555 . 149_545 120.00(2) ?
Ga1 Ga1 Ge1 9_555 . 6_555 60.00(3) ?
Ga1 Ga1 Ge1 9_555 . 150_555 120.00(2) ?
Ga1 Ga1 Ge1 9_555 . 9_555 0 ?
Ga1 Ga1 Ge1 9_555 . 105_554 180 ?
Ga1 Ga1 Ge1 9_555 . 10_555 90.00(5) ?
Ga1 Ga1 Ge1 9_555 . 106_555 90.00(3) ?
Ga1 Ga1 Ga1 105_554 . 10_555 90.00(3) ?
Ga1 Ga1 Ga1 105_554 . 106_555 90.00(7) ?
Ga1 Ga1 Ge1 105_554 . 5_555 120.00(2) ?
Ga1 Ga1 Ge1 105_554 . 149_545 60.00(4) ?
Ga1 Ga1 Ge1 105_554 . 6_555 120.00(2) ?
Ga1 Ga1 Ge1 105_554 . 150_555 60.00(4) ?
Ga1 Ga1 Ge1 105_554 . 9_555 180 ?
Ga1 Ga1 Ge1 105_554 . 105_554 0 ?
Ga1 Ga1 Ge1 105_554 . 10_555 90.00(3) ?
Ga1 Ga1 Ge1 105_554 . 106_555 90.00(7) ?
Ga1 Ga1 Ga1 10_555 . 106_555 180 ?
Ga1 Ga1 Ge1 10_555 . 5_555 60.00(3) ?
Ga1 Ga1 Ge1 10_555 . 149_545 120.00(2) ?
Ga1 Ga1 Ge1 10_555 . 6_555 60.00(3) ?
Ga1 Ga1 Ge1 10_555 . 150_555 120.00(2) ?
Ga1 Ga1 Ge1 10_555 . 9_555 90.00(5) ?
Ga1 Ga1 Ge1 10_555 . 105_554 90.00(3) ?
Ga1 Ga1 Ge1 10_555 . 10_555 0 ?
Ga1 Ga1 Ge1 10_555 . 106_555 180 ?
Ga1 Ga1 Ge1 106_555 . 5_555 120.00(2) ?
Ga1 Ga1 Ge1 106_555 . 149_545 60.00(4) ?
Ga1 Ga1 Ge1 106_555 . 6_555 120.00(2) ?
Ga1 Ga1 Ge1 106_555 . 150_555 60.00(4) ?
Ga1 Ga1 Ge1 106_555 . 9_555 90.00(3) ?
Ga1 Ga1 Ge1 106_555 . 105_554 90.00(7) ?
Ga1 Ga1 Ge1 106_555 . 10_555 180 ?
Ga1 Ga1 Ge1 106_555 . 106_555 0 ?
Ge1 Ga1 Ge1 5_555 . 149_545 180 ?
Ge1 Ga1 Ge1 5_555 . 6_555 90.00(5) ?
Ge1 Ga1 Ge1 5_555 . 150_555 90.00(3) ?
Ge1 Ga1 Ge1 5_555 . 9_555 60.00(3) ?
Ge1 Ga1 Ge1 5_555 . 105_554 120.00(2) ?
Ge1 Ga1 Ge1 5_555 . 10_555 60.00(3) ?
Ge1 Ga1 Ge1 5_555 . 106_555 120.00(2) ?
Ge1 Ga1 Ge1 149_545 . 6_555 90.00(3) ?
Ge1 Ga1 Ge1 149_545 . 150_555 90.00(7) ?
Ge1 Ga1 Ge1 149_545 . 9_555 120.00(2) ?
Ge1 Ga1 Ge1 149_545 . 105_554 60.00(4) ?
Ge1 Ga1 Ge1 149_545 . 10_555 120.00(2) ?
Ge1 Ga1 Ge1 149_545 . 106_555 60.00(4) ?
Ge1 Ga1 Ge1 6_555 . 150_555 180 ?
Ge1 Ga1 Ge1 6_555 . 9_555 60.00(3) ?
Ge1 Ga1 Ge1 6_555 . 105_554 120.00(2) ?
Ge1 Ga1 Ge1 6_555 . 10_555 60.00(3) ?
Ge1 Ga1 Ge1 6_555 . 106_555 120.00(2) ?
Ge1 Ga1 Ge1 150_555 . 9_555 120.00(2) ?
Ge1 Ga1 Ge1 150_555 . 105_554 60.00(4) ?
Ge1 Ga1 Ge1 150_555 . 10_555 120.00(2) ?
Ge1 Ga1 Ge1 150_555 . 106_555 60.00(4) ?
Ge1 Ga1 Ge1 9_555 . 105_554 180 ?
Ge1 Ga1 Ge1 9_555 . 10_555 90.00(5) ?
Ge1 Ga1 Ge1 9_555 . 106_555 90.00(3) ?
Ge1 Ga1 Ge1 105_554 . 10_555 90.00(3) ?
Ge1 Ga1 Ge1 105_554 . 106_555 90.00(7) ?
Ge1 Ga1 Ge1 10_555 . 106_555 180 ?
Sm1 Ge1 Sm1 . . 49_544 171.59(7) ?
Sm1 Ge1 Sm1 . . 13_555 89.692(6) ?
Sm1 Ge1 Sm1 . . 61_545 89.692(6) ?
Sm1 Ge1 Mn1 . . . 85.80(3) ?
Sm1 Ge1 Ga1 . . 5_555 56.600(19) ?
Sm1 Ge1 Ga1 . . 149_545 123.40(4) ?
Sm1 Ge1 Ga1 . . 6_555 116.54(4) ?
Sm1 Ge1 Ga1 . . 150_555 63.46(2) ?
Sm1 Ge1 Ga1 . . 9_555 56.600(19) ?
Sm1 Ge1 Ga1 . . 105_554 123.40(4) ?
Sm1 Ge1 Ga1 . . 10_555 116.54(4) ?
Sm1 Ge1 Ga1 . . 106_555 63.46(2) ?
Sm1 Ge1 Ge1 . . 5_555 56.600(19) ?
Sm1 Ge1 Ge1 . . 149_545 123.40(4) ?
Sm1 Ge1 Ge1 . . 6_555 116.54(4) ?
Sm1 Ge1 Ge1 . . 150_555 63.46(2) ?
Sm1 Ge1 Ge1 . . 9_555 56.600(19) ?
Sm1 Ge1 Ge1 . . 105_554 123.40(4) ?
Sm1 Ge1 Ge1 . . 10_555 116.54(4) ?
Sm1 Ge1 Ge1 . . 106_555 63.46(2) ?
Sm1 Ge1 Sm1 49_544 . 13_555 89.692(6) ?
Sm1 Ge1 Sm1 49_544 . 61_545 89.692(6) ?
Sm1 Ge1 Mn1 49_544 . . 85.80(3) ?
Sm1 Ge1 Ga1 49_544 . 5_555 116.54(4) ?
Sm1 Ge1 Ga1 49_544 . 149_545 63.46(2) ?
Sm1 Ge1 Ga1 49_544 . 6_555 56.600(19) ?
Sm1 Ge1 Ga1 49_544 . 150_555 123.40(4) ?
Sm1 Ge1 Ga1 49_544 . 9_555 116.54(4) ?
Sm1 Ge1 Ga1 49_544 . 105_554 63.46(2) ?
Sm1 Ge1 Ga1 49_544 . 10_555 56.600(19) ?
Sm1 Ge1 Ga1 49_544 . 106_555 123.40(4) ?
Sm1 Ge1 Ge1 49_544 . 5_555 116.54(4) ?
Sm1 Ge1 Ge1 49_544 . 149_545 63.46(2) ?
Sm1 Ge1 Ge1 49_544 . 6_555 56.600(19) ?
Sm1 Ge1 Ge1 49_544 . 150_555 123.40(4) ?
Sm1 Ge1 Ge1 49_544 . 9_555 116.54(4) ?
Sm1 Ge1 Ge1 49_544 . 105_554 63.46(2) ?
Sm1 Ge1 Ge1 49_544 . 10_555 56.600(19) ?
Sm1 Ge1 Ge1 49_544 . 106_555 123.40(4) ?
Sm1 Ge1 Sm1 13_555 . 61_545 171.59(7) ?
Sm1 Ge1 Mn1 13_555 . . 85.80(3) ?
Sm1 Ge1 Ga1 13_555 . 5_555 56.600(19) ?
Sm1 Ge1 Ga1 13_555 . 149_545 123.40(4) ?
Sm1 Ge1 Ga1 13_555 . 6_555 116.54(4) ?
Sm1 Ge1 Ga1 13_555 . 150_555 63.46(2) ?
Sm1 Ge1 Ga1 13_555 . 9_555 116.54(4) ?
Sm1 Ge1 Ga1 13_555 . 105_554 63.46(2) ?
Sm1 Ge1 Ga1 13_555 . 10_555 56.600(19) ?
Sm1 Ge1 Ga1 13_555 . 106_555 123.40(4) ?
Sm1 Ge1 Ge1 13_555 . 5_555 56.600(19) ?
Sm1 Ge1 Ge1 13_555 . 149_545 123.40(4) ?
Sm1 Ge1 Ge1 13_555 . 6_555 116.54(4) ?
Sm1 Ge1 Ge1 13_555 . 150_555 63.46(2) ?
Sm1 Ge1 Ge1 13_555 . 9_555 116.54(4) ?
Sm1 Ge1 Ge1 13_555 . 105_554 63.46(2) ?
Sm1 Ge1 Ge1 13_555 . 10_555 56.600(19) ?
Sm1 Ge1 Ge1 13_555 . 106_555 123.40(4) ?
Sm1 Ge1 Mn1 61_545 . . 85.80(3) ?
Sm1 Ge1 Ga1 61_545 . 5_555 116.54(4) ?
Sm1 Ge1 Ga1 61_545 . 149_545 63.46(2) ?
Sm1 Ge1 Ga1 61_545 . 6_555 56.600(19) ?
Sm1 Ge1 Ga1 61_545 . 150_555 123.40(4) ?
Sm1 Ge1 Ga1 61_545 . 9_555 56.600(19) ?
Sm1 Ge1 Ga1 61_545 . 105_554 123.40(4) ?
Sm1 Ge1 Ga1 61_545 . 10_555 116.54(4) ?
Sm1 Ge1 Ga1 61_545 . 106_555 63.46(2) ?
Sm1 Ge1 Ge1 61_545 . 5_555 116.54(4) ?
Sm1 Ge1 Ge1 61_545 . 149_545 63.46(2) ?
Sm1 Ge1 Ge1 61_545 . 6_555 56.600(19) ?
Sm1 Ge1 Ge1 61_545 . 150_555 123.40(4) ?
Sm1 Ge1 Ge1 61_545 . 9_555 56.600(19) ?
Sm1 Ge1 Ge1 61_545 . 105_554 123.40(4) ?
Sm1 Ge1 Ge1 61_545 . 10_555 116.54(4) ?
Sm1 Ge1 Ge1 61_545 . 106_555 63.46(2) ?
Mn1 Ge1 Ga1 . . 5_555 45.00(3) ?
Mn1 Ge1 Ga1 . . 149_545 135.00(4) ?
Mn1 Ge1 Ga1 . . 6_555 45.00(3) ?
Mn1 Ge1 Ga1 . . 150_555 135.00(4) ?
Mn1 Ge1 Ga1 . . 9_555 45.00(3) ?
Mn1 Ge1 Ga1 . . 105_554 135.00(4) ?
Mn1 Ge1 Ga1 . . 10_555 45.00(3) ?
Mn1 Ge1 Ga1 . . 106_555 135.00(4) ?
Mn1 Ge1 Ge1 . . 5_555 45.00(3) ?
Mn1 Ge1 Ge1 . . 149_545 135.00(4) ?
Mn1 Ge1 Ge1 . . 6_555 45.00(3) ?
Mn1 Ge1 Ge1 . . 150_555 135.00(4) ?
Mn1 Ge1 Ge1 . . 9_555 45.00(3) ?
Mn1 Ge1 Ge1 . . 105_554 135.00(4) ?
Mn1 Ge1 Ge1 . . 10_555 45.00(3) ?
Mn1 Ge1 Ge1 . . 106_555 135.00(4) ?
Ga1 Ge1 Ga1 5_555 . 149_545 180 ?
Ga1 Ge1 Ga1 5_555 . 6_555 90.00(5) ?
Ga1 Ge1 Ga1 5_555 . 150_555 90.00(3) ?
Ga1 Ge1 Ga1 5_555 . 9_555 60.00(3) ?
Ga1 Ge1 Ga1 5_555 . 105_554 120.00(2) ?
Ga1 Ge1 Ga1 5_555 . 10_555 60.00(3) ?
Ga1 Ge1 Ga1 5_555 . 106_555 120.00(2) ?
Ga1 Ge1 Ge1 5_555 . 5_555 0 ?
Ga1 Ge1 Ge1 5_555 . 149_545 180 ?
Ga1 Ge1 Ge1 5_555 . 6_555 90.00(5) ?
Ga1 Ge1 Ge1 5_555 . 150_555 90.00(3) ?
Ga1 Ge1 Ge1 5_555 . 9_555 60.00(3) ?
Ga1 Ge1 Ge1 5_555 . 105_554 120.00(2) ?
Ga1 Ge1 Ge1 5_555 . 10_555 60.00(3) ?
Ga1 Ge1 Ge1 5_555 . 106_555 120.00(2) ?
Ga1 Ge1 Ga1 149_545 . 6_555 90.00(3) ?
Ga1 Ge1 Ga1 149_545 . 150_555 90.00(7) ?
Ga1 Ge1 Ga1 149_545 . 9_555 120.00(2) ?
Ga1 Ge1 Ga1 149_545 . 105_554 60.00(4) ?
Ga1 Ge1 Ga1 149_545 . 10_555 120.00(2) ?
Ga1 Ge1 Ga1 149_545 . 106_555 60.00(4) ?
Ga1 Ge1 Ge1 149_545 . 5_555 180 ?
Ga1 Ge1 Ge1 149_545 . 149_545 0 ?
Ga1 Ge1 Ge1 149_545 . 6_555 90.00(3) ?
Ga1 Ge1 Ge1 149_545 . 150_555 90.00(7) ?
Ga1 Ge1 Ge1 149_545 . 9_555 120.00(2) ?
Ga1 Ge1 Ge1 149_545 . 105_554 60.00(4) ?
Ga1 Ge1 Ge1 149_545 . 10_555 120.00(2) ?
Ga1 Ge1 Ge1 149_545 . 106_555 60.00(4) ?
Ga1 Ge1 Ga1 6_555 . 150_555 180 ?
Ga1 Ge1 Ga1 6_555 . 9_555 60.00(3) ?
Ga1 Ge1 Ga1 6_555 . 105_554 120.00(2) ?
Ga1 Ge1 Ga1 6_555 . 10_555 60.00(3) ?
Ga1 Ge1 Ga1 6_555 . 106_555 120.00(2) ?
Ga1 Ge1 Ge1 6_555 . 5_555 90.00(5) ?
Ga1 Ge1 Ge1 6_555 . 149_545 90.00(3) ?
Ga1 Ge1 Ge1 6_555 . 6_555 0 ?
Ga1 Ge1 Ge1 6_555 . 150_555 180 ?
Ga1 Ge1 Ge1 6_555 . 9_555 60.00(3) ?
Ga1 Ge1 Ge1 6_555 . 105_554 120.00(2) ?
Ga1 Ge1 Ge1 6_555 . 10_555 60.00(3) ?
Ga1 Ge1 Ge1 6_555 . 106_555 120.00(2) ?
Ga1 Ge1 Ga1 150_555 . 9_555 120.00(2) ?
Ga1 Ge1 Ga1 150_555 . 105_554 60.00(4) ?
Ga1 Ge1 Ga1 150_555 . 10_555 120.00(2) ?
Ga1 Ge1 Ga1 150_555 . 106_555 60.00(4) ?
Ga1 Ge1 Ge1 150_555 . 5_555 90.00(3) ?
Ga1 Ge1 Ge1 150_555 . 149_545 90.00(7) ?
Ga1 Ge1 Ge1 150_555 . 6_555 180 ?
Ga1 Ge1 Ge1 150_555 . 150_555 0 ?
Ga1 Ge1 Ge1 150_555 . 9_555 120.00(2) ?
Ga1 Ge1 Ge1 150_555 . 105_554 60.00(4) ?
Ga1 Ge1 Ge1 150_555 . 10_555 120.00(2) ?
Ga1 Ge1 Ge1 150_555 . 106_555 60.00(4) ?
Ga1 Ge1 Ga1 9_555 . 105_554 180 ?
Ga1 Ge1 Ga1 9_555 . 10_555 90.00(5) ?
Ga1 Ge1 Ga1 9_555 . 106_555 90.00(3) ?
Ga1 Ge1 Ge1 9_555 . 5_555 60.00(3) ?
Ga1 Ge1 Ge1 9_555 . 149_545 120.00(2) ?
Ga1 Ge1 Ge1 9_555 . 6_555 60.00(3) ?
Ga1 Ge1 Ge1 9_555 . 150_555 120.00(2) ?
Ga1 Ge1 Ge1 9_555 . 9_555 0 ?
Ga1 Ge1 Ge1 9_555 . 105_554 180 ?
Ga1 Ge1 Ge1 9_555 . 10_555 90.00(5) ?
Ga1 Ge1 Ge1 9_555 . 106_555 90.00(3) ?
Ga1 Ge1 Ga1 105_554 . 10_555 90.00(3) ?
Ga1 Ge1 Ga1 105_554 . 106_555 90.00(7) ?
Ga1 Ge1 Ge1 105_554 . 5_555 120.00(2) ?
Ga1 Ge1 Ge1 105_554 . 149_545 60.00(4) ?
Ga1 Ge1 Ge1 105_554 . 6_555 120.00(2) ?
Ga1 Ge1 Ge1 105_554 . 150_555 60.00(4) ?
Ga1 Ge1 Ge1 105_554 . 9_555 180 ?
Ga1 Ge1 Ge1 105_554 . 105_554 0 ?
Ga1 Ge1 Ge1 105_554 . 10_555 90.00(3) ?
Ga1 Ge1 Ge1 105_554 . 106_555 90.00(7) ?
Ga1 Ge1 Ga1 10_555 . 106_555 180 ?
Ga1 Ge1 Ge1 10_555 . 5_555 60.00(3) ?
Ga1 Ge1 Ge1 10_555 . 149_545 120.00(2) ?
Ga1 Ge1 Ge1 10_555 . 6_555 60.00(3) ?
Ga1 Ge1 Ge1 10_555 . 150_555 120.00(2) ?
Ga1 Ge1 Ge1 10_555 . 9_555 90.00(5) ?
Ga1 Ge1 Ge1 10_555 . 105_554 90.00(3) ?
Ga1 Ge1 Ge1 10_555 . 10_555 0 ?
Ga1 Ge1 Ge1 10_555 . 106_555 180 ?
Ga1 Ge1 Ge1 106_555 . 5_555 120.00(2) ?
Ga1 Ge1 Ge1 106_555 . 149_545 60.00(4) ?
Ga1 Ge1 Ge1 106_555 . 6_555 120.00(2) ?
Ga1 Ge1 Ge1 106_555 . 150_555 60.00(4) ?
Ga1 Ge1 Ge1 106_555 . 9_555 90.00(3) ?
Ga1 Ge1 Ge1 106_555 . 105_554 90.00(7) ?
Ga1 Ge1 Ge1 106_555 . 10_555 180 ?
Ga1 Ge1 Ge1 106_555 . 106_555 0 ?
Ge1 Ge1 Ge1 5_555 . 149_545 180 ?
Ge1 Ge1 Ge1 5_555 . 6_555 90.00(5) ?
Ge1 Ge1 Ge1 5_555 . 150_555 90.00(3) ?
Ge1 Ge1 Ge1 5_555 . 9_555 60.00(3) ?
Ge1 Ge1 Ge1 5_555 . 105_554 120.00(2) ?
Ge1 Ge1 Ge1 5_555 . 10_555 60.00(3) ?
Ge1 Ge1 Ge1 5_555 . 106_555 120.00(2) ?
Ge1 Ge1 Ge1 149_545 . 6_555 90.00(3) ?
Ge1 Ge1 Ge1 149_545 . 150_555 90.00(7) ?
Ge1 Ge1 Ge1 149_545 . 9_555 120.00(2) ?
Ge1 Ge1 Ge1 149_545 . 105_554 60.00(4) ?
Ge1 Ge1 Ge1 149_545 . 10_555 120.00(2) ?
Ge1 Ge1 Ge1 149_545 . 106_555 60.00(4) ?
Ge1 Ge1 Ge1 6_555 . 150_555 180 ?
Ge1 Ge1 Ge1 6_555 . 9_555 60.00(3) ?
Ge1 Ge1 Ge1 6_555 . 105_554 120.00(2) ?
Ge1 Ge1 Ge1 6_555 . 10_555 60.00(3) ?
Ge1 Ge1 Ge1 6_555 . 106_555 120.00(2) ?
Ge1 Ge1 Ge1 150_555 . 9_555 120.00(2) ?
Ge1 Ge1 Ge1 150_555 . 105_554 60.00(4) ?
Ge1 Ge1 Ge1 150_555 . 10_555 120.00(2) ?
Ge1 Ge1 Ge1 150_555 . 106_555 60.00(4) ?
Ge1 Ge1 Ge1 9_555 . 105_554 180 ?
Ge1 Ge1 Ge1 9_555 . 10_555 90.00(5) ?
Ge1 Ge1 Ge1 9_555 . 106_555 90.00(3) ?
Ge1 Ge1 Ge1 105_554 . 10_555 90.00(3) ?
Ge1 Ge1 Ge1 105_554 . 106_555 90.00(7) ?
Ge1 Ge1 Ge1 10_555 . 106_555 180 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 11. STRUCTURE-FACTOR LIST


_exptl_crystal_recrystallization_method 'From the Melt'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_Sm4MnGa86Ge34T100K
_database_code_depnum_ccdc_archive 'CCDC 2312752'
loop_
_audit_author_name
_audit_author_address
'Roman Khalaniya'
;Lomonosov Moscow State University
Russia
;
_audit_update_record             
;
2023-12-07 deposited with the CCDC.	2023-12-13 downloaded from the CCDC.
;
#=======================================================================

_audit_creation_method           'Jana2006 Version : 15/02/2021'

#=======================================================================

# 4. CHECKCIF RESPONSE 

# start Validation Reply Form

#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        Sm4MnGa8.6Ge3.4
_chemical_name_common            ?
_chemical_formula_moiety         'Sm4 Mn Ga8.6 Ge3.4'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_sum            'Ga8.6 Ge3.4 Mn1 Sm4'
_chemical_formula_weight         1502.8
_chemical_melting_point          ?
_chemical_compound_source        ?
_chemical_absolute_configuration .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'I m -3 m'
_symmetry_space_group_name_Hall  '-I 4;2;3'
_symmetry_Int_Tables_number      229

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -x,y,-z
4 x,-y,-z
5 z,x,y
6 z,-x,-y
7 -z,-x,y
8 -z,x,-y
9 y,z,x
10 -y,z,-x
11 y,-z,-x
12 -y,-z,x
13 y,x,-z
14 -y,-x,-z
15 y,-x,z
16 -y,x,z
17 x,z,-y
18 -x,z,y
19 -x,-z,-y
20 x,-z,y
21 z,y,-x
22 z,-y,x
23 -z,y,x
24 -z,-y,-x
25 -x,-y,-z
26 x,y,-z
27 x,-y,z
28 -x,y,z
29 -z,-x,-y
30 -z,x,y
31 z,x,-y
32 z,-x,y
33 -y,-z,-x
34 y,-z,x
35 -y,z,x
36 y,z,-x
37 -y,-x,z
38 y,x,z
39 -y,x,-z
40 y,-x,-z
41 -x,-z,y
42 x,-z,-y
43 x,z,y
44 -x,z,-y
45 -z,-y,x
46 -z,y,-x
47 z,-y,-x
48 z,y,x
49 x+1/2,y+1/2,z+1/2
50 -x+1/2,-y+1/2,z+1/2
51 -x+1/2,y+1/2,-z+1/2
52 x+1/2,-y+1/2,-z+1/2
53 z+1/2,x+1/2,y+1/2
54 z+1/2,-x+1/2,-y+1/2
55 -z+1/2,-x+1/2,y+1/2
56 -z+1/2,x+1/2,-y+1/2
57 y+1/2,z+1/2,x+1/2
58 -y+1/2,z+1/2,-x+1/2
59 y+1/2,-z+1/2,-x+1/2
60 -y+1/2,-z+1/2,x+1/2
61 y+1/2,x+1/2,-z+1/2
62 -y+1/2,-x+1/2,-z+1/2
63 y+1/2,-x+1/2,z+1/2
64 -y+1/2,x+1/2,z+1/2
65 x+1/2,z+1/2,-y+1/2
66 -x+1/2,z+1/2,y+1/2
67 -x+1/2,-z+1/2,-y+1/2
68 x+1/2,-z+1/2,y+1/2
69 z+1/2,y+1/2,-x+1/2
70 z+1/2,-y+1/2,x+1/2
71 -z+1/2,y+1/2,x+1/2
72 -z+1/2,-y+1/2,-x+1/2
73 -x+1/2,-y+1/2,-z+1/2
74 x+1/2,y+1/2,-z+1/2
75 x+1/2,-y+1/2,z+1/2
76 -x+1/2,y+1/2,z+1/2
77 -z+1/2,-x+1/2,-y+1/2
78 -z+1/2,x+1/2,y+1/2
79 z+1/2,x+1/2,-y+1/2
80 z+1/2,-x+1/2,y+1/2
81 -y+1/2,-z+1/2,-x+1/2
82 y+1/2,-z+1/2,x+1/2
83 -y+1/2,z+1/2,x+1/2
84 y+1/2,z+1/2,-x+1/2
85 -y+1/2,-x+1/2,z+1/2
86 y+1/2,x+1/2,z+1/2
87 -y+1/2,x+1/2,-z+1/2
88 y+1/2,-x+1/2,-z+1/2
89 -x+1/2,-z+1/2,y+1/2
90 x+1/2,-z+1/2,-y+1/2
91 x+1/2,z+1/2,y+1/2
92 -x+1/2,z+1/2,-y+1/2
93 -z+1/2,-y+1/2,x+1/2
94 -z+1/2,y+1/2,-x+1/2
95 z+1/2,-y+1/2,-x+1/2
96 z+1/2,y+1/2,x+1/2

_cell_length_a                   8.6283(8)
_cell_length_b                   8.6283(8)
_cell_length_c                   8.6283(8)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     642.36(10)

loop_
_twin_individual_id
_twin_individual_mass_fraction_refined
_twin_individual_twin_matrix_11
_twin_individual_twin_matrix_12
_twin_individual_twin_matrix_13
_twin_individual_twin_matrix_21
_twin_individual_twin_matrix_22
_twin_individual_twin_matrix_23
_twin_individual_twin_matrix_31
_twin_individual_twin_matrix_32
_twin_individual_twin_matrix_33
? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z            2

_cell_measurement_reflns_used    1212
_cell_measurement_theta_min      4.73
_cell_measurement_theta_max      30.29
_cell_measurement_temperature    100
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    7.7696
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             1297

_exptl_absorpt_coefficient_mu    44.359
_exptl_crystal_description       'rectangular cuboid'
_exptl_crystal_size_max          0.4
_exptl_crystal_size_mid          0.3
_exptl_crystal_size_min          0.2
_exptl_crystal_size_rad          ?
_exptl_crystal_colour            grey
_exptl_absorpt_correction_type   multi-scan,gausian
_exptl_absorpt_process_details   
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_absorpt_correction_T_min  0.0041
_exptl_absorpt_correction_T_max  0.0325
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?

_diffrn_ambient_temperature      100
_diffrn_source                   ?
_diffrn_source_power             ?
_diffrn_source_voltage           ?
_diffrn_source_current           ?
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_detector                 ?
_diffrn_detector_area_resol_mean ?
_diffrn_measurement_method       'Bruker CCD'
_diffrn_measurement_specimen_support ?

_diffrn_reflns_number            1758
_diffrn_reflns_theta_min         3.34
_diffrn_reflns_theta_max         30.52
_diffrn_reflns_theta_full        30.52
_diffrn_measured_fraction_theta_max 0.99
_diffrn_measured_fraction_theta_full 0.99
_diffrn_reflns_av_R_equivalents  0.1149
_diffrn_reflns_av_unetI/netI     0.066
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_reduction_process ?

_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
? ? ?

_diffrn_radiation_probe          X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details          
; ?
;

_reflns_number_total             124
_reflns_number_gt                102
_reflns_threshold_expression     I>2σ(I)

_refine_ls_structure_factor_coef F
_refine_ls_R_factor_gt           0.0281
_refine_ls_wR_factor_gt          0.0302
_refine_ls_R_factor_all          0.0360
_refine_ls_wR_factor_ref         0.0328
_refine_ls_goodness_of_fit_ref   1.00
_refine_ls_goodness_of_fit_gt    1.03
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_reflns         124
_refine_ls_number_parameters     15
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     w=1/(σ²(F)+0.000081F²)
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0055
_refine_ls_shift/su_mean         0.0032
_refine_diff_density_max         2.14
_refine_diff_density_min         -0.85
_refine_ls_extinction_method     
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef       280(40)
_refine_ls_extinction_expression ?
_refine_ls_abs_structure_details ?
_refine_ls_abs_structure_Flack   ?
_refine_ls_abs_structure_Rogers  ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ga 0.2307 1.6083 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Ge 0.1547 1.8001 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Mn 0.3368 0.7283 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Sm -0.1638 3.4418 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?

loop_
_restr_angle_atom_site_label_1
_restr_angle_site_symmetry_1
_restr_angle_atom_site_label_2
_restr_angle_site_symmetry_2
_restr_angle_atom_site_label_3
_restr_angle_site_symmetry_3
_restr_angle_target
_restr_angle_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_torsion_atom_site_label_1
_restr_torsion_site_symmetry_1
_restr_torsion_atom_site_label_2
_restr_torsion_site_symmetry_2
_restr_torsion_atom_site_label_3
_restr_torsion_site_symmetry_3
_restr_torsion_atom_site_label_4
_restr_torsion_site_symmetry_4
_restr_torsion_angle_target
_restr_torsion_weight_param
? ? ? ? ? ? ? ? ? ?

loop_
_restr_equal_distance_atom_site_label_1
_restr_equal_distance_site_symmetry_1
_restr_equal_distance_atom_site_label_2
_restr_equal_distance_site_symmetry_2
_restr_equal_distance_class_class_id
_restr_equal_distance_class_target_weight_param
? ? ? ? ? ?

loop_
_restr_equal_angle_atom_site_label_1
_restr_equal_angle_site_symmetry_1
_restr_equal_angle_atom_site_label_2
_restr_equal_angle_site_symmetry_2
_restr_equal_angle_atom_site_label_3
_restr_equal_angle_site_symmetry_3
_restr_equal_angle_class_class_id
_restr_equal_angle_class_target_weight_param
? ? ? ? ? ? ? ?

loop_
_restr_equal_torsion_atom_site_label_1
_restr_equal_torsion_site_symmetry_1
_restr_equal_torsion_atom_site_label_2
_restr_equal_torsion_site_symmetry_2
_restr_equal_torsion_atom_site_label_3
_restr_equal_torsion_site_symmetry_3
_restr_equal_torsion_atom_site_label_4
_restr_equal_torsion_site_symmetry_4
_restr_equal_torsion_class_class_id
_restr_equal_torsion_class_target_weight_param
? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Sm1 Sm 0.25 0.25 0.25 Uani 0.0160(6) 8 1 d . . .
Mn1 Mn 0 0 0 Uiso 0.0138(11) 2 1 d . . .
Ga1 Ga 0.5 0 0.25 Uani 0.0167(8) 12 0.7167 d . . .
Ge1 Ge 0.5 0 0.25 Uani 0.0167(8) 12 0.2833 d . . .
Ga2 Ga 0.2917(3) 0 0 Uani 0.0179(9) 12 0.7167 d . . .
Ge2 Ge 0.2917(3) 0 0 Uani 0.0179(9) 12 0.2833 d . . .


loop_
_jana_atom_site_ADP_C_label
_jana_atom_site_ADP_C_type_symbol
_jana_atom_site_ADP_C_111
_jana_atom_site_ADP_C_112
_jana_atom_site_ADP_C_113
_jana_atom_site_ADP_C_122
_jana_atom_site_ADP_C_123
_jana_atom_site_ADP_C_133
_jana_atom_site_ADP_C_222
_jana_atom_site_ADP_C_223
_jana_atom_site_ADP_C_233
_jana_atom_site_ADP_C_333
Sm1 Sm 0 0 0 0 0 0 0 0 0 0
Ga1 Ga 0 0 0 0 0 0 0 0 0 0
Ge1 Ge 0 0 0 0 0 0 0 0 0 0
Ga2 Ga 0 0 0 0 0 0 0 0 0 0
Ge2 Ge 0 0 0 0 0 0 0 0 0 0

loop_
_jana_atom_site_ADP_D_label
_jana_atom_site_ADP_D_type_symbol
_jana_atom_site_ADP_D_1111
_jana_atom_site_ADP_D_1112
_jana_atom_site_ADP_D_1113
_jana_atom_site_ADP_D_1122
_jana_atom_site_ADP_D_1123
_jana_atom_site_ADP_D_1133
_jana_atom_site_ADP_D_1222
_jana_atom_site_ADP_D_1223
_jana_atom_site_ADP_D_1233
_jana_atom_site_ADP_D_1333
_jana_atom_site_ADP_D_2222
_jana_atom_site_ADP_D_2223
_jana_atom_site_ADP_D_2233
_jana_atom_site_ADP_D_2333
_jana_atom_site_ADP_D_3333
Sm1 Sm 0.0008(4) 0 0 0.00025(14) 0 0.00025(14) 0 0 0 0 0.0008(4) 0 0.00025(14)
0 0.0008(4)
Ga1 Ga 0.0019(9) 0 0 0 0 0 0 0 0 0 0.0019(9) 0 0 0 0
Ge1 Ge 0.0019(9) 0 0 0 0 0 0 0 0 0 0.0019(9) 0 0 0 0
Ga2 Ga 0 0 0 0 0 0 0 0 0 0 0.0016(9) 0 0.0015(4) 0 0.0016(9)
Ge2 Ge 0 0 0 0 0 0 0 0 0 0 0.0016(9) 0 0.0015(4) 0 0.0016(9)

loop_
_jana_atom_site_ADP_E_label
_jana_atom_site_ADP_E_type_symbol
_jana_atom_site_ADP_E_11111
_jana_atom_site_ADP_E_11112
_jana_atom_site_ADP_E_11113
_jana_atom_site_ADP_E_11122
_jana_atom_site_ADP_E_11123
_jana_atom_site_ADP_E_11133
_jana_atom_site_ADP_E_11222
_jana_atom_site_ADP_E_11223
_jana_atom_site_ADP_E_11233
_jana_atom_site_ADP_E_11333
_jana_atom_site_ADP_E_12222
_jana_atom_site_ADP_E_12223
_jana_atom_site_ADP_E_12233
_jana_atom_site_ADP_E_12333
_jana_atom_site_ADP_E_13333
_jana_atom_site_ADP_E_22222
_jana_atom_site_ADP_E_22223
_jana_atom_site_ADP_E_22233
_jana_atom_site_ADP_E_22333
_jana_atom_site_ADP_E_23333
_jana_atom_site_ADP_E_33333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
_jana_atom_site_ADP_F_label
_jana_atom_site_ADP_F_type_symbol
_jana_atom_site_ADP_F_111111
_jana_atom_site_ADP_F_111112
_jana_atom_site_ADP_F_111113
_jana_atom_site_ADP_F_111122
_jana_atom_site_ADP_F_111123
_jana_atom_site_ADP_F_111133
_jana_atom_site_ADP_F_111222
_jana_atom_site_ADP_F_111223
_jana_atom_site_ADP_F_111233
_jana_atom_site_ADP_F_111333
_jana_atom_site_ADP_F_112222
_jana_atom_site_ADP_F_112223
_jana_atom_site_ADP_F_112233
_jana_atom_site_ADP_F_112333
_jana_atom_site_ADP_F_113333
_jana_atom_site_ADP_F_122222
_jana_atom_site_ADP_F_122223
_jana_atom_site_ADP_F_122233
_jana_atom_site_ADP_F_122333
_jana_atom_site_ADP_F_123333
_jana_atom_site_ADP_F_133333
_jana_atom_site_ADP_F_222222
_jana_atom_site_ADP_F_222223
_jana_atom_site_ADP_F_222233
_jana_atom_site_ADP_F_222333
_jana_atom_site_ADP_F_223333
_jana_atom_site_ADP_F_233333
_jana_atom_site_ADP_F_333333
? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sm1 Mn1 . . 3.7362(4) ?
Sm1 Mn1 . 49_555 3.7362(4) ?
Sm1 Ga1 . . 3.0506(4) ?
Sm1 Ga1 . 51_555 3.0506(4) ?
Sm1 Ga1 . 5_555 3.0506(4) ?
Sm1 Ga1 . 55_555 3.0506(4) ?
Sm1 Ga1 . 9_555 3.0506(4) ?
Sm1 Ga1 . 59_555 3.0506(4) ?
Sm1 Ge1 . . 3.0506(4) ?
Sm1 Ge1 . 51_555 3.0506(4) ?
Sm1 Ge1 . 5_555 3.0506(4) ?
Sm1 Ge1 . 55_555 3.0506(4) ?
Sm1 Ge1 . 9_555 3.0506(4) ?
Sm1 Ge1 . 59_555 3.0506(4) ?
Sm1 Ga2 . . 3.0717(5) ?
Sm1 Ga2 . 50_555 3.0717(5) ?
Sm1 Ga2 . 5_555 3.0717(5) ?
Sm1 Ga2 . 54_555 3.0717(5) ?
Sm1 Ga2 . 9_555 3.0717(5) ?
Sm1 Ga2 . 58_555 3.0717(5) ?
Sm1 Ge2 . . 3.0717(5) ?
Sm1 Ge2 . 50_555 3.0717(5) ?
Sm1 Ge2 . 5_555 3.0717(5) ?
Sm1 Ge2 . 54_555 3.0717(5) ?
Sm1 Ge2 . 9_555 3.0717(5) ?
Sm1 Ge2 . 58_555 3.0717(5) ?
Mn1 Ga2 . . 2.517(2) ?
Mn1 Ga2 . 2_555 2.517(2) ?
Mn1 Ga2 . 5_555 2.517(2) ?
Mn1 Ga2 . 6_555 2.517(2) ?
Mn1 Ga2 . 9_555 2.517(2) ?
Mn1 Ga2 . 10_555 2.517(2) ?
Mn1 Ge2 . . 2.517(2) ?
Mn1 Ge2 . 2_555 2.517(2) ?
Mn1 Ge2 . 5_555 2.517(2) ?
Mn1 Ge2 . 6_555 2.517(2) ?
Mn1 Ge2 . 9_555 2.517(2) ?
Mn1 Ge2 . 10_555 2.517(2) ?
Ga1 Ga1 . 53_545 3.0506(4) ?
Ga1 Ga1 . 55_555 3.0506(4) ?
Ga1 Ga1 . 57_544 3.0506(4) ?
Ga1 Ga1 . 59_555 3.0506(4) ?
Ga1 Ge1 . 53_545 3.0506(4) ?
Ga1 Ge1 . 55_555 3.0506(4) ?
Ga1 Ge1 . 57_544 3.0506(4) ?
Ga1 Ge1 . 59_555 3.0506(4) ?
Ga1 Ga2 . . 2.8078(15) ?
Ga1 Ga2 . 2_655 2.8078(15) ?
Ga1 Ga2 . 53_545 2.8078(15) ?
Ga1 Ga2 . 54_555 2.8078(15) ?
Ga1 Ge2 . . 2.8078(15) ?
Ga1 Ge2 . 2_655 2.8078(15) ?
Ga1 Ge2 . 53_545 2.8078(15) ?
Ga1 Ge2 . 54_555 2.8078(15) ?
Ge1 Ge1 . 53_545 3.0506(4) ?
Ge1 Ge1 . 55_555 3.0506(4) ?
Ge1 Ge1 . 57_544 3.0506(4) ?
Ge1 Ge1 . 59_555 3.0506(4) ?
Ge1 Ga2 . . 2.8078(15) ?
Ge1 Ga2 . 2_655 2.8078(15) ?
Ge1 Ga2 . 53_545 2.8078(15) ?
Ge1 Ga2 . 54_555 2.8078(15) ?
Ge1 Ge2 . . 2.8078(15) ?
Ge1 Ge2 . 2_655 2.8078(15) ?
Ge1 Ge2 . 53_545 2.8078(15) ?
Ge1 Ge2 . 54_555 2.8078(15) ?
Ga2 Ga2 . 2_655 3.595(3) ?
Ga2 Ga2 . 5_555 3.559(2) ?
Ga2 Ga2 . 6_555 3.559(2) ?
Ga2 Ga2 . 9_555 3.559(2) ?
Ga2 Ga2 . 10_555 3.559(2) ?
Ga2 Ge2 . 2_655 3.595(3) ?
Ga2 Ge2 . 5_555 3.559(2) ?
Ga2 Ge2 . 6_555 3.559(2) ?
Ga2 Ge2 . 9_555 3.559(2) ?
Ga2 Ge2 . 10_555 3.559(2) ?
Ge2 Ge2 . 2_655 3.595(3) ?
Ge2 Ge2 . 5_555 3.559(2) ?
Ge2 Ge2 . 6_555 3.559(2) ?
Ge2 Ge2 . 9_555 3.559(2) ?
Ge2 Ge2 . 10_555 3.559(2) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Mn1 Sm1 Mn1 . . 49_555 180 ?
Mn1 Sm1 Ga1 . . . 90.000(6) ?
Mn1 Sm1 Ga1 . . 51_555 90.000(6) ?
Mn1 Sm1 Ga1 . . 5_555 90.000(6) ?
Mn1 Sm1 Ga1 . . 55_555 90.000(6) ?
Mn1 Sm1 Ga1 . . 9_555 90.000(6) ?
Mn1 Sm1 Ga1 . . 59_555 90.000(6) ?
Mn1 Sm1 Ge1 . . . 90.000(6) ?
Mn1 Sm1 Ge1 . . 51_555 90.000(6) ?
Mn1 Sm1 Ge1 . . 5_555 90.000(6) ?
Mn1 Sm1 Ge1 . . 55_555 90.000(6) ?
Mn1 Sm1 Ge1 . . 9_555 90.000(6) ?
Mn1 Sm1 Ge1 . . 59_555 90.000(6) ?
Mn1 Sm1 Ga2 . . . 41.99(4) ?
Mn1 Sm1 Ga2 . . 50_555 138.01(4) ?
Mn1 Sm1 Ga2 . . 5_555 41.99(4) ?
Mn1 Sm1 Ga2 . . 54_555 138.01(4) ?
Mn1 Sm1 Ga2 . . 9_555 41.99(4) ?
Mn1 Sm1 Ga2 . . 58_555 138.01(4) ?
Mn1 Sm1 Ge2 . . . 41.99(4) ?
Mn1 Sm1 Ge2 . . 50_555 138.01(4) ?
Mn1 Sm1 Ge2 . . 5_555 41.99(4) ?
Mn1 Sm1 Ge2 . . 54_555 138.01(4) ?
Mn1 Sm1 Ge2 . . 9_555 41.99(4) ?
Mn1 Sm1 Ge2 . . 58_555 138.01(4) ?
Mn1 Sm1 Ga1 49_555 . . 90.000(6) ?
Mn1 Sm1 Ga1 49_555 . 51_555 90.000(6) ?
Mn1 Sm1 Ga1 49_555 . 5_555 90.000(6) ?
Mn1 Sm1 Ga1 49_555 . 55_555 90.000(6) ?
Mn1 Sm1 Ga1 49_555 . 9_555 90.000(6) ?
Mn1 Sm1 Ga1 49_555 . 59_555 90.000(6) ?
Mn1 Sm1 Ge1 49_555 . . 90.000(6) ?
Mn1 Sm1 Ge1 49_555 . 51_555 90.000(6) ?
Mn1 Sm1 Ge1 49_555 . 5_555 90.000(6) ?
Mn1 Sm1 Ge1 49_555 . 55_555 90.000(6) ?
Mn1 Sm1 Ge1 49_555 . 9_555 90.000(6) ?
Mn1 Sm1 Ge1 49_555 . 59_555 90.000(6) ?
Mn1 Sm1 Ga2 49_555 . . 138.01(4) ?
Mn1 Sm1 Ga2 49_555 . 50_555 41.99(4) ?
Mn1 Sm1 Ga2 49_555 . 5_555 138.01(4) ?
Mn1 Sm1 Ga2 49_555 . 54_555 41.99(4) ?
Mn1 Sm1 Ga2 49_555 . 9_555 138.01(4) ?
Mn1 Sm1 Ga2 49_555 . 58_555 41.99(4) ?
Mn1 Sm1 Ge2 49_555 . . 138.01(4) ?
Mn1 Sm1 Ge2 49_555 . 50_555 41.99(4) ?
Mn1 Sm1 Ge2 49_555 . 5_555 138.01(4) ?
Mn1 Sm1 Ge2 49_555 . 54_555 41.99(4) ?
Mn1 Sm1 Ge2 49_555 . 9_555 138.01(4) ?
Mn1 Sm1 Ge2 49_555 . 58_555 41.99(4) ?
Ga1 Sm1 Ga1 . . 51_555 180 ?
Ga1 Sm1 Ga1 . . 5_555 120.000(4) ?
Ga1 Sm1 Ga1 . . 55_555 60.000(4) ?
Ga1 Sm1 Ga1 . . 9_555 120.000(4) ?
Ga1 Sm1 Ga1 . . 59_555 60.000(4) ?
Ga1 Sm1 Ge1 . . . 0 ?
Ga1 Sm1 Ge1 . . 51_555 180 ?
Ga1 Sm1 Ge1 . . 5_555 120.000(4) ?
Ga1 Sm1 Ge1 . . 55_555 60.000(4) ?
Ga1 Sm1 Ge1 . . 9_555 120.000(4) ?
Ga1 Sm1 Ge1 . . 59_555 60.000(4) ?
Ga1 Sm1 Ga2 . . . 54.60(3) ?
Ga1 Sm1 Ga2 . . 50_555 125.40(3) ?
Ga1 Sm1 Ga2 . . 5_555 125.40(3) ?
Ga1 Sm1 Ga2 . . 54_555 54.60(3) ?
Ga1 Sm1 Ga2 . . 9_555 90.000(7) ?
Ga1 Sm1 Ga2 . . 58_555 90.000(7) ?
Ga1 Sm1 Ge2 . . . 54.60(3) ?
Ga1 Sm1 Ge2 . . 50_555 125.40(3) ?
Ga1 Sm1 Ge2 . . 5_555 125.40(3) ?
Ga1 Sm1 Ge2 . . 54_555 54.60(3) ?
Ga1 Sm1 Ge2 . . 9_555 90.000(7) ?
Ga1 Sm1 Ge2 . . 58_555 90.000(7) ?
Ga1 Sm1 Ga1 51_555 . 5_555 60.000(4) ?
Ga1 Sm1 Ga1 51_555 . 55_555 120.000(4) ?
Ga1 Sm1 Ga1 51_555 . 9_555 60.000(4) ?
Ga1 Sm1 Ga1 51_555 . 59_555 120.000(4) ?
Ga1 Sm1 Ge1 51_555 . . 180 ?
Ga1 Sm1 Ge1 51_555 . 51_555 0 ?
Ga1 Sm1 Ge1 51_555 . 5_555 60.000(4) ?
Ga1 Sm1 Ge1 51_555 . 55_555 120.000(4) ?
Ga1 Sm1 Ge1 51_555 . 9_555 60.000(4) ?
Ga1 Sm1 Ge1 51_555 . 59_555 120.000(4) ?
Ga1 Sm1 Ga2 51_555 . . 125.40(3) ?
Ga1 Sm1 Ga2 51_555 . 50_555 54.60(3) ?
Ga1 Sm1 Ga2 51_555 . 5_555 54.60(3) ?
Ga1 Sm1 Ga2 51_555 . 54_555 125.40(3) ?
Ga1 Sm1 Ga2 51_555 . 9_555 90.000(7) ?
Ga1 Sm1 Ga2 51_555 . 58_555 90.000(7) ?
Ga1 Sm1 Ge2 51_555 . . 125.40(3) ?
Ga1 Sm1 Ge2 51_555 . 50_555 54.60(3) ?
Ga1 Sm1 Ge2 51_555 . 5_555 54.60(3) ?
Ga1 Sm1 Ge2 51_555 . 54_555 125.40(3) ?
Ga1 Sm1 Ge2 51_555 . 9_555 90.000(7) ?
Ga1 Sm1 Ge2 51_555 . 58_555 90.000(7) ?
Ga1 Sm1 Ga1 5_555 . 55_555 180 ?
Ga1 Sm1 Ga1 5_555 . 9_555 120.000(4) ?
Ga1 Sm1 Ga1 5_555 . 59_555 60.000(4) ?
Ga1 Sm1 Ge1 5_555 . . 120.000(4) ?
Ga1 Sm1 Ge1 5_555 . 51_555 60.000(4) ?
Ga1 Sm1 Ge1 5_555 . 5_555 0 ?
Ga1 Sm1 Ge1 5_555 . 55_555 180 ?
Ga1 Sm1 Ge1 5_555 . 9_555 120.000(4) ?
Ga1 Sm1 Ge1 5_555 . 59_555 60.000(4) ?
Ga1 Sm1 Ga2 5_555 . . 90.000(7) ?
Ga1 Sm1 Ga2 5_555 . 50_555 90.000(7) ?
Ga1 Sm1 Ga2 5_555 . 5_555 54.60(3) ?
Ga1 Sm1 Ga2 5_555 . 54_555 125.40(3) ?
Ga1 Sm1 Ga2 5_555 . 9_555 125.40(3) ?
Ga1 Sm1 Ga2 5_555 . 58_555 54.60(3) ?
Ga1 Sm1 Ge2 5_555 . . 90.000(7) ?
Ga1 Sm1 Ge2 5_555 . 50_555 90.000(7) ?
Ga1 Sm1 Ge2 5_555 . 5_555 54.60(3) ?
Ga1 Sm1 Ge2 5_555 . 54_555 125.40(3) ?
Ga1 Sm1 Ge2 5_555 . 9_555 125.40(3) ?
Ga1 Sm1 Ge2 5_555 . 58_555 54.60(3) ?
Ga1 Sm1 Ga1 55_555 . 9_555 60.000(4) ?
Ga1 Sm1 Ga1 55_555 . 59_555 120.000(4) ?
Ga1 Sm1 Ge1 55_555 . . 60.000(4) ?
Ga1 Sm1 Ge1 55_555 . 51_555 120.000(4) ?
Ga1 Sm1 Ge1 55_555 . 5_555 180 ?
Ga1 Sm1 Ge1 55_555 . 55_555 0 ?
Ga1 Sm1 Ge1 55_555 . 9_555 60.000(4) ?
Ga1 Sm1 Ge1 55_555 . 59_555 120.000(4) ?
Ga1 Sm1 Ga2 55_555 . . 90.000(7) ?
Ga1 Sm1 Ga2 55_555 . 50_555 90.000(7) ?
Ga1 Sm1 Ga2 55_555 . 5_555 125.40(3) ?
Ga1 Sm1 Ga2 55_555 . 54_555 54.60(3) ?
Ga1 Sm1 Ga2 55_555 . 9_555 54.60(3) ?
Ga1 Sm1 Ga2 55_555 . 58_555 125.40(3) ?
Ga1 Sm1 Ge2 55_555 . . 90.000(7) ?
Ga1 Sm1 Ge2 55_555 . 50_555 90.000(7) ?
Ga1 Sm1 Ge2 55_555 . 5_555 125.40(3) ?
Ga1 Sm1 Ge2 55_555 . 54_555 54.60(3) ?
Ga1 Sm1 Ge2 55_555 . 9_555 54.60(3) ?
Ga1 Sm1 Ge2 55_555 . 58_555 125.40(3) ?
Ga1 Sm1 Ga1 9_555 . 59_555 180 ?
Ga1 Sm1 Ge1 9_555 . . 120.000(4) ?
Ga1 Sm1 Ge1 9_555 . 51_555 60.000(4) ?
Ga1 Sm1 Ge1 9_555 . 5_555 120.000(4) ?
Ga1 Sm1 Ge1 9_555 . 55_555 60.000(4) ?
Ga1 Sm1 Ge1 9_555 . 9_555 0 ?
Ga1 Sm1 Ge1 9_555 . 59_555 180 ?
Ga1 Sm1 Ga2 9_555 . . 125.40(3) ?
Ga1 Sm1 Ga2 9_555 . 50_555 54.60(3) ?
Ga1 Sm1 Ga2 9_555 . 5_555 90.000(7) ?
Ga1 Sm1 Ga2 9_555 . 54_555 90.000(7) ?
Ga1 Sm1 Ga2 9_555 . 9_555 54.60(3) ?
Ga1 Sm1 Ga2 9_555 . 58_555 125.40(3) ?
Ga1 Sm1 Ge2 9_555 . . 125.40(3) ?
Ga1 Sm1 Ge2 9_555 . 50_555 54.60(3) ?
Ga1 Sm1 Ge2 9_555 . 5_555 90.000(7) ?
Ga1 Sm1 Ge2 9_555 . 54_555 90.000(7) ?
Ga1 Sm1 Ge2 9_555 . 9_555 54.60(3) ?
Ga1 Sm1 Ge2 9_555 . 58_555 125.40(3) ?
Ga1 Sm1 Ge1 59_555 . . 60.000(4) ?
Ga1 Sm1 Ge1 59_555 . 51_555 120.000(4) ?
Ga1 Sm1 Ge1 59_555 . 5_555 60.000(4) ?
Ga1 Sm1 Ge1 59_555 . 55_555 120.000(4) ?
Ga1 Sm1 Ge1 59_555 . 9_555 180 ?
Ga1 Sm1 Ge1 59_555 . 59_555 0 ?
Ga1 Sm1 Ga2 59_555 . . 54.60(3) ?
Ga1 Sm1 Ga2 59_555 . 50_555 125.40(3) ?
Ga1 Sm1 Ga2 59_555 . 5_555 90.000(7) ?
Ga1 Sm1 Ga2 59_555 . 54_555 90.000(7) ?
Ga1 Sm1 Ga2 59_555 . 9_555 125.40(3) ?
Ga1 Sm1 Ga2 59_555 . 58_555 54.60(3) ?
Ga1 Sm1 Ge2 59_555 . . 54.60(3) ?
Ga1 Sm1 Ge2 59_555 . 50_555 125.40(3) ?
Ga1 Sm1 Ge2 59_555 . 5_555 90.000(7) ?
Ga1 Sm1 Ge2 59_555 . 54_555 90.000(7) ?
Ga1 Sm1 Ge2 59_555 . 9_555 125.40(3) ?
Ga1 Sm1 Ge2 59_555 . 58_555 54.60(3) ?
Ge1 Sm1 Ge1 . . 51_555 180 ?
Ge1 Sm1 Ge1 . . 5_555 120.000(4) ?
Ge1 Sm1 Ge1 . . 55_555 60.000(4) ?
Ge1 Sm1 Ge1 . . 9_555 120.000(4) ?
Ge1 Sm1 Ge1 . . 59_555 60.000(4) ?
Ge1 Sm1 Ga2 . . . 54.60(3) ?
Ge1 Sm1 Ga2 . . 50_555 125.40(3) ?
Ge1 Sm1 Ga2 . . 5_555 125.40(3) ?
Ge1 Sm1 Ga2 . . 54_555 54.60(3) ?
Ge1 Sm1 Ga2 . . 9_555 90.000(7) ?
Ge1 Sm1 Ga2 . . 58_555 90.000(7) ?
Ge1 Sm1 Ge2 . . . 54.60(3) ?
Ge1 Sm1 Ge2 . . 50_555 125.40(3) ?
Ge1 Sm1 Ge2 . . 5_555 125.40(3) ?
Ge1 Sm1 Ge2 . . 54_555 54.60(3) ?
Ge1 Sm1 Ge2 . . 9_555 90.000(7) ?
Ge1 Sm1 Ge2 . . 58_555 90.000(7) ?
Ge1 Sm1 Ge1 51_555 . 5_555 60.000(4) ?
Ge1 Sm1 Ge1 51_555 . 55_555 120.000(4) ?
Ge1 Sm1 Ge1 51_555 . 9_555 60.000(4) ?
Ge1 Sm1 Ge1 51_555 . 59_555 120.000(4) ?
Ge1 Sm1 Ga2 51_555 . . 125.40(3) ?
Ge1 Sm1 Ga2 51_555 . 50_555 54.60(3) ?
Ge1 Sm1 Ga2 51_555 . 5_555 54.60(3) ?
Ge1 Sm1 Ga2 51_555 . 54_555 125.40(3) ?
Ge1 Sm1 Ga2 51_555 . 9_555 90.000(7) ?
Ge1 Sm1 Ga2 51_555 . 58_555 90.000(7) ?
Ge1 Sm1 Ge2 51_555 . . 125.40(3) ?
Ge1 Sm1 Ge2 51_555 . 50_555 54.60(3) ?
Ge1 Sm1 Ge2 51_555 . 5_555 54.60(3) ?
Ge1 Sm1 Ge2 51_555 . 54_555 125.40(3) ?
Ge1 Sm1 Ge2 51_555 . 9_555 90.000(7) ?
Ge1 Sm1 Ge2 51_555 . 58_555 90.000(7) ?
Ge1 Sm1 Ge1 5_555 . 55_555 180 ?
Ge1 Sm1 Ge1 5_555 . 9_555 120.000(4) ?
Ge1 Sm1 Ge1 5_555 . 59_555 60.000(4) ?
Ge1 Sm1 Ga2 5_555 . . 90.000(7) ?
Ge1 Sm1 Ga2 5_555 . 50_555 90.000(7) ?
Ge1 Sm1 Ga2 5_555 . 5_555 54.60(3) ?
Ge1 Sm1 Ga2 5_555 . 54_555 125.40(3) ?
Ge1 Sm1 Ga2 5_555 . 9_555 125.40(3) ?
Ge1 Sm1 Ga2 5_555 . 58_555 54.60(3) ?
Ge1 Sm1 Ge2 5_555 . . 90.000(7) ?
Ge1 Sm1 Ge2 5_555 . 50_555 90.000(7) ?
Ge1 Sm1 Ge2 5_555 . 5_555 54.60(3) ?
Ge1 Sm1 Ge2 5_555 . 54_555 125.40(3) ?
Ge1 Sm1 Ge2 5_555 . 9_555 125.40(3) ?
Ge1 Sm1 Ge2 5_555 . 58_555 54.60(3) ?
Ge1 Sm1 Ge1 55_555 . 9_555 60.000(4) ?
Ge1 Sm1 Ge1 55_555 . 59_555 120.000(4) ?
Ge1 Sm1 Ga2 55_555 . . 90.000(7) ?
Ge1 Sm1 Ga2 55_555 . 50_555 90.000(7) ?
Ge1 Sm1 Ga2 55_555 . 5_555 125.40(3) ?
Ge1 Sm1 Ga2 55_555 . 54_555 54.60(3) ?
Ge1 Sm1 Ga2 55_555 . 9_555 54.60(3) ?
Ge1 Sm1 Ga2 55_555 . 58_555 125.40(3) ?
Ge1 Sm1 Ge2 55_555 . . 90.000(7) ?
Ge1 Sm1 Ge2 55_555 . 50_555 90.000(7) ?
Ge1 Sm1 Ge2 55_555 . 5_555 125.40(3) ?
Ge1 Sm1 Ge2 55_555 . 54_555 54.60(3) ?
Ge1 Sm1 Ge2 55_555 . 9_555 54.60(3) ?
Ge1 Sm1 Ge2 55_555 . 58_555 125.40(3) ?
Ge1 Sm1 Ge1 9_555 . 59_555 180 ?
Ge1 Sm1 Ga2 9_555 . . 125.40(3) ?
Ge1 Sm1 Ga2 9_555 . 50_555 54.60(3) ?
Ge1 Sm1 Ga2 9_555 . 5_555 90.000(7) ?
Ge1 Sm1 Ga2 9_555 . 54_555 90.000(7) ?
Ge1 Sm1 Ga2 9_555 . 9_555 54.60(3) ?
Ge1 Sm1 Ga2 9_555 . 58_555 125.40(3) ?
Ge1 Sm1 Ge2 9_555 . . 125.40(3) ?
Ge1 Sm1 Ge2 9_555 . 50_555 54.60(3) ?
Ge1 Sm1 Ge2 9_555 . 5_555 90.000(7) ?
Ge1 Sm1 Ge2 9_555 . 54_555 90.000(7) ?
Ge1 Sm1 Ge2 9_555 . 9_555 54.60(3) ?
Ge1 Sm1 Ge2 9_555 . 58_555 125.40(3) ?
Ge1 Sm1 Ga2 59_555 . . 54.60(3) ?
Ge1 Sm1 Ga2 59_555 . 50_555 125.40(3) ?
Ge1 Sm1 Ga2 59_555 . 5_555 90.000(7) ?
Ge1 Sm1 Ga2 59_555 . 54_555 90.000(7) ?
Ge1 Sm1 Ga2 59_555 . 9_555 125.40(3) ?
Ge1 Sm1 Ga2 59_555 . 58_555 54.60(3) ?
Ge1 Sm1 Ge2 59_555 . . 54.60(3) ?
Ge1 Sm1 Ge2 59_555 . 50_555 125.40(3) ?
Ge1 Sm1 Ge2 59_555 . 5_555 90.000(7) ?
Ge1 Sm1 Ge2 59_555 . 54_555 90.000(7) ?
Ge1 Sm1 Ge2 59_555 . 9_555 125.40(3) ?
Ge1 Sm1 Ge2 59_555 . 58_555 54.60(3) ?
Ga2 Sm1 Ga2 . . 50_555 180 ?
Ga2 Sm1 Ga2 . . 5_555 70.81(5) ?
Ga2 Sm1 Ga2 . . 54_555 109.19(5) ?
Ga2 Sm1 Ga2 . . 9_555 70.81(5) ?
Ga2 Sm1 Ga2 . . 58_555 109.19(5) ?
Ga2 Sm1 Ge2 . . . 0 ?
Ga2 Sm1 Ge2 . . 50_555 180 ?
Ga2 Sm1 Ge2 . . 5_555 70.81(5) ?
Ga2 Sm1 Ge2 . . 54_555 109.19(5) ?
Ga2 Sm1 Ge2 . . 9_555 70.81(5) ?
Ga2 Sm1 Ge2 . . 58_555 109.19(5) ?
Ga2 Sm1 Ga2 50_555 . 5_555 109.19(5) ?
Ga2 Sm1 Ga2 50_555 . 54_555 70.81(5) ?
Ga2 Sm1 Ga2 50_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ga2 50_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ge2 50_555 . . 180 ?
Ga2 Sm1 Ge2 50_555 . 50_555 0 ?
Ga2 Sm1 Ge2 50_555 . 5_555 109.19(5) ?
Ga2 Sm1 Ge2 50_555 . 54_555 70.81(5) ?
Ga2 Sm1 Ge2 50_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ge2 50_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ga2 5_555 . 54_555 180 ?
Ga2 Sm1 Ga2 5_555 . 9_555 70.81(5) ?
Ga2 Sm1 Ga2 5_555 . 58_555 109.19(5) ?
Ga2 Sm1 Ge2 5_555 . . 70.81(5) ?
Ga2 Sm1 Ge2 5_555 . 50_555 109.19(5) ?
Ga2 Sm1 Ge2 5_555 . 5_555 0 ?
Ga2 Sm1 Ge2 5_555 . 54_555 180 ?
Ga2 Sm1 Ge2 5_555 . 9_555 70.81(5) ?
Ga2 Sm1 Ge2 5_555 . 58_555 109.19(5) ?
Ga2 Sm1 Ga2 54_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ga2 54_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ge2 54_555 . . 109.19(5) ?
Ga2 Sm1 Ge2 54_555 . 50_555 70.81(5) ?
Ga2 Sm1 Ge2 54_555 . 5_555 180 ?
Ga2 Sm1 Ge2 54_555 . 54_555 0 ?
Ga2 Sm1 Ge2 54_555 . 9_555 109.19(5) ?
Ga2 Sm1 Ge2 54_555 . 58_555 70.81(5) ?
Ga2 Sm1 Ga2 9_555 . 58_555 180 ?
Ga2 Sm1 Ge2 9_555 . . 70.81(5) ?
Ga2 Sm1 Ge2 9_555 . 50_555 109.19(5) ?
Ga2 Sm1 Ge2 9_555 . 5_555 70.81(5) ?
Ga2 Sm1 Ge2 9_555 . 54_555 109.19(5) ?
Ga2 Sm1 Ge2 9_555 . 9_555 0 ?
Ga2 Sm1 Ge2 9_555 . 58_555 180 ?
Ga2 Sm1 Ge2 58_555 . . 109.19(5) ?
Ga2 Sm1 Ge2 58_555 . 50_555 70.81(5) ?
Ga2 Sm1 Ge2 58_555 . 5_555 109.19(5) ?
Ga2 Sm1 Ge2 58_555 . 54_555 70.81(5) ?
Ga2 Sm1 Ge2 58_555 . 9_555 180 ?
Ga2 Sm1 Ge2 58_555 . 58_555 0 ?
Ge2 Sm1 Ge2 . . 50_555 180 ?
Ge2 Sm1 Ge2 . . 5_555 70.81(5) ?
Ge2 Sm1 Ge2 . . 54_555 109.19(5) ?
Ge2 Sm1 Ge2 . . 9_555 70.81(5) ?
Ge2 Sm1 Ge2 . . 58_555 109.19(5) ?
Ge2 Sm1 Ge2 50_555 . 5_555 109.19(5) ?
Ge2 Sm1 Ge2 50_555 . 54_555 70.81(5) ?
Ge2 Sm1 Ge2 50_555 . 9_555 109.19(5) ?
Ge2 Sm1 Ge2 50_555 . 58_555 70.81(5) ?
Ge2 Sm1 Ge2 5_555 . 54_555 180 ?
Ge2 Sm1 Ge2 5_555 . 9_555 70.81(5) ?
Ge2 Sm1 Ge2 5_555 . 58_555 109.19(5) ?
Ge2 Sm1 Ge2 54_555 . 9_555 109.19(5) ?
Ge2 Sm1 Ge2 54_555 . 58_555 70.81(5) ?
Ge2 Sm1 Ge2 9_555 . 58_555 180 ?
Sm1 Mn1 Sm1 . . 49_444 180 ?
Sm1 Mn1 Sm1 . . 2_555 109.471(6) ?
Sm1 Mn1 Sm1 . . 50_554 70.529(6) ?
Sm1 Mn1 Sm1 . . 3_555 109.471(6) ?
Sm1 Mn1 Sm1 . . 51_545 70.529(6) ?
Sm1 Mn1 Sm1 . . 4_555 109.471(6) ?
Sm1 Mn1 Sm1 . . 52_455 70.529(6) ?
Sm1 Mn1 Ga2 . . . 54.736(3) ?
Sm1 Mn1 Ga2 . . 2_555 125.264(3) ?
Sm1 Mn1 Ga2 . . 5_555 54.736(3) ?
Sm1 Mn1 Ga2 . . 6_555 125.264(3) ?
Sm1 Mn1 Ga2 . . 9_555 54.736(3) ?
Sm1 Mn1 Ga2 . . 10_555 125.264(3) ?
Sm1 Mn1 Ge2 . . . 54.736(3) ?
Sm1 Mn1 Ge2 . . 2_555 125.264(3) ?
Sm1 Mn1 Ge2 . . 5_555 54.736(3) ?
Sm1 Mn1 Ge2 . . 6_555 125.264(3) ?
Sm1 Mn1 Ge2 . . 9_555 54.736(3) ?
Sm1 Mn1 Ge2 . . 10_555 125.264(3) ?
Sm1 Mn1 Sm1 49_444 . 2_555 70.529(6) ?
Sm1 Mn1 Sm1 49_444 . 50_554 109.471(6) ?
Sm1 Mn1 Sm1 49_444 . 3_555 70.529(6) ?
Sm1 Mn1 Sm1 49_444 . 51_545 109.471(6) ?
Sm1 Mn1 Sm1 49_444 . 4_555 70.529(6) ?
Sm1 Mn1 Sm1 49_444 . 52_455 109.471(6) ?
Sm1 Mn1 Ga2 49_444 . . 125.264(3) ?
Sm1 Mn1 Ga2 49_444 . 2_555 54.736(3) ?
Sm1 Mn1 Ga2 49_444 . 5_555 125.264(3) ?
Sm1 Mn1 Ga2 49_444 . 6_555 54.736(3) ?
Sm1 Mn1 Ga2 49_444 . 9_555 125.264(3) ?
Sm1 Mn1 Ga2 49_444 . 10_555 54.736(3) ?
Sm1 Mn1 Ge2 49_444 . . 125.264(3) ?
Sm1 Mn1 Ge2 49_444 . 2_555 54.736(3) ?
Sm1 Mn1 Ge2 49_444 . 5_555 125.264(3) ?
Sm1 Mn1 Ge2 49_444 . 6_555 54.736(3) ?
Sm1 Mn1 Ge2 49_444 . 9_555 125.264(3) ?
Sm1 Mn1 Ge2 49_444 . 10_555 54.736(3) ?
Sm1 Mn1 Sm1 2_555 . 50_554 180 ?
Sm1 Mn1 Sm1 2_555 . 3_555 109.471(6) ?
Sm1 Mn1 Sm1 2_555 . 51_545 70.529(6) ?
Sm1 Mn1 Sm1 2_555 . 4_555 109.471(6) ?
Sm1 Mn1 Sm1 2_555 . 52_455 70.529(6) ?
Sm1 Mn1 Ga2 2_555 . . 125.264(3) ?
Sm1 Mn1 Ga2 2_555 . 2_555 54.736(3) ?
Sm1 Mn1 Ga2 2_555 . 5_555 125.264(3) ?
Sm1 Mn1 Ga2 2_555 . 6_555 54.736(3) ?
Sm1 Mn1 Ga2 2_555 . 9_555 54.736(3) ?
Sm1 Mn1 Ga2 2_555 . 10_555 125.264(3) ?
Sm1 Mn1 Ge2 2_555 . . 125.264(3) ?
Sm1 Mn1 Ge2 2_555 . 2_555 54.736(3) ?
Sm1 Mn1 Ge2 2_555 . 5_555 125.264(3) ?
Sm1 Mn1 Ge2 2_555 . 6_555 54.736(3) ?
Sm1 Mn1 Ge2 2_555 . 9_555 54.736(3) ?
Sm1 Mn1 Ge2 2_555 . 10_555 125.264(3) ?
Sm1 Mn1 Sm1 50_554 . 3_555 70.529(6) ?
Sm1 Mn1 Sm1 50_554 . 51_545 109.471(6) ?
Sm1 Mn1 Sm1 50_554 . 4_555 70.529(6) ?
Sm1 Mn1 Sm1 50_554 . 52_455 109.471(6) ?
Sm1 Mn1 Ga2 50_554 . . 54.736(3) ?
Sm1 Mn1 Ga2 50_554 . 2_555 125.264(3) ?
Sm1 Mn1 Ga2 50_554 . 5_555 54.736(3) ?
Sm1 Mn1 Ga2 50_554 . 6_555 125.264(3) ?
Sm1 Mn1 Ga2 50_554 . 9_555 125.264(3) ?
Sm1 Mn1 Ga2 50_554 . 10_555 54.736(3) ?
Sm1 Mn1 Ge2 50_554 . . 54.736(3) ?
Sm1 Mn1 Ge2 50_554 . 2_555 125.264(3) ?
Sm1 Mn1 Ge2 50_554 . 5_555 54.736(3) ?
Sm1 Mn1 Ge2 50_554 . 6_555 125.264(3) ?
Sm1 Mn1 Ge2 50_554 . 9_555 125.264(3) ?
Sm1 Mn1 Ge2 50_554 . 10_555 54.736(3) ?
Sm1 Mn1 Sm1 3_555 . 51_545 180 ?
Sm1 Mn1 Sm1 3_555 . 4_555 109.471(6) ?
Sm1 Mn1 Sm1 3_555 . 52_455 70.529(6) ?
Sm1 Mn1 Ga2 3_555 . . 125.264(3) ?
Sm1 Mn1 Ga2 3_555 . 2_555 54.736(3) ?
Sm1 Mn1 Ga2 3_555 . 5_555 54.736(3) ?
Sm1 Mn1 Ga2 3_555 . 6_555 125.264(3) ?
Sm1 Mn1 Ga2 3_555 . 9_555 125.264(3) ?
Sm1 Mn1 Ga2 3_555 . 10_555 54.736(3) ?
Sm1 Mn1 Ge2 3_555 . . 125.264(3) ?
Sm1 Mn1 Ge2 3_555 . 2_555 54.736(3) ?
Sm1 Mn1 Ge2 3_555 . 5_555 54.736(3) ?
Sm1 Mn1 Ge2 3_555 . 6_555 125.264(3) ?
Sm1 Mn1 Ge2 3_555 . 9_555 125.264(3) ?
Sm1 Mn1 Ge2 3_555 . 10_555 54.736(3) ?
Sm1 Mn1 Sm1 51_545 . 4_555 70.529(6) ?
Sm1 Mn1 Sm1 51_545 . 52_455 109.471(6) ?
Sm1 Mn1 Ga2 51_545 . . 54.736(3) ?
Sm1 Mn1 Ga2 51_545 . 2_555 125.264(3) ?
Sm1 Mn1 Ga2 51_545 . 5_555 125.264(3) ?
Sm1 Mn1 Ga2 51_545 . 6_555 54.736(3) ?
Sm1 Mn1 Ga2 51_545 . 9_555 54.736(3) ?
Sm1 Mn1 Ga2 51_545 . 10_555 125.264(3) ?
Sm1 Mn1 Ge2 51_545 . . 54.736(3) ?
Sm1 Mn1 Ge2 51_545 . 2_555 125.264(3) ?
Sm1 Mn1 Ge2 51_545 . 5_555 125.264(3) ?
Sm1 Mn1 Ge2 51_545 . 6_555 54.736(3) ?
Sm1 Mn1 Ge2 51_545 . 9_555 54.736(3) ?
Sm1 Mn1 Ge2 51_545 . 10_555 125.264(3) ?
Sm1 Mn1 Sm1 4_555 . 52_455 180 ?
Sm1 Mn1 Ga2 4_555 . . 54.736(3) ?
Sm1 Mn1 Ga2 4_555 . 2_555 125.264(3) ?
Sm1 Mn1 Ga2 4_555 . 5_555 125.264(3) ?
Sm1 Mn1 Ga2 4_555 . 6_555 54.736(3) ?
Sm1 Mn1 Ga2 4_555 . 9_555 125.264(3) ?
Sm1 Mn1 Ga2 4_555 . 10_555 54.736(3) ?
Sm1 Mn1 Ge2 4_555 . . 54.736(3) ?
Sm1 Mn1 Ge2 4_555 . 2_555 125.264(3) ?
Sm1 Mn1 Ge2 4_555 . 5_555 125.264(3) ?
Sm1 Mn1 Ge2 4_555 . 6_555 54.736(3) ?
Sm1 Mn1 Ge2 4_555 . 9_555 125.264(3) ?
Sm1 Mn1 Ge2 4_555 . 10_555 54.736(3) ?
Sm1 Mn1 Ga2 52_455 . . 125.264(3) ?
Sm1 Mn1 Ga2 52_455 . 2_555 54.736(3) ?
Sm1 Mn1 Ga2 52_455 . 5_555 54.736(3) ?
Sm1 Mn1 Ga2 52_455 . 6_555 125.264(3) ?
Sm1 Mn1 Ga2 52_455 . 9_555 54.736(3) ?
Sm1 Mn1 Ga2 52_455 . 10_555 125.264(3) ?
Sm1 Mn1 Ge2 52_455 . . 125.264(3) ?
Sm1 Mn1 Ge2 52_455 . 2_555 54.736(3) ?
Sm1 Mn1 Ge2 52_455 . 5_555 54.736(3) ?
Sm1 Mn1 Ge2 52_455 . 6_555 125.264(3) ?
Sm1 Mn1 Ge2 52_455 . 9_555 54.736(3) ?
Sm1 Mn1 Ge2 52_455 . 10_555 125.264(3) ?
Ga2 Mn1 Ga2 . . 2_555 180 ?
Ga2 Mn1 Ga2 . . 5_555 90 ?
Ga2 Mn1 Ga2 . . 6_555 90 ?
Ga2 Mn1 Ga2 . . 9_555 90 ?
Ga2 Mn1 Ga2 . . 10_555 90 ?
Ga2 Mn1 Ge2 . . . 0 ?
Ga2 Mn1 Ge2 . . 2_555 180 ?
Ga2 Mn1 Ge2 . . 5_555 90 ?
Ga2 Mn1 Ge2 . . 6_555 90 ?
Ga2 Mn1 Ge2 . . 9_555 90 ?
Ga2 Mn1 Ge2 . . 10_555 90 ?
Ga2 Mn1 Ga2 2_555 . 5_555 90 ?
Ga2 Mn1 Ga2 2_555 . 6_555 90 ?
Ga2 Mn1 Ga2 2_555 . 9_555 90 ?
Ga2 Mn1 Ga2 2_555 . 10_555 90 ?
Ga2 Mn1 Ge2 2_555 . . 180 ?
Ga2 Mn1 Ge2 2_555 . 2_555 0 ?
Ga2 Mn1 Ge2 2_555 . 5_555 90 ?
Ga2 Mn1 Ge2 2_555 . 6_555 90 ?
Ga2 Mn1 Ge2 2_555 . 9_555 90 ?
Ga2 Mn1 Ge2 2_555 . 10_555 90 ?
Ga2 Mn1 Ga2 5_555 . 6_555 180 ?
Ga2 Mn1 Ga2 5_555 . 9_555 90 ?
Ga2 Mn1 Ga2 5_555 . 10_555 90 ?
Ga2 Mn1 Ge2 5_555 . . 90 ?
Ga2 Mn1 Ge2 5_555 . 2_555 90 ?
Ga2 Mn1 Ge2 5_555 . 5_555 0 ?
Ga2 Mn1 Ge2 5_555 . 6_555 180 ?
Ga2 Mn1 Ge2 5_555 . 9_555 90 ?
Ga2 Mn1 Ge2 5_555 . 10_555 90 ?
Ga2 Mn1 Ga2 6_555 . 9_555 90 ?
Ga2 Mn1 Ga2 6_555 . 10_555 90 ?
Ga2 Mn1 Ge2 6_555 . . 90 ?
Ga2 Mn1 Ge2 6_555 . 2_555 90 ?
Ga2 Mn1 Ge2 6_555 . 5_555 180 ?
Ga2 Mn1 Ge2 6_555 . 6_555 0 ?
Ga2 Mn1 Ge2 6_555 . 9_555 90 ?
Ga2 Mn1 Ge2 6_555 . 10_555 90 ?
Ga2 Mn1 Ga2 9_555 . 10_555 180 ?
Ga2 Mn1 Ge2 9_555 . . 90 ?
Ga2 Mn1 Ge2 9_555 . 2_555 90 ?
Ga2 Mn1 Ge2 9_555 . 5_555 90 ?
Ga2 Mn1 Ge2 9_555 . 6_555 90 ?
Ga2 Mn1 Ge2 9_555 . 9_555 0 ?
Ga2 Mn1 Ge2 9_555 . 10_555 180 ?
Ga2 Mn1 Ge2 10_555 . . 90 ?
Ga2 Mn1 Ge2 10_555 . 2_555 90 ?
Ga2 Mn1 Ge2 10_555 . 5_555 90 ?
Ga2 Mn1 Ge2 10_555 . 6_555 90 ?
Ga2 Mn1 Ge2 10_555 . 9_555 180 ?
Ga2 Mn1 Ge2 10_555 . 10_555 0 ?
Ge2 Mn1 Ge2 . . 2_555 180 ?
Ge2 Mn1 Ge2 . . 5_555 90 ?
Ge2 Mn1 Ge2 . . 6_555 90 ?
Ge2 Mn1 Ge2 . . 9_555 90 ?
Ge2 Mn1 Ge2 . . 10_555 90 ?
Ge2 Mn1 Ge2 2_555 . 5_555 90 ?
Ge2 Mn1 Ge2 2_555 . 6_555 90 ?
Ge2 Mn1 Ge2 2_555 . 9_555 90 ?
Ge2 Mn1 Ge2 2_555 . 10_555 90 ?
Ge2 Mn1 Ge2 5_555 . 6_555 180 ?
Ge2 Mn1 Ge2 5_555 . 9_555 90 ?
Ge2 Mn1 Ge2 5_555 . 10_555 90 ?
Ge2 Mn1 Ge2 6_555 . 9_555 90 ?
Ge2 Mn1 Ge2 6_555 . 10_555 90 ?
Ge2 Mn1 Ge2 9_555 . 10_555 180 ?
Sm1 Ga1 Sm1 . . 2_655 180 ?
Sm1 Ga1 Sm1 . . 51_545 90.000(8) ?
Sm1 Ga1 Sm1 . . 52_555 90.000(8) ?
Sm1 Ga1 Ga1 . . 53_545 120.000(4) ?
Sm1 Ga1 Ga1 . . 55_555 60.000(4) ?
Sm1 Ga1 Ga1 . . 57_544 120.000(4) ?
Sm1 Ga1 Ga1 . . 59_555 60.000(4) ?
Sm1 Ga1 Ge1 . . 53_545 120.000(4) ?
Sm1 Ga1 Ge1 . . 55_555 60.000(4) ?
Sm1 Ga1 Ge1 . . 57_544 120.000(4) ?
Sm1 Ga1 Ge1 . . 59_555 60.000(4) ?
Sm1 Ga1 Ga2 . . . 63.08(2) ?
Sm1 Ga1 Ga2 . . 2_655 116.92(2) ?
Sm1 Ga1 Ga2 . . 53_545 116.92(2) ?
Sm1 Ga1 Ga2 . . 54_555 63.08(2) ?
Sm1 Ga1 Ge2 . . . 63.08(2) ?
Sm1 Ga1 Ge2 . . 2_655 116.92(2) ?
Sm1 Ga1 Ge2 . . 53_545 116.92(2) ?
Sm1 Ga1 Ge2 . . 54_555 63.08(2) ?
Sm1 Ga1 Sm1 2_655 . 51_545 90.000(8) ?
Sm1 Ga1 Sm1 2_655 . 52_555 90.000(8) ?
Sm1 Ga1 Ga1 2_655 . 53_545 60.000(4) ?
Sm1 Ga1 Ga1 2_655 . 55_555 120.000(4) ?
Sm1 Ga1 Ga1 2_655 . 57_544 60.000(4) ?
Sm1 Ga1 Ga1 2_655 . 59_555 120.000(4) ?
Sm1 Ga1 Ge1 2_655 . 53_545 60.000(4) ?
Sm1 Ga1 Ge1 2_655 . 55_555 120.000(4) ?
Sm1 Ga1 Ge1 2_655 . 57_544 60.000(4) ?
Sm1 Ga1 Ge1 2_655 . 59_555 120.000(4) ?
Sm1 Ga1 Ga2 2_655 . . 116.92(2) ?
Sm1 Ga1 Ga2 2_655 . 2_655 63.08(2) ?
Sm1 Ga1 Ga2 2_655 . 53_545 63.08(2) ?
Sm1 Ga1 Ga2 2_655 . 54_555 116.92(2) ?
Sm1 Ga1 Ge2 2_655 . . 116.92(2) ?
Sm1 Ga1 Ge2 2_655 . 2_655 63.08(2) ?
Sm1 Ga1 Ge2 2_655 . 53_545 63.08(2) ?
Sm1 Ga1 Ge2 2_655 . 54_555 116.92(2) ?
Sm1 Ga1 Sm1 51_545 . 52_555 180 ?
Sm1 Ga1 Ga1 51_545 . 53_545 120.000(4) ?
Sm1 Ga1 Ga1 51_545 . 55_555 60.000(4) ?
Sm1 Ga1 Ga1 51_545 . 57_544 60.000(4) ?
Sm1 Ga1 Ga1 51_545 . 59_555 120.000(4) ?
Sm1 Ga1 Ge1 51_545 . 53_545 120.000(4) ?
Sm1 Ga1 Ge1 51_545 . 55_555 60.000(4) ?
Sm1 Ga1 Ge1 51_545 . 57_544 60.000(4) ?
Sm1 Ga1 Ge1 51_545 . 59_555 120.000(4) ?
Sm1 Ga1 Ga2 51_545 . . 63.08(2) ?
Sm1 Ga1 Ga2 51_545 . 2_655 116.92(2) ?
Sm1 Ga1 Ga2 51_545 . 53_545 63.08(2) ?
Sm1 Ga1 Ga2 51_545 . 54_555 116.92(2) ?
Sm1 Ga1 Ge2 51_545 . . 63.08(2) ?
Sm1 Ga1 Ge2 51_545 . 2_655 116.92(2) ?
Sm1 Ga1 Ge2 51_545 . 53_545 63.08(2) ?
Sm1 Ga1 Ge2 51_545 . 54_555 116.92(2) ?
Sm1 Ga1 Ga1 52_555 . 53_545 60.000(4) ?
Sm1 Ga1 Ga1 52_555 . 55_555 120.000(4) ?
Sm1 Ga1 Ga1 52_555 . 57_544 120.000(4) ?
Sm1 Ga1 Ga1 52_555 . 59_555 60.000(4) ?
Sm1 Ga1 Ge1 52_555 . 53_545 60.000(4) ?
Sm1 Ga1 Ge1 52_555 . 55_555 120.000(4) ?
Sm1 Ga1 Ge1 52_555 . 57_544 120.000(4) ?
Sm1 Ga1 Ge1 52_555 . 59_555 60.000(4) ?
Sm1 Ga1 Ga2 52_555 . . 116.92(2) ?
Sm1 Ga1 Ga2 52_555 . 2_655 63.08(2) ?
Sm1 Ga1 Ga2 52_555 . 53_545 116.92(2) ?
Sm1 Ga1 Ga2 52_555 . 54_555 63.08(2) ?
Sm1 Ga1 Ge2 52_555 . . 116.92(2) ?
Sm1 Ga1 Ge2 52_555 . 2_655 63.08(2) ?
Sm1 Ga1 Ge2 52_555 . 53_545 116.92(2) ?
Sm1 Ga1 Ge2 52_555 . 54_555 63.08(2) ?
Ga1 Ga1 Ga1 53_545 . 55_555 90.000(8) ?
Ga1 Ga1 Ga1 53_545 . 57_544 120.000(4) ?
Ga1 Ga1 Ga1 53_545 . 59_555 120.000(4) ?
Ga1 Ga1 Ge1 53_545 . 53_545 0 ?
Ga1 Ga1 Ge1 53_545 . 55_555 90.000(8) ?
Ga1 Ga1 Ge1 53_545 . 57_544 120.000(4) ?
Ga1 Ga1 Ge1 53_545 . 59_555 120.000(4) ?
Ga1 Ga1 Ga2 53_545 . . 174.80(3) ?
Ga1 Ga1 Ga2 53_545 . 2_655 95.20(4) ?
Ga1 Ga1 Ga2 53_545 . 53_545 57.097(19) ?
Ga1 Ga1 Ga2 53_545 . 54_555 57.097(19) ?
Ga1 Ga1 Ge2 53_545 . . 174.80(3) ?
Ga1 Ga1 Ge2 53_545 . 2_655 95.20(4) ?
Ga1 Ga1 Ge2 53_545 . 53_545 57.097(19) ?
Ga1 Ga1 Ge2 53_545 . 54_555 57.097(19) ?
Ga1 Ga1 Ga1 55_555 . 57_544 120.000(4) ?
Ga1 Ga1 Ga1 55_555 . 59_555 120.000(4) ?
Ga1 Ga1 Ge1 55_555 . 53_545 90.000(8) ?
Ga1 Ga1 Ge1 55_555 . 55_555 0 ?
Ga1 Ga1 Ge1 55_555 . 57_544 120.000(4) ?
Ga1 Ga1 Ge1 55_555 . 59_555 120.000(4) ?
Ga1 Ga1 Ga2 55_555 . . 95.20(4) ?
Ga1 Ga1 Ga2 55_555 . 2_655 174.80(3) ?
Ga1 Ga1 Ga2 55_555 . 53_545 57.097(19) ?
Ga1 Ga1 Ga2 55_555 . 54_555 57.097(19) ?
Ga1 Ga1 Ge2 55_555 . . 95.20(4) ?
Ga1 Ga1 Ge2 55_555 . 2_655 174.80(3) ?
Ga1 Ga1 Ge2 55_555 . 53_545 57.097(19) ?
Ga1 Ga1 Ge2 55_555 . 54_555 57.097(19) ?
Ga1 Ga1 Ga1 57_544 . 59_555 90.000(8) ?
Ga1 Ga1 Ge1 57_544 . 53_545 120.000(4) ?
Ga1 Ga1 Ge1 57_544 . 55_555 120.000(4) ?
Ga1 Ga1 Ge1 57_544 . 57_544 0 ?
Ga1 Ga1 Ge1 57_544 . 59_555 90.000(8) ?
Ga1 Ga1 Ga2 57_544 . . 57.097(19) ?
Ga1 Ga1 Ga2 57_544 . 2_655 57.097(19) ?
Ga1 Ga1 Ga2 57_544 . 53_545 95.20(4) ?
Ga1 Ga1 Ga2 57_544 . 54_555 174.80(3) ?
Ga1 Ga1 Ge2 57_544 . . 57.097(19) ?
Ga1 Ga1 Ge2 57_544 . 2_655 57.097(19) ?
Ga1 Ga1 Ge2 57_544 . 53_545 95.20(4) ?
Ga1 Ga1 Ge2 57_544 . 54_555 174.80(3) ?
Ga1 Ga1 Ge1 59_555 . 53_545 120.000(4) ?
Ga1 Ga1 Ge1 59_555 . 55_555 120.000(4) ?
Ga1 Ga1 Ge1 59_555 . 57_544 90.000(8) ?
Ga1 Ga1 Ge1 59_555 . 59_555 0 ?
Ga1 Ga1 Ga2 59_555 . . 57.097(19) ?
Ga1 Ga1 Ga2 59_555 . 2_655 57.097(19) ?
Ga1 Ga1 Ga2 59_555 . 53_545 174.80(3) ?
Ga1 Ga1 Ga2 59_555 . 54_555 95.20(4) ?
Ga1 Ga1 Ge2 59_555 . . 57.097(19) ?
Ga1 Ga1 Ge2 59_555 . 2_655 57.097(19) ?
Ga1 Ga1 Ge2 59_555 . 53_545 174.80(3) ?
Ga1 Ga1 Ge2 59_555 . 54_555 95.20(4) ?
Ge1 Ga1 Ge1 53_545 . 55_555 90.000(8) ?
Ge1 Ga1 Ge1 53_545 . 57_544 120.000(4) ?
Ge1 Ga1 Ge1 53_545 . 59_555 120.000(4) ?
Ge1 Ga1 Ga2 53_545 . . 174.80(3) ?
Ge1 Ga1 Ga2 53_545 . 2_655 95.20(4) ?
Ge1 Ga1 Ga2 53_545 . 53_545 57.097(19) ?
Ge1 Ga1 Ga2 53_545 . 54_555 57.097(19) ?
Ge1 Ga1 Ge2 53_545 . . 174.80(3) ?
Ge1 Ga1 Ge2 53_545 . 2_655 95.20(4) ?
Ge1 Ga1 Ge2 53_545 . 53_545 57.097(19) ?
Ge1 Ga1 Ge2 53_545 . 54_555 57.097(19) ?
Ge1 Ga1 Ge1 55_555 . 57_544 120.000(4) ?
Ge1 Ga1 Ge1 55_555 . 59_555 120.000(4) ?
Ge1 Ga1 Ga2 55_555 . . 95.20(4) ?
Ge1 Ga1 Ga2 55_555 . 2_655 174.80(3) ?
Ge1 Ga1 Ga2 55_555 . 53_545 57.097(19) ?
Ge1 Ga1 Ga2 55_555 . 54_555 57.097(19) ?
Ge1 Ga1 Ge2 55_555 . . 95.20(4) ?
Ge1 Ga1 Ge2 55_555 . 2_655 174.80(3) ?
Ge1 Ga1 Ge2 55_555 . 53_545 57.097(19) ?
Ge1 Ga1 Ge2 55_555 . 54_555 57.097(19) ?
Ge1 Ga1 Ge1 57_544 . 59_555 90.000(8) ?
Ge1 Ga1 Ga2 57_544 . . 57.097(19) ?
Ge1 Ga1 Ga2 57_544 . 2_655 57.097(19) ?
Ge1 Ga1 Ga2 57_544 . 53_545 95.20(4) ?
Ge1 Ga1 Ga2 57_544 . 54_555 174.80(3) ?
Ge1 Ga1 Ge2 57_544 . . 57.097(19) ?
Ge1 Ga1 Ge2 57_544 . 2_655 57.097(19) ?
Ge1 Ga1 Ge2 57_544 . 53_545 95.20(4) ?
Ge1 Ga1 Ge2 57_544 . 54_555 174.80(3) ?
Ge1 Ga1 Ga2 59_555 . . 57.097(19) ?
Ge1 Ga1 Ga2 59_555 . 2_655 57.097(19) ?
Ge1 Ga1 Ga2 59_555 . 53_545 174.80(3) ?
Ge1 Ga1 Ga2 59_555 . 54_555 95.20(4) ?
Ge1 Ga1 Ge2 59_555 . . 57.097(19) ?
Ge1 Ga1 Ge2 59_555 . 2_655 57.097(19) ?
Ge1 Ga1 Ge2 59_555 . 53_545 174.80(3) ?
Ge1 Ga1 Ge2 59_555 . 54_555 95.20(4) ?
Ga2 Ga1 Ga2 . . 2_655 79.61(5) ?
Ga2 Ga1 Ga2 . . 53_545 126.17(3) ?
Ga2 Ga1 Ga2 . . 54_555 126.17(3) ?
Ga2 Ga1 Ge2 . . . 0 ?
Ga2 Ga1 Ge2 . . 2_655 79.61(5) ?
Ga2 Ga1 Ge2 . . 53_545 126.17(3) ?
Ga2 Ga1 Ge2 . . 54_555 126.17(3) ?
Ga2 Ga1 Ga2 2_655 . 53_545 126.17(3) ?
Ga2 Ga1 Ga2 2_655 . 54_555 126.17(3) ?
Ga2 Ga1 Ge2 2_655 . . 79.61(5) ?
Ga2 Ga1 Ge2 2_655 . 2_655 0 ?
Ga2 Ga1 Ge2 2_655 . 53_545 126.17(3) ?
Ga2 Ga1 Ge2 2_655 . 54_555 126.17(3) ?
Ga2 Ga1 Ga2 53_545 . 54_555 79.61(5) ?
Ga2 Ga1 Ge2 53_545 . . 126.17(3) ?
Ga2 Ga1 Ge2 53_545 . 2_655 126.17(3) ?
Ga2 Ga1 Ge2 53_545 . 53_545 0 ?
Ga2 Ga1 Ge2 53_545 . 54_555 79.61(5) ?
Ga2 Ga1 Ge2 54_555 . . 126.17(3) ?
Ga2 Ga1 Ge2 54_555 . 2_655 126.17(3) ?
Ga2 Ga1 Ge2 54_555 . 53_545 79.61(5) ?
Ga2 Ga1 Ge2 54_555 . 54_555 0 ?
Ge2 Ga1 Ge2 . . 2_655 79.61(5) ?
Ge2 Ga1 Ge2 . . 53_545 126.17(3) ?
Ge2 Ga1 Ge2 . . 54_555 126.17(3) ?
Ge2 Ga1 Ge2 2_655 . 53_545 126.17(3) ?
Ge2 Ga1 Ge2 2_655 . 54_555 126.17(3) ?
Ge2 Ga1 Ge2 53_545 . 54_555 79.61(5) ?
Sm1 Ge1 Sm1 . . 2_655 180 ?
Sm1 Ge1 Sm1 . . 51_545 90.000(8) ?
Sm1 Ge1 Sm1 . . 52_555 90.000(8) ?
Sm1 Ge1 Ga1 . . 53_545 120.000(4) ?
Sm1 Ge1 Ga1 . . 55_555 60.000(4) ?
Sm1 Ge1 Ga1 . . 57_544 120.000(4) ?
Sm1 Ge1 Ga1 . . 59_555 60.000(4) ?
Sm1 Ge1 Ge1 . . 53_545 120.000(4) ?
Sm1 Ge1 Ge1 . . 55_555 60.000(4) ?
Sm1 Ge1 Ge1 . . 57_544 120.000(4) ?
Sm1 Ge1 Ge1 . . 59_555 60.000(4) ?
Sm1 Ge1 Ga2 . . . 63.08(2) ?
Sm1 Ge1 Ga2 . . 2_655 116.92(2) ?
Sm1 Ge1 Ga2 . . 53_545 116.92(2) ?
Sm1 Ge1 Ga2 . . 54_555 63.08(2) ?
Sm1 Ge1 Ge2 . . . 63.08(2) ?
Sm1 Ge1 Ge2 . . 2_655 116.92(2) ?
Sm1 Ge1 Ge2 . . 53_545 116.92(2) ?
Sm1 Ge1 Ge2 . . 54_555 63.08(2) ?
Sm1 Ge1 Sm1 2_655 . 51_545 90.000(8) ?
Sm1 Ge1 Sm1 2_655 . 52_555 90.000(8) ?
Sm1 Ge1 Ga1 2_655 . 53_545 60.000(4) ?
Sm1 Ge1 Ga1 2_655 . 55_555 120.000(4) ?
Sm1 Ge1 Ga1 2_655 . 57_544 60.000(4) ?
Sm1 Ge1 Ga1 2_655 . 59_555 120.000(4) ?
Sm1 Ge1 Ge1 2_655 . 53_545 60.000(4) ?
Sm1 Ge1 Ge1 2_655 . 55_555 120.000(4) ?
Sm1 Ge1 Ge1 2_655 . 57_544 60.000(4) ?
Sm1 Ge1 Ge1 2_655 . 59_555 120.000(4) ?
Sm1 Ge1 Ga2 2_655 . . 116.92(2) ?
Sm1 Ge1 Ga2 2_655 . 2_655 63.08(2) ?
Sm1 Ge1 Ga2 2_655 . 53_545 63.08(2) ?
Sm1 Ge1 Ga2 2_655 . 54_555 116.92(2) ?
Sm1 Ge1 Ge2 2_655 . . 116.92(2) ?
Sm1 Ge1 Ge2 2_655 . 2_655 63.08(2) ?
Sm1 Ge1 Ge2 2_655 . 53_545 63.08(2) ?
Sm1 Ge1 Ge2 2_655 . 54_555 116.92(2) ?
Sm1 Ge1 Sm1 51_545 . 52_555 180 ?
Sm1 Ge1 Ga1 51_545 . 53_545 120.000(4) ?
Sm1 Ge1 Ga1 51_545 . 55_555 60.000(4) ?
Sm1 Ge1 Ga1 51_545 . 57_544 60.000(4) ?
Sm1 Ge1 Ga1 51_545 . 59_555 120.000(4) ?
Sm1 Ge1 Ge1 51_545 . 53_545 120.000(4) ?
Sm1 Ge1 Ge1 51_545 . 55_555 60.000(4) ?
Sm1 Ge1 Ge1 51_545 . 57_544 60.000(4) ?
Sm1 Ge1 Ge1 51_545 . 59_555 120.000(4) ?
Sm1 Ge1 Ga2 51_545 . . 63.08(2) ?
Sm1 Ge1 Ga2 51_545 . 2_655 116.92(2) ?
Sm1 Ge1 Ga2 51_545 . 53_545 63.08(2) ?
Sm1 Ge1 Ga2 51_545 . 54_555 116.92(2) ?
Sm1 Ge1 Ge2 51_545 . . 63.08(2) ?
Sm1 Ge1 Ge2 51_545 . 2_655 116.92(2) ?
Sm1 Ge1 Ge2 51_545 . 53_545 63.08(2) ?
Sm1 Ge1 Ge2 51_545 . 54_555 116.92(2) ?
Sm1 Ge1 Ga1 52_555 . 53_545 60.000(4) ?
Sm1 Ge1 Ga1 52_555 . 55_555 120.000(4) ?
Sm1 Ge1 Ga1 52_555 . 57_544 120.000(4) ?
Sm1 Ge1 Ga1 52_555 . 59_555 60.000(4) ?
Sm1 Ge1 Ge1 52_555 . 53_545 60.000(4) ?
Sm1 Ge1 Ge1 52_555 . 55_555 120.000(4) ?
Sm1 Ge1 Ge1 52_555 . 57_544 120.000(4) ?
Sm1 Ge1 Ge1 52_555 . 59_555 60.000(4) ?
Sm1 Ge1 Ga2 52_555 . . 116.92(2) ?
Sm1 Ge1 Ga2 52_555 . 2_655 63.08(2) ?
Sm1 Ge1 Ga2 52_555 . 53_545 116.92(2) ?
Sm1 Ge1 Ga2 52_555 . 54_555 63.08(2) ?
Sm1 Ge1 Ge2 52_555 . . 116.92(2) ?
Sm1 Ge1 Ge2 52_555 . 2_655 63.08(2) ?
Sm1 Ge1 Ge2 52_555 . 53_545 116.92(2) ?
Sm1 Ge1 Ge2 52_555 . 54_555 63.08(2) ?
Ga1 Ge1 Ga1 53_545 . 55_555 90.000(8) ?
Ga1 Ge1 Ga1 53_545 . 57_544 120.000(4) ?
Ga1 Ge1 Ga1 53_545 . 59_555 120.000(4) ?
Ga1 Ge1 Ge1 53_545 . 53_545 0 ?
Ga1 Ge1 Ge1 53_545 . 55_555 90.000(8) ?
Ga1 Ge1 Ge1 53_545 . 57_544 120.000(4) ?
Ga1 Ge1 Ge1 53_545 . 59_555 120.000(4) ?
Ga1 Ge1 Ga2 53_545 . . 174.80(3) ?
Ga1 Ge1 Ga2 53_545 . 2_655 95.20(4) ?
Ga1 Ge1 Ga2 53_545 . 53_545 57.097(19) ?
Ga1 Ge1 Ga2 53_545 . 54_555 57.097(19) ?
Ga1 Ge1 Ge2 53_545 . . 174.80(3) ?
Ga1 Ge1 Ge2 53_545 . 2_655 95.20(4) ?
Ga1 Ge1 Ge2 53_545 . 53_545 57.097(19) ?
Ga1 Ge1 Ge2 53_545 . 54_555 57.097(19) ?
Ga1 Ge1 Ga1 55_555 . 57_544 120.000(4) ?
Ga1 Ge1 Ga1 55_555 . 59_555 120.000(4) ?
Ga1 Ge1 Ge1 55_555 . 53_545 90.000(8) ?
Ga1 Ge1 Ge1 55_555 . 55_555 0 ?
Ga1 Ge1 Ge1 55_555 . 57_544 120.000(4) ?
Ga1 Ge1 Ge1 55_555 . 59_555 120.000(4) ?
Ga1 Ge1 Ga2 55_555 . . 95.20(4) ?
Ga1 Ge1 Ga2 55_555 . 2_655 174.80(3) ?
Ga1 Ge1 Ga2 55_555 . 53_545 57.097(19) ?
Ga1 Ge1 Ga2 55_555 . 54_555 57.097(19) ?
Ga1 Ge1 Ge2 55_555 . . 95.20(4) ?
Ga1 Ge1 Ge2 55_555 . 2_655 174.80(3) ?
Ga1 Ge1 Ge2 55_555 . 53_545 57.097(19) ?
Ga1 Ge1 Ge2 55_555 . 54_555 57.097(19) ?
Ga1 Ge1 Ga1 57_544 . 59_555 90.000(8) ?
Ga1 Ge1 Ge1 57_544 . 53_545 120.000(4) ?
Ga1 Ge1 Ge1 57_544 . 55_555 120.000(4) ?
Ga1 Ge1 Ge1 57_544 . 57_544 0 ?
Ga1 Ge1 Ge1 57_544 . 59_555 90.000(8) ?
Ga1 Ge1 Ga2 57_544 . . 57.097(19) ?
Ga1 Ge1 Ga2 57_544 . 2_655 57.097(19) ?
Ga1 Ge1 Ga2 57_544 . 53_545 95.20(4) ?
Ga1 Ge1 Ga2 57_544 . 54_555 174.80(3) ?
Ga1 Ge1 Ge2 57_544 . . 57.097(19) ?
Ga1 Ge1 Ge2 57_544 . 2_655 57.097(19) ?
Ga1 Ge1 Ge2 57_544 . 53_545 95.20(4) ?
Ga1 Ge1 Ge2 57_544 . 54_555 174.80(3) ?
Ga1 Ge1 Ge1 59_555 . 53_545 120.000(4) ?
Ga1 Ge1 Ge1 59_555 . 55_555 120.000(4) ?
Ga1 Ge1 Ge1 59_555 . 57_544 90.000(8) ?
Ga1 Ge1 Ge1 59_555 . 59_555 0 ?
Ga1 Ge1 Ga2 59_555 . . 57.097(19) ?
Ga1 Ge1 Ga2 59_555 . 2_655 57.097(19) ?
Ga1 Ge1 Ga2 59_555 . 53_545 174.80(3) ?
Ga1 Ge1 Ga2 59_555 . 54_555 95.20(4) ?
Ga1 Ge1 Ge2 59_555 . . 57.097(19) ?
Ga1 Ge1 Ge2 59_555 . 2_655 57.097(19) ?
Ga1 Ge1 Ge2 59_555 . 53_545 174.80(3) ?
Ga1 Ge1 Ge2 59_555 . 54_555 95.20(4) ?
Ge1 Ge1 Ge1 53_545 . 55_555 90.000(8) ?
Ge1 Ge1 Ge1 53_545 . 57_544 120.000(4) ?
Ge1 Ge1 Ge1 53_545 . 59_555 120.000(4) ?
Ge1 Ge1 Ga2 53_545 . . 174.80(3) ?
Ge1 Ge1 Ga2 53_545 . 2_655 95.20(4) ?
Ge1 Ge1 Ga2 53_545 . 53_545 57.097(19) ?
Ge1 Ge1 Ga2 53_545 . 54_555 57.097(19) ?
Ge1 Ge1 Ge2 53_545 . . 174.80(3) ?
Ge1 Ge1 Ge2 53_545 . 2_655 95.20(4) ?
Ge1 Ge1 Ge2 53_545 . 53_545 57.097(19) ?
Ge1 Ge1 Ge2 53_545 . 54_555 57.097(19) ?
Ge1 Ge1 Ge1 55_555 . 57_544 120.000(4) ?
Ge1 Ge1 Ge1 55_555 . 59_555 120.000(4) ?
Ge1 Ge1 Ga2 55_555 . . 95.20(4) ?
Ge1 Ge1 Ga2 55_555 . 2_655 174.80(3) ?
Ge1 Ge1 Ga2 55_555 . 53_545 57.097(19) ?
Ge1 Ge1 Ga2 55_555 . 54_555 57.097(19) ?
Ge1 Ge1 Ge2 55_555 . . 95.20(4) ?
Ge1 Ge1 Ge2 55_555 . 2_655 174.80(3) ?
Ge1 Ge1 Ge2 55_555 . 53_545 57.097(19) ?
Ge1 Ge1 Ge2 55_555 . 54_555 57.097(19) ?
Ge1 Ge1 Ge1 57_544 . 59_555 90.000(8) ?
Ge1 Ge1 Ga2 57_544 . . 57.097(19) ?
Ge1 Ge1 Ga2 57_544 . 2_655 57.097(19) ?
Ge1 Ge1 Ga2 57_544 . 53_545 95.20(4) ?
Ge1 Ge1 Ga2 57_544 . 54_555 174.80(3) ?
Ge1 Ge1 Ge2 57_544 . . 57.097(19) ?
Ge1 Ge1 Ge2 57_544 . 2_655 57.097(19) ?
Ge1 Ge1 Ge2 57_544 . 53_545 95.20(4) ?
Ge1 Ge1 Ge2 57_544 . 54_555 174.80(3) ?
Ge1 Ge1 Ga2 59_555 . . 57.097(19) ?
Ge1 Ge1 Ga2 59_555 . 2_655 57.097(19) ?
Ge1 Ge1 Ga2 59_555 . 53_545 174.80(3) ?
Ge1 Ge1 Ga2 59_555 . 54_555 95.20(4) ?
Ge1 Ge1 Ge2 59_555 . . 57.097(19) ?
Ge1 Ge1 Ge2 59_555 . 2_655 57.097(19) ?
Ge1 Ge1 Ge2 59_555 . 53_545 174.80(3) ?
Ge1 Ge1 Ge2 59_555 . 54_555 95.20(4) ?
Ga2 Ge1 Ga2 . . 2_655 79.61(5) ?
Ga2 Ge1 Ga2 . . 53_545 126.17(3) ?
Ga2 Ge1 Ga2 . . 54_555 126.17(3) ?
Ga2 Ge1 Ge2 . . . 0 ?
Ga2 Ge1 Ge2 . . 2_655 79.61(5) ?
Ga2 Ge1 Ge2 . . 53_545 126.17(3) ?
Ga2 Ge1 Ge2 . . 54_555 126.17(3) ?
Ga2 Ge1 Ga2 2_655 . 53_545 126.17(3) ?
Ga2 Ge1 Ga2 2_655 . 54_555 126.17(3) ?
Ga2 Ge1 Ge2 2_655 . . 79.61(5) ?
Ga2 Ge1 Ge2 2_655 . 2_655 0 ?
Ga2 Ge1 Ge2 2_655 . 53_545 126.17(3) ?
Ga2 Ge1 Ge2 2_655 . 54_555 126.17(3) ?
Ga2 Ge1 Ga2 53_545 . 54_555 79.61(5) ?
Ga2 Ge1 Ge2 53_545 . . 126.17(3) ?
Ga2 Ge1 Ge2 53_545 . 2_655 126.17(3) ?
Ga2 Ge1 Ge2 53_545 . 53_545 0 ?
Ga2 Ge1 Ge2 53_545 . 54_555 79.61(5) ?
Ga2 Ge1 Ge2 54_555 . . 126.17(3) ?
Ga2 Ge1 Ge2 54_555 . 2_655 126.17(3) ?
Ga2 Ge1 Ge2 54_555 . 53_545 79.61(5) ?
Ga2 Ge1 Ge2 54_555 . 54_555 0 ?
Ge2 Ge1 Ge2 . . 2_655 79.61(5) ?
Ge2 Ge1 Ge2 . . 53_545 126.17(3) ?
Ge2 Ge1 Ge2 . . 54_555 126.17(3) ?
Ge2 Ge1 Ge2 2_655 . 53_545 126.17(3) ?
Ge2 Ge1 Ge2 2_655 . 54_555 126.17(3) ?
Ge2 Ge1 Ge2 53_545 . 54_555 79.61(5) ?
Sm1 Ga2 Sm1 . . 50_554 89.215(12) ?
Sm1 Ga2 Sm1 . . 51_545 89.215(12) ?
Sm1 Ga2 Sm1 . . 4_555 166.55(8) ?
Sm1 Ga2 Mn1 . . . 83.28(4) ?
Sm1 Ga2 Ga1 . . . 62.319(12) ?
Sm1 Ga2 Ga1 . . 3_655 127.91(5) ?
Sm1 Ga2 Ga1 . . 57_544 127.91(5) ?
Sm1 Ga2 Ga1 . . 59_555 62.319(12) ?
Sm1 Ga2 Ge1 . . . 62.319(12) ?
Sm1 Ga2 Ge1 . . 3_655 127.91(5) ?
Sm1 Ga2 Ge1 . . 57_544 127.91(5) ?
Sm1 Ga2 Ge1 . . 59_555 62.319(12) ?
Sm1 Ga2 Ga2 . . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 . . 5_555 54.60(2) ?
Sm1 Ga2 Ga2 . . 6_555 114.44(5) ?
Sm1 Ga2 Ga2 . . 9_555 54.60(2) ?
Sm1 Ga2 Ga2 . . 10_555 114.44(5) ?
Sm1 Ga2 Ge2 . . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 . . 5_555 54.60(2) ?
Sm1 Ga2 Ge2 . . 6_555 114.44(5) ?
Sm1 Ga2 Ge2 . . 9_555 54.60(2) ?
Sm1 Ga2 Ge2 . . 10_555 114.44(5) ?
Sm1 Ga2 Sm1 50_554 . 51_545 166.55(8) ?
Sm1 Ga2 Sm1 50_554 . 4_555 89.215(12) ?
Sm1 Ga2 Mn1 50_554 . . 83.28(4) ?
Sm1 Ga2 Ga1 50_554 . . 127.91(5) ?
Sm1 Ga2 Ga1 50_554 . 3_655 62.319(12) ?
Sm1 Ga2 Ga1 50_554 . 57_544 127.91(5) ?
Sm1 Ga2 Ga1 50_554 . 59_555 62.319(12) ?
Sm1 Ga2 Ge1 50_554 . . 127.91(5) ?
Sm1 Ga2 Ge1 50_554 . 3_655 62.319(12) ?
Sm1 Ga2 Ge1 50_554 . 57_544 127.91(5) ?
Sm1 Ga2 Ge1 50_554 . 59_555 62.319(12) ?
Sm1 Ga2 Ga2 50_554 . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 50_554 . 5_555 54.60(2) ?
Sm1 Ga2 Ga2 50_554 . 6_555 114.44(5) ?
Sm1 Ga2 Ga2 50_554 . 9_555 114.44(5) ?
Sm1 Ga2 Ga2 50_554 . 10_555 54.60(2) ?
Sm1 Ga2 Ge2 50_554 . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 50_554 . 5_555 54.60(2) ?
Sm1 Ga2 Ge2 50_554 . 6_555 114.44(5) ?
Sm1 Ga2 Ge2 50_554 . 9_555 114.44(5) ?
Sm1 Ga2 Ge2 50_554 . 10_555 54.60(2) ?
Sm1 Ga2 Sm1 51_545 . 4_555 89.215(12) ?
Sm1 Ga2 Mn1 51_545 . . 83.28(4) ?
Sm1 Ga2 Ga1 51_545 . . 62.319(12) ?
Sm1 Ga2 Ga1 51_545 . 3_655 127.91(5) ?
Sm1 Ga2 Ga1 51_545 . 57_544 62.319(12) ?
Sm1 Ga2 Ga1 51_545 . 59_555 127.91(5) ?
Sm1 Ga2 Ge1 51_545 . . 62.319(12) ?
Sm1 Ga2 Ge1 51_545 . 3_655 127.91(5) ?
Sm1 Ga2 Ge1 51_545 . 57_544 62.319(12) ?
Sm1 Ga2 Ge1 51_545 . 59_555 127.91(5) ?
Sm1 Ga2 Ga2 51_545 . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 51_545 . 5_555 114.44(5) ?
Sm1 Ga2 Ga2 51_545 . 6_555 54.60(2) ?
Sm1 Ga2 Ga2 51_545 . 9_555 54.60(2) ?
Sm1 Ga2 Ga2 51_545 . 10_555 114.44(5) ?
Sm1 Ga2 Ge2 51_545 . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 51_545 . 5_555 114.44(5) ?
Sm1 Ga2 Ge2 51_545 . 6_555 54.60(2) ?
Sm1 Ga2 Ge2 51_545 . 9_555 54.60(2) ?
Sm1 Ga2 Ge2 51_545 . 10_555 114.44(5) ?
Sm1 Ga2 Mn1 4_555 . . 83.28(4) ?
Sm1 Ga2 Ga1 4_555 . . 127.91(5) ?
Sm1 Ga2 Ga1 4_555 . 3_655 62.319(12) ?
Sm1 Ga2 Ga1 4_555 . 57_544 62.319(12) ?
Sm1 Ga2 Ga1 4_555 . 59_555 127.91(5) ?
Sm1 Ga2 Ge1 4_555 . . 127.91(5) ?
Sm1 Ga2 Ge1 4_555 . 3_655 62.319(12) ?
Sm1 Ga2 Ge1 4_555 . 57_544 62.319(12) ?
Sm1 Ga2 Ge1 4_555 . 59_555 127.91(5) ?
Sm1 Ga2 Ga2 4_555 . 2_655 96.72(4) ?
Sm1 Ga2 Ga2 4_555 . 5_555 114.44(5) ?
Sm1 Ga2 Ga2 4_555 . 6_555 54.60(2) ?
Sm1 Ga2 Ga2 4_555 . 9_555 114.44(5) ?
Sm1 Ga2 Ga2 4_555 . 10_555 54.60(2) ?
Sm1 Ga2 Ge2 4_555 . 2_655 96.72(4) ?
Sm1 Ga2 Ge2 4_555 . 5_555 114.44(5) ?
Sm1 Ga2 Ge2 4_555 . 6_555 54.60(2) ?
Sm1 Ga2 Ge2 4_555 . 9_555 114.44(5) ?
Sm1 Ga2 Ge2 4_555 . 10_555 54.60(2) ?
Mn1 Ga2 Ga1 . . . 129.80(4) ?
Mn1 Ga2 Ga1 . . 3_655 129.80(4) ?
Mn1 Ga2 Ga1 . . 57_544 129.80(4) ?
Mn1 Ga2 Ga1 . . 59_555 129.80(4) ?
Mn1 Ga2 Ge1 . . . 129.80(4) ?
Mn1 Ga2 Ge1 . . 3_655 129.80(4) ?
Mn1 Ga2 Ge1 . . 57_544 129.80(4) ?
Mn1 Ga2 Ge1 . . 59_555 129.80(4) ?
Mn1 Ga2 Ga2 . . 2_655 180 ?
Mn1 Ga2 Ga2 . . 5_555 45.00(4) ?
Mn1 Ga2 Ga2 . . 6_555 45.00(4) ?
Mn1 Ga2 Ga2 . . 9_555 45.00(4) ?
Mn1 Ga2 Ga2 . . 10_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 2_655 180 ?
Mn1 Ga2 Ge2 . . 5_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 6_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 9_555 45.00(4) ?
Mn1 Ga2 Ge2 . . 10_555 45.00(4) ?
Ga1 Ga2 Ga1 . . 3_655 100.39(7) ?
Ga1 Ga2 Ga1 . . 57_544 65.81(4) ?
Ga1 Ga2 Ga1 . . 59_555 65.81(4) ?
Ga1 Ga2 Ge1 . . . 0 ?
Ga1 Ga2 Ge1 . . 3_655 100.39(7) ?
Ga1 Ga2 Ge1 . . 57_544 65.81(4) ?
Ga1 Ga2 Ge1 . . 59_555 65.81(4) ?
Ga1 Ga2 Ga2 . . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 . . 5_555 116.915(16) ?
Ga1 Ga2 Ga2 . . 6_555 116.915(16) ?
Ga1 Ga2 Ga2 . . 9_555 84.80(3) ?
Ga1 Ga2 Ga2 . . 10_555 174.80(7) ?
Ga1 Ga2 Ge2 . . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 . . 5_555 116.915(16) ?
Ga1 Ga2 Ge2 . . 6_555 116.915(16) ?
Ga1 Ga2 Ge2 . . 9_555 84.80(3) ?
Ga1 Ga2 Ge2 . . 10_555 174.80(7) ?
Ga1 Ga2 Ga1 3_655 . 57_544 65.81(4) ?
Ga1 Ga2 Ga1 3_655 . 59_555 65.81(4) ?
Ga1 Ga2 Ge1 3_655 . . 100.39(7) ?
Ga1 Ga2 Ge1 3_655 . 3_655 0 ?
Ga1 Ga2 Ge1 3_655 . 57_544 65.81(4) ?
Ga1 Ga2 Ge1 3_655 . 59_555 65.81(4) ?
Ga1 Ga2 Ga2 3_655 . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 3_655 . 5_555 116.915(16) ?
Ga1 Ga2 Ga2 3_655 . 6_555 116.915(16) ?
Ga1 Ga2 Ga2 3_655 . 9_555 174.80(7) ?
Ga1 Ga2 Ga2 3_655 . 10_555 84.80(3) ?
Ga1 Ga2 Ge2 3_655 . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 3_655 . 5_555 116.915(16) ?
Ga1 Ga2 Ge2 3_655 . 6_555 116.915(16) ?
Ga1 Ga2 Ge2 3_655 . 9_555 174.80(7) ?
Ga1 Ga2 Ge2 3_655 . 10_555 84.80(3) ?
Ga1 Ga2 Ga1 57_544 . 59_555 100.39(7) ?
Ga1 Ga2 Ge1 57_544 . . 65.81(4) ?
Ga1 Ga2 Ge1 57_544 . 3_655 65.81(4) ?
Ga1 Ga2 Ge1 57_544 . 57_544 0 ?
Ga1 Ga2 Ge1 57_544 . 59_555 100.39(7) ?
Ga1 Ga2 Ga2 57_544 . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 57_544 . 5_555 174.80(7) ?
Ga1 Ga2 Ga2 57_544 . 6_555 84.80(3) ?
Ga1 Ga2 Ga2 57_544 . 9_555 116.915(16) ?
Ga1 Ga2 Ga2 57_544 . 10_555 116.915(16) ?
Ga1 Ga2 Ge2 57_544 . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 57_544 . 5_555 174.80(7) ?
Ga1 Ga2 Ge2 57_544 . 6_555 84.80(3) ?
Ga1 Ga2 Ge2 57_544 . 9_555 116.915(16) ?
Ga1 Ga2 Ge2 57_544 . 10_555 116.915(16) ?
Ga1 Ga2 Ge1 59_555 . . 65.81(4) ?
Ga1 Ga2 Ge1 59_555 . 3_655 65.81(4) ?
Ga1 Ga2 Ge1 59_555 . 57_544 100.39(7) ?
Ga1 Ga2 Ge1 59_555 . 59_555 0 ?
Ga1 Ga2 Ga2 59_555 . 2_655 50.20(4) ?
Ga1 Ga2 Ga2 59_555 . 5_555 84.80(3) ?
Ga1 Ga2 Ga2 59_555 . 6_555 174.80(7) ?
Ga1 Ga2 Ga2 59_555 . 9_555 116.915(16) ?
Ga1 Ga2 Ga2 59_555 . 10_555 116.915(16) ?
Ga1 Ga2 Ge2 59_555 . 2_655 50.20(4) ?
Ga1 Ga2 Ge2 59_555 . 5_555 84.80(3) ?
Ga1 Ga2 Ge2 59_555 . 6_555 174.80(7) ?
Ga1 Ga2 Ge2 59_555 . 9_555 116.915(16) ?
Ga1 Ga2 Ge2 59_555 . 10_555 116.915(16) ?
Ge1 Ga2 Ge1 . . 3_655 100.39(7) ?
Ge1 Ga2 Ge1 . . 57_544 65.81(4) ?
Ge1 Ga2 Ge1 . . 59_555 65.81(4) ?
Ge1 Ga2 Ga2 . . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 . . 5_555 116.915(16) ?
Ge1 Ga2 Ga2 . . 6_555 116.915(16) ?
Ge1 Ga2 Ga2 . . 9_555 84.80(3) ?
Ge1 Ga2 Ga2 . . 10_555 174.80(7) ?
Ge1 Ga2 Ge2 . . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 . . 5_555 116.915(16) ?
Ge1 Ga2 Ge2 . . 6_555 116.915(16) ?
Ge1 Ga2 Ge2 . . 9_555 84.80(3) ?
Ge1 Ga2 Ge2 . . 10_555 174.80(7) ?
Ge1 Ga2 Ge1 3_655 . 57_544 65.81(4) ?
Ge1 Ga2 Ge1 3_655 . 59_555 65.81(4) ?
Ge1 Ga2 Ga2 3_655 . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 3_655 . 5_555 116.915(16) ?
Ge1 Ga2 Ga2 3_655 . 6_555 116.915(16) ?
Ge1 Ga2 Ga2 3_655 . 9_555 174.80(7) ?
Ge1 Ga2 Ga2 3_655 . 10_555 84.80(3) ?
Ge1 Ga2 Ge2 3_655 . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 3_655 . 5_555 116.915(16) ?
Ge1 Ga2 Ge2 3_655 . 6_555 116.915(16) ?
Ge1 Ga2 Ge2 3_655 . 9_555 174.80(7) ?
Ge1 Ga2 Ge2 3_655 . 10_555 84.80(3) ?
Ge1 Ga2 Ge1 57_544 . 59_555 100.39(7) ?
Ge1 Ga2 Ga2 57_544 . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 57_544 . 5_555 174.80(7) ?
Ge1 Ga2 Ga2 57_544 . 6_555 84.80(3) ?
Ge1 Ga2 Ga2 57_544 . 9_555 116.915(16) ?
Ge1 Ga2 Ga2 57_544 . 10_555 116.915(16) ?
Ge1 Ga2 Ge2 57_544 . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 57_544 . 5_555 174.80(7) ?
Ge1 Ga2 Ge2 57_544 . 6_555 84.80(3) ?
Ge1 Ga2 Ge2 57_544 . 9_555 116.915(16) ?
Ge1 Ga2 Ge2 57_544 . 10_555 116.915(16) ?
Ge1 Ga2 Ga2 59_555 . 2_655 50.20(4) ?
Ge1 Ga2 Ga2 59_555 . 5_555 84.80(3) ?
Ge1 Ga2 Ga2 59_555 . 6_555 174.80(7) ?
Ge1 Ga2 Ga2 59_555 . 9_555 116.915(16) ?
Ge1 Ga2 Ga2 59_555 . 10_555 116.915(16) ?
Ge1 Ga2 Ge2 59_555 . 2_655 50.20(4) ?
Ge1 Ga2 Ge2 59_555 . 5_555 84.80(3) ?
Ge1 Ga2 Ge2 59_555 . 6_555 174.80(7) ?
Ge1 Ga2 Ge2 59_555 . 9_555 116.915(16) ?
Ge1 Ga2 Ge2 59_555 . 10_555 116.915(16) ?
Ga2 Ga2 Ga2 2_655 . 5_555 135.00(4) ?
Ga2 Ga2 Ga2 2_655 . 6_555 135.00(4) ?
Ga2 Ga2 Ga2 2_655 . 9_555 135.00(4) ?
Ga2 Ga2 Ga2 2_655 . 10_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 2_655 0 ?
Ga2 Ga2 Ge2 2_655 . 5_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 6_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 9_555 135.00(4) ?
Ga2 Ga2 Ge2 2_655 . 10_555 135.00(4) ?
Ga2 Ga2 Ga2 5_555 . 6_555 90.00(6) ?
Ga2 Ga2 Ga2 5_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ga2 5_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ge2 5_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 5_555 . 5_555 0 ?
Ga2 Ga2 Ge2 5_555 . 6_555 90.00(6) ?
Ga2 Ga2 Ge2 5_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ge2 5_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ga2 6_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ga2 6_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ge2 6_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 6_555 . 5_555 90.00(6) ?
Ga2 Ga2 Ge2 6_555 . 6_555 0 ?
Ga2 Ga2 Ge2 6_555 . 9_555 60.00(4) ?
Ga2 Ga2 Ge2 6_555 . 10_555 60.00(4) ?
Ga2 Ga2 Ga2 9_555 . 10_555 90.00(6) ?
Ga2 Ga2 Ge2 9_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 9_555 . 5_555 60.00(4) ?
Ga2 Ga2 Ge2 9_555 . 6_555 60.00(4) ?
Ga2 Ga2 Ge2 9_555 . 9_555 0 ?
Ga2 Ga2 Ge2 9_555 . 10_555 90.00(6) ?
Ga2 Ga2 Ge2 10_555 . 2_655 135.00(4) ?
Ga2 Ga2 Ge2 10_555 . 5_555 60.00(4) ?
Ga2 Ga2 Ge2 10_555 . 6_555 60.00(4) ?
Ga2 Ga2 Ge2 10_555 . 9_555 90.00(6) ?
Ga2 Ga2 Ge2 10_555 . 10_555 0 ?
Ge2 Ga2 Ge2 2_655 . 5_555 135.00(4) ?
Ge2 Ga2 Ge2 2_655 . 6_555 135.00(4) ?
Ge2 Ga2 Ge2 2_655 . 9_555 135.00(4) ?
Ge2 Ga2 Ge2 2_655 . 10_555 135.00(4) ?
Ge2 Ga2 Ge2 5_555 . 6_555 90.00(6) ?
Ge2 Ga2 Ge2 5_555 . 9_555 60.00(4) ?
Ge2 Ga2 Ge2 5_555 . 10_555 60.00(4) ?
Ge2 Ga2 Ge2 6_555 . 9_555 60.00(4) ?
Ge2 Ga2 Ge2 6_555 . 10_555 60.00(4) ?
Ge2 Ga2 Ge2 9_555 . 10_555 90.00(6) ?
Sm1 Ge2 Sm1 . . 50_554 89.215(12) ?
Sm1 Ge2 Sm1 . . 51_545 89.215(12) ?
Sm1 Ge2 Sm1 . . 4_555 166.55(8) ?
Sm1 Ge2 Mn1 . . . 83.28(4) ?
Sm1 Ge2 Ga1 . . . 62.319(12) ?
Sm1 Ge2 Ga1 . . 3_655 127.91(5) ?
Sm1 Ge2 Ga1 . . 57_544 127.91(5) ?
Sm1 Ge2 Ga1 . . 59_555 62.319(12) ?
Sm1 Ge2 Ge1 . . . 62.319(12) ?
Sm1 Ge2 Ge1 . . 3_655 127.91(5) ?
Sm1 Ge2 Ge1 . . 57_544 127.91(5) ?
Sm1 Ge2 Ge1 . . 59_555 62.319(12) ?
Sm1 Ge2 Ga2 . . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 . . 5_555 54.60(2) ?
Sm1 Ge2 Ga2 . . 6_555 114.44(5) ?
Sm1 Ge2 Ga2 . . 9_555 54.60(2) ?
Sm1 Ge2 Ga2 . . 10_555 114.44(5) ?
Sm1 Ge2 Ge2 . . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 . . 5_555 54.60(2) ?
Sm1 Ge2 Ge2 . . 6_555 114.44(5) ?
Sm1 Ge2 Ge2 . . 9_555 54.60(2) ?
Sm1 Ge2 Ge2 . . 10_555 114.44(5) ?
Sm1 Ge2 Sm1 50_554 . 51_545 166.55(8) ?
Sm1 Ge2 Sm1 50_554 . 4_555 89.215(12) ?
Sm1 Ge2 Mn1 50_554 . . 83.28(4) ?
Sm1 Ge2 Ga1 50_554 . . 127.91(5) ?
Sm1 Ge2 Ga1 50_554 . 3_655 62.319(12) ?
Sm1 Ge2 Ga1 50_554 . 57_544 127.91(5) ?
Sm1 Ge2 Ga1 50_554 . 59_555 62.319(12) ?
Sm1 Ge2 Ge1 50_554 . . 127.91(5) ?
Sm1 Ge2 Ge1 50_554 . 3_655 62.319(12) ?
Sm1 Ge2 Ge1 50_554 . 57_544 127.91(5) ?
Sm1 Ge2 Ge1 50_554 . 59_555 62.319(12) ?
Sm1 Ge2 Ga2 50_554 . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 50_554 . 5_555 54.60(2) ?
Sm1 Ge2 Ga2 50_554 . 6_555 114.44(5) ?
Sm1 Ge2 Ga2 50_554 . 9_555 114.44(5) ?
Sm1 Ge2 Ga2 50_554 . 10_555 54.60(2) ?
Sm1 Ge2 Ge2 50_554 . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 50_554 . 5_555 54.60(2) ?
Sm1 Ge2 Ge2 50_554 . 6_555 114.44(5) ?
Sm1 Ge2 Ge2 50_554 . 9_555 114.44(5) ?
Sm1 Ge2 Ge2 50_554 . 10_555 54.60(2) ?
Sm1 Ge2 Sm1 51_545 . 4_555 89.215(12) ?
Sm1 Ge2 Mn1 51_545 . . 83.28(4) ?
Sm1 Ge2 Ga1 51_545 . . 62.319(12) ?
Sm1 Ge2 Ga1 51_545 . 3_655 127.91(5) ?
Sm1 Ge2 Ga1 51_545 . 57_544 62.319(12) ?
Sm1 Ge2 Ga1 51_545 . 59_555 127.91(5) ?
Sm1 Ge2 Ge1 51_545 . . 62.319(12) ?
Sm1 Ge2 Ge1 51_545 . 3_655 127.91(5) ?
Sm1 Ge2 Ge1 51_545 . 57_544 62.319(12) ?
Sm1 Ge2 Ge1 51_545 . 59_555 127.91(5) ?
Sm1 Ge2 Ga2 51_545 . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 51_545 . 5_555 114.44(5) ?
Sm1 Ge2 Ga2 51_545 . 6_555 54.60(2) ?
Sm1 Ge2 Ga2 51_545 . 9_555 54.60(2) ?
Sm1 Ge2 Ga2 51_545 . 10_555 114.44(5) ?
Sm1 Ge2 Ge2 51_545 . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 51_545 . 5_555 114.44(5) ?
Sm1 Ge2 Ge2 51_545 . 6_555 54.60(2) ?
Sm1 Ge2 Ge2 51_545 . 9_555 54.60(2) ?
Sm1 Ge2 Ge2 51_545 . 10_555 114.44(5) ?
Sm1 Ge2 Mn1 4_555 . . 83.28(4) ?
Sm1 Ge2 Ga1 4_555 . . 127.91(5) ?
Sm1 Ge2 Ga1 4_555 . 3_655 62.319(12) ?
Sm1 Ge2 Ga1 4_555 . 57_544 62.319(12) ?
Sm1 Ge2 Ga1 4_555 . 59_555 127.91(5) ?
Sm1 Ge2 Ge1 4_555 . . 127.91(5) ?
Sm1 Ge2 Ge1 4_555 . 3_655 62.319(12) ?
Sm1 Ge2 Ge1 4_555 . 57_544 62.319(12) ?
Sm1 Ge2 Ge1 4_555 . 59_555 127.91(5) ?
Sm1 Ge2 Ga2 4_555 . 2_655 96.72(4) ?
Sm1 Ge2 Ga2 4_555 . 5_555 114.44(5) ?
Sm1 Ge2 Ga2 4_555 . 6_555 54.60(2) ?
Sm1 Ge2 Ga2 4_555 . 9_555 114.44(5) ?
Sm1 Ge2 Ga2 4_555 . 10_555 54.60(2) ?
Sm1 Ge2 Ge2 4_555 . 2_655 96.72(4) ?
Sm1 Ge2 Ge2 4_555 . 5_555 114.44(5) ?
Sm1 Ge2 Ge2 4_555 . 6_555 54.60(2) ?
Sm1 Ge2 Ge2 4_555 . 9_555 114.44(5) ?
Sm1 Ge2 Ge2 4_555 . 10_555 54.60(2) ?
Mn1 Ge2 Ga1 . . . 129.80(4) ?
Mn1 Ge2 Ga1 . . 3_655 129.80(4) ?
Mn1 Ge2 Ga1 . . 57_544 129.80(4) ?
Mn1 Ge2 Ga1 . . 59_555 129.80(4) ?
Mn1 Ge2 Ge1 . . . 129.80(4) ?
Mn1 Ge2 Ge1 . . 3_655 129.80(4) ?
Mn1 Ge2 Ge1 . . 57_544 129.80(4) ?
Mn1 Ge2 Ge1 . . 59_555 129.80(4) ?
Mn1 Ge2 Ga2 . . 2_655 180 ?
Mn1 Ge2 Ga2 . . 5_555 45.00(4) ?
Mn1 Ge2 Ga2 . . 6_555 45.00(4) ?
Mn1 Ge2 Ga2 . . 9_555 45.00(4) ?
Mn1 Ge2 Ga2 . . 10_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 2_655 180 ?
Mn1 Ge2 Ge2 . . 5_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 6_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 9_555 45.00(4) ?
Mn1 Ge2 Ge2 . . 10_555 45.00(4) ?
Ga1 Ge2 Ga1 . . 3_655 100.39(7) ?
Ga1 Ge2 Ga1 . . 57_544 65.81(4) ?
Ga1 Ge2 Ga1 . . 59_555 65.81(4) ?
Ga1 Ge2 Ge1 . . . 0 ?
Ga1 Ge2 Ge1 . . 3_655 100.39(7) ?
Ga1 Ge2 Ge1 . . 57_544 65.81(4) ?
Ga1 Ge2 Ge1 . . 59_555 65.81(4) ?
Ga1 Ge2 Ga2 . . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 . . 5_555 116.915(16) ?
Ga1 Ge2 Ga2 . . 6_555 116.915(16) ?
Ga1 Ge2 Ga2 . . 9_555 84.80(3) ?
Ga1 Ge2 Ga2 . . 10_555 174.80(7) ?
Ga1 Ge2 Ge2 . . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 . . 5_555 116.915(16) ?
Ga1 Ge2 Ge2 . . 6_555 116.915(16) ?
Ga1 Ge2 Ge2 . . 9_555 84.80(3) ?
Ga1 Ge2 Ge2 . . 10_555 174.80(7) ?
Ga1 Ge2 Ga1 3_655 . 57_544 65.81(4) ?
Ga1 Ge2 Ga1 3_655 . 59_555 65.81(4) ?
Ga1 Ge2 Ge1 3_655 . . 100.39(7) ?
Ga1 Ge2 Ge1 3_655 . 3_655 0 ?
Ga1 Ge2 Ge1 3_655 . 57_544 65.81(4) ?
Ga1 Ge2 Ge1 3_655 . 59_555 65.81(4) ?
Ga1 Ge2 Ga2 3_655 . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 3_655 . 5_555 116.915(16) ?
Ga1 Ge2 Ga2 3_655 . 6_555 116.915(16) ?
Ga1 Ge2 Ga2 3_655 . 9_555 174.80(7) ?
Ga1 Ge2 Ga2 3_655 . 10_555 84.80(3) ?
Ga1 Ge2 Ge2 3_655 . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 3_655 . 5_555 116.915(16) ?
Ga1 Ge2 Ge2 3_655 . 6_555 116.915(16) ?
Ga1 Ge2 Ge2 3_655 . 9_555 174.80(7) ?
Ga1 Ge2 Ge2 3_655 . 10_555 84.80(3) ?
Ga1 Ge2 Ga1 57_544 . 59_555 100.39(7) ?
Ga1 Ge2 Ge1 57_544 . . 65.81(4) ?
Ga1 Ge2 Ge1 57_544 . 3_655 65.81(4) ?
Ga1 Ge2 Ge1 57_544 . 57_544 0 ?
Ga1 Ge2 Ge1 57_544 . 59_555 100.39(7) ?
Ga1 Ge2 Ga2 57_544 . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 57_544 . 5_555 174.80(7) ?
Ga1 Ge2 Ga2 57_544 . 6_555 84.80(3) ?
Ga1 Ge2 Ga2 57_544 . 9_555 116.915(16) ?
Ga1 Ge2 Ga2 57_544 . 10_555 116.915(16) ?
Ga1 Ge2 Ge2 57_544 . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 57_544 . 5_555 174.80(7) ?
Ga1 Ge2 Ge2 57_544 . 6_555 84.80(3) ?
Ga1 Ge2 Ge2 57_544 . 9_555 116.915(16) ?
Ga1 Ge2 Ge2 57_544 . 10_555 116.915(16) ?
Ga1 Ge2 Ge1 59_555 . . 65.81(4) ?
Ga1 Ge2 Ge1 59_555 . 3_655 65.81(4) ?
Ga1 Ge2 Ge1 59_555 . 57_544 100.39(7) ?
Ga1 Ge2 Ge1 59_555 . 59_555 0 ?
Ga1 Ge2 Ga2 59_555 . 2_655 50.20(4) ?
Ga1 Ge2 Ga2 59_555 . 5_555 84.80(3) ?
Ga1 Ge2 Ga2 59_555 . 6_555 174.80(7) ?
Ga1 Ge2 Ga2 59_555 . 9_555 116.915(16) ?
Ga1 Ge2 Ga2 59_555 . 10_555 116.915(16) ?
Ga1 Ge2 Ge2 59_555 . 2_655 50.20(4) ?
Ga1 Ge2 Ge2 59_555 . 5_555 84.80(3) ?
Ga1 Ge2 Ge2 59_555 . 6_555 174.80(7) ?
Ga1 Ge2 Ge2 59_555 . 9_555 116.915(16) ?
Ga1 Ge2 Ge2 59_555 . 10_555 116.915(16) ?
Ge1 Ge2 Ge1 . . 3_655 100.39(7) ?
Ge1 Ge2 Ge1 . . 57_544 65.81(4) ?
Ge1 Ge2 Ge1 . . 59_555 65.81(4) ?
Ge1 Ge2 Ga2 . . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 . . 5_555 116.915(16) ?
Ge1 Ge2 Ga2 . . 6_555 116.915(16) ?
Ge1 Ge2 Ga2 . . 9_555 84.80(3) ?
Ge1 Ge2 Ga2 . . 10_555 174.80(7) ?
Ge1 Ge2 Ge2 . . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 . . 5_555 116.915(16) ?
Ge1 Ge2 Ge2 . . 6_555 116.915(16) ?
Ge1 Ge2 Ge2 . . 9_555 84.80(3) ?
Ge1 Ge2 Ge2 . . 10_555 174.80(7) ?
Ge1 Ge2 Ge1 3_655 . 57_544 65.81(4) ?
Ge1 Ge2 Ge1 3_655 . 59_555 65.81(4) ?
Ge1 Ge2 Ga2 3_655 . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 3_655 . 5_555 116.915(16) ?
Ge1 Ge2 Ga2 3_655 . 6_555 116.915(16) ?
Ge1 Ge2 Ga2 3_655 . 9_555 174.80(7) ?
Ge1 Ge2 Ga2 3_655 . 10_555 84.80(3) ?
Ge1 Ge2 Ge2 3_655 . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 3_655 . 5_555 116.915(16) ?
Ge1 Ge2 Ge2 3_655 . 6_555 116.915(16) ?
Ge1 Ge2 Ge2 3_655 . 9_555 174.80(7) ?
Ge1 Ge2 Ge2 3_655 . 10_555 84.80(3) ?
Ge1 Ge2 Ge1 57_544 . 59_555 100.39(7) ?
Ge1 Ge2 Ga2 57_544 . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 57_544 . 5_555 174.80(7) ?
Ge1 Ge2 Ga2 57_544 . 6_555 84.80(3) ?
Ge1 Ge2 Ga2 57_544 . 9_555 116.915(16) ?
Ge1 Ge2 Ga2 57_544 . 10_555 116.915(16) ?
Ge1 Ge2 Ge2 57_544 . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 57_544 . 5_555 174.80(7) ?
Ge1 Ge2 Ge2 57_544 . 6_555 84.80(3) ?
Ge1 Ge2 Ge2 57_544 . 9_555 116.915(16) ?
Ge1 Ge2 Ge2 57_544 . 10_555 116.915(16) ?
Ge1 Ge2 Ga2 59_555 . 2_655 50.20(4) ?
Ge1 Ge2 Ga2 59_555 . 5_555 84.80(3) ?
Ge1 Ge2 Ga2 59_555 . 6_555 174.80(7) ?
Ge1 Ge2 Ga2 59_555 . 9_555 116.915(16) ?
Ge1 Ge2 Ga2 59_555 . 10_555 116.915(16) ?
Ge1 Ge2 Ge2 59_555 . 2_655 50.20(4) ?
Ge1 Ge2 Ge2 59_555 . 5_555 84.80(3) ?
Ge1 Ge2 Ge2 59_555 . 6_555 174.80(7) ?
Ge1 Ge2 Ge2 59_555 . 9_555 116.915(16) ?
Ge1 Ge2 Ge2 59_555 . 10_555 116.915(16) ?
Ga2 Ge2 Ga2 2_655 . 5_555 135.00(4) ?
Ga2 Ge2 Ga2 2_655 . 6_555 135.00(4) ?
Ga2 Ge2 Ga2 2_655 . 9_555 135.00(4) ?
Ga2 Ge2 Ga2 2_655 . 10_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 2_655 0 ?
Ga2 Ge2 Ge2 2_655 . 5_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 6_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 9_555 135.00(4) ?
Ga2 Ge2 Ge2 2_655 . 10_555 135.00(4) ?
Ga2 Ge2 Ga2 5_555 . 6_555 90.00(6) ?
Ga2 Ge2 Ga2 5_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ga2 5_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ge2 5_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 5_555 . 5_555 0 ?
Ga2 Ge2 Ge2 5_555 . 6_555 90.00(6) ?
Ga2 Ge2 Ge2 5_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ge2 5_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ga2 6_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ga2 6_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ge2 6_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 6_555 . 5_555 90.00(6) ?
Ga2 Ge2 Ge2 6_555 . 6_555 0 ?
Ga2 Ge2 Ge2 6_555 . 9_555 60.00(4) ?
Ga2 Ge2 Ge2 6_555 . 10_555 60.00(4) ?
Ga2 Ge2 Ga2 9_555 . 10_555 90.00(6) ?
Ga2 Ge2 Ge2 9_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 9_555 . 5_555 60.00(4) ?
Ga2 Ge2 Ge2 9_555 . 6_555 60.00(4) ?
Ga2 Ge2 Ge2 9_555 . 9_555 0 ?
Ga2 Ge2 Ge2 9_555 . 10_555 90.00(6) ?
Ga2 Ge2 Ge2 10_555 . 2_655 135.00(4) ?
Ga2 Ge2 Ge2 10_555 . 5_555 60.00(4) ?
Ga2 Ge2 Ge2 10_555 . 6_555 60.00(4) ?
Ga2 Ge2 Ge2 10_555 . 9_555 90.00(6) ?
Ga2 Ge2 Ge2 10_555 . 10_555 0 ?
Ge2 Ge2 Ge2 2_655 . 5_555 135.00(4) ?
Ge2 Ge2 Ge2 2_655 . 6_555 135.00(4) ?
Ge2 Ge2 Ge2 2_655 . 9_555 135.00(4) ?
Ge2 Ge2 Ge2 2_655 . 10_555 135.00(4) ?
Ge2 Ge2 Ge2 5_555 . 6_555 90.00(6) ?
Ge2 Ge2 Ge2 5_555 . 9_555 60.00(4) ?
Ge2 Ge2 Ge2 5_555 . 10_555 60.00(4) ?
Ge2 Ge2 Ge2 6_555 . 9_555 60.00(4) ?
Ge2 Ge2 Ge2 6_555 . 10_555 60.00(4) ?
Ge2 Ge2 Ge2 9_555 . 10_555 90.00(6) ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
? ? ? ? ? ? ? ? ? ?

loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_site_symmetry_D
_geom_hbond_site_symmetry_H
_geom_hbond_site_symmetry_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_publ_flag
? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 11. STRUCTURE-FACTOR LIST


_exptl_crystal_recrystallization_method 'From the Melt'
